Tensor Properties of Solids Phenomenological Development of the Tensor Properties of Crystals
Copyright © 2008 by Morg...

Author:
Richard F. Tinder

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Tensor Properties of Solids Phenomenological Development of the Tensor Properties of Crystals

Copyright © 2008 by Morgan & Claypool All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means—electronic, mechanical, photocopy, recording, or any other except for brief quotations in printed reviews, without the prior permission of the publisher. Tensor Properties of Solids: Phenomenological Development of the Tensor Properties of Crystals Richard F. Tinder www.morganclaypool.com ISBN: 1598293486

paperback

ISBN: 9781598293487 paperback ISBN: 1598293494

ebook

ISBN: 9781598293494 ebook DOI: 10.2200/S00057ED1V01Y200712ENG04 DOI: 10.2200/S00058ED1V01Y200712ENG05 A Publication in the Morgan & Claypool Publishers series SYNTHESIS LECTURES ON ENGINEERING # 4 Lecture #4 Series ISSN ISSN 1939-5221

print

ISSN 1939-523X

electronic

Tensor Properties of Solids Phenomenological Development of the Tensor Properties of Crystals Richard F. Tinder Washington State University

SYNTHESIS LECTURES ON ENGINEERING # 4

M &C

Mor gan

& Cl aypool

Publishers

iv

ABSTRACT Tensor Properties of Solids presents the phenomenological development of solid state properties represented as matter tensors in two parts: Part I on equilibrium tensor properties and Part II on transport tensor properties. Part I begins with an introduction to tensor notation, transformations, algebra, and calculus together with the matrix representations. Crystallography, as it relates to tensor properties of crystals, completes the background treatment. A generalized treatment of solid-state equilibrium thermodynamics leads to the systematic correlation of equilibrium tensor properties. This is followed by developments covering first-, second-, third-, and higher-order tensor effects. Included are the generalized compliance and rigidity matrices for first-order tensor properties, Maxwell relations, effect of measurement conditions, and the dependent coupled effects and use of interaction diagrams. Part I concludes with the second- and higher-order effects, including numerous optical tensor properties. Part II presents the driving forces and fluxes for the well-known proper conductivities. An introduction to irreversible thermodynamics includes the concepts of microscopic reversibility, Onsager’s reciprocity principle, entropy density production, and the proper choice of the transport parameters. This is followed by the force–flux equations for electronic charge and heat flow and the relationships between the proper conductivities and phenomenological coefficients. The thermoelectric effects in solids are discussed and extended to the piezothermoelectric and piezoresistance tensor effects. The subjects of thermomagnetic, galvanomagnetic, and thermogalvanomagnetic effects are developed together with other higher-order magnetotransport property tensors. A glossary of terms, expressions and symbols are provided at the end of the text, and endof-chapter problems are provided on request. Endnotes provide the necessary references for further reading.

Keywords tensor properties, crystals, thermodynamics, equilibrium, transport

Preface An exhaustive in-depth treatment of the tensor properties of crystals would be a daunting task and would require several books on the subject, each of which would be of considerable length. This would require each property, experimentally known to exist or predicted by theory, to be developed from first principles at the atomic or quantum mechanical level. This is not what this text is about. We purport to develop the physical properties of solids (actually crystals) from the thermodynamic and tensorial points of view, which, if done correctly, provide a valuable introduction to a multitude of physical properties. The phenomenological development used in this text permits a thermodynamic basis for property definitions that is inviolate or nearly so. However, it is correct to say that many of the matter tensor properties defined in this way may not have been studied previously to establish their relative importance. This text is designed to be used as a one-semester or two-quarter course in the subject matter. It also serves as a valuable source of information for practicing engineers and scientists in related fields. Although the text provides the necessary background in tensor analysis, the readership is expected to have some knowledge of calculus and matrix algebra. An understanding of basic vector analysis is also deemed helpful. The necessary information regarding crystallography and point groups as they relate to this text is provided as background material in the text. The contents of this text are based on the author’s notes used for a graduate course taught over several years at Washington State University to graduate students and second-semester seniors in the areas of material science, electrical and mechanical engineering, physics, and chemical physics. An instructor of a course in this subject matter is provided ample opportunity to limit, alter, or expound on any part of the text material as needed to satisfy the course description and needs of the students. Extensive glossaries of terms, expressions, and symbols at the end of the text aid in the learning process. As with any text dealing with complex subject matter, there will undoubtedly be found typos and errors that were overlooked by the author. Hopefully, these have been kept to a minimum. However, should any be found by the instructor or readers, the author would appreciate knowing of them so that corrections can be made. The author may be contacted at the following e-mail address: [email protected]

vii

Acknowledgments The author is deeply indebted to the many senior and graduate students for their countless questions, comments, arguments, and suggestions given during the many years that the contents of this text were used as notes in the conduct of the author’s graduate course taught at Washington State University. As most professors know, students can and do provide the most candid and critical assessments of material presented in a given course. The author also acknowledges the suggestions and contributions of Prof. Elias (Lee) Stefanakos to the subject matter presented in this text, in particular, to the optical effects presented in Chapter 7. Dr. Stefanakos is director of the Clean Energy Research Center at the University of South Florida. Gratefully acknowledged is the encouragement and helpful suggestions offered by Joel Claypool, publisher of Morgan & Claypool Publishers. Finally and most importantly, the author acknowledges the support, care, and understanding of his loving wife, his best friend and confidante, Gloria.

ix

Contents I Equilibrium Tensor Properties of Solids ...............................................................1 1. Introduction ........................................................................................................ 3 1.1 Definition of a Tensor Property . ............................................................. 3 1.2 Concepts of Equilibrium and Reversibility ............................................. 4 1.3 Interaction Diagrams and First-Order Equilibrium Property Nomenclature and Representation........................................................... 5 1.4 Interaction Diagram for the First-Order Nonequilibrium Tensor Properties ................................................................................................ 9 2. Introduction to Tensor Notation, Tensor Transformations, Tensor Calculus, and Matrix Representation ................................................................................ 13 2.1 Introduction to Tensor and Matrix Notation ........................................ 13 2.2 Transformation of Tensors . ................................................................... 14 2.2.1 Transformation of Scalars .......................................................... 15 2.2.2 Transformation of Vectors ......................................................... 15 2.2.3 Transformation of Second-Rank Tensors .................................. 16 2.2.4 Symmetrical and Antisymmetrical Second-Rank Tensors ........ 17 2.2.5 Quadratic Transformation Forms .............................................. 19 2.2.6 Transformation of Third-Rank Tensors . ................................... 20 2.2.7 Transformation of Fourth-Rank Tensors ................................... 22 2.2.8 Summary of Tensor Transformation Laws ................................ 25 2.3 Introduction to Tensor Algebra.............................................................. 25 2.3.1 Tensor Addition . ....................................................................... 26 2.3.2 Tensor Multiplication................................................................. 26 2.3.3 Outer Product . .......................................................................... 27 2.3.4 Tensor Contraction . .................................................................. 27 2.4 Axial Tensors.......................................................................................... 29 2.5 Taylor’s Series Expansion and the Tensor Differentiation Laws ........... 30 2.6 Tensor Fields and Tensor Operators . .................................................... 31 2.6.1 Gradient of a Tensor Field.......................................................... 32

Tensor Properties of Solids

3.

4.

5.

2.6.2 Divergence of a Tensor Field...................................................... 33 2.6.3 Kronecker Delta, Permutation Tensor, Vector Cross Product, and Tensorial Contraction.......................................................... 33 Crystal Systems, Symmetry Elements, and Symmetry Transformations . ....................................................................................... 37 3.1 Introduction .......................................................................................... 37 3.2 Macroscopic Crystal Symmetry and Symmetry Transformations.......... 38 3.2.1 Permissible Rotations................................................................. 38 3.2.2 Center of Symmetry .................................................................. 38 3.3 Space Lattices, Unit Cells, Crystallographic Planes, and Directions—Miller Indices . .................................................................. 41 3.4 The Macroscopic Symmetry of Crystals and the 32 Conventional Point Groups.......................................................................................... 46 3.5 Neumann’s Principle and Its Application to Tensor Properties.............. 46 3.6 Application of Neumann’s Principle to Symmetrical Second-Rank Property Tensors . .................................................................................. 52 3.7 Effect of Neumann’s Principle on the 11 Centrosymmetrical Crystal Classes . ..................................................................................... 56 3.8 Longitudinal and Transverse Effects for Symmetrical Second-Rank Property Tensors . .................................................................................. 57 Generalized Thermostatics and the Systematic Correlation of Physical Properties ............................................................................................ 61 4.1 Energy Representations and the Criteria for Thermodynamic Equilibrium............................................................................................ 61 4.1.1 Energy Density Representation . ............................................... 64 4.2 Thermodynamic Definition of Parameters ............................................ 65 4.3 Generalized Compliance and Rigidity Matrices ................................... 68 4.4 Symmetry of the General Compliance and Rigidity Matrices............... 71 4.5 Systematic Enumeration and Correlation of First-Order Tensor Properties—Generalized Maxwell Relations . ....................................... 74 4.5.1 Principal Effects......................................................................... 74 4.5.2 Independent Coupled Effects . .................................................. 75 4.6 Effect of Measurement Conditions on the First-Order Tensor Properties................................................................ 78 The Dependent Coupled Effects and the Interrelationships Between First-Order Tensor Properties—Use of Interaction Diagrams........................... 85 5.1 The Dependent Coupled Effects .......................................................... 85

Tensor Properties of Solids xi

6.

7.

II

5.2 Interrelationship Between First-Order Properties—Use of Interaction Diagrams . ........................................................................... 87 5.3 The Grüneisen Tensor . ......................................................................... 90 Third- and Fourth-Rank Tensor Properties—Symmetry Considerations.......... 95 6.1 Direct and Converse Piezoelectric Effects . ........................................... 95 6.1.1 Direct Piezoelectric Effect . ....................................................... 95 6.1.2 Converse Piezoelectric Effect .................................................... 97 6.1.3 Crystal Symmetry Considerations . ........................................... 99 6.1.4 Brute-Force Method for the Trigonal and Hexagonal Classes—The Piezoelectric Moduli . ....................................... 100 6.1.5 Longitudinal Piezoelectric Effect ............................................ 106 6.1.6 Transverse Piezoelectric Effect................................................. 108 6.2 Elasticity . ............................................................................................ 108 6.2.1 Hooke’s Law . .......................................................................... 109 6.2.2 Bulk Elastic Behavior .............................................................. 110 6.2.3 Transformation Laws . ............................................................. 112 6.2.4 Elastic Strain Energy Density.................................................. 113 6.2.5 Effect of Crystal Symmetry . ................................................... 113 6.2.6 Homogeneous Elastically Isotropic Solids .............................. 118 6.2.7 Young’s Modulus in a Particular Direction............................... 120 6.2.8 Shear Modulus and Poisson’s Ratio ......................................... 121 Second- and Higher-Order Effects—Symmetry Considerations ................... 123 7.1 Electrostriction and Morphic Effects................................................... 123 7.1.1 Symmetry and Transformation Considerations of Fourth-Rank Tensors . ............................................................. 124 7.2 Generalized Development of the Second-Order Effects . ................... 125 7.3 Phenomenological Development of the Optical Effects...................... 129 7.3.1 Electro-Optical Effects ........................................................... 132 7.3.2 Piezo-Optical and Elasto-Optical Effects . ............................. 134 7.3.3 Piezo-Optical Effect in Cubic Crystals Under Uniaxial Tension ...................................................................... 136 7.3.4 Magneto-Optical (Cotton–Mouton and Faraday) Effects....... 139 7.3.5 Thermo-Optical Effects........................................................... 142

Transport Properties of Solids .......................................................................... 145 8. Introduction to Transport Properties and the Thermodynamics of Irreversible Processes........................................................................................ 147

xii Tensor Properties of Solids

8.1 8.2 8.3 8.4

Gradients, Current Densities, and the Conductivities . ....................... 147 Conjugate or Proper Conductivities..................................................... 149 Cross or Interference Conductivities.................................................... 149 Markoffian Systems, Microscopic Reversibility, and Onsager’s Reciprocity Principle............................................................................ 150 8.4.1 Markoff Processes . .................................................................. 150 8.4.2 Principle of Microscopic Reversibility...................................... 151 8.4.3 Onsager’s Reciprocity Principle................................................ 151 8.4.4 Entropy Production.................................................................. 152 8.5 Proper Choice of Parameters................................................................ 152 8.5.1 Further Restrictions on the Phenomenological Coefficients.... 155 8.6 Flow of Electronic Charge and Heat—The Conductivities................. 156 9. Thermoelectric, Piezothermoelectric, and Diffusive Effects in Solids............. 159 9.1 Seebeck Effect (Thermocouple Effect)................................................ 159 9.2 Peltier Effect (Thermoelectric Heater/Refrigerator Effect)................. 162 9.3 Thomson Effect .................................................................................. 163 9.4 Piezothermoelectric and Elastothermoelectric Effects......................... 166 9.5 Piezoresistance Effect (Strain Gauge Effect)....................................... 169 9.6 Electrodiffusive and Thermodiffusive Effects ..................................... 171 9.6.1 Multiple Diffusing Species....................................................... 171 10. Effect of Magnetic Field on the Transport Properties...................................... 175 10.1 First-Order Thermomagnetic and Galvanomagnetic Effects in an Isotropic Plane . .......................................................................... 175 10.2 Definitions of the Thermomagnetic and Galvanomagnetic Effects in an Isotropic x,y Plane ...................................................................... 178 10.3 Second-Order Effects in a Magnetic Field—The Hall and Magnetoresistance Tensors .................................................................. 181 10.4 First-Order Thermogalvanomagnetic Effects in Isotropic Conductive Media ............................................................................... 184 10.5 Other Higher-Order Magnetotransport Tensor Properties in Anisotropic Media . ............................................................................. 186 Appendices .............................................................................................................. 189 Magnetic Tensor Properties, Magnetic Crystals, and the Combined Space–Time Transformations..................................................................................... 189 A.1 Conditions for Magnetocrystalline Class Application...................................... 189 A.2 Combined Space-Time Transformations......................................................... 190

Tensor Properties of Solids xiii

A.3 Application of Neumann’s Principle to Magnetocrystalline Transformations.... 192 A.4 The Magnetic Point Groups ........................................................................... 198 Endnotes ................................................................................................................. 201 Glossary .................................................................................................................. 205 Terms and Expressions . ............................................................................................ 205 Symbols and Abbreviations . ..................................................................................... 223 Greek Symbols .......................................................................................................... 227 Author Biography..................................................................................................... 229 Index ....................................................................................................................... 231

PA RT I

Equilibrium Tensor Properties of Solids

chapter 1

Introduction 1.1 DEFINITION OF A TENSOR PROPERTY A property, as defined in this text, is a coefficient that linearly relates an intensive (or cause) parameter to an extensive (or effect) parameter. When the intensive and extensive parameters are tensor variables, the property is also a tensor quantity. One way of expressing this is

Tensor

Coefficient Parameter

Parameter

= Property

Tensor

Cause

Tensor

Effect

(1.1)

or its inverse, which places the inverse of the tensor property coefficient on the left-hand side of the equation. The particular tensor property will have a definite physical significance and will be represented by a fixed number of components depending on the nature and tensor character of the intensive and extensive parameters that it relates. One physical significance of the property coefficient may be given as the rate of change of one parameter with respect to the other as implied by Eq. (1.1). One or both of the parameters that define the property coefficient will usually be a field tensor such as stress or strain, electric or magnetic field strength, or temperature (a scalar). The extent to which a property of a crystal exists with respect to the application of a given field depends on the electronic and subatomic structure of the atoms and on the manner in which they are arranged in the lattice. Shown in Table 1.1 are four typical examples of properties of crystals that are directly related by cause and effect tensor parameter. Here, the pyroelectric coefficient pi is a vector–scalar tensor property, hence, a vector, that relates the change in polarization δPi with a change in temperature δT. The thermal expansion coefficient aij is a tensor–scalar tensor property of tensor rank 2 that relates a change in strain εij with a change in temperature δT. The piezoelectric coefficient dijk is a vector– tensor property of tensor rank 3 that relates the polarization Pi to the stress tensor σjk. Finally, the elastic compliance coefficient sijkl is a tensor–tensor property of rank 4 that relates the stress σij to

tensor properties of solids

TABLE 1.1: Typical examples of properties of crystals that are directly related by cause and effect tensor parameters Effect tensor parameter

Cause tensor parameter

Property name

Tensor equation

Tensor rank of coefficient

δPi

δT

Pyroelectricity

δPi = piδT

First (pi)

δεij

δT

Thermal expansion

δεij = αijδT

Second (αij)

Pi

σij

Piezoelectricity

Pi = dijkσjk

Third (dijk)

εij

σkl

Elasticity

εij = sijklσkl

Fourth (sijkl)

Shown are the tensor parameters, property to which they are applicable, and the tensor equations and tensor rank for the property coefficients.

the strain εkl (Hooke’s law). Thus, it is seen that the tensor rank of a property coefficient is the sum of the tensor ranks of the parameters that it relates. Note that all tensor property coefficients given in Table 1.1 are examples of equilibrium properties. A well-known example of a nonequilibrium or transport property is resistivity ρij , a second-rank tensor that relates electric field strength Ei to the current density Jj according to Ei = ρij Jj , which, of course, is the tensor representation of Ohm’s law. The distinction between equilibrium and nonequilibrium transport properties will be made clear in the section that follows, together with Parts I and II of this text.

1.2

CONCEPTS OF EQUILIBRIUM AND REVERSIBILITY

The properties of interest to Part I of this text are those that can be represented by tensors and described with reference to equilibrium states and thermodynamically reversible changes in crystals. Consider a thought experiment on any closed system (e.g., a crystal) in which all imaginable physically measurable quantities are accurately recorded as a function of time. If it is found that all processes, defined by the physically measurable quantities, are macroscopically time independent, thermodynamic equilibrium is said to exist. This requires, for example, the absence of the transport of heat (or entropy), charge, and mass and that all parts of the system be mechanically in static equilibrium. Thus, thermodynamic equilibrium prevails if the system under consideration is in thermal, electrical, magnetic, mechanical, and chemical equilibrium. Thermodynamic equilibrium does permit microscopic fluctuations to occur on the atomic level as long as they are random and do not produce measurable time-dependent changes in the physical state of the system.

introduction

Properties of crystals that represent time-independent processes are called equilibrium properties. Such properties can adequately be described phenomenologically by using equilibrium thermodynamics, that is, thermostatics. Properties that represent time-dependent or spontaneous processes are called nonequilibrium or transport properties. Such properties can be described only by use of the thermodynamics of irreversible processes, a subject that is covered in Part II of this text. The concept of thermodynamic reversibility is intimately connected with the concept of equilibrium. The term reversible applies to a process within a system that has been displaced from equilibrium only to an infinitesimal extent. Therefore, a reversible process may be defined as the hypothetical passage of the system through a series of equilibrium states so close together that they are nearly indistinguishable. Such a process is reversed by an appropriate infinitesimal change of the physical conditions imposed on the system. Actually, no ongoing process is reversible in the strict sense of the word. However, if the conditions to be imposed on the system are applied infinitesimally fast, then, within experimental error, the process may be considered reversible. A reversible process is usually considered to be a linear process over an infinitesimal change in cause and effect parameters. However, a reversible process may be nonlinear, provided that the infinitesimal changes in the system are restored reversibly. In the development of the equilibrium properties, we will assume that the reversible processes are linear and that thermodynamic equilibrium is established at each point in an infinitesimal change.

1.3

INTERACTION DIAGRAMS AND FIRST-ORDER EQUILIBRIUM PROPERTY NOMENCLATURE AND REPRESENTATION

It is appropriate that we now preview the spectrum of first-order equilibrium properties about which we shall later discuss in more detail. To do this, it is necessary to define the conjugate parameters from which the general first-order interaction diagram can be constructed. The four pairs of conjugate 8 parameters are the following: (T,S), (E, P), (B, M ), and (σ,ε), which give rise to ∑n=1 (n - 1) = 28 first-order properties including 4 principal effects and 24 coupled effects. The conjugate parameter pairs are (temperature, entropy), (electric field strength, polarization), (magnetic flux density, magnetization), and (stress, strain), respectively. The conjugate pairs (E, P) and (B, M) are chosen in preference to others for the sake of consistency, with the thermodynamic developments yet to come. Shown in Figure 1.1 is the generalized interaction diagram for the first-order equilibrium properties where the names, symbols, and tensor rank (in parentheses) are given for each of the eight parameters. The four principal effects are represented by horizontal lines (i.e., between conjugate parameters), whereas the coupled effects are given by the nonhorizontal lines. The vertical lines represent dependent coupled properties relating any two intensive parameters (or any two extensive parameters). The set of 16 “compliance” effects are shown by arrows that point to the dependent variables, which,

tensor properties of solids

in this case, are the extensive parameters. Extensive parameters are those that depend on the amount of material of the solid phase system. Parameters that are independent of the amount of material in the solid phase are called intensive parameters and are associated only with the external conditions (fields) imposed on the system. Thus, the arrows in Figure 1.1 are drawn from the intensive (independent) parameters to the extensive (dependent) parameters. Reversal of the arrows defines the set of 16 “rigidity” effects that will later be shown as the collective inverse of the “compliance” effects. For the convenience of the reader, the 16 compliance equilibrium properties are presented in Table 1.2 in the order of increasing tensor rank, first for the principle effects and then for the

Intensive Parameters

T

T emperature (0)

Extensive Parameters

S

Entopy (0)

E

P

Electric Field (1)

Polarization (1)

B

M

Magnetic Flux (1)

Magnetization (1)

σ

Stress (2)

ε

Strain (2)

FIGURE 1.1: Generalized interaction diagram for the 28 first-order effects showing the names, symbols, and tensor rank (in parentheses) for each of the 8 parameters.

introduction

TABLE 1.2: The set of 16 compliance effects and their associated parameter pairs showing the 4 principal effects and 12 coupled effects as listed in the order of increasing tensor rank Parameter pair

Associated property

Tensor rank

Principal effects (S, T )

Heat capacity

0

(P, E)

Dielectric susceptibility

2

(M, B)

Magnetic susceptibility

2

(ε, σ)

Elasticity

4

Interaction (coupled) effects (S, E)

Pyroelectric effect

1

(P, T )

Converse pyroelectric effect

1

(S, B)

Pyromagnetic effect (magnetocaloric effect)

1

(M, T )

Converse pyromagnetic effect

1

(S, σ)

Piezocaloric effect

2

(ε, T )

Thermal expansion (converse piezocaloric effect)

2

(P, B)

Magnetoelectric susceptibility

2

(M, E)

Converse magnetoelectric susceptibility

2

(P, σ)

Direct piezoelectric effect

3

(ε , E)

Converse piezoelectric effect (first-order electrostriction)

3

(M, σ)

Direct piezomagnetic effect

3

(ε, B)

Converse piezomagnetic effect (first-order magnetostriction)

3

tensor properties of solids

T

Temperature (0)

Th erm al

Thermal Stress, – t (2)

ca zo e i P

lo

ric

α ct, e f Ef

Entopy (0)

(2)

Ex pa nsi o

σ

Stress (2)

S

Heat Capacity, C/T (0)

n, α

Heat of Deformation, t (2) (2)

ε

Elasticity, s (4)

Strain (2)

FIGURE 1.2: Interaction diagram representing the thermal, thermoelastic, and elastic effects. The arrows point to the dependent variable.

interaction (coupled) effects. Note that each parameter pair is given in (extensive, intensive) notation form. Other equilibrium properties, not mentioned above, include those in Figure 1.1 for which no one-way arrows are shown. Some of these are of little or no interest to the developments in this text. Most of those equilibrium properties that remain are higher-order effects that can usually be defined in Taylor series expansions of the appropriate parameters. The higher-order effects are usually of high tensor rank and are, accordingly, more complicated. These include such effects as electrostriction, magnetostriction, and a variety of optical effects. Many of these effects will be considered in later chapters. To provide a little more background detail, we will next consider an interaction diagram associated with the thermal and mechanical variables, that is, one that represents the thermal, thermoelastic, and elastic effects. This interaction diagram is shown in Figure 1.2 where the arrows again point toward the dependent variables. Noting from Figure 1.2 that both the stress and temperature fields contribute to an elastic strain, we write in differential form,

dεij = siTjkl dσkl + a σij dT

(1.2)

εij = siTjkl σkl + a σij ∆T .

(1.3)

or in integrated form

introduction

In these equations, sTijkl = (∂εij / ∂σkl)T is the isothermal (temperature independent) elastic compliance, and α σij = (∂εij / ∂T )σ is the isopiestic (stress invariant) coefficient of thermal expansion. The fourthrank tensor property sTijkl represents a principal effect (elasticity) because it relates the conjugate parameters σ and ε. The second-rank tensor property α σij , on the other hand, represents a coupled effect (thermal expansion) because it relates the cross parameters T and ε at constant stress, σ. By similar reasoning, one notes from Figure 1.2 that a positive increase in stress as well as an increase in temperature and strain produces an increase in the entropy of a crystal. In differential form, we write

dS = αTij dσij + (C σ / T )dT

(1.4)

∆S = αTij σij + (C σ / T )∆T .

(1.5)

or in integrated form

Here, αTij = (∂S / ∂σij )T is the isothermal piezocaloric coefficient, equal to the coefficient of thermal expansion measured under constant stress, and C σ = T (∂S / ∂T )σ is the isopiestic (constant stress) heat capacity. The fact that (∂S / ∂σij )T = (∂εij / ∂T )σ is a consequence of thermodynamic arguments to be discussed in detail later. The properties just described have been defined in such a way that only the intensive parameters are held constant. Other coupled effects result from an association of the thermal and mechanical variables but which will have both intensive and extensive parameters held constant. Suppose it is desirable to equate the isothermal elastocaloric (heat of deformation) with the isometric thermal stress coefficient as depicted by the vertical arrows in Figure 1.2. When this is done, we write

(∂S / ∂εij )T = − (∂σij / ∂T )ε = tij ,

(1.6)

a result that follows from developments that will be presented later. Note that the isometric thermal stress coefficient describes the negative or compressive stress produced when a mechanically constrained crystal is heated. Equation (1.6) is one of many Maxwell relations to be discussed later in Chapters 4 and 5.

1.4

INTERACTION DIAGRAM FOR THE FIRST-ORDER NONEQUILIBRIUM TENSOR PROPERTIES

There is another important group of properties common to crystals that deal with thermodynamically irreversible phenomena. These are the transport properties that involve the flow of charge, heat, and mass. A complete understanding of these effects is possible only through the use of

10 tensor properties of solids

fluctuation theory, the principle of microscopic reversibility, and the Onsager reciprocal relations, that is, through the use of the thermodynamics of irreversible processes. In contrast, the interactions between equilibrium properties are easily deduced by using standard thermodynamic (thermostatic) arguments. Although it is not commonly done, the first-order transport properties may also be represented by interaction diagrams. To do this, it must be stated clearly that the use of such diagrams in no way implies thermodynamic reversibility in the same sense as for the equilibrium properties, but rather implies microscopic reversibility as used in fluctuation theory. To construct a useful interaction diagram for first-order nonequilibrium properties, three pairs of conjugate parameters that are physically measurable are used. These pairs are the three current densities (fluxes) and their conjugate driving forces representing the flow of current ( J n, ∇φ E ), heat ( J q, ∇φT ), and mass ( J m, ∇φ C ). Shown in Figure 1.3 is the interaction diagram for the first-order transport properties that positions the temperature gradient (∇φT ), electric potential gradient (∇φ E ), and concentration gradient (∇φC )

=0 (J n

KmE

e siv fu dif tro ec we Po r

oe l ec tri cP ow er

El

Kq E

Electrical Cond., KnE

)

∇φ E

m

(J

Jn

Th

erm

) =0

o al C m r The

∇φ T

KnT

ctiv ndu

ity,

qT

K

KmT

Jq

Jm

KnC

D if fusi vi KqC

Thermodiffusive Power (J m = 0)

ty,

K mC

∇φ C

FIGURE 1.3: Interaction diagram for the first-order nonequilibrium (transport) properties showing the 9 conductivities and 3 power coefficients, all 12 of which are second-rank tensor properties.

introduction 11

in clockwise sequence on the outside of the interaction triangle. The heat current ( J q), electron (or ion) current ( J n), and mass current densities ( J m) are placed inside the gradient triangle nearest their respective conjugate parameters. All transport parameters, it will be noted, are tensors of 6 rank 1, that is, vectors. This diagram represents ∑n =1 (n - 1) = 15 relationships, which include nine conductivities each relating a flux to a gradient, three “power” coefficients each relating one gradient to another, and three relationships between the current densities. The 12 conductivities and power coefficients are each second-rank tensors. The relationships between fluxes are interpreted, for example, as the heat or entropy associated with the flow of charge for the ( Jq , J n) relationship and similarly for the two other pairs. These current density relationships have not been considered as tensor properties. There exist other transport properties not included in the interaction diagram of Figure 1.3. These arise primarily from the application of magnetic and/or stress fields applied to crystals exhibiting one or more of the properties represented in the J − ∇φ interaction diagram. This leads to important thermomagnetic and galvanomagnetic, piezoresistance, piezothermoelectric, and the piezogalvanomagnetic effects and to other higher-order transport properties. The phenomenological developments of the transport properties in crystalline solids are the topics covered in Part II of this text. These properties will be discussed in some depth based on the basic principles of irreversible thermodynamics. The treatment is, by its nature, more difficult than that presented in Part I, dealing with the phenomenological developments of the equilibrium tensor properties—the basic principle of irreversible thermodynamics are statistical in nature, dealing mainly with fluctuation theory. Recognizing this, special care is taken to present the more complex developments in a manner that minimizes this difficulty. • • • •

13

chapter 2

Introduction to Tensor Notation, Tensor Transformations, Tensor Calculus, and Matrix Representation 2.1

INTRODUCTION TO TENSOR AND MATRIX NOTATION

To help understand the tensor notation used in Section 1.3 and in subsequent sections, we provide here an introduction to tensor analysis in the use of scalars, vectors, and tensors of second- and higherorder rank. To define explicitly the various tensor operations involved in a comprehensive treatment of the physical properties of solids, reference must be made to a coordinate system. This leads naturally to subscript notation and matrix forms, which will be used exclusively throughout this book. Tensors are known to be abstract quantities that are used in the study of many physical laws of nature. There are different kinds of tensors (e.g., polar, axial, magnetic, axial–magnetic), and each kind is classified by its tensor rank, r. In general, a tensor is specified by n(r) components, where n is the number of dimensions of space being used. In three-dimensional Euclidean space, the number of components of a given tensor is 3(r). We will be concerned only with orthogonal Euclidean coordinates (Cartesian coordinates) and with Cartesian tensors, thereby allowing the distinction between covariant and contravariant tensors laws to disappear, and hence of no concern to us. A tensor of rank r that is specified by 3(r) components in rectangular Cartesian coordinates is given in tensor subscript notation by Tijk, that is, by r number of subscripts each taking on values 1, 2, 3 corresponding to three-dimensional Cartesian space. The components of these tensors can be represented by a matrix of symbols arranged in rows and columns. Consider, for example, a second- rank tensor Tij relating two vectors pi and qj, with components p1, p2, and p3, and q1, q2, and q3, respectively. The tensor equation becomes

pi = Tij qj

(i, j = 1,2,3),

(2.1)

where summation from 1 to 3 with respect to the repeating (dummy) suffix, j, is understood. This is called the Einstein summation convention, which allows the summation sign Σ to be dropped. Expanding Eq. (2.1), as required by summation, gives the following three equations for pi:

14 tensor properties of solids

p1 = T11q1 + T12q2 + T13q3 p2 = T21q1 + T22q2 + T23q3 p3 = T31q1 + T32q2 + T33q3

(2.2)

which can be represented in matrix form as

p1 T11 T12 T13 q1 p2 = T21 T22 T23 . q2 p3 T31 T32 T33 q3

(2.3)

or simply in matrix symbolic notation p = Tq .

(2.4)

Vectors may be represented either by a (3 × 1 = rows × column) column matrix as in Eq. (2.3) or as a (1 × 3) row matrix

p1 p2 or [ p1 p2 p3] , p3

depending on the type of matrix operation to be performed. The nine components of a secondrank tensor, Tij, may be represented by a (3 × 3) matrix as in Eq. (2.3) or as either a (9 × 1) column matrix or (1 × 9) row matrix, as will be demonstrated later. In any case, it must be understood that a matrix is nothing more than an array of symbols or numbers arranged in rows and columns. The matrix array has no physical meaning in itself but may represent a tensor that does have physical significance.

2.2

TRANSFORMATION OF TENSORS

The tensor concept is intimately connected with the transformation laws for tensors. In fact, a tensor can be regarded as a mathematical entity having the transformation properties required by the physical quantities that it represents. The transformation of a tensor from one set of Cartesian coordinates to another set does not alter the tensor’s physical significance but rather is simply another equivalent way of representing it. A tensor may be classified as to its symmetry, that is, it may be symmetrical (or partially symmetrical), asymmetrical, or antisymmetrical. However, depending on its transformation law, the tensor may be further characterized as polar, axial, magnetic, or axial–magnetic. The components of an axial tensor change sign if the handedness of the coordinate axes is changed, whereas the com-

introduction to tensor and matrix representation 15

ponents of a magnetic tensor change sign only if the atomic magnetic moments are reversed. Polar tensors, on the other hand, are unaffected by either change in handedness or reversal of magnetic moments. In this section, attention will be focused on the transformation laws of polar tensors.

2.2.1 Transformation of Scalars Tensors of rank 0 are nondirectional physical quantities called scalars and are invariant under a coordinate transformation. Typical examples are mass, temperature, entropy, and heat capacity; thus, for example, T ′ = T for the transformation of entropy.

2.2.2 Transformation of Vectors Tensors of rank 1 are called vectors. Polar vectors (as distinguished from axial vectors) transform like the coordinates of a point. Let Tj be a polar vector with respect to axes 0x1, 0x2 , 0x3 that is to be transformed to T ′i with respect to axes 0x ′1, 0x ′2 , 0x ′3 symbolized by T → T ′. Each T ′i is obtained by resolving the Tj along the axes 0x ′1 as shown in Figure 2.1. The components for the three T ′i are given by

T ′1 = a11T1 + a12T2 + a13T3 T ′2 = a21T1 + a22T2 + a23T3 T ′3 = a31T1 + a32T2 + a33T3

(2.5)

T ′i = aijTj (i, j = 1,2,3 = 1 − 3)

(2.6)

or

in convenient tensor subscript notation. Here, the aij are called the direction cosines, for which examples are shown in Figure 2.1. Thus, nine direction cosines are required to specify the transformation of a polar vector where i and j represent the new and old axes, respectively. Equations in (2.5) can also be conveniently represented in the matrix form

T1′ a11 a12 a13 T1 T2′ = a21 a22 a23 . T2 T3′ a31 a32 a33 T3

(2.7)

or simply

T ′= aT

(2.8)

16 tensor properties of solids

x3 x3'

T

-1 a 33

c os

T3'

T3

T2'

cos-1a31

T2

co

x2

cos-1a13

T1 x1

x2'

T1'

s -1 a

11

-1 a 12

s co

x1' FIGURE 2.1: Transformation of the polar vector T → T ′ showing sample direction cosines.

in matrix symbolic notation. The reverse transformation symbolized by T ′ → T is given by T = a~T ′ = a -1T ′,

(2.9)

(2.10)

where a is an orthogonal matrix and

a11 a21 a31 ~ a = a12 a22 a32 a13 a23 a33

is the transpose of a always equal to its inverse, a~ = a -1. Examples of polar vectors are force, electric field, and polarization. Other vectors, such as mechanical moment, angular momentum, and the curl of a polar vector, are examples of axial vectors. Still other vectors, such as magnetic field strength, magnetic flux density, and magnetization, are both axial and magnetic in character and will be considered at a later time.

2.2.3 Transformation of Second-Rank Tensors The transformation law for polar second-rank tensors can be developed from the transformation law for polar vectors. As in Eq. (2.4), consider a second-rank polar tensor that linearly relates two polar vectors p and q. With respect to two sets of axes 0xi and 0x ′i and in matrix symbolic notation, Eq. (2.4) becomes

p = Tq with respect to 0xi

(2.11)

introduction to tensor and matrix representation 17

p′ = T ′q′ with respect to 0x′i

(2.11a)

Transforming the components of p and q′ separately, one obtains in matrix notation

p′ = ap

(2.12)

q = a~q′,

(2.12a)

after which, by introducing Eqs. (2.11) and (2.12a) into Eq. (2.12), there results in matrix notation p′ = ap = aTq = aT a~q′ = T ′q′.

It now follows that

T ′ = aT a~

(2.13)

T ′ij = aikajlTkl (i, j, k, l = 1, 2, 3 = 1 − 3)

(2.14)

or

in tensor subscript notation. Both Eqs. (2.13) and (2.14) represent the transformation law for polar second-rank tensors. In Eq. (2.14), the components of T ′ij are obtained by direct summation of the repeating (dummy) subscripts k and l, whereas in Eq. (2.13), the same components are given in the form

a11 a21 a31 a12 a22 a32 , a13 a23 a33

T11 T12 T13 T21 T22 T23 T31 T32 T33

a11 a12 a13 T ′= a21 a22 a23 a31 a32 a33

(2.15)

which are conformable for matrix multiplication.

2.2.4 Symmetrical and Antisymmetrical Second-Rank Tensors Any second-rank tensor Tij can be expressed as the sum of symmetrical Sij and antisymmetrical Aij tensors. In subscript notation and matrix symbolic notation, this is written as

~ ~ Tij = (Tij + Tji ) / 2 + (Tij − Tji ) / 2 = (T + T ) / 2 + (T − T ) / 2 = Sij + Aij ,

(2.16)

18 tensor properties of solids

where it follows that

S31 ~ S23 = S, S33

½ (T12− T21 ) ½ (T13− T31 ) 0 0 A12 −A31 ~ A23 = −A. A = ½ (T21− T12 ) 0 ½ (T23− T32 ) = −A12 0 0 A31 −A23 0 ½ (T31− T13 ) ½ (T32− T23 )

(2.17)

½ (T12+ T21 ) ½ (T13+ T31 ) T11 S11 S12 S = ½ (T21+ T12 ) S22 T22 ½ (T23+ T32 ) = T33 Sym. ½ (T13+ T31 ) ½ (T32+ T23 )

(2.18)

Clearly, S is specified generally by six independent components, whereas A is specified generally by three independent components. Thus, a symmetrical second-rank tensor is equal to its transpose, ~ S = S , where S11, S22, and S33 are called the principal components that lie along the leading diagonal of the (Sij) matrix. In the case of an antisymmetrical second-rank tensor, the principal components are zero. The stress tensor σij is an example of a symmetrical second-rank tensor, such that σij = σji . Equation (2.17) permits simplification of the matrix forms for symmetrical second-rank tensors. Writing the subscripts in a positive permutation of 123 gives the following results: Tensor notation S11 S22 S33 S23( = S32 ) S31( = S13 ) S12( = S21) Strain notation S1 S2 S3 2S23 2S32 2S12 (2.19) Matrix notation S1 S2 S3 S4 S5 S6 The notation in (2.19) leads to three useful (6 × 1) column forms:

S1 S2 S3 or S4 S5 S6

S1 S2 S3 or 2S4 2S5 2S6

S11 S22 S S = 33 S23 S31 S12

(2.20)

or their (1 × 6) row transpositions. The single subscript form will be the form of choice for use in matrix symbolic equations. The third form in (2.20) is also the accepted matrix form for the strain tensor. Examples of symmetrical second-rank tensors are stress, strain, thermal expansion, dielectric and magnetic susceptibilities, and others. From Eq. (2.18), it is clear that the principal components

introduction to tensor and matrix representation 19

of an antisymmetrical second-rank tensor are null, leaving only three antisymmetrical components, A23, A31, and A12. Examples of antisymmetrical second-rank tensors include the rotational component of a generalized elastic deformation leaving strain εij = εji as a symmetrical second-rank tensor.

2.2.5 Quadratic Transformation Forms The transformation of third- and fourth-rank tensor components is greatly facilitated by the use of quadratic transformation forms, which can be readily obtained from the transformation law for second-rank tensors. It is assumed that any second-rank tensor involved in the description of a third- or fourth-rank tensor is symmetrical such that use can be made of the linear transformation law

a11 a12 a13 S11 S12 S31 a11 a21 a31 a21 a22 a23 . S12 S22 S23 . a12 a22 a32 . a31 a32 a33 S31 S23 S33 a13 a23 a33

(2.21)

S′= aS a~ =

2 a 22 2 a 32

2 a 13 2 a 23 2 a 33

2a 12 a13 2a22 a23

2a13a11

2a11a12

2a23 a21

2a21a22

S2′

2 a11 2 a11

2 a 12

2 a11

S1

S1′

--------------------------------

Carrying out the indicated multiplication and arranging the components of S ′ and S into (6 × 1) column matrices permits Eq. (2.21) to be represented in the quadratic form S2

S3′ = 2a32 a33 2a33a31 2a31 a32 . S3 -----------------------------------------------------------------------------------------------a21 a31 a22 a32 a23 a33 a22 a33 + a23 a32 a21 a33 + a23 a31 a21 a32 + a22 a31 S4 S4′

S6′

S5

a11 a21 a12a22 a13a23 a12 a23+ a13a22 a11a23 + a13 a21 a11 a22 + a12a21 S6

a31a11 a32 a12 a33 a13 a12 a33 + a13 a32 a11 a33 + a13 a31 a11 a32 + a12 a31

S5′

or simply in symbolic matrix notation

S′ = αS.

(2.22)

Here, α is a (6 × 6) matrix called the quadratic transformation matrix for a symmetrical second- rank tensor and where the third single subscript notation of (2.20) has been applied. With few exceptions, the property tensors of higher order, which are commonly encountered, are represented by third- and fourth-rank tensors having some inherent symmetry. Thus, where it is necessary to specify the transformation law for these matter tensors, rather extensive practical use will be made of the α transformation form—a method preferred over the more cumbersome method of direct summation of the repeating suffixes in the tensor subscript forms.

20 tensor properties of solids

A mnemonic diagram for the quadratic transformation matrix α can be constructed by dividing it into four sections as follows:

---------------------

Twice the product of row omissions of [aij ] matrix . -----------------------------------------------------------------------------------Cross product of Product of column minor of element aij omissions of [aij ] matrix

Square of element aij of [aij ] matrix

The content of these four sections can be verified by an inspection of Eq. (2.22) in expanded form. Not all property tensors exhibit inherent symmetry, and for this reason, a similar quadratic transformation law must be written for an asymmetrical second-rank tensor. In this case, the transformation matrix becomes a (9 × 9) quadratic form. The development of this more general form follows from Eq. (2.15) by carrying out the indicated multiplication and arranging the components of T ′ and T as (9 × 1) matrices similar to (2.20) but with no symmetry. The result is given by

T ′ = βT ,

(2.23)

where β is called the (9 × 9) general quadratic transformation matrix for asymmetrical second-rank tensors presented in Eq. (9.31). The β transformation form is useful in describing the transformation laws for the less common piezothermoelectric and elastothermoelectric power properties as well as the piezomagnetoelectric and elastomagnetoelectric effects.

2.2.6 Transformation of T hird-Rank Tensors Consider a third-rank tensor, T, relating a polar vector, p, and a polar second-rank tensor, q, written with respect to two sets of coordinate exes, 0xi and 0x′i :

pi = Tijkqjk or p = Tq for axes 0xi

(2.24)

p′l = T ′lmnq′mn or p′ = T ′q′ for axes 0x′i

(2.25)

and

For the case where q is a symmetrical second-rank tensor (hence, q = q~), it follows that for the transformations p′ = ap, q′ = α q, and q = α −1q′, there results

p′ = ap = aTq = aTα −1q′ = T ′q′,

introduction to tensor and matrix representation 21

giving for the transformation law for T T ′ = aTα −1,

(2.26)

~ in general. In tensor subscript where α −1 is the inverse of α and where it is understood that α −1 ¹ α notation, Eq. (2.26) is written as

T ′ijk = ail ajmaknTlmn (i − n = 1 − 3)

(2.27)

The partial symmetry of T in Eq. (2.24) is implied by the symmetry of q. This is easily shown by using tensor subscript notation giving pi = Tijkqjk = Tikj qkj ,

(2.28)

which permits Tijk = Tikj .

In matrix subscript notation, Eq. (2.28) becomes

pi = Timqm (i = 1 − 3; m = 1 − 6),

(2.29)

where q is now a (6 × 1) column matrix and Eq. (2.29) becomes

p1 T11 T12 T13 T14 T15 T16 p = p2 = T21 T22 T23 T24 T25 T26 p3 T31 T32 T33 T34 T35 T36

q1 q2 q3 = Tq, q4 q5 q6

(2.30)

with respect to axes 0xi . Note that subscript m in Eq. (2.29) is unfolded according to the matrix notation in (2.20). This permits a reduction in the T matrix from a (3 × 9) to a (3 × 6) matrix, as given in Eq. (2.30), both of which avoid the need for a three-dimensional representation. The tensors Tijk and Tikj in Eq. (2.28) are called tensor isomers and represent a certain partial symmetry. The tensor Tijk has a total of 3! = 6 isomers possible, which are obtained by the permutation of pairs of subscripts. In comparison, the transpose of a second-rank tensor Tij is its only isomer. Examples of third-rank tensor properties that exhibit this partial symmetry are the piezoelectric

22 tensor properties of solids

effect, first-order electrostriction, piezomagnetic effect and first-order magnetostriction, the linear electro-optical effect, the thermal–electro-optical effect, and others. The transformation of components for the partially symmetrical third-rank tensor Tijk = Tikj is carried out in accordance with Eq. (2.26) for new and old sets of axes, 0x′i and 0xi , respectively:

−1 α 14 −1 α 24 −1 α 34 −1 α 44 −1 α 54 −1 α 64

−1 α 15 −1 α 25 −1 α 35 −1 α 45 −1 α 54 −1 α 65

−1 α 16 −1 α 26 −1 α 36 −1 α 46 −1 α 56 −1 α 66

−1 α 13 −1 α 23 −1 α 33 −1 α 43 −1 α 53 −1 α 63

−1 α 12 −1 α 22 −1 α 32 −1 α 42 −1 α 52 −1 α 62

a11 a12 a13 T11 T12 T13 T14 T15 T16 T ′ = a21 a22 a23 . T21 T22 T23 T24 T25 T26 a31 a32 a33 T31 T32 T33 T34 T35 T36

−1 α 11 −1 α 21 −1 α 31 −1 α 41 −1 α 51 −1 α 61

which represents the matrix equation

T ′ = aTα −1

(2.31)

It may be recalled that the inverse (or reciprocal) A −ij1 of a matrix A is the transpose of the cofactor (Aij ) of the element Aij divided by the non-zero determinant of Aij . That is,

( Aji) (Aij )−1= or Ai j

( A~ ) A −1= A

(2.32)

where (Aij ) = (−1)(i + j )|Mij | is the cofactor of element Aij and |Mij | is its minor (the determinant that remains after removing the ith row and jth column in |Aij | ). Obviously, transformation of tensors of rank 3 can be quite laborious. Fortunately, the linear and quadratic transformation matrices representing the symmetry operation for crystals are relatively uncomplicated. As will be shown later in Section 3.5, these matrices often consist of compo~, a result that is not true generally. nents that are 0, 1, or -1, and in most cases, α −1 = α

2.2.7 Transformation of Fourth-Rank Tensors In similar fashion, the transformation law for a fourth-rank tensor property can be deduced from the transformation laws of the tensor variables it relates. Consider the fourth-rank tensor property relating two polar second-rank tensor variables with reference to the two sets of axes, 0xi and 0x′i

pij = Tijkl qkl or p = Tq for axes 0xi

(2.33)

introduction to tensor and matrix representation 23

and

p′mn = T ′mnopq′op or p′ = T ′q′ for axes 0x′i .

(2.34)

If both p and q are symmetrical second-rank tensors, convenient use can again be made of the α quadratic transformation form. Because p and q′ transform as p′ = αp and q = α −1q′, then p′ = αp = αTq = αTα −1q′ = T ′q′

or

T ′ = αTα −1

(2.35)

as the transformation equation for T in matrix symbolic notation. In tensor subscript notation, Eq. (2.35) becomes

T ′ijkl = aimajnakoalpTmnop (i − p = 1 − 3)

(2.36)

The partial symmetry of Tijkl is implied by the symmetry of pij = pji = pm and qkl = qlk = qn where it is now proper to write

pm = Tmnqn (m, n = 1 − 6)

(2.37)

The partial symmetry expressed by Eq. (2.37) permits a reduction in the number of independent coefficients needed to specify T from 3(4) = 81 to 36. Because both p and q are represented by (6 × 1) matrices, it follows that T must be a (6 × 6) matrix and that Eq. (2.37) can be presented as

T22 T32 T42 T52

T23 T33 T43 T53

T24 T34 T44 T54

T25 T35 T45 T55

T62 T63 T64 T65

T26 q2 T36 . q3 . T46 q4 T56 q5 T66 q6

p2 T21 p3 = T31 p4 T41 p5 T51 p6 T61

T11 T12 T13 T14 T15 T16 q1

p1

(2.38)

Just as for the case of the partially symmetrical third-rank tensor, the transformation law for the partially symmetrical fourth-rank tensor in Eq. (2.37) is most conveniently represented in matrix form according to T ′ = αTα −1 in Eq. (2.35), giving

24 tensor properties of solids

T12 T22 T32 T42 T52 T62

T13 T14 T23 T24 T33 T34 T43 T44 T53 T54 T63 T64

T15 T25 T35 T45 T55 T65

T16 T26 T36 T46 T56 T66

T11 T21 T31 T41 T51 T61

−1 α 11 −1 α 21 −1 α 31 −1 α 41 −1 α 51 −1 α 61

−1 α 12 −1 α 22 −1 α 32 −1 α 42 −1 α 52 −1 α 62

−1 α 13 −1 α 23 −1 α 33 −1 α 43 −1 α 53 −1 α 63

−1 α 14 −1 α 24 −1 α 34 −1 α 44 −1 α 54 −1 α 64

−1 α 15 −1 α 25 −1 α 35 −1 α 45 −1 α 54 −1 α 65

−1 α 16 −1 α 26 −1 α 36 −1 α 46 −1 α 56 −1 (2.39) α 66

α 16 α 26 α 36 α 46 α 56 α 66

α 15 α 25 α 35 α 45 α 55 α 65

α 14 α 24 α 34 α 44 α 54 α 64

α 13 α 23 α 33 α 43 α 53 α 63

α 12 α 22 α 32 α 42 α 52 α 62

α 11 α 21 α T ′ = 31 α 41 α 51 α 61

Here again, it is shown that numerical manipulation required to transform a higher-rank tensor is considerable, particular for an arbitrary rotation of axes. In such cases, use of the computer is recommended. However, as pointed out earlier, transformation matrices representing most crystal symmetry operations are strikingly simple, allowing tensor transformations in most cases to be carried out with little difficulty by using α −1 = α~ in Eqs. (2.31) and (2.39) or even by the method of direct inspection discussed later. The maximum inherent symmetry possible for fourth-rank tensors is given by

Tmn = Tnm (m, n = 1 − 6) .

(2.40)

In this case, the leading diagonal of components becomes the mn = nm symmetry line. This eliminates the 15 coefficients below the leading diagonal symmetry line as independent components. The remaining 21 coefficients are now represented by the symmetrical (6 × 6) matrix

T16 T26 T36 = [Tnm ] T46 T56 T66

T15 T25 T35 T45 T55

T11 T12 T13 T14 T22 T23 T24 T33 T34 [Tmn ] = T44 (Sym.)

(2.41)

The symmetrical matrix of Eq. (2.41) is used to represent the elastic compliance and stiffness moduli as well as the many properties involving these moduli. The inherent symmetry expressed by Tmn = Tnm results solely from thermodynamic arguments that are presented in Section 4.4. Property tensors with tensor rank greater than four are not as common as some of those of lesser tensor rank. Nevertheless, a few fifth- and sixth-rank tensor properties have either been measured experimentally or have been predicted to exist on theoretical grounds. Examples are the fifth-rank piezoelectro-optical, piezomagneto-optical, and sixth-rank quadratic piezo-optical effects mentioned in Section 7.3.2 and the quadratic piezothermoelectric power and quadratic piezo-

introduction to tensor and matrix representation 25

TABLE 2.1: The transformation laws for polar tensors up through the rank 4 showing tensor rank, tensor subscript notation, matrix symbolic notation, and the referred matrix text equation. Transformation law Rank

Tensor subscript notation

Matrix symbolic notation

Referred matrix equation

0

T ′ = T

—

—

1

T ′i = aijTj

T ′ = at

(2.8)

2

T ′ij = aikajlTkl

T ′ = aT a~

(2.13)

3

T ′ijk = ail ajmaknTlmn

T ′ = aTα −1

(2.31)

4

T ′ijkl = aim ajnakoalpTmnop

T ′ = αTα −1

(2.35)

resistance effects represented in Eqs. (9.26) and (9.38), respectively, both of which are sixth-rank tensor properties.

2.2.8 Summary of Tensor Transformation Laws For the convenience of the reader, Table 2.1 summarizes the transformation laws for polar tensors up through rank 4 that exhibit some inherent symmetry. The transformation equations are given in both tensor subscript form, where summation over the dummy (repeating) subscripts is understood, and in conformable matrix symbolic form, the latter being derived from equations of the form p = Tq. The transformation equations for the fifth- and sixth-rank tensor properties mentioned above will be left as additional exercises for the reader. In the matrix equations, use is made of the quadratic transformation matrix α, which assumes a) some inherent symmetry for a given tensor T and b) that the first and third forms in the column matrices of Eqs. (2.20) are equated. If no inherent symmetry exists in T, the matrix forms of the transformation laws in Table 2.1 may still be used but with the α matrix replaced by the more general β transformation form given in Eq. (9.31) applicable to asymmetrical second-rank tensors.

2.3

INTRODUCTION TO TENSOR ALGEBRA

Up to this point, we have made some use of tensor algebra without specific mention of the laws involved. We will now review various standard operations involving tensor addition and multiplication

26 tensor properties of solids

with some exceptions. The subjects of axial tensors, tensor differentiation, tensor field subject matter, and the vector cross product will be reviewed later in Sections 2.4, 2.5, and 2.6, respectively.

2.3.1 Tensor Addition The addition (or subtraction) of corresponding components of two or more tensors all having the same tensor rank yields a resultant tensor of the same rank. As an example, consider adding components of two symmetrical second-rank polar tensors A and B expressed in both tensor subscript and symbolic matrix notation:

Rij = Aij + Bij or R = A + B

This requires that R11 = A11 + B11, R22 = A22 + B22 , … R12 = A12 + B12 for all six independent components of the resultant matrix R. The sum rule may be generalized by the equation

Rijk... = Aijk... + Bijk... + ... ,

(2.42)

which is restricted to components of tensors having the same rank and tensor character. The sum rule obeys the commutative, associative, and distributive laws of additions well-known in Cartesian algebra.

2.3.2 Tensor Multiplication For the reader’s convenience and by using the symbol ⊗ to represent the outer and inner product operations, we review the following tensor multiplication laws best illustrated by using conformable matrix forms: Cumulative law A⊗B=B⊗A Associative law A ⊗ (B ⊗ C) = (A ⊗ B) ⊗ C Distributive law A ⊗ (B + C) = A ⊗ B + A ⊗ C

(2.43)

These laws are written in the order of increasing extent to which they are obeyed by the tensor multiplication operations. Generally speaking, the distributive law is always obeyed if the sum rule is obeyed, the associative law is obeyed if the permutation tensor is not involved, and the commutative law is never obeyed except for scalar products. The tensor representation of the vector cross product and the properties of the Kronecker delta and permutation tensor will be reviewed later in Section 2.6.3.

introduction to tensor and matrix representation 27

2.3.3 Outer Product The product of two tensors AB that yields a resultant tensor of tensor rank equal to the sum of the tensor ranks of A and B (rA + rB) is called the outer product or dyadic product of A and B. For example, the outer product of a vector Ai and a symmetrical second-rank tensor Bjk yields a tensor of thirdrank Rijk. That is, Rijk = Ai Bjk (i, j, k = 1 − 3)

or

Rim = Ai Bm (i = 1 − 3; m = 1 − 6).

(2.44)

The expanded matrix form of Eq. (2.44) yields a (3 × 6) AB matrix given by A1B1 A1B2 A1B3 A1B4 A1B5 A1B6 A2B1 A2B2 A2B3 A2B4 A2B5 A2B6 . A3B1 A3B2 A3B3 A3B4 A3B5 A3B6

A1 R = A2 . [B1 B2 B3 B4 B5 B6 ] = A3

~ Note that if B ¹ B , then the product AB yields a (3 × 9) matrix. The outer product rule can be generalized by the tensor subscript equation

Rijk...opq... = Aijk...Bopq...,

(2.45)

where R has a tensor rank equal to the sum of the ranks of A and B, that is, rR = rA + rB , a fact that is lost in the use of symbolic matrix notation R = AB.

2.3.4 Tensor Contraction When a single subscript in the product or two tensors of the same rank r are set equal, a single contraction results producing a tensor of rank (r − 2). The product of two tensors of arbitrary rank results in tensor contraction called the inner product and is generalized in tensor subscript notation as

R...ijlm = A...ijkBklm...

(2.46)

or R = A⋅B in tensor symbolic notation. Here, R is a tensor of rank rR = (rA + rB) − 2 having the same tensor character as that of A and B. As an example, consider the single contraction (inner) product of a polar vector and a partially symmetrical third-rank polar tensor (Bijk = Bikj) given by

28 tensor properties of solids

Rjk = Ai Bijk (i, j, k = 1 − 3)

or

Rm = Ai Bim (i = 1 − 3; m = 1 − 6)

In expanded matrix form, this becomes B16 B26 = [R1 R2 R3 R4 R5 R6 ], B36

B15 B25 B35

R = [A1 A2

B11 B12 B13 B14 A3 ] . B21 B22 B23 B24 B31 B32 B33 B34

which yields the components of symmetrical polar second-rank tensor R in the form of a (1 × 6) matrix. Double contraction results when two subscripts in the product of two tensors of the same rank r are set equal, producing a tensor of rank r − 4. The double contraction product of two tensors of arbitrary tensor rank is generalized in tensor subscript notation as

R...hk... = A...hij Bijk...

(2.47)

or R = A ⋅ B in tensor symbolic notation. Here, R is a tensor of rank rR = (rA + rB) − 4 having the same tensor character as that of the A and B combination. An example of double contraction is

Rij = Aijkl Bkl (i, j, k, l = 1 − 3),

(2.48)

which was used in Eq. (2.33) to represent a polar fourth-rank that relates two polar second-rank tensors. Tensor contraction continues through triple, quadruple, etc. contractions and becomes complete when the product of two tensors of the same rank yields a scalar. This product is called the scalar product, which is generalized as

R = Aijk... Bijk... = tr (AB)

(2.49)

called the trace of AB. An example is the scalar product of two symmetrical second-rank tensors,

R = Aij Bij ,

introduction to tensor and matrix representation 29

represented in matrix form as the scalar product

= A1B1 + A2B2 + A3B3 + A4B4+ A5B5 + A6B6

2.4

R = [ A1 A2 A3 A4 A5

B1 B2 B A6] 3 = tr(AB) B4 B5 B6 (2.50)

AXIAL TENSORS

The tensors discussed so far have been polar tensors that transform, such that the sign of their components is unaltered by a transformation that changes the handedness of the coordinate axes. Table 2.1 gives the transformation laws for polar tensors. Tensors having components that change sign when the handedness of the coordinate axes is changed by a transformation are called axial tensors or pseudo tensors. To generalize, axial tensors transform according to T ′ijk... = | a |aimajnako...Tmno... .

(2.51)

Here, for example, the “handedness” factor | a | for a second-rank tensor is the determinant of the transformation matrix (aij ) given symbolically by

| |

a b c |a | = d e f = a . e f − b . d f + c . d e g h g i h i g h i

| |

| | | | | |

e f where, for example, = ei − f h. Thus, | a | = - 1 for a transformation that changes the handedh i ness of the axes, and | a | = 1 if the handedness is left unchanged by the transformation. Table 2.1 for polar tensor transformations applies to axial tensors if the handedness factor | a | = ± 1 is included on the right-hand side of each transformation law. For a scalar, the transformation law becomes T ′ = | a |T. An example of an axial (pseudo)-scalar is the optical rotatory power, ρ. Vectors, such as magnetic field strength, magnetic flux density, and magnetization, are both axial and magnetic in character. As a second example, the Hall tensor Rijk is both antisymmetrical (in subscripts j,k or i,k)

30 tensor properties of solids

and axial–magnetic but which can be represented as a polar–magnetic second-rank tensor as discussed in Section 10.3. The reader must be aware of the fact that axial tensors and antisymmetrical tensors are two entirely different tensor characteristics the distinction of which will be made evident in Section 2.6.3. Magnetic tensor character is discussed in Appendix A.

2.5

TAYLOR’S SERIES EXPANSION AND THE TENSOR DIFFERENTIATION LAWS

Taylor’s series is a type of power series used to express a given function of one or more variables by means of a polynomial in the neighborhood where the function is regular (analytic). A valid Taylor’s series expansion requires that the series be convergent within a finite interval and that all derivatives (or partial derivatives) of the function be continuous in that interval. For the general case of multivariable tensor functions, the Taylor’s series expansion is given symbolically by

∞ 1 ∂ 0 ∂ 0 ∂ 0 f (P, Q , R ...) = ∑ kl j n! (Pi − Pi ) ∂Pi + (Qj − Qj ∂Qj + (Rkl − R kl )∂Rkl +... i n=0

n

f (Pi0, Qj0 , Rkl0 ...), (2.52)

(

where n = 1, 2, 3, ... is an integer and f (P i0, Q 0j , Rk l0 ...) signifies that after the function is operated on, the resulting coefficients are evaluated at the reference values of Pi = Pi0, Qj = Q j0, Rkl = Rk l0 , and so forth. Because the function f may itself be a tensor quantity of arbitrary tensor rank, the resulting coefficients are tensors given in accordance with the tensor differentiation laws

T...ijkl ...

C,D,...

2

,U...ijkl ...rs...

∂ A...ij . . . , et = ∂Bkl... ∂Crs... D,E,...

∂ A...ij = ∂Bkl...

(2.53)

Here, the law expressed by T...ijkl... implies that all remaining components of B and all components of C, D, and so forth are held constant and that T...ijkl... has the tensor rank rA + rB and the combined tensor character of A and B. The law expressed by U...ijkl...rs... for a second-order derivative implies that U has a tensor rank of rA + rB + rC with the combined tensor character of A, B, and C, where it is understood that the remaining components of B and C and all components of D, E, and so forth are held constant. Notice that our rule of subscript order is read from top-to-bottom–left-to-right. However, because other subscript order schemes can be found in literature, care must be taken to recognize which scheme is used.

introduction to tensor and matrix representation 31

As an example of the use of Eq. (2.53), let the electric polarization Pi be a function of electrical field strength Ej and stress σkl and let Pi (Ej , σkl ) be expanded in a Maclaurin series (special case of a Taylor series) about the state of zero electric field and zero stress to give 1 ∂ Pj(Ej, σkl ) = σ ∂ E n! j Ej + σ n=0

∑

∞

n

Pi (0,0),

(2.54)

giving the result 2 ∂ Pi σ kl + 1 ∂ E ∂E 2! j m (0,0)

∂2Pi Ej σkl + ∂ σ ∂σ kl n o (0,0)

(0,0)

Ej Em

(0,0)

∂2Pi ∂ Ej ∂ σkl

+2

∂P Ej + i ∂ σ kl (0,0)

∂P Pj(Ej, σ kl ) = Pi (0,0) + i ∂Ej

σ kl σn o + ...

As will be shown in later chapters, the various coefficients (in parentheses) define certain tensor properties. For example, κ 0−1(∂Pi / ∂Ej ) = χij is the dielectric susceptibility tensor for a crystal and κ 0 is the permittivity in a vacuum. The quantity (∂Pi / ∂σkl) = dikl is the piezoelectric tensor. Here, both χij and dikl are first-order (n = 1) effects evaluated, in this case, at zero electric field and zero stress. The three properties given within the square brackets are second-order (n = 2) effects and are represented by third-, fourth-, and fifth-rank tensors also evaluated at zero electric field and zero stress. Note that had the expansion in Eq. (2.54) also been taken about the state of reference temperature T 0, it would be called a Taylor’s series—hence, the basic distinction between a Maclaurin’s series and a Taylor’s series.

2.6

TENSOR FIELDS AND TENSOR OPERATORS

For purposes of this section, we will use the symbol ψ to represents a Cartesian tensor field of rank r in a region R and specified by 3(r) continuous functions of position ψijk... (x1, x2, x3) or simply ψijk...(x). We will cover only the tensor gradient and divergence, Kronecker delta, permutation tensor, vector cross product, and tensorial contraction because these will be used later in both Parts I and Part II of this text. Other related subjects such as Stoke’s theorem and Green’s theorem in a plane and their application to thermodynamics will be discussed in sufficient detail as they become needed in later developments. The curl of a tensor will be left to further reading (see Endnotes).

32 tensor properties of solids

2.6.1 Gradient of a Tensor Field The components of a field tensor of rank r can be differentiated with respect to the coordinates of a point, resulting in a tensor of rank r + n, where n is the order of the differential operator used. One can generalize the tensor gradient as the outer product of two tensors, a field tensor ψijk...(x) of rank r and the nth-order operator ∂pst... of rank n. That is,

∂ψijk ... Tijk ... pst = ∂pst ...ψijk ... = ∂xp∂xs∂xt ...

(2.55)

written as T = gradψ = ∇ψ in tensor symbolic notation. Here, T transforms as a tensor of rank r + n and is represented by 3(r + n) continuous functions of position T (x) in Cartesian space. Note that Eq. (2.55) has been written by using the rule of subscript order given in Section 2.5. The simplest application of Eq. (2.55), and one in which we are particularly interested, is the gradient of a scalar field. If the scalar field is represented by φ, then its gradient is a Cartesian vector having components given as

∂φ ∂φ ∂φ ∂i φ = x , x , x 1 2 3

(2.56)

or written as gradφ = ∇φ in vector symbolic notation. See Eq. (8.1) in Chapter 8 as an example. The gradient of a scalar points in the direction of the maximum rate of change and that has a magnitude equal to that maximum rate of change. Examples of a scalar field are the electrostatic potential (or voltage), chemical potential, and temperature. Thus, the gradient of any scalar field is always from low to high potential as, for example, from low to high temperature. Thus, Fourier’s law requires that the heat must flow from high to low temperature in a direction opposite to the temperature gradient, hence, the minus sign in Eq. (8.7) presented in Part II of this text. Application of Eq. (2.55) to the field vector ψi(x) results in the asymmetrical dyadic ∂jψi = ∂ψi /∂xj called the vector gradient of the given field with components given by a 3 × 3 Jacobian matrix,

∂1ψ1 / ∂x1 ∂1ψ1 / ∂x2 ∂1ψ1 / ∂x3 = ∂2ψ2 / ∂x1 ∂2ψ2 / ∂x2 ∂2ψ2 / ∂x3 /∂ / / ∂3ψ3 ∂x1 ∂3ψ3 ∂x2 ∂3ψ3 x3

∂ψi Tij = ∂xj

(2.57)

We will have no further need to apply Eq. (2.55) to tensor fields of tensor rank greater than r = 1.

introduction to tensor and matrix representation 33

2.6.2 Divergence of a Tensor Field The divergence of a tensor can be generalized by the single-contraction product of a field tensor ψijk...(x) of rank r with the vector operator ∂i yielding a tensor of rank r − 1 given by Tjk ... = ∂iψijk ... =

∂ψijk...

∂xi

(2.58)

or as T = divψ = ∇.ψ in tensor symbolic notation. Contraction can be carried out on any of the indices of ψijk...(x), but the results will, in general, be different. A physical interpretation of Eq. (2.58) is reasonably straightforward. The divergence of a tensor gives at each point the rate per unit volume at which the physical entity represented by ψ is issuing from that volume. The divergence theorem (also known as Gauss’ theorem) is widely used and provides the integral definition of divergence of a tensor field given by ο∫ dS .ψ divψ ≡ lim s ∆V→0 ∆V

(2.59)

where o∫ sdS.ψ is called the net flux of ψ out of S. Thus, Eq. (2.59) defines the divergence of a tensor field at a point P in V as the limiting value of the flux of ψ per unit volume out of S when ∆V →0. The simplest example is the divergence of a vector field ψi(x) equal to a scalar ∂iψi having magnitude

∂i ψi =

∂ψ1 ∂ψ2 ∂ψ3 + = tr(∂jψi ), + ∂ x1 ∂ x2 ∂ x3

(2.60)

which is equal to the trace of the vector gradient in Eq. (2.57). A well-known example of the application of Eq. (2.60) is the steady state in a thermoelectric system when the divergence of the energy flux vanishes, that is, ∇.J u = 0. This means that the heat energy emitted to the surroundings, say, by Joule (I 2R-type) heating in a volume element must be exactly balanced by the heat energy absorbed by that volume element from the surroundings.

2.6.3 Kronecker Delta, Permutation Tensor, Vector Cross Product, and Tensorial Contraction The Kronecker delta is defined by

0 0 1

0 1 0

or

δ 11 δ 12 δ 13 1 [δij ] = δ 21 δ 22 δ23 = 0 0 δ 31 δ 32 δ33

1 if i = j δij = 0 if i ≠ j

(2.61)

34 tensor properties of solids

Now, if Ti is the ith component of a vector, then with the definitions of Eqs. (2.61), there results the expressions δij Ti = Tj and δij Tj = Ti , or for a tensor Tjk , there results δij Tjk = Tik and δij Tik = Tjk . All express the substitution property of the Kronecker delta, which will be used in Section 9.3 of this text. The permutation tensor eijk (also called the Levi–Civita tensor, alternating tensor, or e-tensor) is an antisymmetrical, axial, third-rank tensor defined by

+ 1 if ijk is an even permutation of 123

eijk ≡ − 1 if ijk is an odd permutation of 123 0 if any two subscripts are the same

→

→

(2.62)

→

A common application of eijk is the vector cross product or R = B × C described by the equation given in tensor notation Ri = eijk BjCk (i, j, k, = 1, 2, 3)

(2.63)

The three components of Ri are readily found by expansion of Eq. (2.63) or by using the matrix form

R1 R2 R 3

B1C1 B2C2 B3C3 B2C3 − B3C2 0 0 0 1 0 0 −1 0 0 B2C3 0 0 1 0 −1 0 B2C1 = B3C1 − B1C3 = 0 0 0 1 0 0 0 −1 B1C2 0 0 0 0 B1C2 − B2C1 B3C2 B1C3 B2C1

(2.64)

Equations in (2.64) can be represented simply by R = e(BC) in matrix symbolic notation, where the dyadic product (BC) has been unfolded as the 9 × 1 form of Tij in Eq. (2.3). The top row of the [3 × 9] matrix is unfolded as 111, 122, 133, 123, 131, 112, 132, 113, 121, then 211, 222, 233, 223, 231, 212, 232, 213, 221 for the second row, and 311, 322, 333, 323, 331, 312, 332, 313, 321 for the third row. The difference between the antisymmetrical and axial character of a tensor is nicely described in terms of the e-tensor. The permutation tensor has been described as antisymmetrical. This is true by virtue of the fact that if any two subscripts of the component eijk are set equal, the component becomes zero—the antisymmetrical property. The e-tensor is also axial due to the fact that if any two subscripts are interchanged, which is equivalent to reversing the handedness of the axes, the

introduction to tensor and matrix representation 35

value of the e-tensor changes sign, 1 to −1, or vice versa. These special features of the e-tensor will be useful in dealing with the magneto-optical and galvanomagnetic effects discussed in Sections 7.3.4 and 10.2. A generalization of the single contraction product involving eijk without restriction on tensor rank and character is given by

Ajklm ... = eijk Tilm ...

(2.65)

or simply by A = e . T in tensor symbolic notation. This equation states that a tensor T of rank r can be represented by its dual A of rank r + 1. Here, A has the combined tensor character of e and T but retains the physical properties of T. Thus, if T represents an axial second-rank tensor (e.g., the magnetoelectric susceptibility discussed in Section 4.5, then A must be an antisymmetrical (nonaxial) tensor with the physical properties of T. A common application of Eq. (2.65) is the case where an axial vector is converted to an antisymmetrical second-rank tensor given by

Ajk = eijk Ri

(2.66)

A generalization of double contraction product involving eijk can be represented, with certain restrictions to tensors of arbitrary tensor rank and character, by the equation

Ailm ... = eijk Tjklm ...

(2.67)

or simply by A = e : T in tensor symbolic notation. Here, the tensor rank of A is r − 1 when the tensor rank of T is r. The restrictions imposed on Eq. (2.67) are simply that tensor T must be of secondrank or higher and that it must be antisymmetrical in j and k if it is necessary that all components of ~ T be retained by A in the conversion. Thus, as an example, eijk Sjk = 0 if S = S . As a second example, the reverse conversion to Eq. (2.66) permits an antisymmetrical second-rank tensor to be converted to an axial vector expressed as

Ri = eijk Ajk

(2.68)

Or, as a third example, if T is an antisymmetrical third-rank tensor in j,k only but is also axial, then A must be a polar (true) second-rank tensor as expressed by

Ail = eijk Tjkl

(2.69)

Here, A is said to be the dual of T. Equation (2.69) will find use in Section 10.3 when dealing with the Hall tensor.

36 tensor properties of solids

Further tensorial contraction using the permutation tensor is possible by highly restricted. A → → → common example is the triple scalar product V = a × b . c , which represents the volume of a general → → → parallelepiped of sides a , b , c In tensor notation, this scalar product is simply written as V = eijk ai bj ck

(2.70)

Thus, V does not transform as a simple scalar but rather as a pseudo (axial) scalar according to V ′ = aV. αβγ = eαβγeijk = ∆K is given by the matrix The generalized Kronecker delta denoted by δijk

δα i δα j δαk ∆ = δβi δβ j δβk δγ i δγ j δγk K

(2.71)

such that the contraction products follow Section 2.3.4, leading to the matrix for triple contraction given by ee~ = 2tr(ee~) = 6 as used in Section 7.3.4. • • • •

37

chapter 3

Crystal Systems, Symmetry Elements, and Symmetry Transformations 3.1

INTRODUCTION

In the previous chapter, it was shown that the possession of inherent symmetry by a tensor of rank r had the effect of reducing the number of independent components representing it from 3(r) to some number that was determined by the number of indices that could be interchanged. In this section, we will discuss certain additional limitations placed on the relationships between the components of a tensor property by the structural symmetry of the crystal within which the property is manifest. Remember, however, that not all tensors are affected by crystal symmetry. Second-rank field tensors such as stress and strain possess certain intrinsic symmetry, but their components are unaffected by the symmetry of the crystal. On the other hand, property tensors, which may relate two or more field tensors and hence possess their intrinsic symmetry, will also acquire the symmetry of the crystal within which the property is evinced. Thus, property tensors may possess a higher symmetry than that possessed by the crystal. When the components representing a given property tensor vary with crystallographic direction, the crystal is said to be anisotropic with respect to that property. Conversely, if the components of a given property tensor are invariant with crystallographic direction, the crystal is said to be isotropic with respect to that particular property. A crystal may possess partial isotropy with respect to a given property if, for example, the components of the property are invariant with direction in a particular crystallographic plane but vary with direction out of that plane. The term crystal symmetry, as used above, refers not to the atomic structure but to the morphology or macroscopic symmetry of the crystal. During the natural growth of some crystals, the planes of highest atomic density have a propensity to form the external faces of the crystal. A naturally occurring quartz crystal is a good example. The special relationship between these faces produces a symmetry that forms the basis of classification of crystals into 32 conventional symmetry classes called point groups. Thus, each of the 32 point groups defines a symmetry class. It is the point group symmetry (i.e., macroscopic symmetry) of a crystal that imposes certain limitations on the relationships between different components of a macroscopic tensor property. For magnetic

38 tensor properties of solids

crystals, the atomic magnetic spin moments, viewed collectively over the crystal, become important in symmetry considerations. This leads to the formation of the 90 magnetic point groups. There are, however, certain microscopic symmetry elements that take place at the atomic level and that are not possible in a point group, conventional or magnetic. Several symmetry operations at the atomic level are used to classify the microscopic symmetry elements in a three-dimensional space lattice, and these are called a space group. There are 230 conventional space groups and 1651 magnetocrystalline space groups, and every crystal must belong to one or more of these groups. We will not further consider space groups, conventional or magnetic, since they fall outside the scope of this text.

3.2

MACROSCOPIC CRYSTAL SYMMETRY AND SYMMETRY TRANSFORMATIONS

There are two fundamental macroscopic symmetry operations that can be performed at a point to generate all 32 point groups representing the 32 crystal classes. These two operations are rotation and center of symmetry. We will consider these in some detail along with the appropriate symmetry transforms and then develop the symbology used to designate the 32 point groups.

3.2.1 Permissible Rotations When a perfect crystal can be brought into congruence with itself by a rotation about an axis, it is said to possess a proper rotation axis of symmetry. One-, two-, three-, four-, and sixfold rotation axes are permissible as expressed by φ = 2π / n, where n = 1, 2, 3, 4, or 6. These permissible rotations are presented in Table 3.1 and are often referred to as monad, diad, triad, tetrad, and hexad axes of rotation, respectively. Rotations for n = 5, 7, ... are not permissible.

3.2.2 Center of Symmetry Taking the origin of coordinates as the center of symmetry, this operation consists of moving each point (x, y, z) to a position (−x, −y, −z) as shown in Figure 3.1. This represents an inversion of axes through the origin of coordinates and is expressed by the transformation matrix (aij) = −(δij), where (δij ) is the unitary matrix. Note that in tensor subscript notation, δij is called the Kronecker delta previously discussed in Section 2.6.3.

TABLE 3.1: Permissible rotations to bring a perfect crystal into self-congruence n

1

2

3

4

6

Rotation, φ = 2π / n

φ = 360°

φ = 180°

φ = 120°

φ = 90°

φ = 60°

Crystal Systems, Symmetry Elements, and Symmetry Transformations 39

x3 z -y

x

x1

-x x2

y -z

FIGURE 3.1: Coordinate axes showing a center of symmetry.

The two operations, an n-fold proper rotation and a center of symmetry, may be combined to produce rotoinversion axes designated by x¯= 1¯, 2¯, 3¯, 4¯, or ¯6. The rotoinversion operation is one of n-fold rotation followed by inversion through a center of coordinates. If the transformation matrices for these two operations are a1 and a2 (= −δij), respectively, then the resultant transformation matrix is a = a2a1 = (−δij)a1 = −a1. A twofold rotoinversion axis of symmetry, ¯2 , is identical to a reflection across a mirror plane (sometimes called a plane of symmetry) lying perpendicular to the ¯2 axis. This is illustrated in Figure 3.2, where the symbol commonly used to designate a plane of symmetry is m ( = 2¯ ). As an example, the rotoinversion transformation matrix representing a reflection across the mirror plane x1, x2 is

180o

Mirror Plane End

FIGURE 3.2: Graphical illustration of a twofold rotoinversion axis of symmetry.

0 1 0

0 0 , −1

Begin

0 1 0 = 0 1 0

0 −1 0 0 −1 0 0 −1 0 = 0 −1 0 0 0 −1 0 1 0

−1 0 0 −1 0 0

a = −( δij )

(3.1)

40 tensor properties of solids

which is obvious from an inspection of Figure 3.2. Here, the first and second matrices represent a center of symmetry and a 180° rotation about the 0x3 axis, respectively—the order is immaterial. Remember that the entries (1’s, −1's, and 0's in this case) in a transformation matrix represent the direction cosines as illustrated in Figure 2.1. Other combinations of the two fundamental symmetry elements are possible and are designated by certain symbology. An n-fold rotoinversion axis lying in a plane of symmetry is designated − as X m = n¯m. An n-fold rotation axis of symmetry perpendicular to a plane of symmetry is designated as X/m = n/m. As an example, consider a fourfold rotation axis of symmetry about 0x3 lying normal to the x1, x2 plane of symmetry. This symmetry operation designated as 4/m(= 42¯), has a transformation matrix

0 0 , −1

0 0 1 0 = −1 0 1 0 0

1 0 0

0 0 0 −1 −1 0

0 1 0

1 a= 0 0

(3.2)

TABLE 3.2: Symmetry transformation symbology used to identify the 32 point groups X

An n-fold rotation axis of symmetry

− X

An n-fold rotoinversion axis of symmetry

m

Plane of symmetry or mirror plane

X/m

Rotation axis with one mirror plane normal to it

X2

Rotation axis with a diad normal to it

− X 2

Rotoinversion axis with a diad normal to it

Xm

Rotation axis with one mirror plane parallel to it

− Xm

Rotoinversion axis with one mirror plane parallel to it

Xmm

Rotation axis with one mirror plane parallel to it*

X/mmm

Rotation axis with one mirror plane normal to it and one mirror plane parallel to it*

* The last element in three- and four-element forms such as Xmm and X/mmm is usually unnecessary to generate the group (see Table 3.6 for examples).

Crystal Systems, Symmetry Elements, and Symmetry Transformations 41

and the 4/m point group would be generated by repeated operations represented by the above transformation matrix product. The symbology used to identify the 32 point groups is presented in Table 3.2, where X and n are interchangeable, and all rotations are taken to be CCW (positive rotations).

3.3

SPACE LATTICES, UNIT CELLS, CRYSTALLOGRAPHIC PLANES, AND DIRECTIONS—MILLER INDICES

A crystal is defined as a special arrangement of atoms that repeats itself periodically in three dimensions. If this periodicity is precise and if it is continuous ad infinitum, the crystal is said to be perfect. Of course, real crystals cannot be perfect because they have finite bounds (free surfaces) and contain internal imperfections such as impurities, vacancies, dislocations, and usually subboundaries. We will treat crystals as being of finite dimensions but without internal defects. The atomic arrangement in a crystal is conveniently represented as a three-dimensional network of straight lines called a space lattice. The intersections of lines are points of the space lattice that may represent the residence of a single atom or a group of atoms distributed in some fashion about the point. There are 14 space lattices called Bravais lattices into which all crystal structures must fall. Each space lattice has some convenient set of axes that is conventionally used with it. Six different systems of axes are commonly used in crystallography. Each set of lattice axes 0x, 0y, 0z → → → represents the directions along which the primitive translation vectors a , b , c lie as illustrated in Figure 3.3. The six different systems of axes define the six crystal systems into which fall the 14 Bravais lattices and hence all the crystal structures possible. These are presented in Table 3.3 together with the unit cell axes and angles, the lattice symbols, and the minimum symmetry elements required for

z

c β

a

α

b

y

γ

x FIGURE 3.3: General space lattice showing the primitive translation vectors and angles.

42 tensor properties of solids

membership in each system. The lattice symbols P, F, I, C, and R are the Hermann–Mauguin notation for primitive (P), face-centered (F), body-centered (I), base-centered (C), and rhombohedral (R) unit cells. Thus, a given crystal system may exist as more than one Bravais lattice. For example, the orthorhombic crystal system exists in primitive, face-centered, body-centered, and base-centered crystal structures. The space lattice is then generated by the translation vector →

→

→

→

T = ma + pb + q c ,

(3.3)

where m, p, and q are integers. The totality of all such translation operations for all values of m, p, and q is called the translation group of the crystal. The magnitudes (a, b, and c) of primitive transla→ → → tion vectors a , b , c are called the lattice parameters, which, together with the lattice angles (α, β, γ ), define the unit cell of a crystal. Before continuing with the subject of macroscopic crystal symmetry elements and symmetry transformations, it will be instructive to review the notation for describing crystallographic planes and directions. Shown in Figure 3.4 are the generalized Miller and Miller–Bravais indices for planes and directions for the six crystal systems in Table 3.3 where the hexagonal and trigonal systems are treated together. Here, referring to Figure 3.4(a), the Miller indices for the plane (hkl ) are the reciprocals of the intercepts (1 / ix , 1 / iy , 1 / iz ). For example, if the intercepts are (ix = 1, iy = 1, iz = 1), then

z

z

(hkl) Plane

iz

ix x

(a) Miller Indices for all crystal systems

[UVTW]

y'

[uvw] Direction

iy

(hkil) Plane

y

Direction

120o

x

o

12 0

y

(b) Miller-Bravais indices for hexagonal and trigonal crystal systems

FIGURE 3.4: Notation for description of planes and directions showing Miller indices for all crystal systems and the Miller–Bravais indices for the hexagonal and trigonal crystal systems.

Crystal Systems, Symmetry Elements, and Symmetry Transformations 43

TABLE 3.3: The 14 Bravais lattices showing the conventional unit cell axes and angles together with their lattice symbols and minimum symmetry elements Crystal system

Unit cell axes and angles

Lattice symbols

Minimum symmetry elements

Triclinic

a ≠ b ≠ c ; α ≠ β ≠ γ

P

1 (or ¯ 1 )

Monoclinic

a ≠ b ≠ c ; α = γ = 90° ≠ β

P, C

2 (or ¯ 2 )

Orthorhombic

a ≠ b ≠ c ; α = β = γ = 90°

P, F, I, C

222 (or ¯ 2 2¯ 2¯)

Tetragonal

a = b ≠ c ; α = β = γ = 90°

P, I

4 (or 4¯ )

Trigonal and

a = b ≠ c ; α = β = 90°; γ = 120°

R, P

3 (or ¯ 3 ); 6 (or ¯ 6 )

a = b = c ; α = β = γ = 90°

P, F, I

4 triads along

hexagonal Cubic

taking the reciprocals of the intercepts gives (111) for the plane. As a second example, if the intercepts are (ix = 1, iy = 1/2, iz = 1/3) along axes 0x, 0y, and 0z, respectively, then the Miller indices for the plane would be (1, 2, 3). For the hexagonal and trigonal crystal systems represented in Figure 3.4(b), the i index in (hkil ) is determined by i = −(h + k) but is sometimes replaced by a dot as (hk.l ). The Miller indices for direction [uvw] are found by “walking” along all axes, x, y, and z in turn, from origin to the end of the lattice vector. Referring to Figure 3.3, one would measure distances along x, y, and z axes in units of a, b, and c, respectively, or their fractions. As an example, and again referring to Figure 3.3, a lattice vector represented by a, b, c would be designated by [111], or a lattice vector (1/2)a, −b, 0 in the x–y plane would be designated as [1/2, 1¯, 0] or clearing fractions [1, 2¯ , 0]. Referring to Figure 3.4(b), the same direction in the hexagonal and trigonal systems would be designated as [UVTW ] = [1, ¯2 , 1, 0], where T = −(U + V ). In the cubic system, for which a = b = c, any direction [uvw] is perpendicular to the plane (hkl ) of the same indices. Planes of the form are designated as {hkl} and {hkil }, whereas the directions of the form are indicated as 〈uvw〉 and 〈UVTW 〉. The four index forms apply specifically to the hexagonal and trigonal systems. The number of non-parallel planes of the form {hkl } is found by multiplying [permutation term] × [sign term]/2. For example {123} has [3!][23]/2 = 24 non-parallel planes of this form. Directions of the form 〈123〉 also have 24 nonparallel directions of that form.

44 tensor properties of solids

TABLE 3.4: The 32 conventional point groups showing crystal system, group number, and the international short symmetry notation Crystal system

Group number

International (short) notation

Triclinic

1

1

2

|| ¯1 ||

3

2

4

m

5

|| 2/m ||

6

222

7

mm2

8

||mmm||

9

4

10

4¯

11

|| 4 /m ||

12

422

13

4mm

14

4¯ 2m

15

|| 4 /mmm ||

Monoclinic

Orthorhombic

Tetragonal

Crystal Systems, Symmetry Elements, and Symmetry Transformations 45

TABLE 3.4: (continued) Crystal system

Group number

International (short) notation

Trigonal (rhombohedral)

16

3

17

|| 3¯ ||

18

32

19

3m

20

|| 3¯m ||

21

6

22

6¯

23

|| 6/m ||

24

622

25

6mm

26

¯6 m2

27

|| 6/mmm ||

28

23

29

|| m3 ||

30

432

31

4¯ 3m

32

|| m3m ||

Hexagonal

Cubic (isometric)

46 tensor properties of solids

3.4

THE MACROSCOPIC SYMMETRY OF CRYSTALS AND THE 32 CONVENTIONAL POINT GROUPS

The 32 conventional point groups are listed in Table 3.4 in the order of increasing symmetry. The symbols used to represent the symmetry elements characteristic of each crystal class belong to the Hermann–Mauguin international short system. There are two other systems used for this purpose. They are the full symbol notation and Schoenflies symbols; neither of which will be used in this text. The 11 point groups, designated by the symbol || X || in the seven crystal systems, each possess a center of symmetry and meet the requirements for complete (maximum) symmetry allowable for classification in that system. These 11 point groups are called the holohedral groups. Finally, it should be noted that a given point group is generated by the repeated symmetry operations required by the elements of that group. This fact will be important in later developments. A point group that contains a center of symmetry is called centrosymmetrical. A group contains a center of symmetry if the product of the transformation matrices, representing the symmetry elements of the group, becomes −(δij ), where (δij ) is the unitary matrix. As an example, the group 2/m has the following transformation matrix

0 cos(pπ) 0

0 0 , 1

0 cos(pπ) 0 0 −1 0

0 1 0

1 0 0

(3.4)

where p is an integer representing the repeated twofold rotation operation and π = 180°. Clearly, cos( pπ) = −1 for p = ±1, ±3, ±5... , and the transformation for 2/m above becomes –(δij), proving that 2/m contains a center of symmetry and is represented by || 2/m || in Table 3.4.

3.5

NEUMANN’S PRINCIPLE AND ITS APPLICATION TO TENSOR PROPERTIES

Basic and most important to a discussion of the effect of crystal symmetry on the tensor properties of crystals is Neumann’s principle, which states, The symmetry elements of any physical property of a crystal must include all the symmetry elements of the point group of the crystal. This means that the component of a tensor representing a property must remain invariant under a transformation of coordinates governed by a symmetry operation valid for the point group of the crystal. Mathematically, this is represented as

Tijk... = Tijk....

(3.5)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 47

TABLE 3.5: The 10 possible generating matrices are shown for both the s and σ forms

0 −1

0

Center of symmetry, −1 0 0 – s (1) = (1 ) = 0 −1 0

Direct inspection method: 1→ −1, 2→ −2, 3→ −3 Twofold CCW rotation about y, −1 0 0 s (2) = (2y) = 0 1 0

0 −1

0

Direct inspection method: 1→ −1, 2→2, 3→ −3 Twofold CCW rotation about z, −1 0 0 (3) s = (2z) = 0 −1 0

1

0

0

Direct inspection method: 1→ −1, 2→ −2, 3→3 Reflection plane ⊥ to x, −1 0 0 (4) s = (m ⊥ x) = 0 1 0

0

1

0

Direct inspection method: 1→ −1, 2→2, 3→3 Reflection plane ⊥ to y, 1 0 0 (5) s = (m ⊥ y) = 0 −1 0 1

0

0

Direct inspection method: 1→1, 2→ −2, 3→3

1 0 0 σ (1) = 0 0 0

0

0

0

0

1

0

0

0

0 1 0 0 0 0 1 0 0 0 0 1 0 0 0 0

0

0 0 =I 0 0 1

~=I σ −1 = σ

I is the identity (unit) matrix

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (2 ) = 0 0 0 −1 0 0 0 0 0 0 1 0 0 0 0 0 0 −1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (3 ) = 0 0 0 −1 0 0 0 0 0 0 −1 0 0 0 0 0 0 1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (4 ) = 0 0 0 1 0 0 0 0 0 0 −1 0 0 0 0 0 0 −1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (5 ) = 0 0 0 −1 0 0 0 0 0 0 1 0 0 0 0 0 0 −1

~ σ −1 = σ

48 tensor properties of solids

TABLE 3.5: (continued)

0 −1

0

Direct inspection method: 1→1, 2→2, 3→ −3 Threefold CCW rotation about z, −1/2 3/2 0 (7) s = (3z) = − 3/2 −1/2 0

0

1

0

Direct inspection method: not applicable Fourfold CCW rotation about x, 1 0 0 (8) s = (4x) = 0 0 1

0

−1

0

Direct inspection method: 1→1, 2→3, 3→ −2 Fourfold CCW rotation about z, 0 1 0 (9) s = (4z) = −1 0 0

0

1

0

Direct inspection method: 1→2, 2→ −1, 3→3 Cyclic interchange of xi, 0 1 0 s(10) = (3[111] ) = 0 0 1 0

0

1

σ (7) =

1/4

3/4

0

0

0

3/4

1/4

0

0

0

0 0 0 3/4 −

Direct inspection method: 1→2, 2→3, 3→1

0 0 0 3/4

1 0 0 0 −1/2 − 3/2 0 3/2 −1/2 0 0 0

− 3/2 3/2 0 0 0 −1/2

To form σ −1. interchange − 3 and 3

1 0 0 0 0 0 0 0 1 0 0 0 0 1 0 0 0 0 σ (8) = 0 0 0 −1 0 0 0 0 0 0 0 −1 0 0 0 0 1 0

~ σ −1 = σ

0 1 0 0 0 0 1 0 0 0 0 0 0 0 1 0 0 0 σ (9 ) = 0 0 0 0 −1 0 0 0 0 1 0 0 0 0 0 0 0 −1

~ σ −1 = σ

0 1 0 0 0 0 0 1 0 0 1 0 0 0 0 = 0 0 0 0 1 0 0 0 0 0 0 0 0 1 0

~ σ −1 = σ

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (6) = 0 0 0 −1 0 0 0 0 0 0 −1 0 0 0 0 0 0 1

Reflection plane ⊥ to z, 1 0 0 s(6) = (m ⊥ z) = 0 1 0

σ (10)

0

0 0 0 1 0

Crystal Systems, Symmetry Elements, and Symmetry Transformations 49

If, on the other hand, a particular component of a tensor changes sign after such a transformation of coordinates, the component must vanish for that crystal in accordance with Neumann’s principle. Mathematically, this is expressed as

Tijk... = −Tijk... = 0

(3.6)

Application of Neumann’s principle to property tensors requires the use of transformation laws for tensors. The transformation laws for both polar and axial property tensors must be valid for any symmetry operation permissible by a given point group. If s represents a symmetry operator, that is, the transformation matrix of a symmetry operation valid for a particular point group, then the generalized transformation laws become

Tijk... = simsjnsko ...Tmno

(3.7)

Tijk... = |s | simsjnsko ...Tmno

(3.8)

for polar property tensors and

for axial tensors, where |s| is the determinant of the symmetry operator (see Section 2.4). For a given crystal class, there will be as many sets of equations for each property tensor as there are symmetry operations valid for the point group of that class. However, the number of operators derived from these symmetry operations can be reduced considerably to some minimum number required to generate the point group. These are called generation operators, which result from the 10 (s) generating matrices given in Table 3.5. The σ generating matrices are the quadratic forms of the s matrices and are applicable only to symmetrical property tensors as represented by ~ (0)= I are Eq. (2.22) in Section 2.2.5. We note here that s(0) = (1) = (δij), σ (0) = I, and [σ (0)]−1 = σ identity (unit) matrices. The minimum number of generating matrices (derived from the 10 generating matrices in Table 3.5) required for each of the 32 point groups are given in Table 3.6. The point groups are designated by using the international short-form symbology as used in Table 3.4. The generating matrices will be used to determine the nonzero components of a given property tensor as required for a particular point group and in accordance with the appropriate transformation law. The symbol || X || appearing in Table 3.6 is used to designate the holohedral group defined earlier. The minimum generating matrices can also be used to generate the stereograms for the 32 point groups (see Endnotes). The work required for simplifying the components of a given tensor can be greatly reduced by recognizing that a tensor of rank r transforms like the products of r coordinates of a point. For example, the center-of-symmetry operator s(1) = (−δij ) requires that

50 tensor properties of solids

TABLE 3.6: Minimum generating matrices for the 32 point groups showing the 11 centrosymmetrical crystal classes designated by || X || Crystal system Triclinic

Monoclinic

Orthorhombic

Tetragonal

International Minimum symbol generating (short form) matrices 1

s(0)

|| 1¯ ||

s(1)

2

s(2)

m

s(5)

|| 2/m ||

s(2), s(5)

222

s(2), s(3)

mm2

s(3), s(5)

|| mmm ||

s(4), s(5), s(6)

4

s(9)

4¯

s(11)

|| 4/m ||

s(6), s(9)

422

s(12), s(9)

4mm

s(4), s(9)

¯4 2m

s(12), s(11)

|| 4/mmm ||

s(4), s(6), s(9)

(4 ¯ z) = s(1) . s(9) = s(11), (2x) = s(1) . s(4) = s(12)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 51

TABLE 3.6: (continued) Crystal system Trigonal

Hexagonal

Cubic

International Minimum symbol generating (short form) matrices 3

s(7)

|| 3¯ ||

s(13)

32

s(12), s(7)

3m

s(4), s(7)

|| 3¯m ||

s(4), s(13)

6

s(14)

6¯

s(15)

|| 6/m ||

s(6), s(14)

622

s(12), s(14)

6mm

s(4), s(14)

¯6 2m

s(4), s(15)

|| 6/mmm ||

s(4), s(6), s(14)

23

s(12), s(10)

|| m3 ||

s(4), s(10)

432

s(8), s(10)

¯4 3m

s(16), s(10)

|| m3m ||

s(4), s(10), s(17)

(3 ¯ z) = s(1) . s(7) = s(13), (6z) = s(3) . s(7) = s(14) (6 ¯ z) = s(1) . s(14) = s(15), (4 ¯x) = s(1) . s(8) = s(16)

m ⊥ (110) = s(4) . s(9) = s17

52 tensor properties of solids

→ −1 → −2 → −3

1 x2 → −x2 or 2 x3 → −x3 3

x1 → −x1

(3.9)

This means that for a polar property tensor of odd rank, any combination of subscripts will result in T ′ = −T = 0 in accordance with Neumann’s principle. Similarly, for an axial property tensor of even rank, any combination of subscripts will result in T ′ = −T = 0 also in accordance with Neumann’s principle. This process of simplification is called the method of direct inspection and is applicable to all point groups except those in the trigonal and hexagonal crystal systems. For a particular crystal class in these two systems, it is necessary to operate on a property tensor with each generating matrix in turn. The use of the quadratic generation operators is then recommended, especially for property tensors of rank greater than two. Note that throughout this text, the notation for crystallographic axes will adhere to the accepted convention x1 = x, x2 = y, and x3 = z in accordance with Figure 3.1.

3.6

APPLICATION OF NEUMANN’S PRINCIPLE TO SYMMETRICAL SECOND-RANK PROPERTY TENSORS

The macroscopic symmetry of a given crystal can dramatically affect the number of nonzero components of a property tensor that are permitted to exist in that crystal. This is easily demonstrated by applying Neumann’s principle to a symmetrical second-rank property tensor Sij , which may repre sent any of several properties to be studied in subsequent chapters. Typical examples are the dielectric susceptibility and thermal expansion coefficient. We begin with the triclinic crystal system and continue in the direction of increasing symmetry to the cubic system. For this purpose, use will be made of the generation matrices for the 11 holohedral point groups in Table 3.6—those possessing a center of symmetry and the necessary generating matrices for complete symmetry. As we progress from the triclinic to cubic system, use will be made of the method of direct inspection except for the trigonal and hexagonal systems as indicated earlier. 1. Triclinic system: Because all symmetrical second-rank property tensors are centrosymmetrical, they cannot be made null by the center-of symmetry operation. The symmetry transformation becomes

(1)

S11 S12 S31 S' = s S˜s = S = S12 S22 S23 S31 S23 S33 (1)

(3.10)

leaving the property Sij unchanged, with all six independent components needed to repre sent it.

Crystal Systems, Symmetry Elements, and Symmetry Transformations 53 (2)

2. Monoclinic system: The monoclinic system requires use of the generation operators s and s(5) via holohedral group || 2/m ||. Beginning with s(2), S′ transforms as

0 0 −1

0 1 0

S11 S12 S31 −1 S12 S22 S23 0 S31 S23 S33 0 S31 −S23 . S33

−1 0 0 0 1 0 0 −1 0 S11 −S12 S22 = Sym.

S' = s (2)S s˜ (2) =

(3.11)

Applying Neumann’s principle requires that S12 = S23 = 0, giving the result

Sym.

S31 0 , S33

0 S2

S11

S=

(3.12)

where S22 = S2 is a principal component along 0x2 = 0y. Application of operator s(5) leaves the result of Eq. (3.12) unchanged. The same result could have been obtained with greater ease by using the direct inspection method. For example, the use of generating matrix s(2) in Table 3.5 gives → −1 → 2 → −3

2 3

1

or

x1 → −x ′1 s(2) → x2 → x ′2 x3 → −x ′3

(3.13)

It now follows that components having a single 1 or single 3 subscript (but not both) must be zero in accordance with Neumann’s principle, that is, S23 = S12 = 0 (all others must remain nonzero), which is applicable to the three classes of the monoclinic crystal system. 3. Orthorhombic system: The holohedral group || mmm || has the generation matrices s(4), s(5), and s(6), which cover all classes of the orthorhombic system. From Table 3.5, these three operators are given by

→ 1 → 2 . → −3

s → 2 3

1 → 1 (6) → −2 s → 2 → 3 3

1

(5)

s → 2 3

→ −1 → 2 → 3

1

(4)

(3.14)

Taken separately and using the direct inspection method together with Neumann’s principle, the generation matrices s(4), s(5), and s(6) require all components having a single 1, a single

54 tensor properties of solids

2, or a single 3 be zero. Thus, S23 = S31= S12 = 0, with all others being nonzero. Therefore, S is now represented by

0 0 . S3

0 0 S1 S2 0 = S33 Sym.

0 S22 0

S11 S= 0 0

(3.15)

The arrays in Eq. (3.15) apply to all crystal classes of the orthorhombic system. The second- rank property components S1, S2, and S3 are the principal components along the crystallographic axes 0x = [100], 0y = [010], and 0z = [001], respectively. 4. Tetragonal system: The holohedral group || 4 /mmm || has the generating matrices s(4), s(6), and s(9), of which s(4) and s(6) have previously been used for the orthorhombic crystal system, and operator s(5) leaves these results unchanged. Then, applying the operator s(9) from Table 3.5 to the results of the orthorhombic system requires, by the direct inspection method, that

→ 2 → −1 . → 3

x1 → x ′2 1 s(9) → x2 → −x ′1 or 2 x3 → x ′3 3

(3.16)

The results are S31 = S32 = −S31 = 0 and S11 = S22 = S1 in accord with Neumann’s principle. This means that the property tensor Sij is everywhere isotropic in the x, y (001) plane. Thus, the components of Sij for all point groups of the tetragonal crystal system are represented by the array 0 0 . S3

Sym.

0 S1

S1

S=

(3.17)

5. Trigonal and hexagonal systems: The holohedral groups || 3¯m || and || 6 /mmm || contain generating operators s(1), s(3), s(4), s(6), and s(7). The application of the operators s(1), s(3), s(4), and s(6) to the tensor Sij will leave unchanged the results obtained for the tetragonal systems. Therefore, there remains only the application of the operator s(7). Because the method of direct inspection is not applicable here, we must perform the transformation given by

S ′ = s(7)S s~(7) = σ (7)S .

(3.18)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 55

But this transformation can be given more conveniently by using the quadratic transformation 0 0 − 3/2 S1 S1 3/2 S2 0 0 S1 S3 0 0 0 S3 = . −1/2 − 3/2 0 0 0 0 0 3/2 −1/2 0 0 0 −1/2 0 0

0 0 1 0 0 0

1/4 3/4 3/4 1/4 0 0 0 0 0 0 3/4 − 3/4

S ′ = σ (7)S =

(3.19)

This indicates that the components of Sij for all point groups of the trigonal and hexagonal crystal systems are the same as those for the tetragonal system. Consequently, these three systems may be treated as a single group with respect to symmetrical second-rank tensor properties. They are often called the optically uniaxial crystal systems. 6. Cubic system: The holohedral group || m3m || contains generation operators s(4), s(9), and s(10), all but s(10), of which have been applied to the previous, less symmetrical systems. So there now remains the application of the generation operator s(10), to the results obtained for the tetragonal, trigonal, and hexagonal systems. The method of direct inspection, which is again applicable, requires that

or

32

→ → →

2 3 . 1

1

→ x2 → x3 →

x′2 x′3 x′1

s

x1 →

(10)

(3.20)

Then by application of Neumann’s principle there results

S1 = S2 = S3 = S,

(3.21)

meaning that any cubic crystal system is isotropic with respect to any symmetrical second-rank property tensor. To summarize, the effect of crystal symmetry on properties that are represented by symmetrical second-rank tensors is given in Table 3.7. The effect of crystal symmetry on other tensor properties will be given at the time the individual properties are considered. This is especially desirable for the property tensors of higher rank because they often possess unique inherent symmetry. This is particularly true for the axial and axial–magnetic property tensors for which both axial and magnetic symmetry must be considered.

56 tensor properties of solids

TABLE 3.7: Effect of crystal symmetry on symmetrical second-rank tensor properties

0 S2

Sym.

S33

0 S1

Sym.

Cubic

s (4), s (9), s (10)

S

S3 0 S

0

Sym.

0 0 S

0

S1

s (1), s (3), s (4), s (6), s (7), s (9)

S3

Tetragonal, trigonal, and hexagonal

0

Sym.

0

0 S2

0

S1

S31

S33

s (4), s (5), s (6)

S 11

S23

Orthorhombic

Sym.

S31

s (2), s (5)

S12 S22

Monoclinic

S11

s (1)

Triclinic

Independent components of the property matrix

System

Holohedral generating matrices

3.7 EFFECT OF NEUMANN’S PRINCIPLE ON THE 11 CENTROSYMMETRICAL CRYSTAL CLASSES With reference to Table 3.6, it is clear that each of the 11 holohedral groups, those designated by || X ||, contain the center-of-symmetry operator s (1) = (−δij), which requires that the symmetry transformations of (3.9) be applied to any crystal system that contains a center of symmetry. As a result, Neumann’s principle requires that for all centrosymmetrical crystal classes

for axial tensors of even rank

for polar tensors of odd rank

T ′= −T = 0 ⇒

.

(3.22)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 57

Thus, all 11 of the centrosymmetrical crystal classes, those that contain a center-of-symmetry, will be lacking in odd-rank polar tensor properties and even-rank axial tensor properties. For example, the piezoelectric tensor dikl , included in Eq. (2.54), is a polar third-rank tensor property whose property components vanish for any of the 11 centrosymmetrical (holohedral) classes designated by || X || in Tables 3.4 and 3.6. Another example is the pyroelectric coefficient defined by ∆Pi = Pi ∆T, where the three components of pi are null for any of the 11 centrosymmetrical crystal classes. All axial and axial–magnetic tensor properties of even rank will be lacking property components for any of the centrosymmetrical crystal classes. The 90 magnetic point groups come into play only for magnetic and axial–magnetic tensor properties of odd rank, further reducing the number of existing components over those required strictly by conventional symmetry arguments.

3.8 LONGITUDINAL AND TRANSVERSE EFFECTS FOR SYMMETRICAL SECOND-RANK PROPERTY TENSORS Use of either the longitudinal or transverse effects, or both, offers a convenient and practical means of measuring the components of symmetrical second-rank property tensors. To demonstrate these effects, it will be helpful to consider the symmetrical second-rank tensor as being a property relating a cause parameter q to an effect parameter p according to pi pj Sij = q = q = Sji . j i

(3.23)

Referring to Figure 2.1, with the transformation matrix represented as

a11 a12 a13 l1 l2 l3 a = a21 a22 a23 = m1 m2 m3 a31 a32 a33 n1 n2 n3

(3.24)

for convenience, the generalized transformation law for longitudinal and transverse effects becomes

m1 m2 m3

n1 n2 . n3

l1 l2 l3

S31 S23 S33

S12 l1 l2 l3 S11 ~ S' = aSa = m1 m2 m3 S22 n1 n2 n3 Sym.

(3.25)

Equation (3.25) is valid for any crystal system in which the property Sij is manifest. We will now explore the effect of crystal symmetry on the longitudinal and transverse effects. 1. Triclinic system: For the triclinic system, no restrictions are placed on the orientation of the reference axes. If the effect parameter p is sensed along the 0x′1 when the cause parameter q is applied in that same direction, the longitudinal effect for the triclinic system is given by

58 tensor properties of solids

S12 S22

S11

S31 l1 l2 l3 . S23 . l2 S33 l3 Sym. = l12 S11 + l22 S22 + l32 S33 + 2l2 l3 S23+ 2l3 l1 S31+ 2l1l2 S12.

p'1 S'11 = q = l1 '1

(3.26)

Here, the longitudinal effect is simply the magnitude of S measured along some arbitrary direction 0x′1. Similarly, if p is sensed along 0x′1 when q is applied along 0x′2 , or vice versa, the transverse effect given by

S11

S31 m1 S23 . m2 S33 m3 Sym. = l1m1S11 + l2m2S22 + l3m3S33 + (l2m3 + l3m2)S23 +

S12 S22

(l3m1 + l1m3)S31 + (l1m2 + l2m1)S12

l3 .

l2

p'1 p'2 S'12 = q = q = l1 '2 '1

(3.27)

is also applicable to the triclinic crystal system. Thus, to measure all six independent components of Sij , six independent measurements must be made using either the longitudinal effect or transverse effect or some suitable combination thereof. The six resulting equations must then be solved simultaneously to obtain the six components. 2. Monoclinic system: Applied to the monoclinic crystal system, Eqs. (3.26) and (3.27) for the triclinic system can be simplified to the extent that S23 = S12 = 0, as indicated in Table 3.7. All other terms in thee expressions remain the same, with S22 = S2 = S[010] being the principal component along 0x2 = 0y = [010]. Four independent measurements, using either the longitudinal or transverse effects or some combination of them, will yield four independent equations from which the four independent components of Sij can be obtained. Note that the magnitude of the property S′11 measured along the axis of symmetry 0x2 = 0y is the principal component S2. 3. Orthorhombic system: The longitudinal and transverse effects can be put into special forms for the orthorhombic crystal system when we note that S23 = S31 = S12 = 0 and that the principal axes lie along the crystallographic axes. The longitudinal effect now becomes

S 11 ′ = p 1′ / q 1′ = l 12S 1 + l 22S 2 + l 32S 3 2 2 2 S[100] + l [010] S[010] + l [001] S[001], = l [100]

(3.28)

where l〈100〉 are the direction cosines between any direction 0x′1 = [uvw] and the crystallographic (principal) axes, [100], [010], and [001], and S〈100〉 represent the three principal

Crystal Systems, Symmetry Elements, and Symmetry Transformations 59

components along these axes. Similarly, if the direction 0x′2 = [m1, m2, m3] is also taken with respect to the crystallographic axes, the transverse effect for the orthorhombic crystal system is given by

S 12 ′ = p 1′ / q 2′ = p 2′ / q 1′ = l1m1S 11 + l2m2S 22 + l3m3S 33 = l[100] m[100]S[100] + l[010]m[010]S[010] + l[001]m[001]S[001]

(3.29)

Thus, knowing the orientation of the principal axes, three independent measurements using either the longitudinal effect or transverse effect or both, will yield the principal values S1, S2, and S3. 4. Tetragonal, trigonal, and hexagonal systems: For the optically uniaxial crystal systems (tetragonal, trigonal, and hexagonal) the longitudinal effect requires measurement of the two independent components, S1 and S3, along any two arbitrary, but different, directions (one direction must be out of the (001) or (0001) plane). Accordingly, the longitudinal effect is established from Eq. (3.28) as

2 2 2 S 11 ′ = p 1′ / q 1′ = (l [100] + l [010] )S[100] + l [001] S[001] 2 2 = (1 - l [001])S[100] + l [001]S[001]

(3.30)

since now S[100] = S[010] due to the isotrophy of property S in the (001) or (0001) plane for the optically uniazial crystal systems. Defining the Eulerian angles θ and φ, as shown in Figure 3.5, the longitudinal effect takes the form S 11 ′ = S⊥sin2φ + S||cos2 φ

z = [001] [uvw]

φ y = [010]

θ x = [100] FIGURE 3.5: Arbitrary direction [uvw] expressed in terms of the Eulerian angles φ and θ.

(3.31)

60 tensor properties of solids

independent of θ. Here S⊥ = S〈uv 0〉 is the magnitude of the property along any direction 〈uv 0〉 perpendicular to the [001], and S|| = S[001] is the magnitude of the property parallel to the [001] direction. Consequently, the magnitude of the property in any direction [uvw] = 0x′1 depends only on the angle φ and the values S⊥ and S||. For the trigonal and hexagonal crystal systems, the longitudinal effect may be represented alternatively as

S 11 ′ = S〈UV T 0〉sin2φ + S[0001]cos2 φ

(3.32)

for measurement in any direction 0x′1 = [UV TW]. The transverse effect for the optically uniaxial crystal systems is established from Eq (3.29) noting again that S[100] = S[010] = S⊥ and S[001] = S||. Therefore, by knowing the direction cosines for directions 0x1′ = [l1, l2, l3] and 0x2′ = [m1, m2, m3] with respect to the crystallographic axes, the transverse effect can be measured. As always, the transverse effect is more difficult to measure than the longitudinal effect. 5. Cubic system: For the cubic system, the magnitude of the property S is the same in all directions, that is, it is isotropic relative to the property S and requires only one measurement of its magnitude in any direction. • • • •

61

chapter 4

Generalized Thermostatics and the Systematic Correlation of Physical Properties 4.1 Energy Representations and the Criteria for Thermodynamic Equilibrium In classical thermodynamics, the first law is expressed as the change in internal energy of a closed system given by

dU = d−Q + d−W,

where d−Q is the thermal energy (heat) transferred to the system and d−W is the external work done on the system. Here, d−Q and d−W are inexact differentials called Pfaffians—they are path-dependent. For a closed solid-phase system, the infinitesimal change in internal energy is given by the first and second laws of thermodynamics as _ dU = d Q +

_

_

Σi dWi = T dS + dW

_ _ _ + dWMag.+ dWMech.+ dWChem.

Elect.

(4.1)

in which d−Q = TdS is the infinitesimal reversible heat absorbed by the solid-phase system at an absolute temperature T, and dS is the infinitesimal entropy change associated with the absorbed heat d−Q. Σd−W is the sum of all infinitesimal reversible work (electrical, magnetic, mechanical and i

i

chemical) done on the solid-phase system by the surroundings. Each work term in Eq. (4.1) is represented by the product of a particular intensive parameter and an infinitesimal change in its conjugate extensive parameter. In crystalline materials, the atoms are essentially immobile compared to the gaseous (or liquid) state. This complicates the energy representation. For example, in classical PVT thermodynamics, pressure P is an adequate intensive parameter for gases, but it is not adequate to describe the effect of applying surface forces to a solid. Similarly, volume V, used as the extensive parameter for gases, must be replaced by reference volume times strain V0e for solids. Thus, –PdV work in the classical sense (for gases) must be replaced by

62 tensor properties of solids

Table 4.1: Intensive and extensive parameters for a solid-state system and their SI units Intensive Parameters

Extensive Parameters

T — Temperature (°K)

S — Entropy ( J/°K)

E — Electric field intensity (V/m)

Pˆ — Total electric dipole moment (Cm)

B — Magnetic flux density (N / A · m = tesla, T)

I — Total magnetic dipole moment (Am2)

s — Stress (N/m2)

V0e — Strain times reference state volume (m3)

m —Chemical potential ( J/mol)

N — Mole number

elastic strain energy sd (V0e) for the case of solids. Furthermore, the fact that solids can develop a net polarization or magnetization adds additional complications to the energy representation— electrical and magnetic work terms must be added. The intensive and extensive parameters that best describe the equilibrium tensor properties of crystals are presented in Table 4.1 along with their SI units. Note that the magnetic intensive parameter is the magnetic flux density B = m0 H measured in the absence of the crystal system (m0 is the permeability in a vacuum and H is the magnetic field strength). Using these parameters, the total infinitesimal change in internal energy for a solid-phase system is given by

dU = T dS + E dPˆ + B dI + σ d (ε V0 ) + µ d N

(4.2)

in agreement with the respective work terms given in Eq. (4.1). From Euler’s theorem on homogeneous first-order forms, the corresponding Euler relation is given by

U = T S + EPˆ + BI + σ (ε V0 ) + µ N .

(4.3)

The Euler relation is a thermodynamic potential seen to combined first and second laws of thermodynamics in terms of the product of conjugate parameters (in energy units of Joules, J ) given in Table 4.1. The Euler relation will later be used in the generation of other useful thermodynamic potentials for a closed solid-phase system of one component (dN = 0). Differentiating Eq. (4.3) gives the result dU = T dS + S d T + E d Pˆ + Pˆ d E + B dI + I dB + σ d (ε V0 ) + (ε V0 ) d σ + µ d N +N d µ ,

Generalized Thermostatics and correlation of Physical properties 63

which compared to Eq. (4.2) requires that

S d T + Pˆ d E + I dB + (ε V0 ) dσ + N d µ = 0

(4.4)

Equation (4.4) is the general form of Gibbs-Duhem equation for a solid-phase system of a single component (d N = 0). The concepts of equilibrium and spontaneous (irreversible) processes are best understood in terms of the thermodynamic potentials G and F called the Gibbs and Helmholtz free energies, respectively. The extended Gibbs free energy for a single component solid-phase system is defined as

G ≡ µ N = U − TS − E Pˆ − BI − σ (ε V0 ),

(4.5)

which follows from the Euler relation. This potential is the Legendre transform of U that simulta- neously replaces S by T, Pˆ by E, I by B and eV0 by s as the independent variables. Differentiating Eq. (4.5) for a closed solid-phase system of one component and introducing Eq. (4.2) gives the infinitesimal change in Gibbs free energy

dG = − S dT − Pˆ d E − I d B − (ε V0 ) dσ

(4.6)

In actual experimental situations, it is often a simple matter to hold the intensive parameters constant. When this is done, that is, when T, E, B, and s are held fixed, the solid-phase system is said to be thermally, electrically, magnetically and mechanically free resulting in

dG = 0

(4.7)

as the criterion for thermodynamic equilibrium. When one or more of the intensive parameters are varied, then

dG < 0 ,

(4.8)

and the process is said to be spontaneous or irreversible. Clearly, the condition dG > 0 applies to a process that will not take place without changing the thermodynamic parameters of the system. The Helmholtz free energy is a thermodynamic potential defined as

F ≡ U − TS .

(4.9)

Thus, the Helmholtz free energy is the Legendre transform that replaces the entropy S by temperature T as the independent variable. Differentiating Eq. (4.9) for a closed solid-phase system of one component and introducing Eq. (4.2) gives the infinitesimal change in the Helmholtz free energy as

d F = − S dT + E d Pˆ + Bd I + σ d(ε V0 )

(4.10)

64 tensor properties of solids

which eliminates the difficult task of holding entropy constant to establish equilibrium but retains the extensive parameters Pˆ, I, and eV0 as the independent variables. Thus, in experimental situations when T, Pˆ, I, and eV0 are held constant, the system is said to be thermally free but electrically, magnetically, and mechanically, clamped. Under these conditions,

d F = 0

(4.11)

as the criterion for thermodynamic equilibrium. It also follows that d F < 0 corresponds to an irreversible or spontaneous thermally free process at constant Pˆ, I, and e, whereas d F > 0 corresponds, to a spontaneous isothermal but electrical, magnetic and mechanical clamped process. Other thermodynamic potentials may also serve usefully as criteria for thermodynamic equilibrium under the appropriate clamped and/or free conditions.

4.1.1 Energy Density Representation In applying thermodynamic arguments to solid-state systems in which the various tensor components must be manipulated, it becomes burdensome to carry the reference volume V0 along with strain to establish the true extensive mechanical parameter. Because the strains are infinitesimal in magnitude, all equations can be divided by the volume of the fiducial or reference state, which is equal to the instantaneous volume V0 of the solid phase. When this is done, the internal energy density and Gibbs free energy density for a closed system of one component (dN = 0) become

d u = dU / V0 = T ds + E d P + B d M + σ d ε

(4.12)

d g = dG / V0 = − s d T − P d E − M d B − ε d σ ,

(4.13)

and

respectively. The extensive parameters are now defined as follows: s = S / V0 = entropy density ( J/°K/m3), P = Pˆ / V0 = total electric dipole moment/unit volume = polarization (C/m2), M = I / V0 = total magnetic dipole moment/unit volume = magnetization (A/m), and e = eV0 / V0 = elastic strain (dimensionless). The criteria for equilibrium still apply but in energy density form, and the Euler relation u = U / V0 and Helmholtz free energy density f ≡ u – Ts follow from the above definitions. By using the energy density representation for simplicity, other thermodynamic potentials, in addition to g and f, can be generated by Legendre transformations of u. Listed in Table 4.2 are the 16 thermodynamic potentials and their differentials for a closed solid-phase system of one component. Some of these will prove to be useful. For example the generalized enthalpy density h, which is given by thermodynamic potential φ5, is used to define the heat capacity of a solid at constant E, B,

Generalized Thermostatics and correlation of Physical properties 65

Table 4.2: The 16 thermodynamic potential densities and their differentials for a closed solid state system of one component Thermodynamic Potentials

Thermodynamic Potential Differentials

φ1 = u − Ts − EP − BM − σε = g

dg=−sdT−PdE−MdB−ε dσ

φ2 = u − Ts − EP − BM

d φ2 = − s d T − P d E − M d B + σ d ε

φ3 = u − Ts − EP − σε

d φ3 = − s d T − P d E + B d M – ε d σ

φ4 = u − Ts − BM − σε

d φ4 = − s d T + E d P − M d B − ε d σ

φ5 = u − EP − BM − σε = h

dh=Tds−PdE−MdB−ε dσ

φ6 = u − Ts − EP

d φ6 = − s d T − P d E + B d M + σ d ε

φ7 = u − Ts − BM

d φ7 = − s d T + E d P − M d B + σ d ε

φ8 = u − Ts − σε

d φ8 = − s d T + E d P + B d M − ε d σ

φ9 = u − EP − BM

d φ9 = T d s − P d E − M d B + σ d ε

φ10 = u − EP − σε

d φ10 = T d s − P d E + B d M − ε d σ

φ11 = u − BM − σε

d φ11 = T d s + E d P − M d B − ε d σ

φ12 = u − Ts

= f

d f = − s d T + P d E + M d B + ε d σ

φ13 = u − EP

d φ13 = T d s − P d E + B d M + σ d ε

φ14 = u − BM

d φ14 = T d s + E d P − M d B + σ d ε

φ15 = u − σε

d φ15 = T d s + E d P + B d M − ε d σ

φ16 = u = u

du=Tds+EdP+BdM+σ dε

and s, which is analogous to CP in the classical sense. Still other potentials, such as φ2, φ3, φ4, and including φ5 are useful in developing Maxwell’s relations for the dependent coupled effects holding certain intensive parameters constant. The reader will note that the differential forms dφi result by differentiating φi followed by introduction of Eq. (4.12), du = T d s + E d P + B d M + σ d ε to complete the Legendre transform of u. For example, differentiating φ13 = u – EP gives dφ 13 = d u − E d P − P d E = T d s + E d P + B d M + σ d ε − E d P − P d E = Td s − P d E + B d M + σ dε

4.2

Thermodynamic Definition of Parameters

Taking any closed solid-state system of one component (d N = 0) in which reversible processes are occurring, the fundamental equation of state becomes u = u (s, Pi , Mi , εij ), where the tensor rank of the

66 tensor properties of solids

extensive parameters is indicated by the number of subscripts. Expanding an infinitesimal change in u in a Taylor series and neglecting the second, and higher-order differential terms, we write the first-order terms of du as

∂u ∂u ∂u d s + dPi + ∂ s P,M,ε ∂ Pi s,M,ε ∂ Mi

du =

∂u d Mi + ∂ε s,P,ε ij

= T d s + Ei d Pi + Bi d Mi + σij dεij (i, j = 1−3).

dεij s,P,Μ (4.14)

By comparing coefficients, we find the following thermodynamic definitions for the intensive parameters by holding certain extensive parameters constant as indicated by the symbols subscripted to the curved brackets: The absolute temperature

(4.15)

∂u ≡T ∂ s P,M,ε

∂u ≡ Ei ∂Pi s,M,ε

The external electric field strength vector

(4.16)

The external magnetic flux density vector

(4.17)

∂u ≡ Bi ∂Mi s,P, ε

The stress tensor.

(4.18)

∂u ∂ε ij

≡ σij s,P,M

In these definitions, T is a scalar and is specified by one component, Ei and Bi are vectors each specified by three components (Bi is axial magnetic in character), and σij is usually a symmetrical secondrank polar tensor (σij = σji ) specified by six components as in Eqs. (2.17) and (2.20). Now, let the letter I represent the intensive parameters (T, Ei , Bi , σij ) and the letter e represent the extensive parameters (s, Pi , Mi , εij ) so that an infinitesimal change in the internal energy density is given in the compact form d u = Im d em

(m = 1–13).

(4.19)

Here, the sequence (T d s + E1 d P1 + E2 d P2 + E3 d P3 + B1 d M1 + B2 d M2 + B3 d M3 + σ1 d ε1 + σ2 d ε 2 + ... σ 6 dε6 )

Generalized Thermostatics and correlation of Physical properties 67

has been written in the form ( I1 d e1 + I2 d e2 + ... + I13 d e13 ), where the stress and strain components have been unfolded according to the matrix scheme of Eq. (2.20) for symmetric second-rank tensors. In a similar manner, the extensive tensor parameters can be defined by using the generalized Gibbs free energy density. For any closed solid-phase system of one component, the fundamental equation of state becomes g = g (T, Ei , Bi , σij ), and we write for the first differential of g ∂g dg = ∂T

E,B,σ

∂g dT + ∂ Ei

∂g d Ei + T,B,σ ∂Bi

d Bi + T,E,σ

∂g ∂σ ij

dσij T,E,B

= − s d T − Pi d Ei − Mi d Bi − εij dσij .

(4.20)

Again, by comparing coefficients there results the following definitions for the extensive parameters of a closed system holding certain intensive parameters constant:

∂g ∂ T E,B,σ

−

≡s

The entropy density

∂g − ≡ Pi The total electric dipole moment per unit volume E ∂ i T,B,σ or (polarization) ∂g − ∂ Bi

(4.22)

≡

Mi The total magnetic dipole moment per unit volume T, E, σ or (magnetization)

∂g − ∂σ ij

(4.21)

≡ εij The strain tensor. T, E, B

(4.23) (4.24)

As with their conjugate intensive parameters, s is a scalar, Pi and Mi are vectors of three components each (Mi is axial magnetic in character), and εij is usually represented as a symmetrical second-rank tensor (εij = εji ) specified by six components as in Eq. (2.20). An infinitesimal change in the Gibbs free energy density may also be represented in the compact form

68 tensor properties of solids

dg = − em dIm

(m = 1 − 13),

(4.25)

where (e1 dI1 + e2 dI2 + ... + e13 dI13) represents the sequence ( s d T + P1 d E 1 + P2 d E 2 + P3 d E 3 + M1 d B1 + M 2 d B 2 + M 3 d B 3 + ε 1d σ 1 + ε 2 d σ 2 + ... ε 6 d σ 6 ). Here again, the stress and strain components have been unfolded according to the scheme given by Eq. (2.20).

4.3

Generalized Compliance and Rigidity Matrices

We now wish to know how the reversible variation of all intensive parameter components affect a given extensive parameter component and vice versa. Consider, as an example, the equation of state for the polarization of a solid-state system of one component as a function of the four intensive parameters given by Pi = Pi(T, Ej , Bj , σkl). In this case, an infinitesimal change in polarization is given by the Taylor series 1 ∂ ∂ ∂ dPi = ∑ dT ∂T + dE k ∂E + dB k ∂B + dσkl n = 1 n! k k ∞

∂ ∂ σkl

n

Pi (T , E , B ,σ ).

(4.26)

Similar Taylor series expansions can also be given for the remaining three equations of state s = s (T , Ek ,Bk , σkl ); Mi = Mi (T , Ek , Bk , σkl )

ε ij = εij (T ,Ek,Bk , σkl ).

(4.27)

Carrying out these Taylor series expansions and accepting only the first-order terms (n = 1), thus neglecting the second- and higher-order differential terms, the infinitesimal changes in the extensive parameters are given by the linear first-order equations:

∂s ∂s ds = dT + ∂ T E,B,σ ∂ Ek ∂P d Pi = i ∂T

E,B,σ

∂ Mi d Mi = ∂T

∂ε dε ij = ij ∂T

∂P dT + i ∂ Ek

E,B,σ

E,B,σ

T,B,σ

∂s d Ek + ∂ Bk

∂P d Ek + i T,B,σ ∂ Bk

T,E,σ

∂ Pi d Bk + T,E,σ ∂σ kl

∂ Mi ∂ Mi dT + dEk + ∂ Ek T,B,σ ∂ Bk

∂ε dT + ij ∂ Ek

T,B,σ

∂ε d Ek + ij ∂ Bk

∂s d Bk + ∂ σkl

T,E,σ

T,E,σ

dσkl T,E,B

dσkl T,E,B

∂ Mi d Bk + ∂ σkl

∂ε d Bk + ij ∂ σkl

dσ kl T,E,B

dσkl . T,E,B

(4.28)

Generalized Thermostatics and correlation of Physical properties 69

The partial derivatives are called the property compliances, where the subscripts indicate those intensive parameters that are held constant. Now, we designate the property compliances by the letter C with the appropriate subscripts and superscripts, such that (∂s / ∂T )E,B,σ = C s,T, (∂s / ∂Ek )T,B,σ = Cks,E, etc., thereby permitting us to set Eqs. (4.28) in the matrix form given by Eq. (4.29). This matrix equation is called the general property compliance matrix for first-order equilibrium properties. The tensor rank of any compliance is indicated by the number of subscripts it has. Thus, it is ε,σ . seen that the tensor rank varies from zero for C s,T to rank 4 for the compliance Cijkl

ds C dP C P,T i= i dMi C M,T i ε,T dεij Cij s,T

Cks,E

Cks,B

CiP,E k

CikP,B

CiM,E k

CiM,B k

Ciεjk,E

Ciεjk,B

Ckls,σ dT CiP,σ kl dEk ⋅ CiM,σ dBk kl ε,σ dσ Cijkl kl

( i, j , k , l = 1 − 3 )

(4.29)

A close inspection of the compliance matrix (4.29) reveals that it is, in reality, a (13 x 13) matrix of tensor components if stress and strain are taken as symmetrical second-rank tensors. This is illustrated in Table 4.3 where the individual property matrices are designated by (r × c), meaning rows by columns. The four principal effects of the property compliance matrix lie along its leading diagonal and are shaded. The off-diagonal compliances represent the coupled (interaction) effects. If we let e represent the extensive parameter components and I represent the intensive parameter components, then the set of linear first-order equations for the compliances in Table 4.3 are expressed in contracted subscript form as

dem = Cmn d In ( m , n = 1 − 13 ),

(4.30)

where it follows that C11 = C s,T = (∂ s / ∂ T )E,B,σ

C12 = C s,E1 = (∂ s / ∂ E1 )T, E

2, E3,B,σ

C29 = CP1, σ2 = (∂P1 / ∂ σ2 )T,E,B,σ ,σ

, σ 1 3 � 6

C46 = CP3, B2 = (∂ P3 / ∂ B2 )T, E, B

1 , B2 , σ

C13,13=C ε6, σ6 = (∂ ε 6 / ∂ σ 6 )T,E,B,σ

,σ ,...σ 1 2 5

(4.31)

70 tensor properties of solids

Table 4.3: Component arrangement of the general compliance matrix emphasizing the principal effects along the leading diagonal (shaded regions), all other being the coupled effects n→

m ↓ 1

s

2 P1 3 P2 P3 4 5 M1 6 M2 7 M3 8 ε1 9 ε2 10 ε 3 11 ε 4 12 ε 5 13 ε 6

1

2

T

E1 E2

3

4

5

E3

B1 B2

6

7

8

9

B3

σ1 σ2

10

11

12

13

σ3

σ4

σ5

σ6

C s,T (0)

C s,E (1 × 3)

C s,B (1× 3)

C s,σ (1 × 6)

C P,T (3 × 1)

C P,E (3 × 3)

C P,B (3 × 3)

C P,σ (3 × 6)

C M,T (3 × 1)

C M,E (3 × 3)

C M,B (3 × 3)

C M,σ (3 × 6)

C ε ,T (6 × 1)

C ε ,E (6 × 3)

C ε ,B (6 × 3)

C ε ,σ (6 × 6)

Thus, a given compliance is a quantity that expresses the rate of change of one particular extensive property component with respect to an intensive property component holding all other intensive parameter components constant. Following the same procedure, the intensive parametric equations of state are

T = T (s ,P,M , ε )

E = E (s , P, M , ε )

B = B (s ,P ,M , ε )

σ = σ (s ,P , M , ε )

(4.32)

From these, there results the following linear first-order equations expressing the infinitesimal changes in intensive parameters as functions of infinitesimal changes in the extensive parameters:

Generalized Thermostatics and correlation of Physical properties 71

dT R dE RE,s i= i dBi RB,s i d σij Riσ,j s

T,s

RkT,P

RkT,M

RiE,P k

RiE,M k

RiE,P k

RikB,M

Riσ,P jk

Rijkσ,Μ

RT,k ε ds REikl,ε dP k ⋅ RiB,klε dMk Rijσ,klε d ε kl

( i, j , k , l = 1 − 3 )

(4.33)

Here, the R matrix is called the general property rigidity matrix for the first-order equilibrium tensor properties. Equations (4.33) can be represented in contracted tensor subscript form as d Im = Rmn d en

(m ,n = 1−13 ),

(4.34)

where it follows that the rigidity and compliance matrices have an inverse relationship given by R = C -1.

(4.35)

The rigidities have the meaning that R11= RT,s = (∂ T / ∂ s )P,M,ε

R46 = RE3,M2 = (∂ E3 / ∂ M2)s,P,M

1,M2 , ε

1

R13,13 = R σ6 , ε6 = (∂σ6 / ∂ε6 )s, P, M, ε

1, ε2, ... ε5.

(4.36) In the above developments, only infinitesimal reversible changes in the intensive and extensive parameters were considered, and all solid-phase systems were assumed closed on their bound- aries. Furthermore, we have suppressed the names of the various property compliances and rigidities until symmetry considerations have been discussed in the next section. Let it suffice for now to say that the properties along the leading diagonals of the general compliance and rigidity matrices each represent four principal effects, whereas the off-diagonal symbols represent the 12 interaction effects often called coupled effects.

4.4

Symmetry of the General Compliance and Rigidity Matrices

The thermodynamic potentials listed in Table 4.2 are functions of thermodynamic properties of a given solid, and each of the thermodynamic properties has only one definite value for any given

72 tensor properties of solids

state of the solid. A thermodynamic property is, therefore, any quantity that depends on the state of the solid and that is independent of the path taken to reach that state. Such quantities are called state functions and form exact differentials. For the intensive and extensive parameters that are field tensors of rank 1 or 2 (T and s are scalars), the term thermodynamic property refers to an individual component of the tensor. For example, φ = g in Table 4.2 represents the Gibbs free energy density g(T , E , B , σ) = g(T , E1 , E2,E3 , B1 , B2 , B3 , σ1, σ2, ... σ3) in which g is given as function of 13 thermodynamic properties (intensive parameter components). Thus, it follows that although g is intensive in nature, internal energy density u is extensive in nature and all other φi in Table 4.2 are of mixed character. Consider any thermodynamic property ζ( p,q) of a solid that is a function of any other two thermodynamic properties, p and q. Now suppose that the substance is taken from its initial thermodynamic state through a series of states allowing p and q to vary independently in some arbitrary manner and that the process may be either reversible or irreversible. Finally, if the substance is returned to its initial state, we would notice that ∆ ζ = 0 since ζ depends only on the initial and final states, which, in this case, are the same. The independence of path of a given thermodynamic property ζ is expressed mathematically by Green’s theorem in a plane (special case of Stoke’s theorem) given by

∫

∂ς ∂ p

∂ς d p + ∂q

d q

ς ( p, q ) =

∫

C

=

∫

(M d p + N d q ) = − C

C

∫

∂ M ∂N d p d q = 0 − S ∂ q p ∂ p q

(4.37)

for any simple closed path C in a given region R′. It follows, therefore, that

∂ N ∂ 2ς ∂ 2ς ∂M = = = ∂ p ∂ p ∂q ∂ q∂ p ∂ q

(4.38)

if M( p,q) and N( p,q) have continuous derivatives in region R′. Simply stated, the order of differentiation of any thermodynamic property ζ is immaterial. This result is essential in describing the symmetry of the generalized compliance and rigidity matrices from which come the Maxwell relations. It will also be most useful when discussing the symmetry of second- and higher-order tensor properties in subsequent chapters. We now apply Eq. (4.38) to the extended Gibbs free energy density. From Eq. (4.25) for any component, em of an extensive parameter is defined by em = −

∂g . ∂Im

(4.39)

Generalized Thermostatics and correlation of Physical properties 73

Also, its infinitesimal change is related to an infinitesimal change in a component of an intensive parameter given by d em = Cmn d In, where the compliance is defined by

Cmn =

∂ em . ∂In

(4.40)

Because the order of differentiation is immaterial, we have the important result that

∂ em ∂e ∂2 g ∂2 g =− =− = n ∂ In ∂ In ∂Im ∂ Im ∂ In ∂ In

(4.41)

or

Cmn = Cnm .

(4.41a)

The meaning of Eq. (4.41) is straightforward. With reference to Table 4.3, only the principle effects (those along the diagonal and shaded) possesses self-symmetry expressed by

~ ~ ~ CP,E = CP,E, CM,B = CM,B, C ε,σ = C ε,σ ,

meaning that the principle property compliance matrices (of components) taken separately are equal to their transpose. All other (coupled) property compliance matrices are related to the corresponding ones across the leading diagonal according to the Maxwell relations given later in Section 4.5.2. ∼ ∼ ∼ ∼ For example, while C P,B = C M,E, it also follows that C P,B ≠ C P,B and C M,E ≠ C M,E ; or while C P,σ = C ε,E, ∼ ∼ it is clear that C P,σ ≠ C P,σ or C ε,E ≠ C ε,E. Consequently, the 13 × 13 compliance component matrix shown in Table 4.3 is symmetric, about the leading diagonal (within the shaded regions), which reduces the number of independent compliance components from 169 to 91. This type of inherent symmetry is called thermodynamic tensor symmetry since it arises from thermodynamic arguments. It must be remembered that the symmetry expressed by Cmn = Cnm applies only to the tensor components on the leading diagonal of the generalized compliance matrix. By similar reasoning, it follows from Eq. (4.19) that Im =

∂u , ∂ en

(4.42) where an infinitesimal change in any intensive parameter is given by dIm = Rm en. Again applying Green’s theorem in a plane yields the result

∂Im ∂I ∂ 2u ∂ 2u =− = = n ∂ en ∂ en ∂ em ∂ em ∂ en ∂ em

(4.43)

74 tensor properties of solids

or Rmn = Rnm.

(4.43a)

We note that this result could have been deduced from Eq. (4.35). Consequently, the 13 × 13 rigidity component matrix is also symmetric about its leading diagonal thereby reducing the number of independent rigidity components from 169 to 91. It must be understood that the so-called thermodynamic tensor symmetry is in no way associated with the symmetry of the crystal in which the tensor properties may or may not be manifest. Thus, the symmetry expressed by Cmn = Cnm and Rmn = Rnm applies generally to all crystal systems. Operation of the minimum generating matrices given in Table 3.6 and the application of Neumann’s principle given in Section 3.6 for symmetric second-rank tensors may result in a reduction of independent components required to specify the property for that point group. This will be done separately and selectively for the tensor properties as they are discussed in later developments.

4.5

Systematic Enumeration and Correlation of First-Order Tensor Properties— Generalized Maxwell Relations

It is desirable at this point to enumerate and correlate the various properties represented by the general compliance and rigidity matrices given by Eqs. (4.29) and (4.33). To do this, we will begin with the principle effects that lie along the leading diagonal of the general compliance matrix and then proceed to the interaction (coupled) effects that are represented by the off-diagonal compliances. Again, we will assume a single solid-phase system that is closed on its boundaries and that all fields applied to it are infinitesimally small so as to avoid second- and higher-order effects.

4.5.1 Principal Effects The principal properties are those that relate conjugate parameters and are defined as follows:

∂s ≡ (C )E, B, σ , specific heat (Heat capacity per unit volume) ∂ T E, B, σ

TC s,T = T

∂ Pi ≡ ( χik )T , B,σ , dielectric susceptibility tensor ∂ Ek T , B, σ

κ −1 CiPk , E = κ −1 0 0

where κ0 is the permittivity of a vacuum.

(4.44)

(4.45)

Generalized Thermostatics and correlation of Physical properties 75

∂ Mi ≡ (ψik )T , E,σ , magnetic susceptibility tensor ∂Bk T , E,σ

B = µ 0 µ 0CiM, k

(4.46)

where µ0 is the permeability of a vacuum.

∂ε Ciε,jklσ = ij ∂ σ kl

≡ (sijkl )T , E , B , elastic compliance tensor T , E , B

(4.47)

By application of the results of the previous section, we find these principal effects have the following thermodynamic tensor symmetry:

~ ( i , k = 1, 2 ,3 ) or χ = χ

(4.48)

~ ψ ik = ψ ki ( i , k = 1, 2 ,3 ) or ψ = ψ

(4.49)

sijkl = sklij ( i , j , k , l = 1, 2 ,3 ) or smn = snm

(4.50)

χ =χ ik

ki

It follows, therefore, that the two susceptibilities are symmetrical second-rank tensors, whereas the fourth-rank elastic compliance tensor sijkl is symmetric with respect to the interchange of pairs (ij ) and (kl ). It will later be shown that σij and εij are nearly always symmetrical second-rank tensors.

4.5.2 Independent Coupled Effects These coupled effects are represented by the off-diagonal compliances of the general compliance matrix and do not relate conjugate parameters. Consequently, they possess no thermodynamic tensor symmetry in themselves (self symmetry) as did the principal effects. However, since the general compliance component matrix is symmetric about its leading diagonal, there results the following six sets of Maxwell relations (57 in all) describing the six independent coupled effects all of which derive from the thermodynamic potential φ1 = g in Table 4.2. 1. Pyroelectric Effect

∂s ∂E 1 T , E ,E 2

3,B,σ

∂s ∂E 3 T , E 1 ,E

∂P = 1 = ( p1)B,σ ∂ T E,B,σ

2,B, σ

∂P = 3 = ( p3)B, σ ∂ T E,B, σ

(4.51)

76 tensor properties of solids

or, collectively, in matrix notation ~ C sE )T ,B,σ = C PT )E,B,σ = ( p)B,σ

(4.52)

These equations state that the electrocaloric coefficients are numerically equal to the corresponding pyroelectric coefficients, and both are represented by the first-rank polar tensor pk (k = 1,2,3). Thus, Eqs.(4.51) derive from dg = -sdt -PdE -MdB -εdσ, to which we apply Stoke’s theorem to give

[(∂ 2 g / ∂ E∂ T ) = (∂ 2g / ∂ T∂ E)]B,σ

or [(∂ / ∂ E)(∂ g / ∂ T ) = (∂ / ∂ T )(∂ g / ∂ E )]B,σ

where ∂g / ∂T = -s and ∂g / ∂E = -P, thereby yielding Eqs. (4.51) at constant B and σ. 2. Pyromagnetic Effect

∂s ∂M = 1 = ( q1)E,σ ∂B1 T ,E , B ,B ,σ ∂ T E,B,σ 2 3 ∂s ∂M = 3 = ( q3)E,σ ∂B3 T ,E , B1 ,B ,σ ∂ T E,B,σ

2

(4.53)

or, collectively, in matrix notation ~ C sB )T ,E,σ = C M,T)E,B,σ = (q )E,σ .

(4.54)

These equations state that the magnetocaloric coefficients are numerically equal to the corresponding pyromagnetic coefficients, and both are represented by the first-rank tensor qk (k = 1,2,3), which is both axial and magnetic in tensor character. 3. Thermal Expansion

∂s ∂ σ 11 T ,E, B,σ

22…σ 12

∂ ε 11 = (α 11) E,B ∂ T E ,B,σ

=

∂s ∂ σ 12 T ,E, B,σ

∂ ε 12 = (α 12 ) E, B ∂ T E , B ,σ

= …σ 11 31

(4.55)

or, collectively, in matrix notation

~ C sσ )T ,E,B = C ε,T )E,B,σ = (α)E,B

(4.56)

Generalized Thermostatics and correlation of Physical properties 77

which states that the piezocaloric coefficients are numerically equal to the corresponding thermal expansion coefficients and that both are represented by the second-rank polar tensor αik(i,k = 1,2,3). It is assumed that stress, strain and thermal expansion are all symmetric second-rank tensors that are unfolded according to the schemes of Eqs. (2.19) or (2.20). 4. Magnetoelectric susceptibility

∂P 1 ∂M 1 = = (λ 11) T, σ ∂B1 T, E, B2, B3,σ ∂E 1 T, E, B2, B3,σ

∂P 2 ∂M 1 = = (λ 21) T, σ ∂B1 T, E, B , B , σ ∂E 2 T, E ,E , B,σ 2

3

(4.57)

1 3

or, collectively, in matrix notation ~ C PB)T,E,σ = C ME)T,B,σ = (λ)T,σ .

(4.58)

Here, the corresponding coefficients of the direct and converse magnetoelectric susceptibility effects are numerically equal and are represented by the asymmetrical second-rank tensor λik which is axial and magnetic in character. Note that the components have been unfolded according to the following schemes: Tensor notation: S11 Matrix notation: S1

S22

S33

S23

S31

S12

S32

S13

S21

(4.59)

S2

S3

S4

S5

S6

S7

S8

S9

(4.60)

5. Piezoelectric Effect

∂P1 ∂ σ 11 T ,E, B,σ

∂ ε 11 E ∂ 1 T,E

= 22…σ 12

= ( d111)

T ,B

2,E3,B,σ

∂P3 ∂ σ 12 T ,E, B,σ

∂ ε 12 ∂ E3 T, E , E

= 11…σ 31

1

2 ,B, σ

= ( d312)

T ,B

(4.61)

or, collectively, in matrix notation

~ C Pσ)T,E,B = C ε,E )T ,B,σ = (d )T ,B .

(4.62)

78 tensor properties of solids

These equations state that the corresponding 18 components of the direct and converse piezoelectric effects are numerically equal and are represented by the third-rank polar tensor dijkl in the form of Tim given by Eq. (2.30) where the partial inherent symmetry is expressed by dikl = dilk = dim. 6. Piezomagnetic Effect

∂M1 ∂ σ 11 T ,E, B, σ

22…σ12

∂ ε 11 = ( Q111) T ,E ∂ B1 T, E,B ,B ,σ

=

2 3

∂M3 ∂ σ 12 T , E, B,σ

11…σ 31

∂ ε 12 = ( Q312) T ,E ∂ B3 T, E,B ,B ,σ

=

1 2

(4.63)

or, collectively, in matrix notation

~ C Mσ)T, E,B = C ε,B )T , E ,σ = (Q)T , E .

(4.64)

Similar to the piezoelectric effects, the corresponding 18 components of the direct and converse piezomagnetic effects are numerically equal. They are represented by the axial-magnetic third-rank tensor with the partial inherent symmetry Qikl = Qilk = Qim, assuming that stress and strain are symmetric second-rank tensors and are expressed by a tensor of the form given by Eq. (2.30). Thus, of the 16 properties represented by the general compliance matrix, only 10 are independent, 4 principal and 6 coupled effects. The same is true for the general rigidity matrix. It will be left as and exercise for the reader to repeat the above correlation procedure for the rigidities.

4.6 Effect of Measurement Conditions on the First-Order Tensor Properties Frequently, it is desirable to convert property coefficients measured under one set of conditions to those measured under another set of conditions. As an example, ultrasonic wave velocity measurements provide isentropic (thermally clamped) elastic coefficients. However, it may be the isothermal (thermally free) elastic coefficients that are desired. A second, and perhaps most common example is the conversion of heat capacity at constant stress (mechanically free) to heat capacity at constant strain (mechanically clamped) or vice versa. There are many other such examples. The problem of

Generalized Thermostatics and correlation of Physical properties 79

converting property coefficients in the clamped state to those in the free state or vice versa is one, which we shall now consider. Let a clamped compliance be that compliance that is measured holding any one of the extensive parameters (s, P, M, or ε) constant. Also, let a free compliance be one that is measured holding any one of the intensive parameters (T, E, B, or σ) constant. Now, consider any two extensive parameters a = a(α , β) and b = b(α , β) that are functions of any two intensive parameters α and β. From the equations dem = Cmn dIn, we write

∂a ∂a dβ da = dα + α ∂ β ∂β α

(4.65)

∂b ∂b db = d α + ∂ α β ∂β

(4.66)

and

d β . α

Holding b constant and multiplying Eq. (4.66) by (∂β / ∂b)α, we obtain

giving the result

∂β ∂b ∂β ∂b 0 = dα + ∂b ∂ β ∂b α ∂ α β α

d β , α b

∂ β ∂b d β = − dα . ∂b α ∂α β

(4.67)

Introducing Eq. (4.67) into Eq. (4.65) gives

∂a ∂ β ∂b ∂a da = d α − dα . α ∂ ∂β ∂b ∂α α β α β

(4.68)

Now, dividing Eq. (4.68) by dα at constant b leads to the final result or

∂a ∂ β ∂b ∂a ∂a − = − ∂β ∂b ∂α ∂α ∂α α β α β b (C a,α)b − (C a,α )β = −(C a,β )α (Rβ,b )α (C b,α )β

(4.69)

80 tensor properties of solids

in symbolic notation. Equation (4.69) gives the difference between the clamped (C a, a)b and free (C a, a)b compliances and requires that all other intensive parameters γ,δ, and so forth be held constant and that b and b be conjugate parameters. Application of Eq. (4.69) is simply accomplished by selecting the desired compliance through choice of a and a, and the clamped and free conditions through choice of the conjugate parameters b and b. For example, the difference between the mechanically clamped and free heat capacities is obtained by the following choice of parameters

a = s b = ε

α = T

(E, B constant)

β =σ

Introducing these parameters into Eq. (4.69) results in

∂ s ∂ σ ij ∂s ∂s − = − ∂ σ ∂ T ε ∂ T σ ij T ∂ ε kl

∂ ε kl , T ∂ T σ

(4.70)

where E and B are assumed to be held constant. But (∂s / ∂σij)T = (∂εij / ∂T )σ = aj by Maxwell’s relation and (∂σij / ∂εkl )T = (cijkl )T where (cijkl )T is the isothermal elastic stiffness coefficient. From this, we find the difference between the mechanically clamped and free heat capacities to be Cε − Cσ = − Tα ij (c ij k l ) α k l

( i , j , k , l = 1 − 3)

in tensor subscript notation or, alternatively,

Cε − Cσ = − Tα i (c ij ) α j = − T α~ ( c ) α T

T

( i , j = 1 − 6 )

(4.71)

in contracted tensor subscript and conformable matrix notation, respectively. Now suppose we wish to know the difference between the isentropic (constant entropy) and isothermal dielectric susceptibilities. For this purpose the choice of parameters becomes

a = P b = s

α = E β = T

(B constant),

resulting in the equation

∂Pi ∂E j

∂Pi − ∂E s j

= − ∂Pi ∂ T ∂ s ∂ T E ∂ s E ∂Ej T

, T

(4.72)

Generalized Thermostatics and correlation of Physical properties 81

where B and σ are held constant. However, because (∂Pi / ∂T )E = (∂s / Ei)T = pi from Maxwell’s relations, there results (χ ) − (χ ) = −

ij T

ij s

T

κ 0 CE

( i , j = 1 − 3 ),

pi pj

(4.73)

where T (∂s / T )E = CE with B and σ held constant, and pi pj is the dyadic or outer product of the pyroelectric coefficients. The above two examples demonstrate how one could obtain the difference between clamped and free principal effects. However, the difference between clamped and free coupled effects can be obtained with equal ease. As a third example, suppose it is desired to know the difference between the electrically clamped and electrically free coefficients of thermal expansion. For this purpose, the choice of parameters must be

a = ε b = P

α=T

β = E

(B constant),

resulting in the equation

∂ ε ij ∂ ε ij ∂T − ∂T P

∂ε = − ij ∂E E k

∂E k ∂P m ∂P ∂ T . E T m T

(4.74)

But according to Maxwell’s relations, (∂εij / ∂Ek)T = (∂Pk / ∂σij )E = dkij , with the result that

(α ij ) − ( αij) = −κ 0−1 (dkij ) ( χkm)−1 ( pm ) E

P

T,σ

T

σ

(i , j , k , m = 1 − 3 )

in tensor subscript notation or, alternatively,

(αi ) − (αi ) = −κ 0-1 ( dki ) ( χ km) -1 ( pm) P

E

T

T,σ

σ

(i = 1 − 6; k , m = 1 − 3)

(4.75)

or

~ αP − αE = −κ 0−1 dT ( χ −1)T,σ pσ

in conformable matrix notation. Because there are four principal effects each with three ways to vary the clamped and free compliances and six independent coupled effects each with two ways to vary the clamped and free compliances, there are a total of 24 equations of the type illustrated above. These are presented in

82 tensor properties of solids

Table 4.4: Differences between clamped and free first-order property compliances given in conformable matrix order for the principal and coupled effects. Principal Effects

Coupled Effects

}

Q s − QT = −(T / C B ,σ )qσ α~ B}E

(1)

C P − C E = −κ 0 T ~ p ( χ T ) −1 p

(2)

~ (ψ ) −1 q C M − C B = −µ 0−1T q T

(3)

~ c α} Cε − Cσ = − T α E, B T

(15)

(4)

p }B , σ χ − χ T = − (T / κ 0 ) C E p ~

(16)

dM − d B = − µ 0 λσ ( χ E ,σ ) − 1 QE

(17)

α P − α E = −κ 0− 1 d T ( χ T ,σ ) −1 pσ

(18)

~ α M − α B = −µ 0 QT (ψ T ,σ) − 1 qσ

(19)

~ qP − q E = −κ 0−1λT ( χ T , B ) −1 p B

(5)

(13)

B ,σ

}

(14)

E,σ

s

−1 ~ χM − χE = − ( µ 0 / κ 0 )λ (ψ E ) λ

}

T,σ

(6)

~ −1 χε − χσ = −κ o dcE d

(7)

ψs − ψT = − ( µ0 T / C B ) q q~}E ,σ

(8)

~ −1 ψ P − ψ E = − ( µ 0 / κ 0 )λ ( χ B ) λ

}

T, B

}

T, σ

QP − QE = −κ 0− 1 λσ ( χ B ,σ ) − 1 d B

T

ds − d T = −(T / C E ,σ ) pσ ~ p E}B

}

~

T

}

B

}

E

}

qε − qσ = − Q T cT , B α B

pM − p B = − µ 0 λ T ( ψ T , E )

E

~ ψε − ψσ = − µ 0 Q cB Q }T , E

(21)

(10)

~} * ss − sT = −(T / Cσ )α α E,B

(22)

pε − pσ = − dT c T , E α E

(11)

~ sP − sE = − κ 0− 1 d ( χσ ) − 1 d}T , B

(23)

λ s − λ T = − (T / C E , B) p B q~ E

(12)

~ s M − sB = − µ0 Q (ψσ ) −1 Q}

(24)

−1

qE

}

}

B

}

~ λε − λσ = −d B c E, B QE

* Difference between the isentropic (constant entropy density) and isothermal elastic compliances.

σ

}

(20)

(9)

T, E

}

}

T

σ

σ

Generalized Thermostatics and correlation of Physical properties 83

Table 4.4 in conformable matrix order. To use the table, one only needs to replace the symbols by their respective matrices and carry out the multiplication as indicated. The tilde appearing above some of the symbols indicates the transpose of the normal matrix form. This may be illustrated by expanding Eq. (4.75), which is Eq. (17) in Table 4.4 (all at constant B), as follows:

α 1 α 1 d11 α α d 2 2 12 α 3 α 3 1 d13 − = − κ 0 d14 α4 α4 α α d 5 5 15 α6 α6 d16 P E

d21 d22 d23 d24 d25 d26

d31 d32 χ −1 d33 11 χ −1 d34 12 χ −1 d35 31 d36 T

χ −1 12 χ −1 22 χ −1 23

χ −1 p1 31 χ −1 p2 . 23 χ −1 p3 σ 33 T,σ

(4.76)

Keep in mind that crystal symmetry considerations can greatly reduce the number of property components needed for use in equations of the type just given and, as a consequence, greatly reduce the matrix calculation time and effort to obtain a result. The matrix equations in Table 4.4 may be used to obtain order-of-magnitude values for the differences between clamped and free compliances. However, in using any one equation, great care must be exercised in choosing representative magnitudes of the properties. Remember that the values of the components usually differ somewhat within each tensor and that these magnitudes my vary dramatically from crystal to crystal if, in fact, they exist at all by reason of normal crystal and magnetic symmetry. It can be easily verified that the inverse of Eq. (4.69) is

R α, a )β − ( R α, a )b = − (R α, b )b (C α, b )b ( R β , α )b

(4.77)

giving the difference between free and clamped rigidity coefficients. In the case of rigidities, it is required that all other extensive parameters c, d, …, and so forth. be held constant and that b and β be conjugate parameters. This also leads to 24 equations of the type shown in Table 4.4. • • • •

85

chapter 5

The Dependent Coupled Effects and the Interrelationships Between First-Order Tensor Properties— Use of Interaction Diagrams The independent principal and coupled first-order effects are featured in Table 4.3, which gives the component arrangement of the general compliance matrix. The four principal effects are those relating the conjugate parameters along the leading diagonal (the shaded regions) and possess thermodynamic self-symmetry. The six coupled effects are the off-diagonal regions in Table 4.3 and relate intensive parameters to nonconjugate extensive parameters—the opposite being true for the general rigidity matrix. Consequently, off-diagonal effects exhibit no self-symmetry. However, they do possess thermodynamic tensor symmetry expressed by the six Maxwell relations in Section 4.5.2 and by Eqs. (4.41a) and (4.43a). For this reason, they are labeled independent coupled effects.

5.1

THE DEPENDENT COUPLED EFFECTS

Additional coupled effects relating any two intensive parameters (or two extensive parameters) can be defined by suitable choice of the thermodynamic potentials given in Table 4.2 followed by application of Stoke’s theorem (actually Green’s theorem in a plane) discussed in Section 4.4. As an example, suppose it is desired to equate the isothermal elastocaloric coefficient (∂s / ∂ε )T to the isometric thermal stress coefficient (∂σ / ∂T )ε at constant P and B. For this purpose, φ7 in Table 4.2 must be used together with Stoke’s theorem. Thus, for dφ7 = - s d T + E d P – M d B + σ d e, we have

∂ 2φ 7 ∂ 2φ 7 = ∂ ε ∂T ∂ T ∂ ε P ,B

∂ ∂φ ∂ or 7 = ∂ ε ∂ T ∂ T

∂φ 7 ∂ ε

, P ,B

86 Tensor properties of solids

with the result that ∂s ∂ε ij

T,P ,B

∂σ = − ij ∂T

( )

= t ij P ,B,ε

P ,B

There are many other examples of dependent coupled effects. In fact, an examination of Table 4.2 will indicate that there are four sets of clamped and/or free conditions for each of the six dependent coupled effects and their inverse, leading to a total of 48 equations of the type exemplified above. Thus, the choice of the thermodynamic potential used to obtain a given Maxwell relation will depend not only on the particular coupled effect involved but on what parameters are desired to be held constant. For the sake of illustration here, let us require that all effects be defined in such a way that only the intensive parameters are held constant. By using just four thermodynamic potentials φ2, φ3, φ4, and φ5, the following six Maxwell relations, representing the six additional coupled effects, are given in the order of increasing tensor rank.

∂ Pi ∂s

∂s ∂ M i

∂s ∂ε ij

∂ Mj ∂ P i

E,B,σ

∂εjk ∂ P i

∂T = − ∂ Ei

T ,E,σ

T,E,B

∂εjk ∂ M i

B,σ

s ,B,σ

∂B = − i ∂T

= (ηi )

(from φ3)

(5.2)

∂σ = − ij ∂T

= t ij

( )

(from φ2)

(5.3)

( )

(from φ4)

(5.4)

( )

(from φ4)

(5.5)

(from φ3)

(5.6)

E,σ

E ,M,σ

E,B,ε

E,B

∂E = − i = υij ∂ Bj T ,P ,σ T ,B,σ

T ,B,σ

T ,E,σ

(from φ5) (5.1)

= ( hi )

∂ Ei = − ∂σ jk

= εijk T,P ,B

∂ Bi = − ∂σ jk

T ,σ

T ,B

( )

= mijk T,E,M

T,E

The inverse of each of the above relations is readily obtained from a different thermodynamic potential chosen from the same group φ2, φ3, φ4, and φ5. For example, (hi-1)B,σ results from φ4.

Dependent Coupled Effects 87

5.2

INTERRELATIONSHIP BETWEEN FIRST-ORDER PROPERTIES—USE OF INTERACTION DIAGRAMS

An inspection of the general interaction diagram in Figure 1.1 reveals the important fact that the six interaction effects in Eqs. (5.1)–(5.6) are not independent effects because each can be expressed in terms of the first-order properties defined in Section 4.5. To illustrate, consider the interaction diagram in Figure 5.1 representing (hi)B,σ in Eq. (5.1) for which the arrows point toward the dependent variable. From Figure 5.1, there results the equation

∂ T ∂ T ∂ s = ∂ Ei ∂ s ∂ Ei

or

− ( hi )

B,σ

B,σ

T = σ pi C B,σ

(5.7)

giving an additional expression for the dependant pyroelectric effect vector, all at constant B and σ. But it is easily verified that three other interaction diagrams shown in Figure 5.2 can also be used to describe hi , leading to the three additional equations that follow, all at constant B and σ. −hi = κ 0 p−j 1 χ ji = qj−1 λ ji = α jk−1 d jki B,σ

(5.8) Similarly, the interaction diagram shown in Figure 5.3 represents the Maxwell relation in Eq. (5.4) for the dependent coupled effect -νij = (∂Ei / ∂Bj)P. From this diagram, there results the equation −ν j = p−1 q i j T , σ i

(5.9)

at constant T and σ and involving the outer or dyadic product pi-1qj . However, it is clear that three other equations for νij can be derived from the three interaction diagrams given in Figure 5.4. Three additional equations are −1 λ−1 λ = µ−1 − νij = κ −1 ψ = d i−1kl Qklj 0 χ ik kj 0 ik kj

(5.10)

all at constant T and σ. T/Cρ

T

s

−h p E FIGURE 5.1: Interaction diagram for dependent coupled effect h in Eq. (5.1) at constant B and σ.

88 Tensor properties of solids

T

T –1

p

−h E

κ 0χ

T

−h P

−h

q–1

E

α–1

E

λ

M

d

ε

FIGURE 5.2: Additional interaction diagrams representing the dependent coupled effect h in Eq (5.1), all at constant B and σ.

Following the same procedure, the four expressions for each of the remaining four dependent coupled effects are readily obtained. These, together with those illustrated previously, are given by the following six sets of equations all given in conformable matrix order:

~ − h = (T /Cσ ) p = κ 0 χ p−1 = λ q−1 = dα −1

(B,σ constant)

(5.11)

− η = (Cσ / T ) q−1 = λ−1 p = µ0ψ −1 q = Q−1α

(E,σ constant)

(5.12)

~ ~ − t = (Cσ / T )α −1 = d −1 p = Q−1 q = s−1α

(E, B constant)

(5.13)

~ − ν = p−1 q~ = κ 0−1 χ −1λ = µ0−1 λ−1ψ = d −1 Q

(T,σ constant)

(5.14)

~ = κ −1χ −1d = λ −1Q = d −1 s − ε = p−1α 0

(T, B constant)

(5.15)

− m = q−1 α~ = λ−1 d = µ0ψ −1 Q = Q−1s

(T, E constant)

(5.16)

The various tensor properties are used in the above six sets of equations to represent the dependent coupled effects defined by Eqs. (5.1)–(5.6) in Section 5.1. The tilde (~) appearing above some of p–1

s

E q

−υ B

FIGURE 5.3: Interaction diagram for dependent coupled effect υ in Eq. (5.4) at constant T and σ.

Dependent Coupled Effects 89

E

−υ

(κ 0χ)–1

P

E

λ–1

−υ

λ B

E

B

ψ /µ 0

−υ M

d –1

B

Q

ε

FIGURE 5.4: Additional interaction diagrams representing the dependent coupled effect υ in Eq (5.4), all at constant T and σ.

the property symbols indicates the transpose of the normal matrix form of the tensor. The normal matrix dimensions (rows × columns) for first- and third-rank tensors are (3 × 1) and (3 × 6), respectively. The normal matrix dimensions for a second-rank tensor property are either (3 × 3) or (6 × 1), the latter being the column form of symmetrical second-rank tensor properties such as α, χ and ψ, all of which are polar in character. As defined by Eqs. (4.57) in Section 4.5, the magnetoelectric susceptibility λ is an asymmetrical axial–magnetic second-rank tensor and has normal matrix dimensions of (3 × 3). However, unfolded according to arrays given by Eqs. (4.59) and (4.60), it would be represented as a (9 × 1) column matrix with axial character. Because the properties q, λ, and Q are axial–magnetic (first-, second-, and third-rank tensors, respectively), the dependent coupled effects η, ν, and m are also axial–magnetic in tensor character. The three remaining dependent coupled effects are polar tensors. The six sets of equations, Eqs. (5.11) to (5.16), have some important uses. First they can be used to obtain the components for any dependent coupled tensor property from known components of the more common first-order properties defined in Section 4.5. As an example, suppose it is desired to know the six components of the isometric thermal stress coefficient tij given by Eqs. (5.13) and determined at constant E and B fields subjected to a particular crystal. If the heat capacity Cσ and coefficients for thermal expansion αij are known for the crystal, as they commonly are, or if the piezoelectric moduli d and the pyroelectric coefficients p are known, then Eqs. (5.13) give two alternatives for the determination of tij at constant E and B.

t1 t 2 t C − 3 = σ t 4 T t 5 t 6

α −1 d −1 11 1 −1 −1 α d 2 21 α −1 d −1 3 31 −1 = −1 α d 4 41 α −1 d −1 5 −1 51 −1 α 6 d 61

−1 d 12 d −1 22 −1 d 32 −1 d 42 −1 d 52 −1 d 62

−1 d 13 −1 d 23 p 1 d −1 33 p −1 2 d 43 p −1 3 d 53 d −1 63

(5.17)

90 Tensor properties of solids

~ Here, it should be understood that quantities such as d -1 represent the component inverse (reciprocal) of its transpose, a two-stage operation from the normal (3 × 6) form. There are many other such examples, including the inverse of the six dependent coupled effects given by Eqs. (5.11)–(5.16). For example, with reference to Eq. (5.3), the components of the effect (∂Ti / ∂σij)s , which describes the adiabatic application of stress, can be obtained by taking the inverse of Eq. (5.17) to give (∂Ti / ∂σij)s = -(T / Cσ)αij all at constant E and B. These same results can also be obtained from the application of Stoke’s theorem to the generalized enthalpy, φ5 = h given in Table 4.2, followed by the appropriate interaction diagram. Another important use of the six sets of equations, Eqs. (5.11)–(5.16), is to interrelate the various first-order effects. Suppose, as a typical example, it is desired to find the components of the magnetoelectric susceptibility λ for a particular crystal under conditions of constant T and σ. If the components of the dielectric susceptibility χ, those of the piezoelectric coefficient d, and those of the piezomagnetic coefficient Q are all known for a particular crystal, Eqs. (5.14) yield the result ~ κ −1 χ−1 λ = d −1 Q 0

(5.18)

Then, solving for λ gives

χ χ d −1 χ 11 11 31 12 −1 λ = κ 0 χ χ χ d 21 23 22 12 χ χ χ d −1 31 31 33 23

−1 d 12 d −1 22 −1 d 32

d −1 13 d −1 23 d −1 33

d −1 14 d −1 24 −1 d 34

−1 d 15 d −1 25 d −1 35

Q11 Q −1 21 d 16 Q31 d −1 26 Q 41 d −1 36 Q 51 Q61

Q12 Q22 Q32 Q42 Q52 Q62

Q13 Q23 Q33 Q43 Q53 Q63

(5.19)

where λ is given generally as an asymmetrical (3 × 3) matrix. If, however, all components of the four effects are known, then Eq. (5.18) could be used to check the internal consistency of the tensor properties involved. This internal consistency check can be used on other interrelated first-order effects.

5.3

THE GRÜNEISEN TENSOR

There are other interaction effects that may be deduced from the interaction diagram in Figure 1.1, and the Grüneisen tensor is one such example. The Grüneisen parameter can be used to show that the quantity (Cε)-1cα remains constant as the temperature T is changed. In its classical form, the Grüneisen parameter is represented by the relation

∂P γ = −V ∂ U V

(5.20)

Dependent Coupled Effects 91

Here, P is the pressure, U is the internal energy, and V is the volume, which is held constant. This equation may be written in a more general form, applicable to crystal systems, if -P is replaced by σij, dU is replaced by Vdu, and V is replaced by strain to give the Grüneisen tensor as

∂σ γ = ij . ij ∂ u ε

(5.21)

But in the absence of any polarization and magnetization (P and M are zero under constant E and B) and at constant strain, such that no mechanical work is done, we recognize that du = Tds for any process in which reversible heat is absorbed by the system. Therefore, Eq. (5.21) becomes

γ = ij

1 ∂σ ij , =γ ji T ∂s ε

(5.22)

indicating that the Grüneisen tensor is proportional to the inverse of the isometric piezocaloric coefficient αij-1 (see Eqs. (4.55)), which is symmetrical. Shown in Figure 5.5 is the interaction diagram that is descriptive of the Grüneisen parameter as presented in Eq. (5.22). Here, as before, the arrows point toward the dependent variable. From the diagram, there results the tensor equation (note that the T ’s cancel)

γ ij =

1 ∂σ ij = ( 1 /Cε ) cijkl α kl T ∂ s ε

(5.23)

all taken at constant E, B, and ε, and where Cε represents the heat capacity at constant strain, αkl is the thermal expansion tensor, and cij represents the elastic stiffness moduli. The properties Cε, αkl, and cijkl can all be obtained in the region of zero strain, P and M, which satisfies the condition of constant strain, and constant E and B.

T

T/C ε

s

α−1 α

σ

c

ε

FIGURE 5.5: Interaction diagram descriptive of the Grüneisen parameter.

92 Tensor properties of solids

Equation (5.23) may be represented in matrix form by

γ i = (Cε )−1 cij α j

(5.24)

or in expanded form shown in Eq. (5.25). This holds generally for any of the seven crystal systems with the proper choice of cij and αj,.

γ 1 c11 c12 c13 γ c 22 c 23 2 γ 3 c33 −1 = (Cε ) γ 4 γ Sym 5 γ 6

c14 c 24 c34 c 44

c15 c 25 c 35 c 45 c 55

c16 α 1 c 26 α 2 c 36 α 3 c 46 α 4 c 56 α 5 c66 α 6

(5.25)

Of particular interest is the Grüneisen tensor specified for the cubic crystal system. See Section 6.2.5 and Table 6.3 for cubic elastic stiffness moduli. In expanded form, we can write

γ 1 γ 2 γ 1 γ = 3 = 0 Cε 0 0

c 11 c12 c 12 0 c 11 c 12 0 c11 0 c 44 Sym.

0 0 0 0 c44

0 α 1 1 0 α 0 α α (c11 + 2c12) 1 = , 0 0 Cε 0 0 0 0 c 44 0 0

(5.26)

giving the six components of γ . From Eq. (5.26), it follows that the Grüneisen invariant is

γ=

αK γ 1 α (c 11 + 2c 12) α = = = 3Cε 3 3Cε ( s 11 + 2 s 12) Cε

(5.27)

which is the classical result, with K = (c11 + 2c12) / 3 being the bulk elastic modulus for the cubic crystal system. The quantity K is also the reciprocal of the volume compressibility. Because of its close relationship with stress (or strain), the Grüneisen parameter may be decomposed into spherical and deviatoric components given by where γij* = λij - γ is the Grüneisen deviator.

γ ij = γ δ ij + γ i*j

(5.28)

Dependent Coupled Effects 93

There are other ways of representing the Grüneisen parameter as can be seen from five of the six dependent coupled effects given by Eqs. (5.11)–(5.13), (5.15), and (5.16). Keep in mind from Figure 5.5 that the Grüneisen tensor is the inverse of the piezocaloric coefficient, αij-1. However, most of these other expressions involve axial–magnetic and/or first-rank property tensors that greatly restrict their application in obtaining the components of γij for many crystals. Eqs. (5.11) and (5.13) would appear to be the most useful as alternative means of representing the Grüneisen tensor. • • • •

95

chapter 6

Third- and Fourth-Rank Tensor Properties—Symmetry Considerations Before we can discuss the second- and higher-order effects presented in the next chapter, it is necessary to lay a proper foundation for that discussion. The best means of accomplishing this is to revisit the third- and fourth-rank tensor properties defined earlier in Section 4.5. We do this by considering, as good examples, the piezoelectric and elastic effects.

6.1 DIRECT AND CONVERSE PIEZOELECTRIC EFFECTS Beyond mere definitions as in Eqs. (4.61) and (4.62), little was said about the direct or converse piezoelectric coefficient. It is important that these subjects be covered at this time because they illustrate the typical symmetry and transformation characteristics displayed by several other thirdrank polar tensor properties.

6.1.1 Direct Piezoelectric Effect When a stress σij is applied to certain crystals, they will develop a total electric dipole moment per unit volume ( polarization) Pi proportional to that stress as represented in tensor subscript notation by

Pi = dijkσjk

(i, j, k = 1 - 3)

(6.1)

The effect represented by Eq. (6.1) is called the direct piezoelectric effect, and dijk are the piezoelectric moduli. Thus, dijk is a third-rank polar tensor property relating a vector to a second-rank tensor, hence, a vector-tensor property. If only “pure” stresses (no body torques) are applied, then σjk = σkj , which allows dijk = dikj = dim and permits us to write the direct piezoelectric effect in the contracted form

Pi = dimσm

(i = 1-3; m = 1- 6),

(6.2)

96 tensor properties of solids

thereby reducing the number of independent components of dijk from 27 to 18 according to Eq. (2.30). Thus, to convert between tensor subscript notation and matrix notation, the stress components become

σ 1 σ6 σ2 ↔ Sym.

σ5 σ4 σ3

σ 11 σ 12 σ 31 σ22 σ23 Sym. σ33

.

(6.3)

However, because stress is a symmetric second-rank tensor σjk = σjk , we follow the tensor-to-matrix conversion rule (recommended in “Standards on Piezoelectric Crystals,” see Endnotes)

d ijk = d im 2d ijk = dim

for

m =1− 3

for

m = 4 − 6

(6.4)

to avoid the appearance of factors of 2 in Eq. (6.2) in terms for which m = 4, 5, and 6. As a result, we represent Eq. (6.2) as P = d:σ or in matrix notation as P = dσ.

(6.5)

Recall that the double dot (:) indicates a double contraction product as in Eq. (2.47). In expanded form, the three components of P in Eq. (6.5) can be written in the conformable matrix array form given by

P1 P = 2 P3

d 11 d 21 d 31

d12

d13

d14

d15

d 22

d 23

d 24

d 25

d32

d 33

d 34

d 35

σ1 σ d16 2 σ d 26 3 σ d 36 4 σ 5 σ6 .

(6.6)

Here, σ1, σ2, and σ3 are the tensile stresses (positive by convention), and σ4, σ5, and σ6 are shear stresses, with the understanding that σ23 = σ32 = σ4, σ31 = σ13 = σ5, and σ12 = σ21= σ6. Shown in Table 6.1 are five common stress arrays. Note that for hydrostatic pressure p = -σ applied on each of the axis normals. The transformation law for piezoelectric moduli, d, can now be established. First, let P = dσ be true relative to the “old” axes and let P ′ = d ′σ ′ hold relative to a “new” set of axes. Then, because P and σ transform as P ′ = aP and σ ′ = ασ or σ = α −1 σ ′, respectively, it follows that

Third- and Fourth-Rank Tensor Properties 97

TABLE 6.1: Sample stress arrays assuming a symmetric stress tensor σij = σji Uniaxial stress

Biaxial stress

Hydrostatic pressure

Pure shear stress

σ1 0 0 0 0 Sym. 0

0 0 σ1 σ2 0 0 Sym.

0 0 − σ −σ 0 − σ Sym.

− σ 0 0 0 σ 0 0 0 σ 0 = 0 0 Sym. Sym.

P ′ = aP = adσ = adα −1σ ′ = d′σ ′

from which we conclude that

d′ = adα −1,

(6.7)

where α is the quadratic transformation form as presented in Eq. (2.22). Equation (6.7) is the appropriate transformation law for the piezoelectric moduli and is identical to Eq. (2.31), assuming ∼. that stress is a symmetrical second-rank field tensor, σ = σ

6.1.2 Converse Piezoelectric Effect When an arbitrarily oriented electric field Ei is applied to a piezoelectric crystal, the shape of the crystal changes slightly, that is, a strain is produced that is proportional to the electric field strength. This is the converse piezoelectric effect expressed by

εjk = dijkEi

(i, j, k = 1-3).

(6.8)

As a result, Eq. (6.8) is succinctly represented by ε = d ⋅ E or simply as

~ ε = dE

(6.9)

in conformable matrix form. The single dot (⋅) indicates a single contraction product as in Eq. (2.46). The converse piezoelectric effect is also called the first-order electrostrictive effect, and dijk are the first-order electrostrictive moduli. From Eqs. (4.61) and (4.62), it is clear that the direct and converse piezoelectric moduli are numerically equal.

98 tensor properties of solids

Because strain is usually a symmetrical second-rank tensor, εjk = εjk, the tensor symmetry for dijk becomes dijk = dikj = dim, which permits Eq. (6.8) to be written as

εm = dimEi

(i = 1 - 3; m = 1 - 6).

(6.10)

∼ The transpose of d, expressed as d in Eq. (6.9), indicates that its rows and columns of the normal form in Eq. (2.30) must be interchanged to a 6 × 3 matrix if the product of Eq. (6.9) is to be conformable. Thus, Eq. (6.9) is written in extended matrix form as

ε1 ε 2 ε3 = ε4 ε 5 ε 6

d11 d 12 d 13 d 14 d 15 d 16

d 31

d 21

E d 33 1 ~ E = d E. d 34 2 E 3 d 35 d 36

d 22

d 32

d 23 d 24 d 25 d 26

(6.11)

Equation (6.11) is valid because the symmetric part of the strain tensor εjk, defined by Eq. (2.17), is

εjk =

1 2

( εjk + ε kj ) ,

(6.12)

which, in turn, permits the strain matrix to be given by

ε11 Sym.

ε12 ε22

ε 11 ε23 = ε33 Sym. ε31

1 2

(ε 12 + ε21 )

1 2

ε22

1 2

(ε 31 + ε 13 )

(ε 23 + ε 32 ) . ε 33

(6.13)

The tensor-to-matrix conversion scheme for strain now becomes

ε11 Sym.

ε12 ε22

ε1 ε23 → Sym. ε33 ε31

1 2

ε6

ε2

1 2 1 2

ε5

ε4 ,

ε 3

(6.14)

where ε1, ε2, and ε3 are the elastic tensile strains or stretches, and the three remaining, ε4, ε5, and ε6, are the elastic shear strains. As a result of the conversion scheme of Eq. (6.14), the shear strain components of Eq. (6.10) will have factors of ½ on both sides of the equations that cancel. This

Third- and Fourth-Rank Tensor Properties 99

permits Eq. (6.11) to be written in simple two-subscript form exclusive of the factors of 2 in the shear components that would otherwise be present. As it turns out, matrix shear strain is identical to engineering shear strain (i.e., ε4 = γyz, ε5 = γzx, and ε6 = γxy ). The antisymmetrical part of εjk is the axial second-rank tensor given by ϖjk = − 21 (εjk − εkj) which is the rotation resulting from elastic shear. The transformation law for converse piezoelectric moduli, d, is now established in a manner ∼ similar to that for the direct effect given earlier. First, let ε = d E be true relative to the “old” axes and ∼ let ε ′= d ′E ′ hold relative to a “new” set of axes. Now, because ε and E transform as ε ′= α∼ -1ε and ∼ ∼ ∼ E ′ = aE or E = a∼E ′ (a-1 = a∼ ), respectively, it follows that ε ′ = α∼ -1ε = α∼ -1 d E = α∼ -1 d a∼ E ′ = d ′E ′, from which we conclude that ~ ~−1 ~ ~ d′=α d a .

(6.15)

∼ -1ε, results from the tensor-to-matrix converThe transformation for matrix shear strain, ε′ = α sion rule given by Eq. (6.14). Note that α∼ -1 requires two separate operations because α∼ ≠ α -1 in general.

6.1.3 Crystal Symmetry Considerations The method of direct inspection can be used to determine the effect of crystal symmetry on the components of the third-rank tensor properties. To do this, the full tensor subscript notation must be used and then only on crystal systems other than the trigonal and hexagonal crystal systems as explained in Section 3.6. Application of Neumann’s principle to the direct (or converse) piezoelectric moduli, dijk, results in dijk = dijk d = − = 0 .. dijk ijk

(6.16)

For example, all holohedral crystal systems, those represented as Xin Table 3.6, are centrosymmetrical, and as a result, dijk = −dijk = 0. Thus, the 11 centrosymmetrical crystal groups will be lacking in all piezoelectric moduli. To illustrate, we apply Neumann’s principle to the 222 crystal group. By using Table 3.6, we observe that the 222 group requires the use of generating matrices s(2) and s(3). From Table 3.5, the transform of axes are given in compact form according to (2)

s

1 → −1 1 → −1 (3) → 2 → 2 and and s → 2 → −2 3 → −3 3 → 3

(6.17)

100 tensor properties of solids

and are applied in any sequence. Applying s(2) first, it is clear that dijk = 0 for all moduli containing an odd number of 1’s and/or 3’s. Application of s (3) requires that dijk = 0 for all moduli for which there is an odd number of 1’s and/or 2’s. Therefore, the only moduli to survive are those containing all three, 1, 2, and 3 in any order. As a result, the array of piezoelectric moduli becomes

d 111 d 122 d 133 d 123 d 131 d 112 d 211 d 222 d 233 d 223 d 231 d 212 d 311 d 322 d 333 d 323 d 331 d 312 ⇓

0 0 0 0 d 14 0 0 0 0 0 d 123 0 0 0 0 0 d 0 = 0 0 0 0 d 25 0 231 0 0 0 0 0 d 312 0 0 0 0 0 d 36

(6.18)

in both three- and two-suffix notation. Application of Neumann’s principle to the trigonal or hexagonal crystal systems requires the “brute-force” method involving Eq. (6.7) for all threefold and sixfold rotations.

6.1.4 Brute-Force Method for the Trigonal and Hexagonal Classes— The Piezoelectric Moduli 1. If generating matrices other than s(7) are involved in the particular crystal class, apply them first each in turn by using the method of direct inspection to obtain a simplified array of the moduli. 2. By using the appropriate transformation law, for example, Eq. (6.7), complete the matrix calculations with the generating matrices s(7) and σ ( 7) to obtain a set of equations for the new property moduli. 3. As a final sep, equate each old modulus with the new and solve the resulting equations simultaneously for the moduli appropriate for the given crystal class. As an example, let us apply Neumann’s principle to the hexagonal class 6. From Table 3.6, we see that this requires the application of generating matrices s(3) ⋅ s(7) = s(14). To simplify the calculations, it is advantageous to apply s(3) first, then follow with s(7) as required by the brute-force method. From generating matrices given by Eq. (6.17), application of s(3) allows the dijk to survive only for moduli with an odd number of 3’s, a total number of eight independent moduli. When this is done, application of s(7) to the piezoelectric transformation law given by Eq. (6.7) takes the form

Third- and Fourth-Rank Tensor Properties 101

[dijk] s

s(7)

3 − 12 2 d′ = 3 1 − 2 − 2 0 0

0 0 1

(3)

(σ (7)) −1

0 0 d 123 d 131 0 0 0 0 d 223 d 231 0 0 d 311 d 322 d 333 0 0 d 312

41 43 0 0 0 − 43

3 2

3 4

0

0

0

1 4

0

0 1

0 0

0 − 23 0 0

0

0

− 12

0

0 −

3 4

0

3 2

0

3 2

0

− 12

0

0

− 12

. (6.19)

When the matrix multiplication operations of Eq. (6.19) are carried out, there result the following equations relating the old moduli to the new moduli: d123 =

d 123 4

−

3 1 −d 3 d223 − 131 + d231 3 4 2 2 2

d131 =

1 −d123 3 + d223 2 2 2

d223 =

d 3 1 d123 + 223 − 4 4 2

d231 =

1 2

3+

d131 4

−

3 d 4 231

− 3 d d131 − 231 3 2 2

− 3 d d123 − 223 2 2

3+

d 3 d131 231 4 4

d311 = d322 =

d311 4

+

3 3 d − d 4 322 4 312

d 3 3 d311 + 322 + d 4 4 4 312

d333 = d333 d312 =

d 3 3 d311 − d322 − 312 2 2 2

Solving these eight equations simultaneously gives the following class 6 piezoelectric moduli in both three- and two-suffix notation where the eight independent moduli in Eq. (6.19) have been reduced to four in Eq. (6.20).

0 0 d123 d131 0 0 0 0 d 14 0 0 0 d 131 −d 123 0 = 0 0 0 d 15 0 d 311 d 311 d 333 0 0 0 d31 d31 d33 0

d 15 0 −d 14 0 0 0

(6.20)

From Table 3.6, we note that the generating matrices for class 622 are s(12) and s(14). Because the moduli arrays of Eq. (6.20) result from the application of s(14), there remains only the application of s(12) = s(1) ⋅ s(4) to the three-suffix form of Eq. (6.20) to obtain the moduli for class 622. From Table 3.5 for s(12) and using the method of direct inspection, it is clear that the only moduli to survive

102 tensor properties of solids

are those for which an odd number of 1’s exists. Thus, d131 = d311 = d333 = 0, resulting in the array for class 622 given by 0 0 0 0 0 d14 0 0 0 d123 0 0 0 0 −d123 0 = 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 . 0

0 − d14 0

(6.21)

Continuing on to class 6mm, we see from Table 3.6 that the generation matrices required for this crystal class are s(3), s(4), and s(7). So there remains only the application of s(4) in Table 3.5 to the three-suffix result of matrix arrays (6.20). When this is done, the only moduli to survive are those for which an even number of 1’s or no 1’s exist. Thus, d123 = 0 in arrays (6.19) resulting in the moduli arrays for class 6mm given by 0 0 0 d131 0 0 0 0 0 0 0 0 d131 0 0 = 0 0 0 d15 0 0 0 d 31 d 31 d 33 0 d 311 d 311 d 333 0

0 0 0

d15 0 0

(6.22)

By applying similar analyses to the 32 crystal classes, there result the matrices for the direct and converse piezoelectric moduli given in Table 6.2 where dijk = 0 for all centrosymmetrical classes. TABLE 6.2: Piezoelectric moduli for both the direct and converse effects Triclinic

Class 1 d 11 d 12 d 21 d 22 d 31 d 32

d 13

d 14

d 23 d 24 d 33

d 34

d 15

d 16

d 25 d 26 d 35 d 36

Class 1 centrosymmetrical, dijk = 0 Monoclinic Class 2 (2 x2)

0 d21 0

0

0

d 14

0

d 22

d23

0

d 25

0

0

d34

0

Class m (m ⊥ x2) d 16

0 d 36

d 11 d 12 0 0 d 31 d 32

Class 2 / m centrosymmetrical, dijk = 0

d 13 0 d 33

0

d 15

d24 0 0 d 35

0

d 26 0

Third- and Fourth-Rank Tensor Properties 103

TABLE 6.2: (continued) Orthorhombic Class 222

Class 2mm 0 0 0 0 d 31 d 32

0

0

d 15

0

d 24

0

d 33

0

0

0

0 0 0 0 0 0 0 0 0

0 0

d 14

0

0

0

d25

0

0

0 d36

Class mmm centrosymmetrical, dijk = 0 Tetragonal _ Class 4

Class 4 0 0 0 0 0 0 d 31 d 31 d 33

d14 d 15 0

d 15 0 −d 14 0 0 0

0 0 0 0 d 31 −d 31

0

0

0

0 d 36

d 14 d 15 −d 15 d 14 0 0 0

Class 4 / m centrosymmetrical, dijk = 0 _ Class 42m

Class 4mm

0 0 d31

0

0

0

0

d 31 d 33

0 d 15 0

0 0 0 0 0 0 0 0 0

d15 0 0 0 0 0 Class 422

0 0 0 0 0 0 0 0 0

d 14 0 0

0

0

−d 14 0 0 0

Class 4 / mmm centrosymmetrical, dijk = 0

d 14

0

0

0

d 14

0

0

0 d 36

104 tensor properties of solids

TABLE 6.2: (continued) Trigonal Class

Class 3

d 11 − d 22 d 31

−d 11

d 22 d 31

0 0 d 33

d 14 d 15 0

d 15 _ d 14 0

0 − d22 d31

_ 2d 22

−2d 11 0

3m

(m ⊥ x1)

0

0

0

d15

−2d 22

d 22

0

0

0

d31

d 33

d 15 0

0

0

Class 3 centrosymmetrical, dijk = 0 Class 32 (quartz)

d 11 0 0

−d 11 0 0

0

d 14 0 0 0 0

0 − d 14 0

0

− 2d 11

0

Class 3 m centrosymmetrical, dijk = 0 Hexagonal

_ Class 6

Class 6 0 0 0 0 0 0 d 31 d 31 d 33

d 14 d 15 0

d 15 0 −d 14 0 0 0

d 11 −d 22 0

_d

11

d 22 0

0 0 0 _ 2d 22 0 0 0 _ 2 d 11 0 0 0 0

Class 6 centrosymmetrical, dijk = 0 Class 6mm (same as 4mm )

0 0 d31

0

0

0

d 15

0

0

d 15

0

d 31 d 33

0

0

Class 622 (same as 422)

0

0 0 0 0 0 0 0 0 0

0 0 _ Class 62m

d 11 −d 11 0 0 0 0

0 0 0

0

0 0 0

−2 d 11

0 0 0

0

Class 6 mmm centrosymmetrical, dijk = 0

d 14 0 0

0

0

−d 14 0 0 0

Third- and Fourth-Rank Tensor Properties 105

TABLE 6.2: (continued) Cubic

_ Class 23 and 4 3m

0 0 0 0 0 0 0 0 0

Class 432

d 14

0

0

0

d 14

0

0

0 d 14

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Class m3 centrosymmetrical, dijk = 0 Class m3m centrosymmetrical, dijk = 0

To demonstrate the use of the piezoelectric moduli in Table 6.2, we will work a couple of problems involving quartz, which belongs to the crystal class 32. Consider the direct piezoelectric effect represented by Eq. (6.2) as applied to class 32 and the application of normal and shear stresses. Shown in Figure 6.1(a) is the array of piezoelectric moduli for class 32 together with the corresponding polarization and stress components. In Figure 6.1(b) is the stereogram for class 32 giving the x1 and x2 axes in the (0001) plane with its normal along the threefold (optic) axis, x3. Clearly, there are only two independent piezoelastic moduli, d11 and d14. Referring to Figure 6.1 for quartz, a polarization P1 can be produced along the x1 direction under the following conditions: 1. By a tensile stress σ1 applied along the x1, resulting in P1 = d11σ1, where P2 = P3 = 0. 2. By a compressive stress σ2 applied along x1, resulting in P1 = -d11σ2 where P2 = P3 = 0. 3. By a shear stress σ4 = σ23, resulting in P1 = d14σ4, where P2 = P3 = 0. Normal

Shear

{ { σ1

σ2

σ3 σ4

σ5

σ6

P1 d11 –d11 0 d14 0 Along x1 0 d = P2 0 0 0 0 –d14 –2d11 Along x2 P3 0 0 0 0 0 0 Along x3

(a)

y' z,x3 y x2 x,x1

(b)

FIGURE 6.1: (a) Piezoelectric moduli for quartz (class 32) and the corresponding polarization and stress components. (b) Stereogram for class 32.

106 tensor properties of solids

A polarization P2 along x2 can be produced only by negative shear stresses σ31 and σ12 giving P2 = -d14σ31 and P2 = -2d11σ12, where for both P1 = P3 = 0. From Figure 6.1(a), it is evident that a polarization P3 along x3 is not possible under any set of conditions.

6.1.5 Longitudinal Piezoelectric Effect The polarization can be found in an arbitrary direction P1′ according to P1′ = d 111 ′ σ11′ = d 11 ′ σ 1′.

(6.23)

Here, d1′1, measures the longitudinal piezoelectric effect in the x1x2 plane, meaning the charge per unit area on the surface of a plate divided by the force per unit area applied normal to that surface, which is in the 0x3 direction. To find d1′1, we will need to find α -1 by making use of the equations σ = ∼a σ ′a = α -1σ ′, which are the inverse of Eqs. (2.21) and (2.22). Recall that the stress tensor is a symmetric second-rank tensor. Once α -1 is known, then d1′1, can be found from the transformation equation d ′ = adα -1, where a given moduli array is chosen from Table 6.2. As an example, we will find d1′1 for a quartz crystal. Shown in Figure 6.2 is the longitudinal direction 0x′1 and direction cosines relative to a set of coordinate axes such that lie in the (0001) plane of a quartz crystal. Thus, as required, the surface of the crystal must conform to the point group symmetry. Because a polarization cannot be produced alone 0x3, a direction 0x′1 out of the x1x2 plane will produce a polarization only due to the projection of 0x′1 onto the x1x2 plane. Thus, we are entitled, but not required, to set a13 = l3 = 0, not shown in Figure 6.2. To facilitate the calculations, we will make the following transformation simplifications: a11 = l1, a12 = l2, a13 = l3, with mi and ni used for the remaining direction cosines following Eq. (3.24). First, we will find α -1 as follows:

l1 σ =a%σ ′a = l2 l 3

m1 m2 m3

l2 n1 σ 1′ 0 0 l1 n2 0 0 0 m1 m2 n3 0 0 0 n1 n2

l3 l 12 m3 = l1 l2 n l l 3

3 1

l1 l2 l22 l2 l3

l3 l1 l2 l3 σ 1′ . l 2 3

(6.24)

Then, reconfiguring yields the result

σ1 σ2 σ σ = 3= σ4 σ 5 σ6

l12 2 l2 l2 3 l2 l3 l l 3 1 l1 l2

0

0

0

0

0 σ 1′

0

0

0

0

0

0

0

0

0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

−1 = α σ′ .

(6.25)

Third- and Fourth-Rank Tensor Properties 107

x2 x'2

x'1

cos–1�2 90 o - θ θ

x3

cos–1�1

x1

0

FIGURE 6.2: Longitudinal direction x1 relative to a set of coordinate axes, where x1 and x2 lie in the (0001) plane of crystal class 32.

Now with α-1 known, we will set up the matrix equation for d ′ = ada-1 where d is the class 32 array obtained from Table 6.2. Thus, there results l1 l2 d ′ = m1 m2 n 1 n 2 l1d11 = m1d11 n1d 11

l 3 d 11 −d 11 0 d 14 m3 0 0 0 0 n 3 0 0 0 0 − l1d11 0 l1d14 −m1d11 0 m1d14 − n1d 11 0 n1d 14

− l2 d14 −m2 d14 − n2d 14

0 −d14 0

0 −2d 11 α −1 = a d α − 1 0

−2l 2 d11 −2m2 d 11 −2n2 d 11

l 12 l 22 l 32 l 2 l3 l3 l1 l1l 2

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 . 0 0 0 0 (6.26)

0 0 0 0 0 0

Therefore, d11′ = l13 d11 − l1 l22 d11 + l1 l2 l3 d14 − l1 l2 l3 d14 − 2 l1 l22 d11

= l13 d11 − 3 l1 l22 d11 = l1 ( l12 − 3 l22 ) d11 ,

(6.27)

which is seen to depend only on d11. Furthermore, from Figure 6.2, it follows that l1 = cosθ and l2 = cos(90° - θ) = sinθ. Therefore, with the help of trigonometric identities, we find d11′ = d11 cos θ (cos2 θ − 3 sin2 θ )

= d11 cos θ (cos2 θ + 3 cos2 θ − 3)

= d11 ( 4 cos3 θ − 3 cosθ ) = d11 cos 3θ .

(6.28)

The result d1′1 = d11 cos 3θ forms a three-petal (each almond shaped) rosette in the (0001) plane, indicating that the polarization is a maximum along the directions x, y, and y ′ spaced 120° apart (see Figure 6.1(b)) and that it is zero at 60° intervals between the x, y , and y ′ directions.

108 tensor properties of solids

6.1.6 Transverse Piezoelectric Effect A similar procedure to that used for the longitudinal piezoelectric effect can be used for the transverse piezoelectric effect. However, the calculations are necessarily made more complex because the direction cosines li , mj , and nk (i, j, k = 1, 2, 3) will, in general, be involved. To demonstrate, let us set up the equations σ = a∼σ ′ a = α -1 σ ′ for the case of a shear stress σ 6 ′ = σ12′ applied to a quartz crystal relative to axes x′1 and x′2 . The results become

l1 σ = a% σ ′ a = l2 l3

m1 m2 m3

n1 0 σ6′ n2 σ6′ 0 n3 0 0

σ 1 0 σ 0 2 σ 0 σ = 3 = σ 4 0 σ 5 0 σ 6 0

0 0 0 0 0 0

l2 0 l1 0 m3 m3 0 n3 n3 0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

l3 2 l1 m1 m3 = n3 Sym.

l1m2 + l2 m1 2 l2 m2

2l 1m 1 0 2l2m 2 0 2l3m 3 0 −1 = α σ′ l2m 3 + l3m 2 0 l3m 1 + l1m 3 0 l1m 2 + l2m 1 σ 6′

l3 m1 + l1m3 l2m3 + l3m2 σ ′ 2 l3 m3

(6.29)

Knowing α -1 permits us to evaluate d ′ = ad α -1, which will be more complex to evaluate than in the case of the longitudinal effect given by Eqs. (6.26), (6.27), and (6.28).

6.2 ELASTICITY The concept of elasticity can best be understood by considering a one-dimensional lattice shown in Figure 6.3. Here, the equilibrium condition is demonstrated in Figure 6.3(a), where the lattice parameter is given by a0. Then, if a tensile force is applied along the 0x direction the atoms are displaced by an amount l = a - a0 to an atom separation of a as in Figure 6.3(b). At a state of equia0

a f

(a)

f (b)

FIGURE 6.3: A one-dimensional lattice. (a) Atoms at equilibrium with lattice parameter a0. (b) Atoms reversibly displaced after the application of a tensile force f along the 0x direction.

Third- and Fourth-Rank Tensor Properties 109

+ Binding Energy 0 E(l)

a0

l

_

(dE/dl) l

=0=

0 Position of stability

Attraction

Force

f(l) 0

Repulsion

l f=0

FIGURE 6.4: Binding energy and tensile force showing position of stability in a one-dimensional lattice.

librium, the force f0 would represent a short-ranged attractive force between atoms along 0x where the lattice parameter between atoms is maintained at a0. The binding energy of the atoms in the one-dimensional lattice is a function of the atom displacement l and is shown in Figure 6.4. Here, at static equilibrium, the minimum in the energy curve occurs at (dE / dl )l = 0 = 0,

(6.30)

for which the applied tensile force f = 0 and where a = a0. So, as f → 0, a position of stability between the atoms is approached. Of course, the force f can be either a tensile force r a compressive force. The convention followed in this text is as follows:

If

f > 0

tensile

a > a0 and

l>0

If

f < 0

compressive

a < a0 and

l < 0.

In any case, the cohesive force between atoms is a reversible function of displacement.

110 tensor properties of solids

6.2.1 Hooke’s Law Assuming that the elastic strain energy E is everywhere a continuous function of displacement l, we can expand E in a Maclaurin series about the state of displacement l = 0, there results

1 d2E dE l + 2 2 dl d l (0)

E ( l ) = E0 +

2 .. . l + . (0)

(6.31)

For very small l, small linear strains exist, and applying Eq. (6.30), we have

E ( l ) ≅ E0 +

1 d2E

l 2 + .... 2 d l 2 (0)

(6.32)

Taking the derivative of Eq. (6.32) with respect to displacement l leads to Hooke’s law given as

f =

d E(l ) dl

d2 E l =Y⋅l, 2 d l (0)

=

(6.33)

where

d2 E = Young's Modulus. Y = 2 d l (0)

(6.34)

Here, Young’s modulus (d2 E / dl 2) is the curvature of the E(l ) versus l curve in Figure 6.4. Thus, the sharper the minimum in the E(l ) versus l curve, the greater will be the Young’s modulus, Y, and vice versa.

6.2.2 Bulk Elastic Behavior Up to this point, we have dealt with a one-dimensional lattice to express the simplest form of Hooke’s law. Now we must move to bulk elastic representations that have practical application. To expand the one-dimensions model to bulk elastic behavior require summing all individual elastic deformations between atoms (neighbors, next nearest neighbors, etc.) taken over all directions in the crystal. Clearly, ∑i( fi = Yli ) applied in this manner would be an impossible task. This apparent dilemma can be overcome by making the following transformations:

f ⇒ σ = stress l ⇒ ε = strain.

(6.35)

Now, the two alternative forms of Hooke’s law may be expressed in terms of the new parameters, σ and ε, as

Third- and Fourth-Rank Tensor Properties 111

σ = c ε , ε = sσ

(6.36)

where

c = E lastic stiffness coefficient (N/m2) S

= E lastic compliance coefficient = c −1.

(6.36a)

Following the developments given in Section 6.1 with regard to stress and strain, we can express Hooke’s law σ = cε in tensor and matrix form, respectively, as

σij = cijkl εkl

(i, j, k, l = 1 - 3)

(6.37)

(m, n = 1 - 6).

(6.38)

and

σm = cmn εn

Here, the first and last suffix pairs of cijkl permit the cmn coefficients to be unfolded according to the following scheme.

Tensor Notation 11 22 33 23, 32 31, 13 12, 21 Matrix Notation 1 2 3 4 5 6

(6.39)

Then, by thermodynamic arguments presented in Section 4.4, we can write

cmn = cnm.

(6.40)

In expanded matrix form, Eq. (6.38) becomes

σ 1 c11 c12 c13 σ c 22 c23 2 σ3 c33 = σ 4 σ Sym. 5 σ 6

c14 c24 c34 c44

c15 c 25 c35 c45 c55

c16 ε1 c26 ε 2 c36 ε 3 ⋅ c46 ε 4 c56 ε5 c66 ε6

(6.41)

where, as before in Section 6.1, σ1, σ2, and σ3 are the tensile stresses (positive by convention) and σ4, σ5, and σ6 are shear stresses, with the understanding that σ23 = σ32 = σ4, σ31 = σ13 = σ5, and σ12 = σ21 = σ6. With the convention used in Eq. (6.14), the strains ε1, ε2 and ε3 are the elastic tensile strains or stretches, and the three remaining, ε4, ε5 and ε6, are the elastic shear strains.

112 tensor properties of solids

The alternative form of Hooke’s law ε = sσ is presented in the tensor form as

εij = sijkl σkl ,

(6.42)

which represents nine equations each with nine terms—a total of 81 sijkl coefficients. Equation (6.42) can be represented in the simplified matrix form

εm = smnσn

(m, n = 1 - 6),

(6.43)

provided that 2’s and 4’s are introduced into the definitions of simn according to the following: sijkl = smn when m and n are 1, 2, or 3 2sijkl = smn when either m and n are 4, 5, or 6 4sijkl = smn when either m and n are 4, 5, or 6. These definitions avoid the appearance of the 2’s and 4’s in Eq. (6.42), thereby making the simplified matrix form possible. Note that in the case of Eq. (6.38), no introductions of 2’s and 4’s were necessary to allow Eq. (6.41). By the thermodynamic arguments presented in Section 4.4, we can write smn = snm ,

(6.44)

giving the expanded matrix form of Eq. (6.43) as

ε 1 s11 s12 s13 ε s22 s23 2 ε3 s33 = ε 4 ε Sym. 5 ε 6

s14 s24 s34 s44

s15 s16 σ1 s25 s26 σ 2 s35 s36 σ3 ⋅ s45 s46 σ4 s55 s56 σ5 s66 σ6

(6.45)

6.2.3 Transformation Laws The transformation laws for the elastic stiffness coefficients and elastic compliances are easily determined by using matrix notation together with the quadratic transformation matrix, α. The reader may find it helpful to review Section 6.1 because it pertains to the transformation laws for the direct and converse piezoelectric effects. Beginning with the stiffness coefficients, the procedure is as follows: Let σ = cε be true relative to the “old” axes and let σ ′ = c ′ε ′ hold relative to the “new” axes. Stress transforms to the “new” axes as

Third- and Fourth-Rank Tensor Properties 113

σ ′ = ασ. Then referring to the developments leading to Eq. (6.15), the strain transforms to the new ∼ -1ε or ε = α ∼ ε ′. Therefore, it follows that σ ′ = ασ = αcε = αcα ∼ ε′ = c ′ε ′, or finally, axes as ε ′ = α ~ . c ′ = α cα

(6.46)

A procedure similar to that for the stiffness coefficients is followed for the elastic compliance coefficients. Let ε = sσ and ε ′ = s ′σ ′ be valid for the old and new axes, respectively. From the pre ∼ -1ε = α∼ -1 sσ = α∼ -1 sα -1σ ′ = s ′σ ′ from which results ceding, σ = α -1σ ′, such that we can write ε ′ = α ~ −1 sα −1 s′ = α ,

(6.47)

∼ . Here, α∼ -1 is the transpose of the inverse of α, two operations. where it is understood that α -1 ≠ α

6.2.4 Elastic Strain Energy Density Referring to the thermodynamic potentials in Table 4.2, the elastic strain energy density can be given by

df = dw = σi dεi = ci j εj dεi

(i, j = 1 − 6)

(6.48)

or

−dg = εi dσi = si j σj dσi

(i, j = 1 − 6)

(6.49)

for a reversible, isothermal deformation in the absence of all electrical and magnetic fields and their conjugate effects. For a linear elastic solid under these conditions, σi dεi = εi dσi. Making use of the substitution property of the Kronecker delta dij (see Section 2.6.3), there results εj = dij εi permitting Eq. (6.48) to be integrated for the elastic strain energy density

wElastic = =

∫ ci

j

1

2

( δij εi ) dεi =

cij εi εj =

1

2

1

2

cij ( δij ε i2 ) + C

σi εi

(i = 1 − 6),

(6.50)

where the constant of integration C = 0 because welastic = 0 if εiεj = 0. For the total strain energy, Eq. (6.50) must be integrated over the volume of the deformed crystal,

ETotal =

∫V σi εi dV .

(6.51)

6.2.5 Effect of Crystal Symmetry Because the procedure to be followed here is similar to that used in Section 6.1 for the piezoelectric moduli, the reader may find it useful to review that material. First of all, it should be recalled that all

114 tensor properties of solids

polar tensors of even rank are “centrosymmetrical.” This means that by Neumann’s principle, their property coefficients are left unchanged by the transformation operation of a center of symmetry. The procedure to be followed for property coefficients of polar fourth-rank tensor properties is as follows: 1. Use the method of direct inspection for all crystal classes for which the s generating matrices, other than s(7), are required as indicated in Table 3.6. This method provides the easiest means of obtaining the independent coefficients of polar fourth-rank tensors. The 10 possible generating matrices are given in Table 3.5 for both s and quadratic σ forms. In applying the direct inspection method to the two suffix coefficient arrays in Eqs. (6.41) and (6.45), the four suffix notation they represent must be kept in mind. Remember that it is actually the four suffix notation to which the method of direct inspection is applied via the tensor/matrix notation of Eq. (6.39). 2. The brute-force method must be used in applying the generating matrix σ(7) to the trigonal and hexagonal crystal systems of polar fourth-rank tensor properties. However, if generating matrices other than s(7) are involved in the particular crystal class, apply them first each in turn by using the method of direct inspection to obtain a simplified array of the moduli. By using the appropriate transformation law, c ′ = α c α∼ or ∼-1sα -1, complete the matrix calculations with the generating matrix σ (7), together s ′ = α with its inverse and transpose as needed, to obtain a set of equations for the new property moduli. As a final step, equate each of the old moduli with the new and solve the resulting set of equations simultaneously for the moduli appropriate for the given crystal class. It is strongly recommended that application of the brute-force method be computer assisted. As an example, let us apply the method of direct inspection to the centrosymmetrical cubic crystal class ||m3|| having the generating (s) matrices s(4) and s(10) given in Table 3.6 and their respective generation operators provided in Table 3.5. Referring to the tensor/matrix suffix notations of Eq. (6.39), we apply the transformation of axes for the generating matrices s(4) and s(10) as follows:

s

(4)

− 1 0 0 = (m ⊥ x) = 0 1 0 0 0 1

Direct inspection method: 1 → -1, 2 → 2, 3 → 3. This means that all c stiffness moduli in Eq. (6.41) containing a single 5 or single 6 (but not containing both) are zero. As examples, c15 = c1131 = 0, c25 = c2231 = 0, c46 = c2312 = 0, and so forth, for a total of eight vanishing coefficients. Application of s(10) then follows accordingly:

Third- and Fourth-Rank Tensor Properties 115

s

(10)

0 1 0 = ( 3[111] ) = 0 0 1 1 0 0

Direct inspection method: 1 → 2, 2 → 3, 3 → 1 and 4 → 5, 5 → 6, 6 → 4. Together with s(4), this means that c16 = c24 = c2223 = 0, c36 = c14 = c1123 = 0, and so forth. Also, c11 = c22 = c33, c44 = c55 = c66 , and c12 = c23 = c31. If, for class ||m3m||, the transformation of axes for s(4) and s(9) together with that for s(10) is applied to the remainder of the cubic classes, the results are found to be the same as above. Thus, the elastic stiffness and compliance coefficients for all classes of the cubic system are given by the following arrays in which there are three independent coefficients, c11, c12 , c44, and s11 , s22 , s44:

c11 c =

c12

c12

0

0

0

s12

s12

0

0

c11

c12

0

0

0

s11

s12

0

0

c11

0

0

0

s11

0

0

c44

0

0

s44

0

c44

0

Sym.

c44

s11 and s =

Sym.

s44

0

0 0 0 s44 0

Continuing in this way, the independent elastic stiffness coefficients are identified for the remainder of the seven crystal systems and are presented in Table 6.3. The case of an isotropic solid is added for completeness and will be considered separately below as an extension of the cubic crystal system. TABLE 6.3: The independent elastic stiffness coefficients for the seven crystal systems with the addition of the case for the isotropic solid Triclinic

c 11

c 12

1, 1 c 13 c 14

c 15

c 16

c 22

c 23

c24

c 25

c33

c 34

c 35 c 36

c44

c 45

Sym.

c55

c 26

c46

c 56 c66

116 tensor properties of solids

TABLE 6.3: (continued) Monoclinic m, 2, 2 / m for diad parallel to x2 c 11 c 12 c 13 0 c 15 0

c 22

c 23

0

c 25

0

c 33

0

c 35

0

c 44

0

c 46

Sym.

c55

0

c 66 Orthorhombic 2mm, 222, mmm c 12 c 13 0 0

c 11 c 22 c 23 c 33 Sym. _ 4, 4, 4 / m c 13 0 0

c 11 c 12 c 11 c 13 c 33 Sym.

0

0

0

0

c 44

0 c 44

0

0

0 0

0

0

0

c 44

0

0 0

Tetragonal c 16 − c 16

0 0 0 c 66

c 55

c 66 _ 4mm, 42m, 422, 4 / mmm 0 c 11 c 12 c13 0 0

c 11

Sym.

c 13

0

0

0

c 33

0

0

0

c 44

0

0

c 44

0 c 66

Third- and Fourth-Rank Tensor Properties 117

TABLE 6.3: (continued) Trigonal

_ 3, 3

c 11 c 12 c 13 c 11 c 13 c 33 Sym.

c 14

−c 14 0 c44

−c 25 c25 0 0 c 44

c 11

0 0 (c 25 ) (c14 ) 1 ( c 11 − c12 ) 2 0

{

_ 3m, 32, 3m

}

c 12

c 13

c 14

0

c 11

c 13

− c14

0

0

0

c 44

0

c 33 Sym.

c 44

( c25 ) → 2s25 , ( c14 ) → − 2s 14

{

}

1 ( c11 − c 12) → 2 (s11 − s12 ) 2

Hexagonal _ _ 6, 6, 6 / m , 6mm, 622, 62m, 6 / mmm 0 c 11 c 12 c 13 0 0

c 11

c 13

0

0

c 33

0

0

c 44

0

Sym.

c 44

0 0 0 1 ( c11 − c12) 2 0

{

}

Cubic _ 23, m3 , 432, 432, m3m , c 11 c 12 c 12 0 0 0 c11 c 12 0 0 0

c 11 Sym.

0

0

0

c 44

0

0 0

c 44

c 44

0 0 0 c ( 14 ) 1 (c 11 − c 12 ) 2 0

{

}

118 tensor properties of solids

TABLE 6.3: (continued) Isotropic

c 11

c 12

c 12

0

0

c 11

c 12

0

0

c 11

0

0

{

1 ( c11 − c12) 2

}

Sym.

{

0

{

0 0 0 0 1 (c 11 − c 12 ) 2 0

1 (c 11 − c12) 2

}

}

{

}

1 (c 11 − c 12 ) → 2( s11 − s12 ) 2

The classes to which a given coefficient array belongs are indicated above the array. Note that the elastic compliance coefficients sij are obtained from the elastic stuffiness coefficients by replacing c by s except where noted by parentheses and braces {x}.

6.2.6 Homogeneous Elastically Isotropic Solids Consider the ′ = σ 6′ to the cubic system, where x′1 , = [110] _ application of a pure shear stress σ 12 ′ = σ 21 and x′2 , = [1 10] as shown by the 45° rotation in Figure 6.5. In the absence of all other stresses, σ ′1 = σ 2′ = σ 3′ = σ ′4 = σ 5′ = 0, the stress tensor transforms as the inverse of Eq. (2.13) or x3, z 450

x2' x2, y

x1, x FIGURE 6.5: Rotation of 45° about the z axis.

x1'

Third- and Fourth-Rank Tensor Properties 119

1 2 a σ ′ a = 1 2 σ =~ 0

−1

2

1

2 0

0 0

0 1

σ6′

0 σ 6′ 1 0

2

1

2

0 − 1 2 1 2 0 0 0

0 0

0

0 = 1

− 1 0 0 0 1 0 σ ′ 6 0 0 0

(6.52) Introducing the results of Eq. (6.52) into Eq. (6.43) for the cubic system yields

s11 εm′ = smn σn′ =

s12

s12

0

0

0 − 1

s11

s12

0

0

0

s11

0

0

0

s44

0

0

s44

0

Sym.

s44

1 0 0 0 0

− ( s11 − s12 ) (s − s ) 11 12 0 σ 6′ = σ 6′ 0 0 0

(6.53)

Then, transforming shear strain to the new axes gives

εi′j = aikajl ε kl or ε12 ′ = a11a21ε 11 + a12a22ε 22 = −ε 11/2 + ε 22 /2.

Therefore, by Eq. (6.53), we have ε′12 = [(s11 - s12) / 2 + (s11 - s12) / 2] σ′12 = (s11 - s12) σ′12 where use of the matrix-to-tensor strain conversion of Eq. (6.14) yields the results

ε 6′ = 2ε 12 ′ = 2(s11 − s12)σ 6′ = s44σ 6′ or s44 = 2(s11 − s12)

(6.54)

as the necessary and sufficient condition for elastic isotropy, in agreement with Table 6.3. Obviously, the application of any other pure shear stress, σ′4 or σ′5 , would lead to the same result. Let us now compare the elastically isotropic compliance array in Table 6.3 with those frequently found in engineering textbooks:

ε1 ε 2 ε3 = ε4 ε 5 ε6

s11

s12

s12

0

0

0

s11

s12

0

0

0

s11

0

0

0

2 ( s11 − s12 )

0

0

2 ( s11 − s12 )

0

Sym.

2 ( s11 −

σ1 σ 2 σ3 σ 4 σ 5 s12 ) σ6

(6.55)

120 tensor properties of solids

ε 1 ε 2 ε 3 = ε 4 ε 5 ε 6

1 / Y

− ν /Y

− ν /Y

1 /Y

− ν /Y 1 /Y

Sym.

0

0

0 σ1

0

0

0

σ2 0 σ3 0 0 1/G 0 0 σ4 1/G 0 σ5 1 / G σ6

(6.56)

A comparison of Eqs. (6.55) and (6.56) indicates the following relationships: s12 = −ν / Y

s11 = 1 / Y

and 2(s11 − s12) = 1 / G,

(6.57)

where Y is Young’s modulus, ν is Poisson’s ratio, and G is thes modulus of rigidity with the combined relation, derived from Eq. (6.57), given by G = Y / {2(1 + ν)} .

(6.58)

Here, Y is a measure of the elongation of an elastically isotropic solid under tension, and ν is a measure of the transverse contraction (at right angles to the elongation). The rigidity modulus measures the stuffiness to shear.

6.2.7 Young’s Modulus in a Particular Direction Consider a bar-shaped crystal of axis 0x1′, along which is applied a unit tensile stress σ 1′ as shown in Figure 6.6.

σ1'

x3 x1'

x3' x2'

x2 x1

(a)

(b)

FIGURE 6.6: (a) Application of a unit tensile stress to a crystal rod along the 0x1′ direction. (b) Orientation of the rod axis 0x′1 relative to reference axes 0xi.

Third- and Fourth-Rank Tensor Properties 121

From Eq. (6.57), Young’s modulus can be defined in the 0x direction ′ as 1 s′11 = 1 / Y = ε 1′ / σ 1′

(6.59)

′ of the rod such that where it is understood that σ 1′ is a unit tensile stress applied along the 0x axis 1 σ 2′ = σ 3′ = σ 4′ = σ 5′ = σ 6′ = 0. Referring to Figure 2.1, let the direction cosines for 0x in ′ Figure 6.6(b) 1 relative to reference axes 0xi be represented as follows: a11 = l1, a12 = l2, and a13 = l3. Then, s′11 is found for any crystal system by Eq. (6.47), which is ~ −1 s α −1 s′ = α

(6.60)

where α-1 is found from σ = a∼σ ′ a = α -1 σ ′ as in Eq. (6.25). Proceeding, having determined α -1, we apply Eq. (6.60) to the cubic system to give l 12 l 22 0 0 0 0 s′ = 0 0 0 0 0 0

or

l 32 l2 l3 0 0 0 0 0 0 0 0 0 0

l3 l 1 0 0 0 0 0

l1 l2 s11 0 0 0 0 0

s12 s11

s12 s12 s11

0 0 0 s44

Sym.

0 0 0 0 s44

0 0 0 0 0 s44

l12 l22 l32 l2 l 3 l 3 l1 l1 l2

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

s′11 = s11(l 14 + l 24 + l 34 ) + s44(l 22 l 32 + l 32 l 12 + l 12 l 22 ) + 2s12(l 22 l 32 + l 32 l 12 + l 12 l 22 ).

But (l 41 + l 42 + l 43 ) = (l 21 + l 22 + l 23 ) -2(l 22 l 23 + l 23 l 21 + l 21 l 22) which, when introduced into the equation for s′11, yields the well-known result

′ = s11

1 = s11 + { s44 − 2 ( s11 − s12 )} Y

(l

2 2 l + l32 l12 2 3

)

+ l12 l22 ,

′ [uvw], such that which is not isotropic. Now, as examples, let 0x = 1

l1 = u / u 2 + v 2 + w 2 , l2 = v / u 2 + v 2 + w 2 , l3 = w / u 2 + v 2 + w 2

where ( l22l 32 + l 23 l 21 + l 21 l 22 ) = (u 2v 2 + v 2 w 2 + w 2u 2 ) (u 2 + v 2 + w 2 ) which is always positive.

(6.61)

122 tensor properties of solids

Along (l 22 l 23 + l 23 l 21 + l 21 l 22 ) = 0 and Y = 1/ s11 = Ymin ′ ) / 3 ; Y = Ymax . Along (l 22 l 23 + l 23 l 21 + l 21 l 22 ) = 1/ 3 and 1 / Y = s11 + ( s44 − s44 Also, because (s44 − s4′4) = 3(Y -1 − Y -1), then

−1 −1 −1 −1 Y = Y + 3 (Y − Y ).

(6.62)

The results for other crystal systems can be found in Nye cited in Endnotes.

6.2.8 Shear Modulus and Poisson’s Ratio The analysis for the shear modulus follows in a similar manner to that for Young’s Modulus. Con′ the 0x direction ′ on a plane whose normal is the 0x′2 sider the application of a shear stress σ in 6 1 direction. Thus, we define 1 = ε 6′ . G σ 6′ (6.63) The method of solution is the same as for Young’s modulus, namely, s′ = α∼ -1 sα -1, where α -1 is found from σ = a∼ σ ′a and σ = α -1σ ′. After simplifying the result, the rigidity modulus is

2 2 2 2 2 2 1 G = s44 − 2 {( s44 − 2( s11 −s12 )} (a11 a21 + a12 a22 + a13 a33 ) ,

(6.64)

which is easily seen not to be isotropic. If we take [uvw] = 0x1′ and [hkl ] = 0x′2, then

(a112 a212 + a122 a222 + a132 a332 ) = {(uh)2 + (vk) 2 + (wl )2 }

(u 2 + v 2 + w 2 )( h 2 + k 2 + l 2 )

Poisson’s ratio, defined as v = −ε2′ / ε1′ = −ε3′ / ε1′, is more difficult to obtain by using the procedure above. However, knowing Y and G, it is easily found from Eq. (6.58) to be

ν = Y / 2 G − 1. • • • •

(6.65)

123

chapter 7

Second- and Higher-Order Effects— Symmetry Considerations First, as we move into a discussion of the second- and higher-order effects, it quickly becomes apparent that their number is far too large for a detailed inclusion in this text. However, we will give specific examples, for instructional purposes, and then provide a generalized approach to their development. Second, it is often the case that the second-order effects do not depend strongly on the magnitudes of the intensive and extensive parameters and may be regarded as weak correction terms (if they exist at all) to the first-order effects under a given set of small intensive or extensive fields. Remember that the first-order effects were developed under the assumption of infinitesimally small fields. However, some second-order effects may actually dominate the first-order effects particularly under field strengths that are not infinitesimally small. If the second-order effects are but weak correction terms to the first-order effects, then it is safe to say that the third- and higher-order effects may be disregarded as we do in our treatment.

7.1 ELECTROSTRICTION AND MORPHIC EFFECTS

~ Recall that the piezoelectric moduli were given earlier by Eq. (4.62) as C P, σ )T,E,B = C ε,E )T,B,σ = dT, B . Here, the converse piezoelectric effect is the first-order electrostriction effect expressed in integrated tensor form as

εij = dijk Ek = εji ,

(7.1)

which applies for very small electric fields and very small stresses and strains all at constant T, B, and σ. At large stresses and strains, quadratic (second-order) terms must be introduced. To do this, we can expand dijk in a Taylor series to give

∂d 1 ∂ 2dijk dijk = dijk0 + ijk E E + …, El + 2 ∂El ∂Em T , B,σ l m ∂ El T , B,σ

(7.2)

0 is the value for dijk at infinitesimal field strength. Introducing Eq. (7.2) into Eq. (7.1) gives where dijk the result

124 tensor properties of solids

{

}

E + … Ek , (7.3) ijkl l 0 where the third-rank tensor terms γijkl El + ... are the correction terms to dijk proportional to field strength and that must conform to both tensor and crystal symmetry. 0 vanish for the 11 centrosymmetrical crystal classes given in All electrostrictive moduli dijk Table 3.4. However, the correction terms γijkl El + ... are not centrosymmetrical and can create new electrostrictive moduli proportional to the field strength E and a strain proportional to E 2. These new moduli create what is called a morphic effect. Thus, an electrostrictive effect in a centrosymmetrical class can exist but only as a morphic effect. 0 + γ εij = dijk

7.1.1 Symmetry and Transformation Considerations of Fourth-Rank Tensors Given the second-order electrostrictive effect from Eq. (7.3),

εij = γ ijkl El Ek ,

xxx(7.4)

it follows that the symmetry for γ becomes

γ

ijkl

=γ

jikl

=γ

ijlk

=γ

jilk

=γ

mn

,

(7.5)

since strain is commonly taken to be symmetrical, εij = εji. Therefore, we can write

εm = γmn (EE )n or ε = γ ( EE )

where

γmn ≠ γnm .

(7.6)

Now, the transformation law for γ can be determined in matrix form from Eqs. (6.46), (7.5), and (7.6) as follows: First, we recognize that all principal compliance and rigidity effects, respectively, those along the leading diagonals in Eqs. (4.29) and (4.33), exhibit thermodynamic symmetry as illustrated by Eqs. (4.48) to (4.50). Accordingly, the elastic stiffness tensor cijkl (a property rigidity) is symmetrical to the extent that cmn = cnm, which derives from the fact that both stress and strain are taken to be symmetrical ∼ , where a is the second-rank tensors. Thus, cijkl transforms in matrix notation as in Eq. (6.46) or c ′ = a c a quadratic transformation form discussed in Section 2.2. In matrix notation, we can write that σ = cε with respect to the “old” set of axes 0xi and that σ ′ = c ′ε ′ with respect to the “new” set of axes 0xi′ . Now, with appropriate substitutions we write

∼ε′ = acε σ ′ = aσ = c ′ε ′ = ac a

Solving for ε ′ by acknowledging the transformation for the dyadic EE and using Eq. (7.6), there results

∼ -1 ε and ε ′ = a

(EE)′ = a(EE) or

(EE) = a -1(EE)′

∼ -1ε = a ∼ -1γ (EE) = a ∼ -1γa -1 (EE)′ = γ (EE)′, resulting in the transformation form Therefore, ε ′ = a

Second- and Higher-Order Effects—Symmetry Considerations 125

~−1γ α −1, γ ′ =α

(7.7)

which transforms exactly like the elastic compliance coefficient, s ′ = a∼ -1 sa -1 given in Eq. (6.47).

7.2

GENERALIZED DEVELOPMENT OF THE SECOND-ORDER EFFECTS

Let the intensive parameters be represented by a , β , γ, ... and their conjugate extensive parameters represented by a, b, c, ... , such that the state equations for the extensive parameters are a = a (α ,β ,γ , …)b ,c , ... b = b (α ,β ,γ , …)a ,c , ... �

�

(7.8)

Similarly, the state equations for the intensive parameters are

α = α (a ,b, c , …)β , γ , … β = β ( a , b, c , …)α, γ , … �

�

(7.9)

We now expand each state equation in Eqs. (7.8) in a differential Taylor’s series with the result

∞ 1

∂ ∂ ∂ … n d a (α ,β ,γ , …) d d + + + α β γ ∂α b, c,… ∂β ∂γ n=1 n !

da = ∑

∞ 1

∂ ∂ ∂ … n b (α ,β ,γ , …) dα + dβ + dγ + a, c,… ∂α ∂β ∂γ n=1 n !

db = ∑

M

M

(7.10)

Similarly, the Taylor series expansion of the intensive state equations in (7.9) become

∞ 1 ∂ ∂ ∂ … n c d d a b d + + +

dα = ∑ n =1

n!

∂a

∂b

∂c

α (a , b , c ,…)

β ,γ ,…

∞ 1

∂ ∂ ∂ … n + db + dc + d a ∂a ∂b ∂c n =1 n !

dβ = ∑

M

β (a , b, c, …)

α ,γ ,…

M

(7.11)

Now, for the sake of illustration, consider any two intensive parameters α and β and their corresponding (conjugate) extensive parameters a and b with all other extensive parameters held

126 tensor properties of solids

constant, i.e., γ,δ, ... = constant. Then, if Eqs. (7.10) apply to the compliance effects as in Eq. (4.26), we can use Taylor’s expansions to evaluate the integrals ∫da and ∫db, giving

∆ a = (C

a,α

)β ∆α + (C

1 ∂ (C )α ∆β + 2 ∂α

)β

1 ∂ (C 2 ∂α

)β

a, α

a, β

∆ b = (C b, α )β ∆ α + (C b , β)α ∆β +

b,α

( ∆α )

2

1 ∂ (C + 2 ∂β

)α

1 ∂ (C 2 ∂β

)α

a, β

b, β

( ∆α )2 +

( ∆β )2 + …

(7.12)

(∆β )2 + …,

(7.13)

where now ∆α = α - α and ∆b = b - b, indicating that the Taylor series (7.12) and (7.13) are to be evaluated around initial values α0 and b0 that become vanishingly small. After differentiating Eqs. (7.12) and (7.13), there results

d a = (C a, α)β d α + (C a, β)α d β +

d b = (C

)β dα + (C )α dβ +

b ,α

b, β

∂ (C a, α)β ∂α ∂ (C b, α )β ∂α

α dα +

α dα +

∂ (C a,β )α ∂β ∂ (C b,β )α ∂β

β d β + …

(7.14)

β dβ + …,

(7.15)

where use was made of

d l im (∆α )2 = 2 α dα and d l im (∆β ) 2 = 2 β dβ . α → 0 β → 0 0

(7.16)

0

If only the first- and second-order effects are considered, Eqs. (7.14) and (7.15) can be represented approximately in the matrix form ∂ C a, α (C a, α)β + α ∂α β d a d b = b, α C b,α + α ∂ C ( ) ∂α β β

a,β ∂ C a,β (C )α + β ∂β α dα . dβ b, β ∂ C b, β (C )α + β ∂β α

(7.17)

Here, other second-order terms such as ∂ 2a / ∂α∂β and ∂ 2b / ∂α∂β together with the third- and higher-order terms have been neglected. We will revisit the issue of first- and second-order terms later when we consider the phenomenological development of the optical effects. Assuming that Eqs. (7.17) are a valid approximate representation of the extensive differentials da and db as functions of the intensive α and β, then an interesting and useful relationship between the second-order terms can be derived. Since from the application of Stoke’s theorem in Eq. (4.38), we established the symmetrical nature of the compliance effects given by Cmn = Cnm , it

Second- and Higher-Order Effects—Symmetry Considerations 127

follows that a symmetrical relationship can also be established between the second-order effects in Eqs. (7.17). Thus,

(C a, β )α = ∂∂βa

permits

α

∂b = = (C b, α )β ∂α

∂ (C b,β) ∂ C a, β ∂ ∂b α = = ∂β ∂α ∂ β β α ∂ β α α

and

∂ (C a, α) ∂ C b, α β ∂ ∂a = = β ∂ α β ∂ ∂ ∂ α α β β α

(7.18)

β

(7.19)

(7.20)

because the order of differentiation is immaterial. The meaning of (∂(Cb,β)α/∂α)β in Eq. (7.19) is that Cb,β is evaluated at constant α and that its change with α is evaluated at constant β. The expressions in Eqs. (7.19) and (7.20) are second-order Maxwell relations. Introducing these expressions into Eqs. (7.17) gives the results ∂ (C b, β) a, β α (C )α + β β ∂ α dα . dβ ∂ C b,β b, β (C )α + β ∂β α (7.21) By thermodynamic symmetry, the Maxwell relations lead to the equality of cross (bracketed) terms a, α (C a, α ) + α ∂ C β ∂α β d a = db ∂ C a, α ) β C b, α + α ( )β ∂β ( α

∂ (C a, α) ∂ (C b,β )α β b, , = (C α)β + α β α ∂ α ∂ β

(C a,β )α + β

(7.22)

where it follows that ∂ (C a, α ) ∂ (C b,β )α β = β α . ∂α β ∂β α

(7.23)

Note that the expressions in Eq. (7.23) result from the symmetry expressed by Eq. (7.18) and that the second-order cross terms in Eqs. (7.21), (7.22), and (7.23) are no longer multiplied by an intensive parameter that is not held constant as in the case of Eqs. (7.17).

128 tensor properties of solids

Consider the use of Eqs. (7.21) to develop the first- and second-order electrostrictive effects as was done in Section 7.1, but from a different approach. To do this, we select the following extensive and intensive parameters:

Equations (7.21) now become

a = ε = b P

ε, σ (C ε,σ ) + σ ∂ C E ∂ E E d ε d P = ∂ (C ε, σ ) E (C P , σ ) E + σ ∂E σ

α = σ . β = E ∂ (C P,E )σ ε,E (C )σ + E E σ ∂ dσ , d E P, E P, E ∂C (C )σ + E ∂ E σ T ,B

(7.24)

(7.25)

where it is understood that T and B are held constant. By thermodynamics symmetry, the cross (braced) terms are equal giving the results

(

C ε,E

)σ

∂ (C P, E )σ ∂ (C ε, σ) E , P,σ + E = (C ) E + σ ∂σ E ∂ σ E

(7.26)

where it follows that

∂ (C P , E ) ∂ (C ε, σ) σ E , = σ E ∂σ E E ∂ σ

(7.27)

because (C ε,E)σ = (CP,σ)E . The compliances CP,E and C ε,σ are defined by Eqs. (4.45) and (4.47), respectively. Written in tensor notation, Eq. (7.27) becomes

∂χ j ∂s κ 0 i E l = ijkl σlm = ψ ijk . ∂σ kl E ∂ Em σ

(7.28)

What Eq. (7.28) indicates is that the components of the polar third-rank tensor ψijk on left side of the equation are numerical equal to those on the right side or vice versa. However, the frequency of the E and σ field changes must be the same if the equality of Eq. (7.28) is to be valid. As another approach to the evaluation of second-order effects, consider the application of the parameter selection in Eq. (7.24) to Eqs. (7.17) expressed as

Second- and Higher-Order Effects—Symmetry Considerations 129

,σ ∂ C ε ,σ ε ,E ∂ C ε ,E C + E (C ε )E + σ ( ) ∂ E σ ∂σ E σ dε dσ . d P = dE E P , , P σ P,σ ∂ C P , E ∂ C (C ) + σ (C )σ + E E ∂σ E ∂ E σ

(7.29)

The first- and second-order converse piezoelectric (electrostrictive) effects are represented by the equation for dε under constant stress σ given in tensor notation by ∂ d jk dε ij = ( dijk)σ dEk + i Ek d El ∂El σ

or in integrated form

{

ε ij = d ijk + γ ijkl E l

}

σ

Ek ,

(7.30)

which is the same as Eq. (7.3). Here, dijk are the converse piezoelectric moduli or the first-order electrostrictive moduli, and γijkl are second-order electrostrictive moduli. In conformable matrix form, ∼ q. (7.30) is given by ε = d E + λ(EE c ), where (EE c ) is the self-conjugate (dyadic) product of electric fields. In expanded matrix form, the strain matrix of Eq. (7.30) becomes

ε 1 d 11 ε d 2 12 ε 3 d 13 = ε 4 d 14 ε d 15 5 ε 6 d 16

d 21 d 22 d 23 d 24 d 25 d 26

d 31 γ 11 γ d 32 E 21 d 33 1 γ 31 E + d 34 2 γ 41 E d 35 3 γ 51 d 36 γ 61

γ 12 γ 22 γ 32 γ 42 γ 52 γ 62

γ 13 γ 23 γ 33 γ 43 γ 53 γ 63

γ 14 γ 24 γ 34 γ 44 γ 54 γ 64

γ 15 γ 25 γ 35 γ 45 γ 55 γ 65

γ 16 E E 1 1 γ 26 E2 E 2 γ 36 E3 E 3 γ 46 E2 E 3 γ 56 E3 E 1 γ 66 E1 E 2

(7.31)

where it is recalled from Section 7.1 that γmn ≠ γnm.

7.3

PHENOMENOLOGICAL DEVELOPMENT OF THE OPTICAL EFFECTS

In the presence of external fields, the dielectric constant (relative permittivity) Kij = κij / κ0 and, hence, the refractive index of a crystal may change. For example, in the presence of an external electric field, an isotropic solid may become optically anisotropic, a uniaxial crystal may become biaxial, and so forth. The effect of the external electric field on the optical symmetry of the crystal is commonly

130 tensor properties of solids

called the electro-optical effect. Similar effects are obtained by the application of other external fields such as magnetic, stress, and temperature changes. The corresponding effects are referred to as magneto-optical, piezo-optical, and thermo-optical effects, respectively. There are several ways to phenomenologically develop the previously mentioned optical effects. For example, we could expand the relative permittivity tensor, Kij in a power series as a function of electric field E, magnetic field H, and stress σ. Two of the coefficients resulting from this expansion would be called the electro-optical and piezo-optical coefficients. Alternatively, we could expand the electric field strength E as a function of the polarization P, magnetic flux density B, and strain ε,thereby obtaining the electro-optical, magneto-optical, and elasto-optical coefficients, and so forth, the choice being arbitrary and a matter of convenience. For our purposes, we will choose as the dependent variable the dielectric impermeability tensor defined as

(

)

Bij = K i−1j = κ 0 ∂Ei / ∂ Dj = Bji ,

(7.32)

→ → → where Dj is the electric flux density given vectorially as D = κ0E + P . The refractive index of a crystal is specified generally by an ellipsoid called the indicatrix whose coefficients at optical frequencies are the components of the dielectric impermeability tensor Bij given by Bijxixj =1. Expansion of the dielectric impermeability in a Taylor’s series about the state of a reference temperature T 0, zero electric field, zero magnetic flux density, and zero stress yields

∞ 1

n

∂ ∂ ∂ ∂ 0 (T − T 0 ) + Ek + Bl + σmn Bij (T , 0 , 0 ,0 ) ∂ ∂ ∂ n ! T E B ∂ σ n= 0 k l mn

Bij ( T , Ek , Bl , σmn ) = ∑

∂ Bij ∂ Bij ∂ B ij ∂ Bij = Bij (T 0 , 0, 0, 0) + ∆ T + E + B + ∂E k ∂B l ∂σ σ mn ∂ T l k mn

+

(7.33)

2 2 ∂ 2 B ij ∂ 2B ij ∂ Bij 1 ∂ Bij 2 B E B ∆ T + E + + ( ) l p σmn σqr 2 ! ∂ T 2 ∂ Ek ∂ Eo k o ∂Bl ∂ Bp ∂ σmn σqr

2 2 2 2 ∂ B ij ∂ Bij ∂ B ij ∂ Bij +2 Ek ∆ T + 2 ∂ T ∂ B Bl ∆ T + 2 ∂T ∂σ σ mn ∆T + 2 ∂ E B Ek Bl ∂ T ∂ Ek k l mn l 2 2 ∂ Bij ∂ Bij E σ 2 +2 + Bl σmn + …. k mn ∂ Ek∂σmn ∂ Bl σ mn

(7.34)

Second- and Higher-Order Effects—Symmetry Considerations 131

Here, Bij (T 0,0,0,0) and all coefficients (in parentheses) are evaluated at a reference temperature T 0 and at zero electric field, zero magnetic field, and zero stress. We now develop phenomenologically the 14 linear and quadratic optical effects expressed in Eq. (7.34). ∂ Bij = tij = linear thermo-optical effect ∂ T (T 0,0 ,0 ,0 ) 1 2

∂ 2Bij = T j = quadratic thermo-optical effect ∂T 2 (T 0,0 ,0 ,0 ) i

∂ Bij ∂ E

k (T 0,0 ,0 ,0 )

1 2

l

= fijl = linear magneto-optical (Faraday) effect (T 0,0 ,0 ,0 )

∂ 2Bij = Fijlp = quadratic magneto-optical (Cotton–Mouton) effect ∂Bl ∂Bp (T 0,0 ,0 ,0 )

∂ Bij ∂σ mn 1 2

∂ 2Bij = Rijko = quadratic electro-optical (Kerr) effect ∂ E ∂E k o (T 0,0 ,0 ,0 )

∂ Bij ∂ B 1 2

= rijk = linear electro-optical effect

= π ijmn = linear piezo-optical effect (T 0,0 ,0 ,0 )

∂ 2Bij = Πijmnqr = quadratic piezo-optical effect ∂ σ mnσ qr (T 0,0 ,0 ,0 )

∂ 2Bij ∂T ∂E k ∂ 2Bij ∂T ∂B l

) = thermoelectro-optical effect = ri(T jk (T 0,0 ,0 ,0 )

= f jl(T ) = thermomagneto-optical effect i (T 0,0 ,0 ,0 )

∂ 2Bij ∂ T∂σ mn

= π i(Tjmn) = thermopiezo-optical effect (T 0,0 ,0 ,0 )

132 tensor properties of solids

∂ 2Bij ∂E B k l

∂ 2Bij ∂ E ∂σ k mn

(T 0,0 ,0 ,0 )

∂ 2Bij ∂B σ l mn

= mijkl = magnetoelectro-optical effect

(T 0,0 ,0 ,0 )

= zijkmn = piezoelectro-optical effect

= wijlmn = piezomagneto-optical effect. (T 0,0 ,0 ,0 )

Only a few of these effects have been experimentally investigated and their tensor rank and symmetry considered. In what follows, we will briefly examine a few of the more common effects.

7.3.1 Electro-Optical Effects The linear and quadratic electro-optical effects can be obtained by applying very small electric fields to a crystal at constant reference temperature T 0 and zero magnetic field and stress. The Taylor’s series expansion of the dielectric impermeability tensor reduces to

2 ∂ Bij ∂ Bij 1 Bij (Ek ) = Bij ( 0) + E + 2 Ek Eo + L ∂Ek k ∂Ek ∂Eo

(7.35)

∆Bij = rijk Ek + Rijko Ek Eo + �.

(7.36)

or

where rijk and Rijko represent the linear and quadratic electro-optical effects, respectively. The coefficients rijk, which describe the linear electro-optical effect in crystals, form a polar nonmagnetic third-rank tensor with symmetry rijk = rjik = rmk such that the linear electro-optical effect can be written as

∆Bm = rmk Ek

( m = 1 − 6; k = 1 − 3) .

(7.37)

In simplified notation, Eq. (7.37) can be expressed as ∆B = r ⋅ E or simply as ∆B = r∼ E in conformable matrix form. Thus, the matrix representation of Eq. (7.37) is the same as the converse piezoelectric effect given by Eq. (6.11). with ε replaced by ∆B and d replaced by r. Because rijk and dijk are both third-rank polar tensors, the symmetry restrictions on their coefficients must be the same. Thus, rijk = 0 for all 11 centrosymmetrical crystal classes and the rmk for the linear electro-optical moduli are the same as those in Table 6.2 if the transpose of each array is taken with the subscripts mk reversed as in Eqs. (6.10) and (6.11). Remember that the d moduli arrays in Table 6.2 are given in normal form.

Second- and Higher-Order Effects—Symmetry Considerations 133

Because the linear electro-optical effect is possible only in piezoelectric crystals, the presence of an externally applied electric field will produce a slight change in the shape of the crystal by the converse piezoelectric effect. The change in crystal shape results in the elasto-optical effect, to be considered in Section 7.3.2. As a result, the electro-optical effect will consist of two components: 1) the true (primary) linear electro-optical effect and 2) the false (secondary) linear electro-optical effect. Combined, these effects are given by ∆Bij = rijkEk = rijk∗ E k + pij lm εlm,

(7.38) rijk* are the true electro-optical coefficients and pijlm are the elasto-optical coefficients. The where elasto-optical coefficients are related to the linear piezo-optical coefficients, as in Eqs. (7.50), by

pijlm = π ijrs crslm

and

π ijlm = pijrs Srslm ,

(7.39)

where c and s represent the elastic stiffness and elastic compliance moduli of a crystal, respectively. Equation (7.38) can be cast into an alternative form by using Eq. (6.8), yielding

∆Bij = (ri∗jk + pijlm dklm ) E k

or

∆Bm = (rm∗k + pmr dkr )Ek ,

(7.40)

so that the product pd appears as a correction factor for the true linear electro-optical effect. At high-field frequencies, the pd correction factor is usually much smaller than the true linear electrooptical effect, but at low frequencies, it can become relatively important. The quadratic electro-optical effect, or Kerr effect, is represented by the coefficients Rijko in Eq. (7.36), which is a polar nonmagnetic fourth-rank tensor. Thus, contrary to the linear electro-optical effect, the quadratic effect may exist in all crystal classes. From its definition ∂ 2Bij / ∂Ek∂Eo there exists symmetry in the subscript pairs (i, j ) and (k, o) permitting the Kerr coefficients to be represented in either form ∆Bij = RijkoEk Eo or

∆Bm = Rmn En2

(m, n = 1 − 6),

and

Rmn ≠ Rnm .

(7.41)

R 16 E1 E 1 R 26 E2 E 2 R 36 E3 E 3 . . R 46 E2 E 3 R 56 E3 E 1 R66 E1 E 2

(7.42)

In expanded matrix form, Eq. (7.41) becomes

∆B1 R 11 ∆B R 2 21 ∆B3 R 31 = ∆B4 R 41 ∆B5 R 51 ∆B6 R 61

R 12 R 22 R 32 R 42 R 52

R 13 R 23 R 33 R 43 R 53

R 14 R 24 R 34 R44 R 54

R 62 R 63 R 64

R 15 R 25 R 35 R 45 R 55 R 65

134 tensor properties of solids

Here, the Rmn coefficients are related to the Rijko coefficients by the rules: Rmn = Rijko if n = 1 - 3, and Rmn = 2Rijko if n = 4 - 6. The restrictions imposed by crystal symmetry on the coefficients Rmn are exactly the same as those imposed on the linear piezo-optical coefficients considered in Section 7.3.2. As in the case of the linear electro-optical effect, the quadratic effect will normally contain two parts: 1) the true (primary) quadratic electro-optical effect and 2) the false (secondary) quadratic electro-optical effect. This can be expressed as

∆Bij = Rijko Ek Eo = Ri∗jko Ek Eo + pijlm εlm,

(7.43)

where R are * the coefficients for the true quadratic electro-optical effect and pijlm are the compoijko nents for the elasto-optical effect. Equation (7.43) can be cast into an alternative form by use of second-order electrostrictive coefficients given in Eq. (7.4). When this is done, Eq. (7.43) becomes

∗ ∆Bij = ( Rijko + pijlm γlmko )Ek Eo ,

(7.44)

where now the pγ product appears as a correction to the true quadratic electro-optical (Kerr) effect. The pγ correction factor is usually weak but can become important in some ferroelectric crystals.

7.3.2 Piezo-Optical and Elasto-Optical Effects The linear and quadratic piezo-optical effects can be obtained by applying small stress components to a crystal at a reference temperature T 0 under zero magnetic and electrical field conditions. The Taylor’s series expansion of the dielectric impermeability tensor in Eq. (7.34) reduces to ∂ 2Bij ∂Bij 1 σ Bij (σmn ) = Bij ( 0) + + σmnσqr + � 2 ∂σmn mn ∂ σmnσqr or

∆Bij = πijmnσmn + Πijmnqrσmn σ qr + L ,

(7.45)

where πijmn and ∏ijmnqr represent the linear and quadratic piezo-optical coefficients, respectively. The coefficients πijmn represent a polar fourth-rank tensor with partial symmetry implied by Bij and σmn thereby permitting the linear effect to be presented in reduced suffix notation as

∆Bo = π op σ p

( o, p = 1 − 6 )

and

π op ≠ π po

(7.46)

Second- and Higher-Order Effects—Symmetry Considerations 135

or in expanded matrix form ∆B1 π 11 ∆B π 2 21 ∆B3 π 31 = ∆B4 π 41 ∆B5 π 51 ∆B6 π 61

π 13 π 14 π 15 π 16 σ 1 π 23 π 24 π 25 π 26 σ 2 π 33 π 34 π 35 π 36 σ 3 . , π 43 π 44 π 45 π 46 σ 4 π 53 π 54 π 55 π 56 σ 5 π 63 π 64 π 65 π 66 σ 6

π 12 π 22 π 32 π 42 π 52 π 62

(7.47)

The elasto-optical coefficients can be obtained in a similar manner by expressing the impermeability tensor as functions of the strain components of the crystal, as in Eq. (7.43), to give ∆Bij = pijlm ε lm ( i , j, m , n = 1 − 3) (7.48) or in reduced suffix notation

∆Bo = pop εp

(o, p = 1 − 6)

and

pop ≠ ppo

(7.49)

Now, Pop = Pijlm for all o and p with no factors of 2 or 1 2 present. The elasto-optical and piezo- optical coefficients are related through the elastic moduli c and s, respectively, by the equations

∂B ∂σq pop = o = πoq cqp ∂σq ∂εp

and

∂Bo ∂ε p πoq = = pop spq . ∂εp ∂σq

(7.50)

The effect of crystal symmetry on the piezo-optical coefficients πoq can be determined by applying the direct inspection method to all crystal classes except the trigonal and hexagonal systems for which the “brute-force” method must be used. Thus, for the trigonal and hexagonal systems, the transformation equation must be used:

π ′ = απα −1.

(7.51)

which also applies to the quadratic electro-optical coefficients R given in Eq. (7.42). Note that Eq. (7.51) derives from B ′ = αB = απσ = απα-1σ ′ = π ′σ ′ because B = πσ applies to the old axes 0xi , whereas B ′ = π ′σ ′ applies to the new axes 0xi′ . Here, the linear quadratic electro-optical coefficients Rmn will be affected by crystal symmetry exactly as will be πmn . Shown in Table 7.1 are the piezo-optical coefficients πmn for the seven crystal systems and the isotropic solid with the understanding that πij ≠ πji. This table can also be applied to the elasto-optical coefficients with some minor changes.

136 tensor properties of solids

7.3.3 Piezo-Optical Effect in Cubic Crystals Under Uniaxial Tension

Consider the application of a uniaxial stress on a cubic crystal of the class 4− 32, 432 or m3m. For any direction of stress, the matrix equation Eq. (7.46) becomes 0 π π π 12 0 ∆ B 0 0 σ1 B B − 1 11 12 1 ∆B B − B 0 π π 11 π 12 0 0 0 σ 2 12 2 2 ∆B3 B3 − B 0 π 12 π 12 π 11 0 0 0 σ 3 = = . , 0 0 π 44 0 0 σ 4 ∆B4 B4 0 ∆B5 B 0 0 0 0 π 44 0 σ 5 5 0 0 0 0 π 44 σ 6 ∆B6 B6 0 (7.52) where B 0 is the reference dielectric impermeability defined by the indicatrix sphere for the undeformed crystal in the absence of temperature, electric, and magnetic fields

x2 x2 x2 B 0 ( x12 + x22 + x32 ) = 01 2 + 02 2 + 03 2 = 1 (n ) (n ) (n )

(7.53)

because B 0 = 1(n0)2. Here, n0 is the refractive index in the absence of all external fields. Now, let a uniaxial tensile stress σ2 be applied along the 0x2 direction, with 0x1 and 0x3 being the other cubic unit cell axes. Because ∆B4 = ∆B5 = ∆B6 = 0, Eq. (7.52) reduces to

∆B1 = π12σ2 ∆B2 = π11σ 2 ∆B 3 = π12σ 2 .

(7.54)

The changes in the three principal refractive indices can be determined by noting, for example, that Bi = 1 / ni2. Then, after differentiation, there results ∆Bi = -(2 / ni3 )∆ni = Bi = Bi0 0 (s. in units of Energy/l 3tT ),

(8.13)

where l is length (e.g., meter, m), t is time (e.g., second, s), and T is temperature (e.g., °K) as in the SI system of units for which energy is given in joules, (1 W = 1 J/s). Thus, we take entropy density production as the time variation of unrecoverable work per unit volume per unit temperature inside the system and whose quadratic form must be positive definite. In general, we assert the requirements that s. = 0 (reversible process) s. > 0 (irreversible process) s. < 0 (a process that cannot occur without altering the system conditions).

8.5

PROPER CHOICE OF PARAMETERS

The entropy production criterion allows for some latitude of “proper choice” for the fluxes J α and affinities X α. Thus, authors may differ in their choice for the fluxes and affinities. We will consider the conjugate parameters for the flow of electrical current, entropy (heat), and matter as they relate to reciprocal Ohm’s, Fourier’s, and Fick’s laws, respectively, given in Section 8.1. But in doing this, we will require that the product of the conjugate parameters each have the units of entropy density production s., that is, s. in SI units of Energy / l 3tT as in Eq. (8.13). 1. Flow of electronic charge: J 1 = Jin = −Jie /e = Electron flux (in units of no. electrons/l 2t ),

transport properties and irreversible thermodynamics 153

where J e is the charged electron flux in the direction of the electrostatic potential gradient. The affinity (force) is given by – – µ ∇µ X 1 = ∇i = i (in units of Energy/lT ), T T

( )(

)

where

µ− = µc + eφ

(8.14)

is the electrochemical potential (total energy per particle, also called the Fermi level in the equilibrium state), µc is the chemical potential per particle, eφ is the electrostatic potential per particle, and e is the charge on the particle assumed to be a positive test charge equal to + | e | = 1.60 × 10−19 C. Thus, the inner product of the conjugate parameters for the flow of electronic charge gives the entropy density production per particle as

(

− µ

T

(

s· = − J ni ∇i

(in units of Energy/l 3tT ),

(8.15)

which will later be shown to satisfy the corresponding reciprocity relations. Be aware of the fact that we are using the positive current convention and that high electrostatic potential is more positive than low electrostatic potential. Thus, Jin is always in a direction counter to the electrostatic potential gradient, which is from low potential to high potential. 2. Flow of entropy or heat: J 2 = Jis = Entropy flux (in units of Energy/l 2t)

(

∇i T (in units of l −1). T =− T The inner product of the conjugate parameters for the flow of entropy yields the entropy production as

(

1

(

s· = J si T ∇i

1

(

X 2 = T ∇i

3 T (in units of Energy/l tT ),

(8.16)

which will be shown to satisfy the corresponding reciprocity relations. Alternatively, for our purpose, because J q = T J s, the conjugate parameters become

X 2 = ∇i

(

1

T

(

and

J 2 = Jjq = Heat flux (in units of Energy /l 2t ) =−

∇i T (in units of (lT )−1, T 2

154 tensor properties of solids

which gives the entropy density production 1

(

(

s· = J qi ∇i

T

(in units of Energy/l 3tT ),

(8.17)

3. Flow of matter (uncharged single component): J 3 = J m = Matter flux (in units of mole number N /l 2t )

µ X 3 = ∇i c

= T

∇i µc

(in units of Energy/lT ).

T

Here, the mole number N is defined as the actual number of the diffusing species divided by Avogadro’s number. The inner product of the conjugate parameters for the flow of uncharged mass (kg-moles) counter to the concentration gradient of one component gives the entropy density production as

µ s· = − J mi ∇i c

(in units of Energy/l 3tT ),

T

(8.18)

which will also be shown to satisfy the corresponding reciprocity relations. Combining Eqs. (8.15), (8.17), and (8.18) yields the total entropy density production for all three processes as

s· =

∑i Ji

α

µ Xiα = − Jin ∇i

+ J q ∇ 1 − J m ∇ µc , i i T i i T

T

(8.19)

which are each represented in units of Energy/l 3tT ). Thus, the phenomenological relations for the three types of flow can be written in the following matrix forms

− Jin q Ji − J m i

=

Li11j Li12j 21 22 Li j Li j L 31 L 32 ij ij

( µ T ) Li23 ∇j (1 T ) . j ∇ ( µ T ) Li33 c j j Li13j ∇j

(8.20)

Here, diagonal Lijαα are the principal phenomenological coefficients and the Lijαβ are the cross or interference coefficients. Onsager’s reciprocity theorem permits the following relationships between the phenomenological coefficients in the absence of a magnetic field ~ ~ Liβα = Ljαβ or Lβα = Lαβ for α ≠ β but Lβα ≠ Lαβ, that is, Lijαβ ≠ Ljαβ j i i and ~ Liαα = Ljαα or Lαα = Lαα for α = β. j i

transport properties and irreversible thermodynamics 155

Thus, only the Lijαα are self-symmetrical. The reciprocal relations are best illustrated for a three-dimensional system in which only electric current and heat flow occurs. Accordingly, Eqs. (8.20) now become

− J1n n − J2 − J n q3 J1 Jq 2 J3q

11 L11 11 L12 L11 = 31 L12 11 L12 12 12 L13

11 L12

11 L31

12 L11

12 L12

∇1 L12 13

11 L22 11 L23 12 L21 12 L22 12 L23

11 L23 11 L33 12 L31 12 L32 12 L33

12 L21 12 L31 L22 11 22 L12 22 L31

L12 22 12 L32 22 L12 22 L22 22 L23

L12 23 L12 33 22 L31 22 L23 22 L33

( ) ( ) ( ) , µ

T

µ ∇2 T ∇ µ T ⋅ 3 1 ∇1 ( T) ∇ ( 1 T) 2 1 ∇3 ( T )

(8.21)

11 11 22 22 21 12 12 12 where L = L˜ , L = L˜ , and L = L˜ , meaning that Lij21 = Lji12, but L ≠ L˜ .

8.5.1 Further Restrictions on the Phenomenological Coefficients Relating the entropy production given in Equation (8.13) to the phenomenological coefficients provides a first step in formalizing a unified theory of the cross (interaction) effects as they relate to the conjugate effects for linear, first-order, irreversible processes. For conditions under which Eq. (8.10) is valid, the quadratic form of the entropy production as given earlier is s⋅ =

∑L

αβ

X α X β > 0,

(8.22)

αβ

which is positive definite and implies that the matrix of phenomenological coefficients Lαβ also be positive definite. For this to be so requires that that determinant of the Lαβ matrix and all of its minors be positive definite. Take, for example, a two-flow process involving a two-dimensional matrix Lαβ given by

J 1 L11 2 = 21 J L

12

L12 X 1

, L22 X 2

(8.23)

21

where L = L according to Onsager’s principle. The necessary and sufficient condition for Eq. (8.23) to be positive definite is that the 2 × 2 determinant of Lαβ be positive definite. Thus,

L11

L12

L21

L22

= L11 L22 − (L12) 2 > 0.

(8.24)

Generally, the diagonal coefficients Lαα > 0 (i.e., are positive), but the Lαβ coefficients can be positive or negative. Applying Eq. (8.13) to the flow of electric charge and heat given in Eq. (8.20), we would write the entropy production for any two-flow process as

156 tensor properties of solids

s· =

∑L

αβ

(

X α X β = L αα X α X α + 2 Lαβ X α X β + Lββ X β X β

αβ

) > 0

(8.25)

or specifically for the flow of electric charge and heat

2

2

µ µ 1 1 + 2 L12 ∇ ⋅ ∇ + L22 ∇ > 0, T T T T

s· = L11 ∇

(8.26)

where each of the quadratic terms is given in units of Energy/l 3tT. Now back to Eq. (8.23), the value of the 2 × 2 determinant given by Eq. (8.24) requires that L11L22 > (L12)2,

(8.27)

which must be valid if the Lαβ matrix is to obey Onsager’s reciprocal relations L12 = L21. Note that L11L22 and (L12)2 both have units of T 2(l . t)−2 for the flow of electric charge and heat.

8.6 FLOW OF ELECTRONIC CHARGE AND HEAT— THE CONDUCTIVITIES A basic postulate in irreversible thermodynamics states that “every observed flux depends on all the affinities (driving forces) applied.” This means that the electronic and heat fluxes must depend on their conjugate affinities as well as the cross affinities. Thus, the flow of electrons not only transport charge but also heat (recall what Joule heat is when electric current flows through a resistor). The flow of mass in this case is considered negligible. With these concepts in mind, consider the simultaneous flow of electron current and heat in a system whose phenomenological equations for the thermoelectric effects are from Eq. (8.20) given by

(

+ L12 ∇ j ij

1

T

Jiq = Lj12i ∇j µ + Li22 ∇j j T

(

1

T

(

µ − Jin = L11 ∇ ij j

(

T

(8.28) (8.29)

The phenomenological coefficients Lij in Eqs. (8.28) and (8.29) can now be related to the familiar conductivities σij and kij. We begin with the electrical conductivity σij , which is defined as the electric current density −eJin per unit potential gradient ∇φ = ∇µ−/e in an isothermal system, the latter being essentially an electromotive force because ∇µc = 0, giving ∇µ− = e ∇φ. Therefore, under isothermal conditions, Eq. (8.28) becomes − Jin = Li11j

(

1

(

11 T ∇j µ = eLij

∇j φ T

for ∇T = 0

transport properties and irreversible thermodynamics 157

and

σ ij ≡

− eJin ∇j φ

= e 2 Li11j / T = σji ,

(8.30)

which indicates symmetry of the electrical conductivity, σij = σji because Lij11 Lji11 . Thus, the electrical conductivity is a symmetrical second-rank tensor with the component array given by Eq. (2.17). Solving for Lij11 in Eq. (8.30) gives Li11 = Tσij /e 2. j

(8.31)

Next, we turn to the heat conductivity defined as the heat current density per unit temperature gradient for zero electric current, J n = 0. For this purpose, Eqs. (8.28) and (8.29) become

µ 0 = Li11 ∇j j

− L12 ∇j T ij T 2

(8.32)

T

and

− L22 ∇ ∇j T . 2 j j i T T

µ Jiq = Lj12 ∇j i

µ Solving for ∇ j

(8.33)

in Eq. (8.32) gives, with subscripts excluded for simplicity, T µ ( 11)−1 12 ∇ T L ∇ = L , for J n = 0 T 2 T

which when substituted into Eq. (8.33) yields 12

(L11)−1 L12 − L22

{

{~L

(

(

Jq =

∇T T 2 .

(8.34)

The thermal conductivity tensor, defined as the heat current density − Jiq per unit temperature gradient ∇jT, now becomes

kij = −

Jiq ∇j T

=

1 T

2

{L

22 ij

}=L

( Li11j ) Li12j − Lj12 i −1

11 22 Lij

ij

− ( L12) 2

Li11j T 2

=

| DL | Li11j T 2

,

(8.35)

~ where by Eq. (8.11) Lji12 = Lij12 = L12, and | DL | > 0 is the determinant of the phenomenological coef~ ficients. Here, (L12)2 is a symmetrical square matrix often represented as L12L12 in matrix symbology. Because L11, L22, and (L12)2 are all symmetrical square matrices, we are permitted to state that

kij = kji

(8.36)

158 tensor properties of solids

~ ~ ~~ ~ t Thus, kij = kji if (L12 (L11)−1 L12) = L12 (L11)−1 L12, which it does since (ABC )t = (C B A ) or in this ~ ~ case, (A B −1A )t = A B −1A. A potential problem with this has been pointed out by Casimir in Nye’s Physical Properties of Crystals (see Endnotes). Only if the antisymmetrical part of kij (see Eq. (2.16)) is negligibly small or unobservable can Eq. (8.36) be justified. Given the validity of Eq. (8.36), the component array for kij as a symmetrical second-rank tensor is given by Eq. (2.17). Solving for Lij22 in Eq. (8.35) and introducing Eq. (8.31) yields the results Lij22 = (L12)

2

(Li11j )−1 + kij T 2 = e

(L12 )2 (σ )−1 + T 2 k . ij ij

2

T

(8.37)

We can now write Eqs. (8.28) and (8.29) in terms of the conductivities σij and kij by introducing the expressions for Lij11 and Lij22 in Eqs. (8.31) and (8.37) with the results

T σ ij − Jin = 2 e

(

µ 1 ∇j + Li12j ∇j T T

(

(

2 + T 2 k + e (L12)2 (σ ) −1 ∇ 1 , j T ij ij T T

µ Jiq = Lj12i ∇j

(8.38)

(

(8.39)

~ where (L12)2 = Lji12Lij12 = L12L12. Equations (8.38) and (8.39) give the generalized force–flux expressions for the dual flows of electricity and heat in an anisotropic solid both in terms of the conductivities σij and kij and the cross-coupled phenomenological coefficient Lij12 yet to be determined in Section 9.1. By dropping the subscripts i and j, these equations can be applied to the one-dimensional flow of electricity and heat in a homogeneous isotropic wire or rod. We end this section by defining thermal resistivity tensor rij as the inverse of the thermal conductivity tensor. Following Eq. (2.35), the inverse of kij is rij given by rij = −

or in matrix notation r = k−1. ( kij ) −1 =

∇i T Jjq

|Mji | | kij |

( − 1)(i + j )

(8.40)

= rij = rji ,

(8.41)

where | Mji | is the ji th minor of | kij |, indicating that any individual component of rij is not the simple reciprocal of kij component. The same reasoning applies to the relationship between the electrical conductivity σij and resistivity ρij expressed by (σij)−1 = ρij . • • • •

159

chapt e r 9

Thermoelectric, Piezothermoelectric, and Diffusive Effects in Solids In previous sections, we dealt mainly with the conduction of electricity and heat as two separate processes. This was done to formalize the conductivity definitions and define the phenomenological coefficients Lij11 and Lij22 in terms of the proper conductivities σij and kij . Now we will consider the simultaneous flow of electricity and heat usually referred to as the thermoelectric effects or, more specifically, the Seebeck, Peltier, and Thomson effects. In doing this, we will recognize that the irreversible processes involved interfere with one another. Thus, we will have to take into account the cross coupled or interference effects by making use of the developments given in Section 8.4. To simplify the treatment given here, we will begin with the isotropic case and then move to the generalized case of the anisotropic solids. In fact, it will be instructive to switch back and forth between the isotropic and anisotropic nomenclature as needed.

9.1

SEEBECK EFFECT (THERMOCOUPLE EFFECT)

The Seebeck effect is defined as the production of an open-circuit voltage or thermoelectric electromotive force between two dissimilar conductors held at different temperatures under conditions of J n = 0. This is, of course, the means by which one can measure a temperature difference by means of a calibrated thermocouple. The physical picture of the thermocouple is illustrated in Figure 9.1 where an ideal capacitor is placed in a circuit that consists of the two dissimilar conducting wires A and B attached to large heat reservoirs held at high and low temperatures designated as TH and TL. The presence of the ideal capacitor ensures that J n = 0. The potential difference ∆φ is the thermoelectric voltage difference between high and low potential measured across the capacitor held at the reference temperature T0. High potential is taken as being more positive than low potential. From Eq. (8.32), with subscripts removed and with ∇µc = 0, we have

∇ µ = e ∇φ =

L12 TL11

∇ T .

(9.1)

In a continuous conducting media, the absolute thermoelectric power ∑ is defined generally as the electrostatic potential gradient per unit temperature gradient when J n = 0. However, in the case of

160 tensor properties of solids A

TL (3)

T0

B

(4)

(2)

B

TH

(1)

∆φ = φ 1 – φ 4

FIGURE 9.1: Thermocouple setup showing two dissimilar metals A and B joined at junctions that are maintained at different temperature TH and TL. Figure 9.1, there can be no temperature gradient across the open circuit of the ideal capacitor. Thus, the absolute thermoelectric power ∑ must be defined as the change in electrostatic voltage potential per unit change in temperature relative to the heat reservoirs. Thus, by using Eqs. (9.1) and (8.31), we have

∑≡

∇φ ∇T

12

=

L

11

eTL

12

=

eL 2

T σ

in units of (V/°K)

(9.2)

in terms of L12 and σ. Solving for L12 then gives the result L12 =

T 2σ ∑. e

(9.3)

From Figure 9.1, because there is no temperature gradient across the capacitor held at temperature T 0, we can sum the electrostatic potential differences as

∆φ = φ 1 − φ4 = (φ1 − φ2 ) + (φ2 − φ3 ) + (φ3 − φ4 ) =

∫

=

∫

T0

TH TH TL

∑ B dT +

∫

TH

TL

∑ A dT +

∫

TL

T0

∑ B dT

(∑ A − ∑ B ) dT .

Therefore, the resulting absolute thermoelectric power for the thermocouple becomes

∑AB =

L12 = A 11 ∆T eTLA

∆φAB

L12 − B 11 eTLB

=∑ −∑ A B

(9.4)

In tensor notation, we write Eq. (9.2) applied to an anisotropic medium as since Lij12 ≠ Lji12.

( Li11j )−1 ∇i φ L12 ij ∑ij = = ≠∑ ji ∇j T eT

(9.5)

Thermoelectric, Piezothermoelectric, and diffusive effects 161

By introducing Eq. (9.3) into Eqs. (8.38) and (8.39), we can cast these thermoelectric equations into forms containing physically measurable quantities (σ, k, and ∑) as they apply to a thermoelectric junction composed of two different isotropic conductors. When this is done, the results are, excluding subscripts,

(

Tσ µ T 2σ ∑ 1 ∇ + e ∇ T 2 T e

(

(9.6)

T2σ ∑ µ ∇ + T 2 k + T σ ∑2 ∇ 1 . e T T

(

Jq =

(

− Jn =

µ between Eqs. (9.6) and (9.7), there results T e2 J n eΣ ∇ µ = − + ∇T . T Tσ T

(9.7)

Then, by eliminating ∇

(9.8)

Finally, by introducing Eq. (9.8) into Eq. (9.7) with ∇(1/T ) = −∇T /T 2 and with a little algebra, Eq. (9.7) can be written in the useful alternative form J q = –eT ∑ J n − k∇T = TJ s

(9.9)

which provides another definition for the thermoelectric power given by

∑≡−

1 Jq

Js = , eT J n ∇T = 0 J e ∇T = 0

(9.10)

where J n = −J e /e and J q = T J s.

TABLE 9.1: Effect of crystal symmetry on ∑ij for the tetragonal, trigonal, and hexagonal systems, all others being the same as in Table 3.7 except that ∑ij ≠ ∑ji Classes

Classes

− − 4, 4 , || 4/m ||, 3, || 3 || − 6, 6 , || 6/m ||

− − 4mm, 4 2m, 422, || 4/mmm ||, 3m, 32, || 3 m || || − 6 m2 ||, 6mm, 622, || 6 /mmm ||

∑11 −∑ 12 0

∑12 ∑11 0

0

0 ∑ 33

∑11 0 0

0

∑11 0

0

∑ 33 0

162 tensor properties of solids

To apply Eqs. (9.6) and (9.7) to an anisotropic solid, one need only reinstall the subscripts and take into account the affect of crystal symmetry on the property tensors—all of which are second-rank tensors but only ∑ij is nonsymmetrical. The effect of crystal symmetry on the ∑ij components follows Table 3.7 for Sij with the following changes: 1) crystal systems are the same as Sij except that ∑ij ≠ ∑ji and 2) the uniaxial group of tetragonal, trigonal, and hexagonal systems is given as in Table 9.1.

9.2

PELTIER EFFECT (THERMOELECTRIC HEATER/REFRIGERATOR EFFECT)

The Peltier effect is defined as the evolution or absorption of heat accompanying the flow of electric current across an isothermal junction between two dissimilar conductors or semiconductors. That is, when J n flows across a junction, heat must be removed or added continuously to maintain the junction at constant temperature, T. This is illustrated in Figure 9.2. Because ∇T = 0 at the junction (the junction is at constant T ), Eq. (9.9) applies as J q = –eT ∑ J n = TJ s .

(9.11)

J Aq − J Bq = –eT ( ∑A − ∑B ) J n = –eT ∑AB J n ,

(9.12)

Then the difference in heat flow is

where ∑AB is the thermoelectric power of the AB junction. Heat evolved Constant T junction

A

(J

(J q)A > (J q)B

Jn B (J q)B

q) A

(J q)A < (J q)B Heat absorbed

FIGURE 9.2: Schematic illustrating the Peltier effect.

Thermoelectric, Piezothermoelectric, and diffusive effects 163

By definition, the Peltier coefficient ∏ is the heat that must be removed from the isothermal junction AB per unit electric current flux from conductor A to conductor B as depicted in Figure 9.2. This is expressed by J Bq − JAq = T ∑AB , ΠAB ≡ (9.13) n eJ ∇T = 0

giving the relationship between the Peltier and Seebeck (thermoelectric power) coefficients. Equation (9.13) is known as the first Kelvin relation. Thus, if ( J Aq − J B q ) > 0, heat must be issued from the isothermal junction AB to the surroundings (thermoelectric heating). Or if ( J Aq − J B q ) < 0, heat must be supplied to (absorbed by) the isothermal junction from the surroundings (thermoelectric cooling) as illustrated in Figure 9.2. In tensor notation, applicable to anisotropic crystals, the Peltier and Seebeck coefficients are related according to ∏ij = T ∑ij ≠ ∏ji since ∑ij ≠ ∑ji ,

(9.14)

where the effect of crystal symmetry for ∏ij is the same as that for ∑ij given in Table 9.1. It should be noted that the developments presented by Eqs. (9.11), (9.12), and (9.13) apply to homogeneous isotropic conducting materials.

9.3

THOMSON EFFECT

Consider a homogeneous conducting rod of uniform cross section that has established a steadystate heat flow J q in the absence of an electric current. Assume that the surroundings are heat reservoirs having the same temperature distribution as the rod. Now, if an electric current J n is allowed to flow through this material, heat must be emitted to or absorbed from the surroundings

φ + ∆φ

Thomson Heat Heat Reservoir

T+∆T

∇φ ∇T

Jn Jq

Jn' J q' ∆x

Heat Reservoir Thomson Heat

FIGURE 9.3: Schematic illustrating the Thomson effect in a homogenous rod element ∆x of a constant cross section carrying heat and electric currents and surrounded by heat reservoirs.

164 tensor properties of solids

to maintain the steady temperature distribution. This is what is called the Thomson effect (after Sir William Thomson, who later became Lord Kelvin), and the heat that is exchanged in this process is called the Thomson heat as depicted by the closed system in Figure 9.3. Whether the Thomson heat is emitted to or absorbed from the surroundings depends on the direction and magnitude of the electric current relative to the heat flow. We now establish an energy flow balance given by fluxes Jiu = Jiq + µ− Jin ,

(9.15)

− is the total energy carried per particle. Thus, as where Jiu is the total energy flow along the rod and µ the electric current flows through the conducting rod, any change in the total energy flow must be supplied by a Thomson heat interchange with the surroundings. Introducing Eq. (9.9) into (9.15) yields

Jiu = –eT ∑ji Jjn − kij∇jT + µ− Jin = (eT ∑ji + δji µ− ) Jjn − kij∇jT ,

(9.16)

where the substitution property of the Kronecker delta δji has been used (see Section 2.6.3). The rate at which energy is interchanged between the rod element and the surroundings in Figure 9.3 is the divergence (Section 2.6.2) of Eq. (9.16) represented by

∇i Jiu = –eT ∇i ( Jjn ∑ji ) – (e ∑ji ∇iT – δji∇i µ− ) Jjn − ∇i (kij∇jT ).

(9.17)

But from Eq. (9.8)

µ ∇j µ = T ∇j

= − e 2J nσ −1+ e ∑ ∇ T ji i i ji T

(9.18)

or

−1

e 2σji Jin = (e ∑ji∇iT − δji ∇i µ )

(9.19)

because δji∇i µ− = ∇j µ−. Introducing Eq. (9.19) into Eq. (9.17) yields

∇i Jiu = − eT ∇i ( Jjn ∑ji ) − e 2 ρji Jin Jj n − ∇i ( kij ∇j T ) , Thermoelectric heat

Joule heat

(9.20)

Conduction

where σij−1 = ρij and e 2ρji Jin Jjn is the Joule (I 2R) heat that is generated by current flow through a conductor even in the absence of a temperature gradient. But for the steady-state conditions, J n = 0 and ∇ . J n = 0, it follows that ∇ . J u must vanish. If we set ∇ . J n = 0 and ∇ . J u = 0, we have

{∇i ( k i ∇ T )} j

j

∇ ⋅J n = 0 ∇ ⋅J u = 0

= 0 ,

Thermoelectric, Piezothermoelectric, and diffusive effects 165

which gives the result

∇i Jiu = − eT ∇i ( Jjn Σj ) − e 2 ρji Jin Jjn . i Thermoelectric heat

(9.21)

Joule heat

We now note that the thermoelectric power ∑ji is a function of the local temperature represented as ∇i ∑ji / ∇iT = ∂ ∑ji / ∂T, which allows

∂ Σji ∇i Σj = i ∂T

∇i T .

(9.22)

Introducing Eq. (9.22) into Eq. (9.21) yields ∇i Jiu = − T

∂ Σji ∂T

∇i T e Jjn − e 2 ρji Jin Jjn Joule heat

T homson heat

= − τ ji ∇i T e Jjn − e 2 ρji Jin Jjn T homson heat

(9.23)

Joule heat

Here,

τ ji = T

∂ Σji ∂T

≠ τ ij

(9.24)

is the Thomson heat coefficient, which is seen to be an asymmetrical second-rank tensor where the effect of crystal symmetry follows that for ∑ji ≠ ∑ij in Table 9.1. Equation (9.24) is known as the second Kelvin relation. Thus, the Thomson heat is the heat evolved or absorbed per unit volume per unit time depending on the direction and magnitude of the current Jin relative to the Joule heat it produces. The Thomson coefficient is usually (but not always) defined as positive if heat must be added to (absorbed by) the element in Figure 9.3 so as to maintain the steady-state temperature distribution in the element. Notice that the Thomson heat (proportional to J n) changes sign when the current density is reversed but that the Joule heat does not because it is proportional to the square of the current density. The foregoing results apply generally to an anisotropic conducting material. However, they can be applied to homogeneous isotropic conductors or semiconductors by dropping subscripts except for a suffix indicating a specific direction along which the heat effects are generated. When this is done, for example, Eq. (9.23) becomes

∇ J u = − τ ∇ T e J n − e 2 ρ ( J n )2 . T homson heat

Joule heat

(9.25)

166 tensor properties of solids

This single direction would apply to one-dimensional flow in the longitudinal direction of the conducting rod (e.g., the x direction). In the isotropic case, the Thomson coefficient is given by the known isotropic value for τ when substituted for the S cubic (diagonal) values presented in Table 3.7.

9.4

PIEZOTHERMOELECTRIC AND ELASTOTHERMOELECTRIC EFFECTS

From what we have learned so far in this chapter, the thermoelectric power tensor ∑ij is fundamental to a general description of the three thermoelectric effects discussed in Sections 9.1, 9.2, and 9.3. However, in practical experimental situations, both temperature and stress variation of the thermoelectric power may be involved. Assuming that ∑ij is everywhere, a continuous function of temperature and stress and that its derivatives with respect to temperature T and stress σkl are real, we may expand ∑ij in a Taylor’s series about the state of reference temperature T0 and zero applied stress (neglecting gravitational forces and body torques). When this is done, we have 1

n

∑ij (T , σ kl ) = ∑ (T − T0 ) + σ kl ∑ j (T0 , 0 ) n = 0 n! ∂T ∂ σ kl i ∂ Σij ∂ Σij = ∑ij (T0 , 0 ) + ( T − T ) + 0 ∂σ T ∂ ( T0 , 0 ) kl ∞

+

2 1 ∂ Σij

2! ∂ T 2

∂

∂

∂ 2 Σij ( T − T 0) + 2 ∂ T∂ σ kl ( T0 , 0 )

∂ 2 Σij + ∂σ ∂σ op kl

2

σ kl σ op ( T0 , 0 )

(T

σ kl 0

, 0)

( T − T 0 )σ kl ( T0 , 0 )

+…,

(9.26)

where ∑ij (T0, 0) and all coefficients (in parentheses) are evaluated at temperature T0 and zero stress. Assuming that all measurements are to be conducted at a reference temperature of T = T0 and that all second- and higher-order terms in stress can be neglected, Eq. (9.26) becomes

∂Σ ∆∑ij = ∑ij (T0 , σ kl ) − ∑ij (T0 , 0 ) = ij ∂ σ kl

(T

σ kl = ∏ijkl σ kl , 0

, 0)

(9.27)

Thermoelectric, Piezothermoelectric, and diffusive effects 167

where ∏ijkl is a fourth-rank polar tensor called the piezothermoelectric power tensor, not to be confused with the Peltier coefficient ∏. Because σkl is symmetrical but ∆∑ij is not, then ∏ijkl = ∏ijlk or ∆∑i = ∏ij σj (i = 1 − 9; j = 1 − 6)

(9.28)

in matrix subscript notation. Thus ∏ij in Eq. (9.28) is completely specified by 54 independent coefficients for the triclinic crystal system given by

∆Σ1 ∆Σ 2 ∆Σ3 ∆Σ4 ∆Σ = 5 ∆Σ 6 ∆Σ 7 ∆Σ 8 ∆Σ 9

∏11 ∏ 21 ∏31 ∏ 41 ∏ 51 ∏61 ∏ 71 ∏81 ∏ 91

∏12

∏13

∏14

∏15

∏16

∏ 22

∏ 23

∏24

∏ 25

∏26

∏ 32

∏33

∏34

∏35

∏36

∏ 42

∏ 43

∏44

∏ 45

∏ 46

∏ 52

∏53

∏54

∏ 55

∏56

∏ 62

∏ 63

∏64

∏ 65

∏66

∏ 72

∏ 73

∏74

∏ 75

∏76

∏82

∏83

∏84

∏85

∏86

∏ 92

∏93

∏94

∏95

∏96

σ 1 σ 2 σ 3 σ 4 σ 5 σ 6

(9.29)

The transformation law for the piezothermoelectric power tensor ∏ is easily determined from the transformation laws for stress and thermoelectric power. These transformation laws are σ ′ = ασ or σ = α−1σ ′, as given in Section 6.1.1, and ∑ is ∑′ = β∑, where α is the quadratic transformation form for symmetrical second-rank polar tensors and β is the general quadratic transformation form for asymmetrical second-rank polar tensors. If ∑′ = ∏′σ ′ relative to coordinate axes 0x′ and ∑ = ∏σ relative to axes 0x, then it follows that ∑′ = β∑ = β∏σ = β∏α −1σ ′ = ∏′σ ′

or

∏′ = β∏α −1

(9.30)

↔

in matrix symbolic notation. The quadratic transformation form β is given by Eq. (9.31), where it is divided into nine 3 × 3 submatrices (numbered in parentheses), 4 of which are replicated as indicated by the symbols ↔ and . Eq. (9.31) can be deduced from that of α given by Eq. (2.22).

168 tensor properties of solids (1) 2 a 212 a 213 a 11 a2 a 222 a 223 21 a 232 a 233 a 231 (4) a21 a31 a22 a32 a23 a33 β = a a 31 11 a32 a12 a33 a13 a11 a21 a12 a22 a13 a23 (7) (4) b (7)

(2)

a13 a11

a11 a12

a12 a23

a23 a21

a21 a 22

a32 a33

a33 a31

a31 a 32

a22 a33

a21 a33

a21 a32

a23 a32

a12 a33

a11 a33

a11 a32

a13 a32

a12 a23

a11 a23

a11 a22

a13 a22

(5)

(8)

(2) ↔ (3) (6) a23 a31 a22 a31 a13 a31 a12 a31 a13 a21 a12 a21 (9) (5) ↔ (9) (3)

a12 a13

(6) ↔ (8)

(9.31)

The variation in thermoelectric power with strain can also be established. For this purpose, Eq. (9.27) is altered to give

∂ Σij ∂εmn ∆Σij = ∂ εmn ∂ σkl

σkl = Εijmn smnkl σkl

(9.32)

or

∆Σi = Εik skj σj = Εik εk

(9.33)

in matrix subscript notation. Here Eik = (∂∑i /∂εk ) is a polar fourth-rank tensor called the elastothermoelectric power tensor and skj is the elastic compliance tensor given by Eq. (4.47). By comparing Eqs. (9.28) and (9.33), the piezothermoelectric and elastothermoelectric power coefficients can be related by reciprocity

∏ ij = Eikskj

(9.34)

Eij = ∏ ik ckj ,

(9.35)

or its inverse

where ckj is the elastic stiffness modulus given by c = s−1 as deduced from Eq. (6.36a) and thermodynamic symmetry discussed in Section 4.4. The transformation law for the elastothermoelectric power tensor E is easily found from the ~ −1ε or ε = α ~ ε ′ transformation laws for strain and thermoelectric power. Strain transforms as ε ′ = α (see Section 6.1.2) and ∑ transforms as ∑′ = β∑. Because from Eq. (9.33) ∑ = Esσ = Eε relative to coordinate axes 0xi and ∑′ = E′ε′ relative to axes 0xi′, it follows that

~ ε ′ = E′ε′ ∑′ = β ∑ = β Eε = β Eα

Thermoelectric, Piezothermoelectric, and diffusive effects 169

or

~ E′ = β Eα

(9.36)

all in matrix notation. A complete description of the first-order piezothermoelectric and elastothermoelectric properties must necessarily include the piezo- and elasto-Seebeck, Peltier, and Thomson effects. From Eq. (9.24) in contracted subscript form and using Eqs. (9.28) and (9.34), there results

τi = T

∂ Σi ∂T

∂ ∏ij ∂Ε s σj = T ik kj ∂T ∂T

= T

σj ,

(9.37)

giving the Thomson effect in terms of the piezothermoelectric and elastothermoelectric coefficients. Here, it has been assumed that all thermal stresses are absent and that the tensor character and aelotropism of ∏ and E are the same. The anisotropy of the piezothermoelectric and elastothermoelectric coefficients ∏ and E is determined by the standard methods emphasized in this text. Consider the ∏ array in Eq. (9.29), which applies to the triclinic crystal system. The anisotropy of all crystal systems, other than the trigonal and hexagonal, can be determined by the method of direct inspection as was done for the piezoelectric moduli in Section 6.1.3. For the trigonal and hexagonal crystal systems, the “bruteforce” method described in Section 6.1.4 must be used. Remember that the generalized quadratic transformation form β must be used together with α in Eqs. (9.30) and (9.36) when applying the brute-force method. For the coefficient arrays of ∏ and E, see Tinder in Endnotes, Section VII.

9.5

PIEZORESISTANCE EFFECT (STRAIN GAUGE EFFECT)

The application of a mechanical stress can significantly change the electrical resistivity of a given conducting medium. The calibrated sensitivity of piezoresistive elements made from metal or semiconductor thin wires are used as gauges to measure the surface strains resulting from a stressed solid member to which the strain gauges are firmly attached. The strain gauges can be aligned with specific crystallographic axes for meaningful measurements. Such measurements are usually in the form of a fractional change in the resistance associated with elongation or contraction of the piezoresistive elements. For cubic crystals, the piezoresistive sensitivity is similar to that discussed for Young’s modulus in Section 6.2.7. To determine the tensor nature of the piezoresistance effect, we can expand the resistivity tensor ρij in a Taylor’s series about the state of reference temperature T0 and zero applied stress (neglecting gravitational forces and body torques) much the same as in the previous section for the

170 tensor properties of solids

piezothermoelectric effect. Here again, we assume that ρij is everywhere a continuous function of temperature and stress and that its derivatives with respect to temperature T and stress σkl are real. The resulting expansion is ∞

ρij (T , σkl ) = ∑

n=0

1

∂

n!

∂T

( T − T0 )

∂ ρij = ρij (T0 , 0 ) + ∂T +

2! ∂T 2

+

∂ 2 ρij

∂σ ∂σ kl op

ρij (T0 , 0 )

+ σkl

∂ σkl

∂ ρij ( T − T ) + 0 ∂σ ( T0 , 0 ) kl

2 1 ∂ ρij

n

∂

∂ 2 ρij (T − T0 ) + 2 ∂ T∂ σ kl ( T0 , 0 ) 2

σkl σop ( T0 , 0 )

σkl ( T0 , 0 )

(T − T0 ) σkl ( T0 , 0 )

+ L,

(9.38)

where ρij (T0, 0) and all tensor coefficients (in parentheses) are evaluated at temperature T0 and zero stress. Notice that the second-order effects, ∂ 2ρij / ∂ T∂σkl and ∂ 2ρij / ∂σkl ∂σop, represent the piezothermoresistive and quadratic piezoresistive effects, respectively. There will be no further discussion of the second-order effects, the remainder of which are self-explanatory. Assuming that all measurements are to be conducted at a reference temperature of T = T0 and that all second- and higher-order terms in stress can be neglected, Eq. (9.38) becomes

∂ ρij ∆ ρij = ρij (T0 , σ kl ) − ρij (T0 , 0 ) = ∂ σkl

σkl = Ρijkl σkl , ( T0 , 0 )

(9.39)

where Pijkl is a fourth-rank polar tensor called the piezoresistance tensor. Because both ρij and σkl are symmetrical second-rank tensors, we can write

∆ρi = Pijσj (i = 1 − 6; j = 1 − 6),

(9.40)

where it is understood that Pij ≠ Pji . Thus, the piezoresistance tensor transforms the same as the linear piezo-optical coefficients given by Eq. (7.51) and is affected by crystal symmetry the same as presented in Table 7.1.

Thermoelectric, Piezothermoelectric, and diffusive effects 171

9.6

ELECTRODIFFUSIVE AND THERMODIFFUSIVE EFFECTS

There are two other two-flow processes that derive from Eqs. (8.20) and that are worthwhile mentioning, the electrodiffusive and thermodiffusive effects. These are represented as follows.

µ T

− J n = L11∇

13 µc + L ∇ T

µ µ − J = L ∇ + L33 ∇ c T T m

Electrodiffusive effects

31

1 23 µ c + L ∇ T T

(9.41)

J q = L22 ∇

µ 1 − J = L32 ∇ + L33 ∇ c T T

Thermodiffusive effects

m

(9.42)

The reader has already been introduced to the phenomenological developments of the thermoelectric effects in some detail including the application of Onsager’s reciprocity principle as applied to the phenomenological coefficients given in Eqs. (8.20). The interaction effects in Eqs.(8.20) can be complex considering that charged matter (electrons, holes, ions) can carry charge, heat, and mass at the same time and that different species can influence other species. Although it is not our intention to explore the electrodiffusive and thermodiffusive effects in detail, a short discussion of the diffusive effects is necessary when dealing with the coupled effects in Eqs. (9.41) and (9.42).

9.6.1 Multiple Diffusing Species In dealing with diffusion of matter, one must understand that several species could be diffusing simultaneous and that the different species may not all be independent. Thus, the flow of one species may influence the flow of another. The entropy density production associated only with the simultaneous diffusion of several species in the absence of an electrostatic field potential gradient (∇φ = 0) and temperature gradient is from Eq. (8.19)

s& = − ∑ Jim ∇ i

µi

,

T

(9.43)

where Jim is the mass flux of the ith species and µi is the chemical potential for the i th species. From this we can generalize Fick’s law in the modified form of Eq. (8.8) and under isothermal conditions as the sum of diffusing species given by

Jim = − ∑ j

Lij T

∇ Nj = − ∑ Dij ∇ Nj ( x ). j

(9.44)

172 tensor properties of solids

Here, Nj (x) is the concentration (mole number) of the j th component at any position in Cartesian space of the medium in which the diffusion is occurring. The problem now remains to relate the phenomenological coefficient L ij with the physically measurable diffusion constant D ij . This requires the use of Gibbs–Duhem relation, Eq. (4.4) under constant temperature, electric, magnetic, and stress fields together with the use of chemical thermodynamics as applied to the condensed state. For example, at constant T, E, B, and σ, the Gibbs–Duhem relation for a non-independent, two-species system and for arbitrary dx, is expressed as N1 d µ1 + N2 d µ2 = N1∇µ1 + N2∇µ2 = 0,

(9.45)

where N1 is the mole number concentration of the (dilute) diffusing species and N2 >> N1 is the mole number concentration of the host medium. Because diffusion flows do not produce a volume change, it follows that →

→

J 1v1 + J 2v2 = 0,

(9.46)

where vi is the partial molar volume of the species i. Now, by introducing Eqs. (9.45) and (9.46) into (9.43), the isothermal entropy density production for the two-component system becomes

r ∇µ r ∇µ r N r ∇µ1 N v r ∇µ 1 1 2 (9.47) s& = − J1 ⋅ − J2 ⋅ = − J1 − 1 J2 ⋅ = − 1 + 1 1 J1 ⋅ T T N2 T N2 v 2 T

in vector notation. With the information in Eq. (9.47), Eqs. (9.44) and (9.45) combine to give the linear force flux equation for the diffusing species as

r N v J1 = − L11 1 + 1 1 N2 v2

µ1 ∇ = − D11 ∇ N1 . T

(9.48)

But ∇µ1/∇N1 = (∂µ1 / ∂N1), which allows

r N v 1 J1 = − L11 1 + 1 1 T N2 v2

resulting in L11 =

∂ µ1 ∂ N1

D11T

v N 1 + 1 1 v2 N2

∂ µ1 ∂N1

since v1N1

Copyright © 2008 by Morgan & Claypool All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means—electronic, mechanical, photocopy, recording, or any other except for brief quotations in printed reviews, without the prior permission of the publisher. Tensor Properties of Solids: Phenomenological Development of the Tensor Properties of Crystals Richard F. Tinder www.morganclaypool.com ISBN: 1598293486

paperback

ISBN: 9781598293487 paperback ISBN: 1598293494

ebook

ISBN: 9781598293494 ebook DOI: 10.2200/S00057ED1V01Y200712ENG04 DOI: 10.2200/S00058ED1V01Y200712ENG05 A Publication in the Morgan & Claypool Publishers series SYNTHESIS LECTURES ON ENGINEERING # 4 Lecture #4 Series ISSN ISSN 1939-5221

ISSN 1939-523X

electronic

Tensor Properties of Solids Phenomenological Development of the Tensor Properties of Crystals Richard F. Tinder Washington State University

SYNTHESIS LECTURES ON ENGINEERING # 4

M &C

Mor gan

& Cl aypool

Publishers

iv

ABSTRACT Tensor Properties of Solids presents the phenomenological development of solid state properties represented as matter tensors in two parts: Part I on equilibrium tensor properties and Part II on transport tensor properties. Part I begins with an introduction to tensor notation, transformations, algebra, and calculus together with the matrix representations. Crystallography, as it relates to tensor properties of crystals, completes the background treatment. A generalized treatment of solid-state equilibrium thermodynamics leads to the systematic correlation of equilibrium tensor properties. This is followed by developments covering first-, second-, third-, and higher-order tensor effects. Included are the generalized compliance and rigidity matrices for first-order tensor properties, Maxwell relations, effect of measurement conditions, and the dependent coupled effects and use of interaction diagrams. Part I concludes with the second- and higher-order effects, including numerous optical tensor properties. Part II presents the driving forces and fluxes for the well-known proper conductivities. An introduction to irreversible thermodynamics includes the concepts of microscopic reversibility, Onsager’s reciprocity principle, entropy density production, and the proper choice of the transport parameters. This is followed by the force–flux equations for electronic charge and heat flow and the relationships between the proper conductivities and phenomenological coefficients. The thermoelectric effects in solids are discussed and extended to the piezothermoelectric and piezoresistance tensor effects. The subjects of thermomagnetic, galvanomagnetic, and thermogalvanomagnetic effects are developed together with other higher-order magnetotransport property tensors. A glossary of terms, expressions and symbols are provided at the end of the text, and endof-chapter problems are provided on request. Endnotes provide the necessary references for further reading.

Keywords tensor properties, crystals, thermodynamics, equilibrium, transport

Preface An exhaustive in-depth treatment of the tensor properties of crystals would be a daunting task and would require several books on the subject, each of which would be of considerable length. This would require each property, experimentally known to exist or predicted by theory, to be developed from first principles at the atomic or quantum mechanical level. This is not what this text is about. We purport to develop the physical properties of solids (actually crystals) from the thermodynamic and tensorial points of view, which, if done correctly, provide a valuable introduction to a multitude of physical properties. The phenomenological development used in this text permits a thermodynamic basis for property definitions that is inviolate or nearly so. However, it is correct to say that many of the matter tensor properties defined in this way may not have been studied previously to establish their relative importance. This text is designed to be used as a one-semester or two-quarter course in the subject matter. It also serves as a valuable source of information for practicing engineers and scientists in related fields. Although the text provides the necessary background in tensor analysis, the readership is expected to have some knowledge of calculus and matrix algebra. An understanding of basic vector analysis is also deemed helpful. The necessary information regarding crystallography and point groups as they relate to this text is provided as background material in the text. The contents of this text are based on the author’s notes used for a graduate course taught over several years at Washington State University to graduate students and second-semester seniors in the areas of material science, electrical and mechanical engineering, physics, and chemical physics. An instructor of a course in this subject matter is provided ample opportunity to limit, alter, or expound on any part of the text material as needed to satisfy the course description and needs of the students. Extensive glossaries of terms, expressions, and symbols at the end of the text aid in the learning process. As with any text dealing with complex subject matter, there will undoubtedly be found typos and errors that were overlooked by the author. Hopefully, these have been kept to a minimum. However, should any be found by the instructor or readers, the author would appreciate knowing of them so that corrections can be made. The author may be contacted at the following e-mail address: [email protected]

vii

Acknowledgments The author is deeply indebted to the many senior and graduate students for their countless questions, comments, arguments, and suggestions given during the many years that the contents of this text were used as notes in the conduct of the author’s graduate course taught at Washington State University. As most professors know, students can and do provide the most candid and critical assessments of material presented in a given course. The author also acknowledges the suggestions and contributions of Prof. Elias (Lee) Stefanakos to the subject matter presented in this text, in particular, to the optical effects presented in Chapter 7. Dr. Stefanakos is director of the Clean Energy Research Center at the University of South Florida. Gratefully acknowledged is the encouragement and helpful suggestions offered by Joel Claypool, publisher of Morgan & Claypool Publishers. Finally and most importantly, the author acknowledges the support, care, and understanding of his loving wife, his best friend and confidante, Gloria.

ix

Contents I Equilibrium Tensor Properties of Solids ...............................................................1 1. Introduction ........................................................................................................ 3 1.1 Definition of a Tensor Property . ............................................................. 3 1.2 Concepts of Equilibrium and Reversibility ............................................. 4 1.3 Interaction Diagrams and First-Order Equilibrium Property Nomenclature and Representation........................................................... 5 1.4 Interaction Diagram for the First-Order Nonequilibrium Tensor Properties ................................................................................................ 9 2. Introduction to Tensor Notation, Tensor Transformations, Tensor Calculus, and Matrix Representation ................................................................................ 13 2.1 Introduction to Tensor and Matrix Notation ........................................ 13 2.2 Transformation of Tensors . ................................................................... 14 2.2.1 Transformation of Scalars .......................................................... 15 2.2.2 Transformation of Vectors ......................................................... 15 2.2.3 Transformation of Second-Rank Tensors .................................. 16 2.2.4 Symmetrical and Antisymmetrical Second-Rank Tensors ........ 17 2.2.5 Quadratic Transformation Forms .............................................. 19 2.2.6 Transformation of Third-Rank Tensors . ................................... 20 2.2.7 Transformation of Fourth-Rank Tensors ................................... 22 2.2.8 Summary of Tensor Transformation Laws ................................ 25 2.3 Introduction to Tensor Algebra.............................................................. 25 2.3.1 Tensor Addition . ....................................................................... 26 2.3.2 Tensor Multiplication................................................................. 26 2.3.3 Outer Product . .......................................................................... 27 2.3.4 Tensor Contraction . .................................................................. 27 2.4 Axial Tensors.......................................................................................... 29 2.5 Taylor’s Series Expansion and the Tensor Differentiation Laws ........... 30 2.6 Tensor Fields and Tensor Operators . .................................................... 31 2.6.1 Gradient of a Tensor Field.......................................................... 32

Tensor Properties of Solids

3.

4.

5.

2.6.2 Divergence of a Tensor Field...................................................... 33 2.6.3 Kronecker Delta, Permutation Tensor, Vector Cross Product, and Tensorial Contraction.......................................................... 33 Crystal Systems, Symmetry Elements, and Symmetry Transformations . ....................................................................................... 37 3.1 Introduction .......................................................................................... 37 3.2 Macroscopic Crystal Symmetry and Symmetry Transformations.......... 38 3.2.1 Permissible Rotations................................................................. 38 3.2.2 Center of Symmetry .................................................................. 38 3.3 Space Lattices, Unit Cells, Crystallographic Planes, and Directions—Miller Indices . .................................................................. 41 3.4 The Macroscopic Symmetry of Crystals and the 32 Conventional Point Groups.......................................................................................... 46 3.5 Neumann’s Principle and Its Application to Tensor Properties.............. 46 3.6 Application of Neumann’s Principle to Symmetrical Second-Rank Property Tensors . .................................................................................. 52 3.7 Effect of Neumann’s Principle on the 11 Centrosymmetrical Crystal Classes . ..................................................................................... 56 3.8 Longitudinal and Transverse Effects for Symmetrical Second-Rank Property Tensors . .................................................................................. 57 Generalized Thermostatics and the Systematic Correlation of Physical Properties ............................................................................................ 61 4.1 Energy Representations and the Criteria for Thermodynamic Equilibrium............................................................................................ 61 4.1.1 Energy Density Representation . ............................................... 64 4.2 Thermodynamic Definition of Parameters ............................................ 65 4.3 Generalized Compliance and Rigidity Matrices ................................... 68 4.4 Symmetry of the General Compliance and Rigidity Matrices............... 71 4.5 Systematic Enumeration and Correlation of First-Order Tensor Properties—Generalized Maxwell Relations . ....................................... 74 4.5.1 Principal Effects......................................................................... 74 4.5.2 Independent Coupled Effects . .................................................. 75 4.6 Effect of Measurement Conditions on the First-Order Tensor Properties................................................................ 78 The Dependent Coupled Effects and the Interrelationships Between First-Order Tensor Properties—Use of Interaction Diagrams........................... 85 5.1 The Dependent Coupled Effects .......................................................... 85

Tensor Properties of Solids xi

6.

7.

II

5.2 Interrelationship Between First-Order Properties—Use of Interaction Diagrams . ........................................................................... 87 5.3 The Grüneisen Tensor . ......................................................................... 90 Third- and Fourth-Rank Tensor Properties—Symmetry Considerations.......... 95 6.1 Direct and Converse Piezoelectric Effects . ........................................... 95 6.1.1 Direct Piezoelectric Effect . ....................................................... 95 6.1.2 Converse Piezoelectric Effect .................................................... 97 6.1.3 Crystal Symmetry Considerations . ........................................... 99 6.1.4 Brute-Force Method for the Trigonal and Hexagonal Classes—The Piezoelectric Moduli . ....................................... 100 6.1.5 Longitudinal Piezoelectric Effect ............................................ 106 6.1.6 Transverse Piezoelectric Effect................................................. 108 6.2 Elasticity . ............................................................................................ 108 6.2.1 Hooke’s Law . .......................................................................... 109 6.2.2 Bulk Elastic Behavior .............................................................. 110 6.2.3 Transformation Laws . ............................................................. 112 6.2.4 Elastic Strain Energy Density.................................................. 113 6.2.5 Effect of Crystal Symmetry . ................................................... 113 6.2.6 Homogeneous Elastically Isotropic Solids .............................. 118 6.2.7 Young’s Modulus in a Particular Direction............................... 120 6.2.8 Shear Modulus and Poisson’s Ratio ......................................... 121 Second- and Higher-Order Effects—Symmetry Considerations ................... 123 7.1 Electrostriction and Morphic Effects................................................... 123 7.1.1 Symmetry and Transformation Considerations of Fourth-Rank Tensors . ............................................................. 124 7.2 Generalized Development of the Second-Order Effects . ................... 125 7.3 Phenomenological Development of the Optical Effects...................... 129 7.3.1 Electro-Optical Effects ........................................................... 132 7.3.2 Piezo-Optical and Elasto-Optical Effects . ............................. 134 7.3.3 Piezo-Optical Effect in Cubic Crystals Under Uniaxial Tension ...................................................................... 136 7.3.4 Magneto-Optical (Cotton–Mouton and Faraday) Effects....... 139 7.3.5 Thermo-Optical Effects........................................................... 142

Transport Properties of Solids .......................................................................... 145 8. Introduction to Transport Properties and the Thermodynamics of Irreversible Processes........................................................................................ 147

xii Tensor Properties of Solids

8.1 8.2 8.3 8.4

Gradients, Current Densities, and the Conductivities . ....................... 147 Conjugate or Proper Conductivities..................................................... 149 Cross or Interference Conductivities.................................................... 149 Markoffian Systems, Microscopic Reversibility, and Onsager’s Reciprocity Principle............................................................................ 150 8.4.1 Markoff Processes . .................................................................. 150 8.4.2 Principle of Microscopic Reversibility...................................... 151 8.4.3 Onsager’s Reciprocity Principle................................................ 151 8.4.4 Entropy Production.................................................................. 152 8.5 Proper Choice of Parameters................................................................ 152 8.5.1 Further Restrictions on the Phenomenological Coefficients.... 155 8.6 Flow of Electronic Charge and Heat—The Conductivities................. 156 9. Thermoelectric, Piezothermoelectric, and Diffusive Effects in Solids............. 159 9.1 Seebeck Effect (Thermocouple Effect)................................................ 159 9.2 Peltier Effect (Thermoelectric Heater/Refrigerator Effect)................. 162 9.3 Thomson Effect .................................................................................. 163 9.4 Piezothermoelectric and Elastothermoelectric Effects......................... 166 9.5 Piezoresistance Effect (Strain Gauge Effect)....................................... 169 9.6 Electrodiffusive and Thermodiffusive Effects ..................................... 171 9.6.1 Multiple Diffusing Species....................................................... 171 10. Effect of Magnetic Field on the Transport Properties...................................... 175 10.1 First-Order Thermomagnetic and Galvanomagnetic Effects in an Isotropic Plane . .......................................................................... 175 10.2 Definitions of the Thermomagnetic and Galvanomagnetic Effects in an Isotropic x,y Plane ...................................................................... 178 10.3 Second-Order Effects in a Magnetic Field—The Hall and Magnetoresistance Tensors .................................................................. 181 10.4 First-Order Thermogalvanomagnetic Effects in Isotropic Conductive Media ............................................................................... 184 10.5 Other Higher-Order Magnetotransport Tensor Properties in Anisotropic Media . ............................................................................. 186 Appendices .............................................................................................................. 189 Magnetic Tensor Properties, Magnetic Crystals, and the Combined Space–Time Transformations..................................................................................... 189 A.1 Conditions for Magnetocrystalline Class Application...................................... 189 A.2 Combined Space-Time Transformations......................................................... 190

Tensor Properties of Solids xiii

A.3 Application of Neumann’s Principle to Magnetocrystalline Transformations.... 192 A.4 The Magnetic Point Groups ........................................................................... 198 Endnotes ................................................................................................................. 201 Glossary .................................................................................................................. 205 Terms and Expressions . ............................................................................................ 205 Symbols and Abbreviations . ..................................................................................... 223 Greek Symbols .......................................................................................................... 227 Author Biography..................................................................................................... 229 Index ....................................................................................................................... 231

PA RT I

Equilibrium Tensor Properties of Solids

chapter 1

Introduction 1.1 DEFINITION OF A TENSOR PROPERTY A property, as defined in this text, is a coefficient that linearly relates an intensive (or cause) parameter to an extensive (or effect) parameter. When the intensive and extensive parameters are tensor variables, the property is also a tensor quantity. One way of expressing this is

Tensor

Coefficient Parameter

Parameter

= Property

Tensor

Cause

Tensor

Effect

(1.1)

or its inverse, which places the inverse of the tensor property coefficient on the left-hand side of the equation. The particular tensor property will have a definite physical significance and will be represented by a fixed number of components depending on the nature and tensor character of the intensive and extensive parameters that it relates. One physical significance of the property coefficient may be given as the rate of change of one parameter with respect to the other as implied by Eq. (1.1). One or both of the parameters that define the property coefficient will usually be a field tensor such as stress or strain, electric or magnetic field strength, or temperature (a scalar). The extent to which a property of a crystal exists with respect to the application of a given field depends on the electronic and subatomic structure of the atoms and on the manner in which they are arranged in the lattice. Shown in Table 1.1 are four typical examples of properties of crystals that are directly related by cause and effect tensor parameter. Here, the pyroelectric coefficient pi is a vector–scalar tensor property, hence, a vector, that relates the change in polarization δPi with a change in temperature δT. The thermal expansion coefficient aij is a tensor–scalar tensor property of tensor rank 2 that relates a change in strain εij with a change in temperature δT. The piezoelectric coefficient dijk is a vector– tensor property of tensor rank 3 that relates the polarization Pi to the stress tensor σjk. Finally, the elastic compliance coefficient sijkl is a tensor–tensor property of rank 4 that relates the stress σij to

tensor properties of solids

TABLE 1.1: Typical examples of properties of crystals that are directly related by cause and effect tensor parameters Effect tensor parameter

Cause tensor parameter

Property name

Tensor equation

Tensor rank of coefficient

δPi

δT

Pyroelectricity

δPi = piδT

First (pi)

δεij

δT

Thermal expansion

δεij = αijδT

Second (αij)

Pi

σij

Piezoelectricity

Pi = dijkσjk

Third (dijk)

εij

σkl

Elasticity

εij = sijklσkl

Fourth (sijkl)

Shown are the tensor parameters, property to which they are applicable, and the tensor equations and tensor rank for the property coefficients.

the strain εkl (Hooke’s law). Thus, it is seen that the tensor rank of a property coefficient is the sum of the tensor ranks of the parameters that it relates. Note that all tensor property coefficients given in Table 1.1 are examples of equilibrium properties. A well-known example of a nonequilibrium or transport property is resistivity ρij , a second-rank tensor that relates electric field strength Ei to the current density Jj according to Ei = ρij Jj , which, of course, is the tensor representation of Ohm’s law. The distinction between equilibrium and nonequilibrium transport properties will be made clear in the section that follows, together with Parts I and II of this text.

1.2

CONCEPTS OF EQUILIBRIUM AND REVERSIBILITY

The properties of interest to Part I of this text are those that can be represented by tensors and described with reference to equilibrium states and thermodynamically reversible changes in crystals. Consider a thought experiment on any closed system (e.g., a crystal) in which all imaginable physically measurable quantities are accurately recorded as a function of time. If it is found that all processes, defined by the physically measurable quantities, are macroscopically time independent, thermodynamic equilibrium is said to exist. This requires, for example, the absence of the transport of heat (or entropy), charge, and mass and that all parts of the system be mechanically in static equilibrium. Thus, thermodynamic equilibrium prevails if the system under consideration is in thermal, electrical, magnetic, mechanical, and chemical equilibrium. Thermodynamic equilibrium does permit microscopic fluctuations to occur on the atomic level as long as they are random and do not produce measurable time-dependent changes in the physical state of the system.

introduction

Properties of crystals that represent time-independent processes are called equilibrium properties. Such properties can adequately be described phenomenologically by using equilibrium thermodynamics, that is, thermostatics. Properties that represent time-dependent or spontaneous processes are called nonequilibrium or transport properties. Such properties can be described only by use of the thermodynamics of irreversible processes, a subject that is covered in Part II of this text. The concept of thermodynamic reversibility is intimately connected with the concept of equilibrium. The term reversible applies to a process within a system that has been displaced from equilibrium only to an infinitesimal extent. Therefore, a reversible process may be defined as the hypothetical passage of the system through a series of equilibrium states so close together that they are nearly indistinguishable. Such a process is reversed by an appropriate infinitesimal change of the physical conditions imposed on the system. Actually, no ongoing process is reversible in the strict sense of the word. However, if the conditions to be imposed on the system are applied infinitesimally fast, then, within experimental error, the process may be considered reversible. A reversible process is usually considered to be a linear process over an infinitesimal change in cause and effect parameters. However, a reversible process may be nonlinear, provided that the infinitesimal changes in the system are restored reversibly. In the development of the equilibrium properties, we will assume that the reversible processes are linear and that thermodynamic equilibrium is established at each point in an infinitesimal change.

1.3

INTERACTION DIAGRAMS AND FIRST-ORDER EQUILIBRIUM PROPERTY NOMENCLATURE AND REPRESENTATION

It is appropriate that we now preview the spectrum of first-order equilibrium properties about which we shall later discuss in more detail. To do this, it is necessary to define the conjugate parameters from which the general first-order interaction diagram can be constructed. The four pairs of conjugate 8 parameters are the following: (T,S), (E, P), (B, M ), and (σ,ε), which give rise to ∑n=1 (n - 1) = 28 first-order properties including 4 principal effects and 24 coupled effects. The conjugate parameter pairs are (temperature, entropy), (electric field strength, polarization), (magnetic flux density, magnetization), and (stress, strain), respectively. The conjugate pairs (E, P) and (B, M) are chosen in preference to others for the sake of consistency, with the thermodynamic developments yet to come. Shown in Figure 1.1 is the generalized interaction diagram for the first-order equilibrium properties where the names, symbols, and tensor rank (in parentheses) are given for each of the eight parameters. The four principal effects are represented by horizontal lines (i.e., between conjugate parameters), whereas the coupled effects are given by the nonhorizontal lines. The vertical lines represent dependent coupled properties relating any two intensive parameters (or any two extensive parameters). The set of 16 “compliance” effects are shown by arrows that point to the dependent variables, which,

tensor properties of solids

in this case, are the extensive parameters. Extensive parameters are those that depend on the amount of material of the solid phase system. Parameters that are independent of the amount of material in the solid phase are called intensive parameters and are associated only with the external conditions (fields) imposed on the system. Thus, the arrows in Figure 1.1 are drawn from the intensive (independent) parameters to the extensive (dependent) parameters. Reversal of the arrows defines the set of 16 “rigidity” effects that will later be shown as the collective inverse of the “compliance” effects. For the convenience of the reader, the 16 compliance equilibrium properties are presented in Table 1.2 in the order of increasing tensor rank, first for the principle effects and then for the

Intensive Parameters

T

T emperature (0)

Extensive Parameters

S

Entopy (0)

E

P

Electric Field (1)

Polarization (1)

B

M

Magnetic Flux (1)

Magnetization (1)

σ

Stress (2)

ε

Strain (2)

FIGURE 1.1: Generalized interaction diagram for the 28 first-order effects showing the names, symbols, and tensor rank (in parentheses) for each of the 8 parameters.

introduction

TABLE 1.2: The set of 16 compliance effects and their associated parameter pairs showing the 4 principal effects and 12 coupled effects as listed in the order of increasing tensor rank Parameter pair

Associated property

Tensor rank

Principal effects (S, T )

Heat capacity

0

(P, E)

Dielectric susceptibility

2

(M, B)

Magnetic susceptibility

2

(ε, σ)

Elasticity

4

Interaction (coupled) effects (S, E)

Pyroelectric effect

1

(P, T )

Converse pyroelectric effect

1

(S, B)

Pyromagnetic effect (magnetocaloric effect)

1

(M, T )

Converse pyromagnetic effect

1

(S, σ)

Piezocaloric effect

2

(ε, T )

Thermal expansion (converse piezocaloric effect)

2

(P, B)

Magnetoelectric susceptibility

2

(M, E)

Converse magnetoelectric susceptibility

2

(P, σ)

Direct piezoelectric effect

3

(ε , E)

Converse piezoelectric effect (first-order electrostriction)

3

(M, σ)

Direct piezomagnetic effect

3

(ε, B)

Converse piezomagnetic effect (first-order magnetostriction)

3

tensor properties of solids

T

Temperature (0)

Th erm al

Thermal Stress, – t (2)

ca zo e i P

lo

ric

α ct, e f Ef

Entopy (0)

(2)

Ex pa nsi o

σ

Stress (2)

S

Heat Capacity, C/T (0)

n, α

Heat of Deformation, t (2) (2)

ε

Elasticity, s (4)

Strain (2)

FIGURE 1.2: Interaction diagram representing the thermal, thermoelastic, and elastic effects. The arrows point to the dependent variable.

interaction (coupled) effects. Note that each parameter pair is given in (extensive, intensive) notation form. Other equilibrium properties, not mentioned above, include those in Figure 1.1 for which no one-way arrows are shown. Some of these are of little or no interest to the developments in this text. Most of those equilibrium properties that remain are higher-order effects that can usually be defined in Taylor series expansions of the appropriate parameters. The higher-order effects are usually of high tensor rank and are, accordingly, more complicated. These include such effects as electrostriction, magnetostriction, and a variety of optical effects. Many of these effects will be considered in later chapters. To provide a little more background detail, we will next consider an interaction diagram associated with the thermal and mechanical variables, that is, one that represents the thermal, thermoelastic, and elastic effects. This interaction diagram is shown in Figure 1.2 where the arrows again point toward the dependent variables. Noting from Figure 1.2 that both the stress and temperature fields contribute to an elastic strain, we write in differential form,

dεij = siTjkl dσkl + a σij dT

(1.2)

εij = siTjkl σkl + a σij ∆T .

(1.3)

or in integrated form

introduction

In these equations, sTijkl = (∂εij / ∂σkl)T is the isothermal (temperature independent) elastic compliance, and α σij = (∂εij / ∂T )σ is the isopiestic (stress invariant) coefficient of thermal expansion. The fourthrank tensor property sTijkl represents a principal effect (elasticity) because it relates the conjugate parameters σ and ε. The second-rank tensor property α σij , on the other hand, represents a coupled effect (thermal expansion) because it relates the cross parameters T and ε at constant stress, σ. By similar reasoning, one notes from Figure 1.2 that a positive increase in stress as well as an increase in temperature and strain produces an increase in the entropy of a crystal. In differential form, we write

dS = αTij dσij + (C σ / T )dT

(1.4)

∆S = αTij σij + (C σ / T )∆T .

(1.5)

or in integrated form

Here, αTij = (∂S / ∂σij )T is the isothermal piezocaloric coefficient, equal to the coefficient of thermal expansion measured under constant stress, and C σ = T (∂S / ∂T )σ is the isopiestic (constant stress) heat capacity. The fact that (∂S / ∂σij )T = (∂εij / ∂T )σ is a consequence of thermodynamic arguments to be discussed in detail later. The properties just described have been defined in such a way that only the intensive parameters are held constant. Other coupled effects result from an association of the thermal and mechanical variables but which will have both intensive and extensive parameters held constant. Suppose it is desirable to equate the isothermal elastocaloric (heat of deformation) with the isometric thermal stress coefficient as depicted by the vertical arrows in Figure 1.2. When this is done, we write

(∂S / ∂εij )T = − (∂σij / ∂T )ε = tij ,

(1.6)

a result that follows from developments that will be presented later. Note that the isometric thermal stress coefficient describes the negative or compressive stress produced when a mechanically constrained crystal is heated. Equation (1.6) is one of many Maxwell relations to be discussed later in Chapters 4 and 5.

1.4

INTERACTION DIAGRAM FOR THE FIRST-ORDER NONEQUILIBRIUM TENSOR PROPERTIES

There is another important group of properties common to crystals that deal with thermodynamically irreversible phenomena. These are the transport properties that involve the flow of charge, heat, and mass. A complete understanding of these effects is possible only through the use of

10 tensor properties of solids

fluctuation theory, the principle of microscopic reversibility, and the Onsager reciprocal relations, that is, through the use of the thermodynamics of irreversible processes. In contrast, the interactions between equilibrium properties are easily deduced by using standard thermodynamic (thermostatic) arguments. Although it is not commonly done, the first-order transport properties may also be represented by interaction diagrams. To do this, it must be stated clearly that the use of such diagrams in no way implies thermodynamic reversibility in the same sense as for the equilibrium properties, but rather implies microscopic reversibility as used in fluctuation theory. To construct a useful interaction diagram for first-order nonequilibrium properties, three pairs of conjugate parameters that are physically measurable are used. These pairs are the three current densities (fluxes) and their conjugate driving forces representing the flow of current ( J n, ∇φ E ), heat ( J q, ∇φT ), and mass ( J m, ∇φ C ). Shown in Figure 1.3 is the interaction diagram for the first-order transport properties that positions the temperature gradient (∇φT ), electric potential gradient (∇φ E ), and concentration gradient (∇φC )

=0 (J n

KmE

e siv fu dif tro ec we Po r

oe l ec tri cP ow er

El

Kq E

Electrical Cond., KnE

)

∇φ E

m

(J

Jn

Th

erm

) =0

o al C m r The

∇φ T

KnT

ctiv ndu

ity,

qT

K

KmT

Jq

Jm

KnC

D if fusi vi KqC

Thermodiffusive Power (J m = 0)

ty,

K mC

∇φ C

FIGURE 1.3: Interaction diagram for the first-order nonequilibrium (transport) properties showing the 9 conductivities and 3 power coefficients, all 12 of which are second-rank tensor properties.

introduction 11

in clockwise sequence on the outside of the interaction triangle. The heat current ( J q), electron (or ion) current ( J n), and mass current densities ( J m) are placed inside the gradient triangle nearest their respective conjugate parameters. All transport parameters, it will be noted, are tensors of 6 rank 1, that is, vectors. This diagram represents ∑n =1 (n - 1) = 15 relationships, which include nine conductivities each relating a flux to a gradient, three “power” coefficients each relating one gradient to another, and three relationships between the current densities. The 12 conductivities and power coefficients are each second-rank tensors. The relationships between fluxes are interpreted, for example, as the heat or entropy associated with the flow of charge for the ( Jq , J n) relationship and similarly for the two other pairs. These current density relationships have not been considered as tensor properties. There exist other transport properties not included in the interaction diagram of Figure 1.3. These arise primarily from the application of magnetic and/or stress fields applied to crystals exhibiting one or more of the properties represented in the J − ∇φ interaction diagram. This leads to important thermomagnetic and galvanomagnetic, piezoresistance, piezothermoelectric, and the piezogalvanomagnetic effects and to other higher-order transport properties. The phenomenological developments of the transport properties in crystalline solids are the topics covered in Part II of this text. These properties will be discussed in some depth based on the basic principles of irreversible thermodynamics. The treatment is, by its nature, more difficult than that presented in Part I, dealing with the phenomenological developments of the equilibrium tensor properties—the basic principle of irreversible thermodynamics are statistical in nature, dealing mainly with fluctuation theory. Recognizing this, special care is taken to present the more complex developments in a manner that minimizes this difficulty. • • • •

13

chapter 2

Introduction to Tensor Notation, Tensor Transformations, Tensor Calculus, and Matrix Representation 2.1

INTRODUCTION TO TENSOR AND MATRIX NOTATION

To help understand the tensor notation used in Section 1.3 and in subsequent sections, we provide here an introduction to tensor analysis in the use of scalars, vectors, and tensors of second- and higherorder rank. To define explicitly the various tensor operations involved in a comprehensive treatment of the physical properties of solids, reference must be made to a coordinate system. This leads naturally to subscript notation and matrix forms, which will be used exclusively throughout this book. Tensors are known to be abstract quantities that are used in the study of many physical laws of nature. There are different kinds of tensors (e.g., polar, axial, magnetic, axial–magnetic), and each kind is classified by its tensor rank, r. In general, a tensor is specified by n(r) components, where n is the number of dimensions of space being used. In three-dimensional Euclidean space, the number of components of a given tensor is 3(r). We will be concerned only with orthogonal Euclidean coordinates (Cartesian coordinates) and with Cartesian tensors, thereby allowing the distinction between covariant and contravariant tensors laws to disappear, and hence of no concern to us. A tensor of rank r that is specified by 3(r) components in rectangular Cartesian coordinates is given in tensor subscript notation by Tijk, that is, by r number of subscripts each taking on values 1, 2, 3 corresponding to three-dimensional Cartesian space. The components of these tensors can be represented by a matrix of symbols arranged in rows and columns. Consider, for example, a second- rank tensor Tij relating two vectors pi and qj, with components p1, p2, and p3, and q1, q2, and q3, respectively. The tensor equation becomes

pi = Tij qj

(i, j = 1,2,3),

(2.1)

where summation from 1 to 3 with respect to the repeating (dummy) suffix, j, is understood. This is called the Einstein summation convention, which allows the summation sign Σ to be dropped. Expanding Eq. (2.1), as required by summation, gives the following three equations for pi:

14 tensor properties of solids

p1 = T11q1 + T12q2 + T13q3 p2 = T21q1 + T22q2 + T23q3 p3 = T31q1 + T32q2 + T33q3

(2.2)

which can be represented in matrix form as

p1 T11 T12 T13 q1 p2 = T21 T22 T23 . q2 p3 T31 T32 T33 q3

(2.3)

or simply in matrix symbolic notation p = Tq .

(2.4)

Vectors may be represented either by a (3 × 1 = rows × column) column matrix as in Eq. (2.3) or as a (1 × 3) row matrix

p1 p2 or [ p1 p2 p3] , p3

depending on the type of matrix operation to be performed. The nine components of a secondrank tensor, Tij, may be represented by a (3 × 3) matrix as in Eq. (2.3) or as either a (9 × 1) column matrix or (1 × 9) row matrix, as will be demonstrated later. In any case, it must be understood that a matrix is nothing more than an array of symbols or numbers arranged in rows and columns. The matrix array has no physical meaning in itself but may represent a tensor that does have physical significance.

2.2

TRANSFORMATION OF TENSORS

The tensor concept is intimately connected with the transformation laws for tensors. In fact, a tensor can be regarded as a mathematical entity having the transformation properties required by the physical quantities that it represents. The transformation of a tensor from one set of Cartesian coordinates to another set does not alter the tensor’s physical significance but rather is simply another equivalent way of representing it. A tensor may be classified as to its symmetry, that is, it may be symmetrical (or partially symmetrical), asymmetrical, or antisymmetrical. However, depending on its transformation law, the tensor may be further characterized as polar, axial, magnetic, or axial–magnetic. The components of an axial tensor change sign if the handedness of the coordinate axes is changed, whereas the com-

introduction to tensor and matrix representation 15

ponents of a magnetic tensor change sign only if the atomic magnetic moments are reversed. Polar tensors, on the other hand, are unaffected by either change in handedness or reversal of magnetic moments. In this section, attention will be focused on the transformation laws of polar tensors.

2.2.1 Transformation of Scalars Tensors of rank 0 are nondirectional physical quantities called scalars and are invariant under a coordinate transformation. Typical examples are mass, temperature, entropy, and heat capacity; thus, for example, T ′ = T for the transformation of entropy.

2.2.2 Transformation of Vectors Tensors of rank 1 are called vectors. Polar vectors (as distinguished from axial vectors) transform like the coordinates of a point. Let Tj be a polar vector with respect to axes 0x1, 0x2 , 0x3 that is to be transformed to T ′i with respect to axes 0x ′1, 0x ′2 , 0x ′3 symbolized by T → T ′. Each T ′i is obtained by resolving the Tj along the axes 0x ′1 as shown in Figure 2.1. The components for the three T ′i are given by

T ′1 = a11T1 + a12T2 + a13T3 T ′2 = a21T1 + a22T2 + a23T3 T ′3 = a31T1 + a32T2 + a33T3

(2.5)

T ′i = aijTj (i, j = 1,2,3 = 1 − 3)

(2.6)

or

in convenient tensor subscript notation. Here, the aij are called the direction cosines, for which examples are shown in Figure 2.1. Thus, nine direction cosines are required to specify the transformation of a polar vector where i and j represent the new and old axes, respectively. Equations in (2.5) can also be conveniently represented in the matrix form

T1′ a11 a12 a13 T1 T2′ = a21 a22 a23 . T2 T3′ a31 a32 a33 T3

(2.7)

or simply

T ′= aT

(2.8)

16 tensor properties of solids

x3 x3'

T

-1 a 33

c os

T3'

T3

T2'

cos-1a31

T2

co

x2

cos-1a13

T1 x1

x2'

T1'

s -1 a

11

-1 a 12

s co

x1' FIGURE 2.1: Transformation of the polar vector T → T ′ showing sample direction cosines.

in matrix symbolic notation. The reverse transformation symbolized by T ′ → T is given by T = a~T ′ = a -1T ′,

(2.9)

(2.10)

where a is an orthogonal matrix and

a11 a21 a31 ~ a = a12 a22 a32 a13 a23 a33

is the transpose of a always equal to its inverse, a~ = a -1. Examples of polar vectors are force, electric field, and polarization. Other vectors, such as mechanical moment, angular momentum, and the curl of a polar vector, are examples of axial vectors. Still other vectors, such as magnetic field strength, magnetic flux density, and magnetization, are both axial and magnetic in character and will be considered at a later time.

2.2.3 Transformation of Second-Rank Tensors The transformation law for polar second-rank tensors can be developed from the transformation law for polar vectors. As in Eq. (2.4), consider a second-rank polar tensor that linearly relates two polar vectors p and q. With respect to two sets of axes 0xi and 0x ′i and in matrix symbolic notation, Eq. (2.4) becomes

p = Tq with respect to 0xi

(2.11)

introduction to tensor and matrix representation 17

p′ = T ′q′ with respect to 0x′i

(2.11a)

Transforming the components of p and q′ separately, one obtains in matrix notation

p′ = ap

(2.12)

q = a~q′,

(2.12a)

after which, by introducing Eqs. (2.11) and (2.12a) into Eq. (2.12), there results in matrix notation p′ = ap = aTq = aT a~q′ = T ′q′.

It now follows that

T ′ = aT a~

(2.13)

T ′ij = aikajlTkl (i, j, k, l = 1, 2, 3 = 1 − 3)

(2.14)

or

in tensor subscript notation. Both Eqs. (2.13) and (2.14) represent the transformation law for polar second-rank tensors. In Eq. (2.14), the components of T ′ij are obtained by direct summation of the repeating (dummy) subscripts k and l, whereas in Eq. (2.13), the same components are given in the form

a11 a21 a31 a12 a22 a32 , a13 a23 a33

T11 T12 T13 T21 T22 T23 T31 T32 T33

a11 a12 a13 T ′= a21 a22 a23 a31 a32 a33

(2.15)

which are conformable for matrix multiplication.

2.2.4 Symmetrical and Antisymmetrical Second-Rank Tensors Any second-rank tensor Tij can be expressed as the sum of symmetrical Sij and antisymmetrical Aij tensors. In subscript notation and matrix symbolic notation, this is written as

~ ~ Tij = (Tij + Tji ) / 2 + (Tij − Tji ) / 2 = (T + T ) / 2 + (T − T ) / 2 = Sij + Aij ,

(2.16)

18 tensor properties of solids

where it follows that

S31 ~ S23 = S, S33

½ (T12− T21 ) ½ (T13− T31 ) 0 0 A12 −A31 ~ A23 = −A. A = ½ (T21− T12 ) 0 ½ (T23− T32 ) = −A12 0 0 A31 −A23 0 ½ (T31− T13 ) ½ (T32− T23 )

(2.17)

½ (T12+ T21 ) ½ (T13+ T31 ) T11 S11 S12 S = ½ (T21+ T12 ) S22 T22 ½ (T23+ T32 ) = T33 Sym. ½ (T13+ T31 ) ½ (T32+ T23 )

(2.18)

Clearly, S is specified generally by six independent components, whereas A is specified generally by three independent components. Thus, a symmetrical second-rank tensor is equal to its transpose, ~ S = S , where S11, S22, and S33 are called the principal components that lie along the leading diagonal of the (Sij) matrix. In the case of an antisymmetrical second-rank tensor, the principal components are zero. The stress tensor σij is an example of a symmetrical second-rank tensor, such that σij = σji . Equation (2.17) permits simplification of the matrix forms for symmetrical second-rank tensors. Writing the subscripts in a positive permutation of 123 gives the following results: Tensor notation S11 S22 S33 S23( = S32 ) S31( = S13 ) S12( = S21) Strain notation S1 S2 S3 2S23 2S32 2S12 (2.19) Matrix notation S1 S2 S3 S4 S5 S6 The notation in (2.19) leads to three useful (6 × 1) column forms:

S1 S2 S3 or S4 S5 S6

S1 S2 S3 or 2S4 2S5 2S6

S11 S22 S S = 33 S23 S31 S12

(2.20)

or their (1 × 6) row transpositions. The single subscript form will be the form of choice for use in matrix symbolic equations. The third form in (2.20) is also the accepted matrix form for the strain tensor. Examples of symmetrical second-rank tensors are stress, strain, thermal expansion, dielectric and magnetic susceptibilities, and others. From Eq. (2.18), it is clear that the principal components

introduction to tensor and matrix representation 19

of an antisymmetrical second-rank tensor are null, leaving only three antisymmetrical components, A23, A31, and A12. Examples of antisymmetrical second-rank tensors include the rotational component of a generalized elastic deformation leaving strain εij = εji as a symmetrical second-rank tensor.

2.2.5 Quadratic Transformation Forms The transformation of third- and fourth-rank tensor components is greatly facilitated by the use of quadratic transformation forms, which can be readily obtained from the transformation law for second-rank tensors. It is assumed that any second-rank tensor involved in the description of a third- or fourth-rank tensor is symmetrical such that use can be made of the linear transformation law

a11 a12 a13 S11 S12 S31 a11 a21 a31 a21 a22 a23 . S12 S22 S23 . a12 a22 a32 . a31 a32 a33 S31 S23 S33 a13 a23 a33

(2.21)

S′= aS a~ =

2 a 22 2 a 32

2 a 13 2 a 23 2 a 33

2a 12 a13 2a22 a23

2a13a11

2a11a12

2a23 a21

2a21a22

S2′

2 a11 2 a11

2 a 12

2 a11

S1

S1′

--------------------------------

Carrying out the indicated multiplication and arranging the components of S ′ and S into (6 × 1) column matrices permits Eq. (2.21) to be represented in the quadratic form S2

S3′ = 2a32 a33 2a33a31 2a31 a32 . S3 -----------------------------------------------------------------------------------------------a21 a31 a22 a32 a23 a33 a22 a33 + a23 a32 a21 a33 + a23 a31 a21 a32 + a22 a31 S4 S4′

S6′

S5

a11 a21 a12a22 a13a23 a12 a23+ a13a22 a11a23 + a13 a21 a11 a22 + a12a21 S6

a31a11 a32 a12 a33 a13 a12 a33 + a13 a32 a11 a33 + a13 a31 a11 a32 + a12 a31

S5′

or simply in symbolic matrix notation

S′ = αS.

(2.22)

Here, α is a (6 × 6) matrix called the quadratic transformation matrix for a symmetrical second- rank tensor and where the third single subscript notation of (2.20) has been applied. With few exceptions, the property tensors of higher order, which are commonly encountered, are represented by third- and fourth-rank tensors having some inherent symmetry. Thus, where it is necessary to specify the transformation law for these matter tensors, rather extensive practical use will be made of the α transformation form—a method preferred over the more cumbersome method of direct summation of the repeating suffixes in the tensor subscript forms.

20 tensor properties of solids

A mnemonic diagram for the quadratic transformation matrix α can be constructed by dividing it into four sections as follows:

---------------------

Twice the product of row omissions of [aij ] matrix . -----------------------------------------------------------------------------------Cross product of Product of column minor of element aij omissions of [aij ] matrix

Square of element aij of [aij ] matrix

The content of these four sections can be verified by an inspection of Eq. (2.22) in expanded form. Not all property tensors exhibit inherent symmetry, and for this reason, a similar quadratic transformation law must be written for an asymmetrical second-rank tensor. In this case, the transformation matrix becomes a (9 × 9) quadratic form. The development of this more general form follows from Eq. (2.15) by carrying out the indicated multiplication and arranging the components of T ′ and T as (9 × 1) matrices similar to (2.20) but with no symmetry. The result is given by

T ′ = βT ,

(2.23)

where β is called the (9 × 9) general quadratic transformation matrix for asymmetrical second-rank tensors presented in Eq. (9.31). The β transformation form is useful in describing the transformation laws for the less common piezothermoelectric and elastothermoelectric power properties as well as the piezomagnetoelectric and elastomagnetoelectric effects.

2.2.6 Transformation of T hird-Rank Tensors Consider a third-rank tensor, T, relating a polar vector, p, and a polar second-rank tensor, q, written with respect to two sets of coordinate exes, 0xi and 0x′i :

pi = Tijkqjk or p = Tq for axes 0xi

(2.24)

p′l = T ′lmnq′mn or p′ = T ′q′ for axes 0x′i

(2.25)

and

For the case where q is a symmetrical second-rank tensor (hence, q = q~), it follows that for the transformations p′ = ap, q′ = α q, and q = α −1q′, there results

p′ = ap = aTq = aTα −1q′ = T ′q′,

introduction to tensor and matrix representation 21

giving for the transformation law for T T ′ = aTα −1,

(2.26)

~ in general. In tensor subscript where α −1 is the inverse of α and where it is understood that α −1 ¹ α notation, Eq. (2.26) is written as

T ′ijk = ail ajmaknTlmn (i − n = 1 − 3)

(2.27)

The partial symmetry of T in Eq. (2.24) is implied by the symmetry of q. This is easily shown by using tensor subscript notation giving pi = Tijkqjk = Tikj qkj ,

(2.28)

which permits Tijk = Tikj .

In matrix subscript notation, Eq. (2.28) becomes

pi = Timqm (i = 1 − 3; m = 1 − 6),

(2.29)

where q is now a (6 × 1) column matrix and Eq. (2.29) becomes

p1 T11 T12 T13 T14 T15 T16 p = p2 = T21 T22 T23 T24 T25 T26 p3 T31 T32 T33 T34 T35 T36

q1 q2 q3 = Tq, q4 q5 q6

(2.30)

with respect to axes 0xi . Note that subscript m in Eq. (2.29) is unfolded according to the matrix notation in (2.20). This permits a reduction in the T matrix from a (3 × 9) to a (3 × 6) matrix, as given in Eq. (2.30), both of which avoid the need for a three-dimensional representation. The tensors Tijk and Tikj in Eq. (2.28) are called tensor isomers and represent a certain partial symmetry. The tensor Tijk has a total of 3! = 6 isomers possible, which are obtained by the permutation of pairs of subscripts. In comparison, the transpose of a second-rank tensor Tij is its only isomer. Examples of third-rank tensor properties that exhibit this partial symmetry are the piezoelectric

22 tensor properties of solids

effect, first-order electrostriction, piezomagnetic effect and first-order magnetostriction, the linear electro-optical effect, the thermal–electro-optical effect, and others. The transformation of components for the partially symmetrical third-rank tensor Tijk = Tikj is carried out in accordance with Eq. (2.26) for new and old sets of axes, 0x′i and 0xi , respectively:

−1 α 14 −1 α 24 −1 α 34 −1 α 44 −1 α 54 −1 α 64

−1 α 15 −1 α 25 −1 α 35 −1 α 45 −1 α 54 −1 α 65

−1 α 16 −1 α 26 −1 α 36 −1 α 46 −1 α 56 −1 α 66

−1 α 13 −1 α 23 −1 α 33 −1 α 43 −1 α 53 −1 α 63

−1 α 12 −1 α 22 −1 α 32 −1 α 42 −1 α 52 −1 α 62

a11 a12 a13 T11 T12 T13 T14 T15 T16 T ′ = a21 a22 a23 . T21 T22 T23 T24 T25 T26 a31 a32 a33 T31 T32 T33 T34 T35 T36

−1 α 11 −1 α 21 −1 α 31 −1 α 41 −1 α 51 −1 α 61

which represents the matrix equation

T ′ = aTα −1

(2.31)

It may be recalled that the inverse (or reciprocal) A −ij1 of a matrix A is the transpose of the cofactor (Aij ) of the element Aij divided by the non-zero determinant of Aij . That is,

( Aji) (Aij )−1= or Ai j

( A~ ) A −1= A

(2.32)

where (Aij ) = (−1)(i + j )|Mij | is the cofactor of element Aij and |Mij | is its minor (the determinant that remains after removing the ith row and jth column in |Aij | ). Obviously, transformation of tensors of rank 3 can be quite laborious. Fortunately, the linear and quadratic transformation matrices representing the symmetry operation for crystals are relatively uncomplicated. As will be shown later in Section 3.5, these matrices often consist of compo~, a result that is not true generally. nents that are 0, 1, or -1, and in most cases, α −1 = α

2.2.7 Transformation of Fourth-Rank Tensors In similar fashion, the transformation law for a fourth-rank tensor property can be deduced from the transformation laws of the tensor variables it relates. Consider the fourth-rank tensor property relating two polar second-rank tensor variables with reference to the two sets of axes, 0xi and 0x′i

pij = Tijkl qkl or p = Tq for axes 0xi

(2.33)

introduction to tensor and matrix representation 23

and

p′mn = T ′mnopq′op or p′ = T ′q′ for axes 0x′i .

(2.34)

If both p and q are symmetrical second-rank tensors, convenient use can again be made of the α quadratic transformation form. Because p and q′ transform as p′ = αp and q = α −1q′, then p′ = αp = αTq = αTα −1q′ = T ′q′

or

T ′ = αTα −1

(2.35)

as the transformation equation for T in matrix symbolic notation. In tensor subscript notation, Eq. (2.35) becomes

T ′ijkl = aimajnakoalpTmnop (i − p = 1 − 3)

(2.36)

The partial symmetry of Tijkl is implied by the symmetry of pij = pji = pm and qkl = qlk = qn where it is now proper to write

pm = Tmnqn (m, n = 1 − 6)

(2.37)

The partial symmetry expressed by Eq. (2.37) permits a reduction in the number of independent coefficients needed to specify T from 3(4) = 81 to 36. Because both p and q are represented by (6 × 1) matrices, it follows that T must be a (6 × 6) matrix and that Eq. (2.37) can be presented as

T22 T32 T42 T52

T23 T33 T43 T53

T24 T34 T44 T54

T25 T35 T45 T55

T62 T63 T64 T65

T26 q2 T36 . q3 . T46 q4 T56 q5 T66 q6

p2 T21 p3 = T31 p4 T41 p5 T51 p6 T61

T11 T12 T13 T14 T15 T16 q1

p1

(2.38)

Just as for the case of the partially symmetrical third-rank tensor, the transformation law for the partially symmetrical fourth-rank tensor in Eq. (2.37) is most conveniently represented in matrix form according to T ′ = αTα −1 in Eq. (2.35), giving

24 tensor properties of solids

T12 T22 T32 T42 T52 T62

T13 T14 T23 T24 T33 T34 T43 T44 T53 T54 T63 T64

T15 T25 T35 T45 T55 T65

T16 T26 T36 T46 T56 T66

T11 T21 T31 T41 T51 T61

−1 α 11 −1 α 21 −1 α 31 −1 α 41 −1 α 51 −1 α 61

−1 α 12 −1 α 22 −1 α 32 −1 α 42 −1 α 52 −1 α 62

−1 α 13 −1 α 23 −1 α 33 −1 α 43 −1 α 53 −1 α 63

−1 α 14 −1 α 24 −1 α 34 −1 α 44 −1 α 54 −1 α 64

−1 α 15 −1 α 25 −1 α 35 −1 α 45 −1 α 54 −1 α 65

−1 α 16 −1 α 26 −1 α 36 −1 α 46 −1 α 56 −1 (2.39) α 66

α 16 α 26 α 36 α 46 α 56 α 66

α 15 α 25 α 35 α 45 α 55 α 65

α 14 α 24 α 34 α 44 α 54 α 64

α 13 α 23 α 33 α 43 α 53 α 63

α 12 α 22 α 32 α 42 α 52 α 62

α 11 α 21 α T ′ = 31 α 41 α 51 α 61

Here again, it is shown that numerical manipulation required to transform a higher-rank tensor is considerable, particular for an arbitrary rotation of axes. In such cases, use of the computer is recommended. However, as pointed out earlier, transformation matrices representing most crystal symmetry operations are strikingly simple, allowing tensor transformations in most cases to be carried out with little difficulty by using α −1 = α~ in Eqs. (2.31) and (2.39) or even by the method of direct inspection discussed later. The maximum inherent symmetry possible for fourth-rank tensors is given by

Tmn = Tnm (m, n = 1 − 6) .

(2.40)

In this case, the leading diagonal of components becomes the mn = nm symmetry line. This eliminates the 15 coefficients below the leading diagonal symmetry line as independent components. The remaining 21 coefficients are now represented by the symmetrical (6 × 6) matrix

T16 T26 T36 = [Tnm ] T46 T56 T66

T15 T25 T35 T45 T55

T11 T12 T13 T14 T22 T23 T24 T33 T34 [Tmn ] = T44 (Sym.)

(2.41)

The symmetrical matrix of Eq. (2.41) is used to represent the elastic compliance and stiffness moduli as well as the many properties involving these moduli. The inherent symmetry expressed by Tmn = Tnm results solely from thermodynamic arguments that are presented in Section 4.4. Property tensors with tensor rank greater than four are not as common as some of those of lesser tensor rank. Nevertheless, a few fifth- and sixth-rank tensor properties have either been measured experimentally or have been predicted to exist on theoretical grounds. Examples are the fifth-rank piezoelectro-optical, piezomagneto-optical, and sixth-rank quadratic piezo-optical effects mentioned in Section 7.3.2 and the quadratic piezothermoelectric power and quadratic piezo-

introduction to tensor and matrix representation 25

TABLE 2.1: The transformation laws for polar tensors up through the rank 4 showing tensor rank, tensor subscript notation, matrix symbolic notation, and the referred matrix text equation. Transformation law Rank

Tensor subscript notation

Matrix symbolic notation

Referred matrix equation

0

T ′ = T

—

—

1

T ′i = aijTj

T ′ = at

(2.8)

2

T ′ij = aikajlTkl

T ′ = aT a~

(2.13)

3

T ′ijk = ail ajmaknTlmn

T ′ = aTα −1

(2.31)

4

T ′ijkl = aim ajnakoalpTmnop

T ′ = αTα −1

(2.35)

resistance effects represented in Eqs. (9.26) and (9.38), respectively, both of which are sixth-rank tensor properties.

2.2.8 Summary of Tensor Transformation Laws For the convenience of the reader, Table 2.1 summarizes the transformation laws for polar tensors up through rank 4 that exhibit some inherent symmetry. The transformation equations are given in both tensor subscript form, where summation over the dummy (repeating) subscripts is understood, and in conformable matrix symbolic form, the latter being derived from equations of the form p = Tq. The transformation equations for the fifth- and sixth-rank tensor properties mentioned above will be left as additional exercises for the reader. In the matrix equations, use is made of the quadratic transformation matrix α, which assumes a) some inherent symmetry for a given tensor T and b) that the first and third forms in the column matrices of Eqs. (2.20) are equated. If no inherent symmetry exists in T, the matrix forms of the transformation laws in Table 2.1 may still be used but with the α matrix replaced by the more general β transformation form given in Eq. (9.31) applicable to asymmetrical second-rank tensors.

2.3

INTRODUCTION TO TENSOR ALGEBRA

Up to this point, we have made some use of tensor algebra without specific mention of the laws involved. We will now review various standard operations involving tensor addition and multiplication

26 tensor properties of solids

with some exceptions. The subjects of axial tensors, tensor differentiation, tensor field subject matter, and the vector cross product will be reviewed later in Sections 2.4, 2.5, and 2.6, respectively.

2.3.1 Tensor Addition The addition (or subtraction) of corresponding components of two or more tensors all having the same tensor rank yields a resultant tensor of the same rank. As an example, consider adding components of two symmetrical second-rank polar tensors A and B expressed in both tensor subscript and symbolic matrix notation:

Rij = Aij + Bij or R = A + B

This requires that R11 = A11 + B11, R22 = A22 + B22 , … R12 = A12 + B12 for all six independent components of the resultant matrix R. The sum rule may be generalized by the equation

Rijk... = Aijk... + Bijk... + ... ,

(2.42)

which is restricted to components of tensors having the same rank and tensor character. The sum rule obeys the commutative, associative, and distributive laws of additions well-known in Cartesian algebra.

2.3.2 Tensor Multiplication For the reader’s convenience and by using the symbol ⊗ to represent the outer and inner product operations, we review the following tensor multiplication laws best illustrated by using conformable matrix forms: Cumulative law A⊗B=B⊗A Associative law A ⊗ (B ⊗ C) = (A ⊗ B) ⊗ C Distributive law A ⊗ (B + C) = A ⊗ B + A ⊗ C

(2.43)

These laws are written in the order of increasing extent to which they are obeyed by the tensor multiplication operations. Generally speaking, the distributive law is always obeyed if the sum rule is obeyed, the associative law is obeyed if the permutation tensor is not involved, and the commutative law is never obeyed except for scalar products. The tensor representation of the vector cross product and the properties of the Kronecker delta and permutation tensor will be reviewed later in Section 2.6.3.

introduction to tensor and matrix representation 27

2.3.3 Outer Product The product of two tensors AB that yields a resultant tensor of tensor rank equal to the sum of the tensor ranks of A and B (rA + rB) is called the outer product or dyadic product of A and B. For example, the outer product of a vector Ai and a symmetrical second-rank tensor Bjk yields a tensor of thirdrank Rijk. That is, Rijk = Ai Bjk (i, j, k = 1 − 3)

or

Rim = Ai Bm (i = 1 − 3; m = 1 − 6).

(2.44)

The expanded matrix form of Eq. (2.44) yields a (3 × 6) AB matrix given by A1B1 A1B2 A1B3 A1B4 A1B5 A1B6 A2B1 A2B2 A2B3 A2B4 A2B5 A2B6 . A3B1 A3B2 A3B3 A3B4 A3B5 A3B6

A1 R = A2 . [B1 B2 B3 B4 B5 B6 ] = A3

~ Note that if B ¹ B , then the product AB yields a (3 × 9) matrix. The outer product rule can be generalized by the tensor subscript equation

Rijk...opq... = Aijk...Bopq...,

(2.45)

where R has a tensor rank equal to the sum of the ranks of A and B, that is, rR = rA + rB , a fact that is lost in the use of symbolic matrix notation R = AB.

2.3.4 Tensor Contraction When a single subscript in the product or two tensors of the same rank r are set equal, a single contraction results producing a tensor of rank (r − 2). The product of two tensors of arbitrary rank results in tensor contraction called the inner product and is generalized in tensor subscript notation as

R...ijlm = A...ijkBklm...

(2.46)

or R = A⋅B in tensor symbolic notation. Here, R is a tensor of rank rR = (rA + rB) − 2 having the same tensor character as that of A and B. As an example, consider the single contraction (inner) product of a polar vector and a partially symmetrical third-rank polar tensor (Bijk = Bikj) given by

28 tensor properties of solids

Rjk = Ai Bijk (i, j, k = 1 − 3)

or

Rm = Ai Bim (i = 1 − 3; m = 1 − 6)

In expanded matrix form, this becomes B16 B26 = [R1 R2 R3 R4 R5 R6 ], B36

B15 B25 B35

R = [A1 A2

B11 B12 B13 B14 A3 ] . B21 B22 B23 B24 B31 B32 B33 B34

which yields the components of symmetrical polar second-rank tensor R in the form of a (1 × 6) matrix. Double contraction results when two subscripts in the product of two tensors of the same rank r are set equal, producing a tensor of rank r − 4. The double contraction product of two tensors of arbitrary tensor rank is generalized in tensor subscript notation as

R...hk... = A...hij Bijk...

(2.47)

or R = A ⋅ B in tensor symbolic notation. Here, R is a tensor of rank rR = (rA + rB) − 4 having the same tensor character as that of the A and B combination. An example of double contraction is

Rij = Aijkl Bkl (i, j, k, l = 1 − 3),

(2.48)

which was used in Eq. (2.33) to represent a polar fourth-rank that relates two polar second-rank tensors. Tensor contraction continues through triple, quadruple, etc. contractions and becomes complete when the product of two tensors of the same rank yields a scalar. This product is called the scalar product, which is generalized as

R = Aijk... Bijk... = tr (AB)

(2.49)

called the trace of AB. An example is the scalar product of two symmetrical second-rank tensors,

R = Aij Bij ,

introduction to tensor and matrix representation 29

represented in matrix form as the scalar product

= A1B1 + A2B2 + A3B3 + A4B4+ A5B5 + A6B6

2.4

R = [ A1 A2 A3 A4 A5

B1 B2 B A6] 3 = tr(AB) B4 B5 B6 (2.50)

AXIAL TENSORS

The tensors discussed so far have been polar tensors that transform, such that the sign of their components is unaltered by a transformation that changes the handedness of the coordinate axes. Table 2.1 gives the transformation laws for polar tensors. Tensors having components that change sign when the handedness of the coordinate axes is changed by a transformation are called axial tensors or pseudo tensors. To generalize, axial tensors transform according to T ′ijk... = | a |aimajnako...Tmno... .

(2.51)

Here, for example, the “handedness” factor | a | for a second-rank tensor is the determinant of the transformation matrix (aij ) given symbolically by

| |

a b c |a | = d e f = a . e f − b . d f + c . d e g h g i h i g h i

| |

| | | | | |

e f where, for example, = ei − f h. Thus, | a | = - 1 for a transformation that changes the handedh i ness of the axes, and | a | = 1 if the handedness is left unchanged by the transformation. Table 2.1 for polar tensor transformations applies to axial tensors if the handedness factor | a | = ± 1 is included on the right-hand side of each transformation law. For a scalar, the transformation law becomes T ′ = | a |T. An example of an axial (pseudo)-scalar is the optical rotatory power, ρ. Vectors, such as magnetic field strength, magnetic flux density, and magnetization, are both axial and magnetic in character. As a second example, the Hall tensor Rijk is both antisymmetrical (in subscripts j,k or i,k)

30 tensor properties of solids

and axial–magnetic but which can be represented as a polar–magnetic second-rank tensor as discussed in Section 10.3. The reader must be aware of the fact that axial tensors and antisymmetrical tensors are two entirely different tensor characteristics the distinction of which will be made evident in Section 2.6.3. Magnetic tensor character is discussed in Appendix A.

2.5

TAYLOR’S SERIES EXPANSION AND THE TENSOR DIFFERENTIATION LAWS

Taylor’s series is a type of power series used to express a given function of one or more variables by means of a polynomial in the neighborhood where the function is regular (analytic). A valid Taylor’s series expansion requires that the series be convergent within a finite interval and that all derivatives (or partial derivatives) of the function be continuous in that interval. For the general case of multivariable tensor functions, the Taylor’s series expansion is given symbolically by

∞ 1 ∂ 0 ∂ 0 ∂ 0 f (P, Q , R ...) = ∑ kl j n! (Pi − Pi ) ∂Pi + (Qj − Qj ∂Qj + (Rkl − R kl )∂Rkl +... i n=0

n

f (Pi0, Qj0 , Rkl0 ...), (2.52)

(

where n = 1, 2, 3, ... is an integer and f (P i0, Q 0j , Rk l0 ...) signifies that after the function is operated on, the resulting coefficients are evaluated at the reference values of Pi = Pi0, Qj = Q j0, Rkl = Rk l0 , and so forth. Because the function f may itself be a tensor quantity of arbitrary tensor rank, the resulting coefficients are tensors given in accordance with the tensor differentiation laws

T...ijkl ...

C,D,...

2

,U...ijkl ...rs...

∂ A...ij . . . , et = ∂Bkl... ∂Crs... D,E,...

∂ A...ij = ∂Bkl...

(2.53)

Here, the law expressed by T...ijkl... implies that all remaining components of B and all components of C, D, and so forth are held constant and that T...ijkl... has the tensor rank rA + rB and the combined tensor character of A and B. The law expressed by U...ijkl...rs... for a second-order derivative implies that U has a tensor rank of rA + rB + rC with the combined tensor character of A, B, and C, where it is understood that the remaining components of B and C and all components of D, E, and so forth are held constant. Notice that our rule of subscript order is read from top-to-bottom–left-to-right. However, because other subscript order schemes can be found in literature, care must be taken to recognize which scheme is used.

introduction to tensor and matrix representation 31

As an example of the use of Eq. (2.53), let the electric polarization Pi be a function of electrical field strength Ej and stress σkl and let Pi (Ej , σkl ) be expanded in a Maclaurin series (special case of a Taylor series) about the state of zero electric field and zero stress to give 1 ∂ Pj(Ej, σkl ) = σ ∂ E n! j Ej + σ n=0

∑

∞

n

Pi (0,0),

(2.54)

giving the result 2 ∂ Pi σ kl + 1 ∂ E ∂E 2! j m (0,0)

∂2Pi Ej σkl + ∂ σ ∂σ kl n o (0,0)

(0,0)

Ej Em

(0,0)

∂2Pi ∂ Ej ∂ σkl

+2

∂P Ej + i ∂ σ kl (0,0)

∂P Pj(Ej, σ kl ) = Pi (0,0) + i ∂Ej

σ kl σn o + ...

As will be shown in later chapters, the various coefficients (in parentheses) define certain tensor properties. For example, κ 0−1(∂Pi / ∂Ej ) = χij is the dielectric susceptibility tensor for a crystal and κ 0 is the permittivity in a vacuum. The quantity (∂Pi / ∂σkl) = dikl is the piezoelectric tensor. Here, both χij and dikl are first-order (n = 1) effects evaluated, in this case, at zero electric field and zero stress. The three properties given within the square brackets are second-order (n = 2) effects and are represented by third-, fourth-, and fifth-rank tensors also evaluated at zero electric field and zero stress. Note that had the expansion in Eq. (2.54) also been taken about the state of reference temperature T 0, it would be called a Taylor’s series—hence, the basic distinction between a Maclaurin’s series and a Taylor’s series.

2.6

TENSOR FIELDS AND TENSOR OPERATORS

For purposes of this section, we will use the symbol ψ to represents a Cartesian tensor field of rank r in a region R and specified by 3(r) continuous functions of position ψijk... (x1, x2, x3) or simply ψijk...(x). We will cover only the tensor gradient and divergence, Kronecker delta, permutation tensor, vector cross product, and tensorial contraction because these will be used later in both Parts I and Part II of this text. Other related subjects such as Stoke’s theorem and Green’s theorem in a plane and their application to thermodynamics will be discussed in sufficient detail as they become needed in later developments. The curl of a tensor will be left to further reading (see Endnotes).

32 tensor properties of solids

2.6.1 Gradient of a Tensor Field The components of a field tensor of rank r can be differentiated with respect to the coordinates of a point, resulting in a tensor of rank r + n, where n is the order of the differential operator used. One can generalize the tensor gradient as the outer product of two tensors, a field tensor ψijk...(x) of rank r and the nth-order operator ∂pst... of rank n. That is,

∂ψijk ... Tijk ... pst = ∂pst ...ψijk ... = ∂xp∂xs∂xt ...

(2.55)

written as T = gradψ = ∇ψ in tensor symbolic notation. Here, T transforms as a tensor of rank r + n and is represented by 3(r + n) continuous functions of position T (x) in Cartesian space. Note that Eq. (2.55) has been written by using the rule of subscript order given in Section 2.5. The simplest application of Eq. (2.55), and one in which we are particularly interested, is the gradient of a scalar field. If the scalar field is represented by φ, then its gradient is a Cartesian vector having components given as

∂φ ∂φ ∂φ ∂i φ = x , x , x 1 2 3

(2.56)

or written as gradφ = ∇φ in vector symbolic notation. See Eq. (8.1) in Chapter 8 as an example. The gradient of a scalar points in the direction of the maximum rate of change and that has a magnitude equal to that maximum rate of change. Examples of a scalar field are the electrostatic potential (or voltage), chemical potential, and temperature. Thus, the gradient of any scalar field is always from low to high potential as, for example, from low to high temperature. Thus, Fourier’s law requires that the heat must flow from high to low temperature in a direction opposite to the temperature gradient, hence, the minus sign in Eq. (8.7) presented in Part II of this text. Application of Eq. (2.55) to the field vector ψi(x) results in the asymmetrical dyadic ∂jψi = ∂ψi /∂xj called the vector gradient of the given field with components given by a 3 × 3 Jacobian matrix,

∂1ψ1 / ∂x1 ∂1ψ1 / ∂x2 ∂1ψ1 / ∂x3 = ∂2ψ2 / ∂x1 ∂2ψ2 / ∂x2 ∂2ψ2 / ∂x3 /∂ / / ∂3ψ3 ∂x1 ∂3ψ3 ∂x2 ∂3ψ3 x3

∂ψi Tij = ∂xj

(2.57)

We will have no further need to apply Eq. (2.55) to tensor fields of tensor rank greater than r = 1.

introduction to tensor and matrix representation 33

2.6.2 Divergence of a Tensor Field The divergence of a tensor can be generalized by the single-contraction product of a field tensor ψijk...(x) of rank r with the vector operator ∂i yielding a tensor of rank r − 1 given by Tjk ... = ∂iψijk ... =

∂ψijk...

∂xi

(2.58)

or as T = divψ = ∇.ψ in tensor symbolic notation. Contraction can be carried out on any of the indices of ψijk...(x), but the results will, in general, be different. A physical interpretation of Eq. (2.58) is reasonably straightforward. The divergence of a tensor gives at each point the rate per unit volume at which the physical entity represented by ψ is issuing from that volume. The divergence theorem (also known as Gauss’ theorem) is widely used and provides the integral definition of divergence of a tensor field given by ο∫ dS .ψ divψ ≡ lim s ∆V→0 ∆V

(2.59)

where o∫ sdS.ψ is called the net flux of ψ out of S. Thus, Eq. (2.59) defines the divergence of a tensor field at a point P in V as the limiting value of the flux of ψ per unit volume out of S when ∆V →0. The simplest example is the divergence of a vector field ψi(x) equal to a scalar ∂iψi having magnitude

∂i ψi =

∂ψ1 ∂ψ2 ∂ψ3 + = tr(∂jψi ), + ∂ x1 ∂ x2 ∂ x3

(2.60)

which is equal to the trace of the vector gradient in Eq. (2.57). A well-known example of the application of Eq. (2.60) is the steady state in a thermoelectric system when the divergence of the energy flux vanishes, that is, ∇.J u = 0. This means that the heat energy emitted to the surroundings, say, by Joule (I 2R-type) heating in a volume element must be exactly balanced by the heat energy absorbed by that volume element from the surroundings.

2.6.3 Kronecker Delta, Permutation Tensor, Vector Cross Product, and Tensorial Contraction The Kronecker delta is defined by

0 0 1

0 1 0

or

δ 11 δ 12 δ 13 1 [δij ] = δ 21 δ 22 δ23 = 0 0 δ 31 δ 32 δ33

1 if i = j δij = 0 if i ≠ j

(2.61)

34 tensor properties of solids

Now, if Ti is the ith component of a vector, then with the definitions of Eqs. (2.61), there results the expressions δij Ti = Tj and δij Tj = Ti , or for a tensor Tjk , there results δij Tjk = Tik and δij Tik = Tjk . All express the substitution property of the Kronecker delta, which will be used in Section 9.3 of this text. The permutation tensor eijk (also called the Levi–Civita tensor, alternating tensor, or e-tensor) is an antisymmetrical, axial, third-rank tensor defined by

+ 1 if ijk is an even permutation of 123

eijk ≡ − 1 if ijk is an odd permutation of 123 0 if any two subscripts are the same

→

→

(2.62)

→

A common application of eijk is the vector cross product or R = B × C described by the equation given in tensor notation Ri = eijk BjCk (i, j, k, = 1, 2, 3)

(2.63)

The three components of Ri are readily found by expansion of Eq. (2.63) or by using the matrix form

R1 R2 R 3

B1C1 B2C2 B3C3 B2C3 − B3C2 0 0 0 1 0 0 −1 0 0 B2C3 0 0 1 0 −1 0 B2C1 = B3C1 − B1C3 = 0 0 0 1 0 0 0 −1 B1C2 0 0 0 0 B1C2 − B2C1 B3C2 B1C3 B2C1

(2.64)

Equations in (2.64) can be represented simply by R = e(BC) in matrix symbolic notation, where the dyadic product (BC) has been unfolded as the 9 × 1 form of Tij in Eq. (2.3). The top row of the [3 × 9] matrix is unfolded as 111, 122, 133, 123, 131, 112, 132, 113, 121, then 211, 222, 233, 223, 231, 212, 232, 213, 221 for the second row, and 311, 322, 333, 323, 331, 312, 332, 313, 321 for the third row. The difference between the antisymmetrical and axial character of a tensor is nicely described in terms of the e-tensor. The permutation tensor has been described as antisymmetrical. This is true by virtue of the fact that if any two subscripts of the component eijk are set equal, the component becomes zero—the antisymmetrical property. The e-tensor is also axial due to the fact that if any two subscripts are interchanged, which is equivalent to reversing the handedness of the axes, the

introduction to tensor and matrix representation 35

value of the e-tensor changes sign, 1 to −1, or vice versa. These special features of the e-tensor will be useful in dealing with the magneto-optical and galvanomagnetic effects discussed in Sections 7.3.4 and 10.2. A generalization of the single contraction product involving eijk without restriction on tensor rank and character is given by

Ajklm ... = eijk Tilm ...

(2.65)

or simply by A = e . T in tensor symbolic notation. This equation states that a tensor T of rank r can be represented by its dual A of rank r + 1. Here, A has the combined tensor character of e and T but retains the physical properties of T. Thus, if T represents an axial second-rank tensor (e.g., the magnetoelectric susceptibility discussed in Section 4.5, then A must be an antisymmetrical (nonaxial) tensor with the physical properties of T. A common application of Eq. (2.65) is the case where an axial vector is converted to an antisymmetrical second-rank tensor given by

Ajk = eijk Ri

(2.66)

A generalization of double contraction product involving eijk can be represented, with certain restrictions to tensors of arbitrary tensor rank and character, by the equation

Ailm ... = eijk Tjklm ...

(2.67)

or simply by A = e : T in tensor symbolic notation. Here, the tensor rank of A is r − 1 when the tensor rank of T is r. The restrictions imposed on Eq. (2.67) are simply that tensor T must be of secondrank or higher and that it must be antisymmetrical in j and k if it is necessary that all components of ~ T be retained by A in the conversion. Thus, as an example, eijk Sjk = 0 if S = S . As a second example, the reverse conversion to Eq. (2.66) permits an antisymmetrical second-rank tensor to be converted to an axial vector expressed as

Ri = eijk Ajk

(2.68)

Or, as a third example, if T is an antisymmetrical third-rank tensor in j,k only but is also axial, then A must be a polar (true) second-rank tensor as expressed by

Ail = eijk Tjkl

(2.69)

Here, A is said to be the dual of T. Equation (2.69) will find use in Section 10.3 when dealing with the Hall tensor.

36 tensor properties of solids

Further tensorial contraction using the permutation tensor is possible by highly restricted. A → → → common example is the triple scalar product V = a × b . c , which represents the volume of a general → → → parallelepiped of sides a , b , c In tensor notation, this scalar product is simply written as V = eijk ai bj ck

(2.70)

Thus, V does not transform as a simple scalar but rather as a pseudo (axial) scalar according to V ′ = aV. αβγ = eαβγeijk = ∆K is given by the matrix The generalized Kronecker delta denoted by δijk

δα i δα j δαk ∆ = δβi δβ j δβk δγ i δγ j δγk K

(2.71)

such that the contraction products follow Section 2.3.4, leading to the matrix for triple contraction given by ee~ = 2tr(ee~) = 6 as used in Section 7.3.4. • • • •

37

chapter 3

Crystal Systems, Symmetry Elements, and Symmetry Transformations 3.1

INTRODUCTION

In the previous chapter, it was shown that the possession of inherent symmetry by a tensor of rank r had the effect of reducing the number of independent components representing it from 3(r) to some number that was determined by the number of indices that could be interchanged. In this section, we will discuss certain additional limitations placed on the relationships between the components of a tensor property by the structural symmetry of the crystal within which the property is manifest. Remember, however, that not all tensors are affected by crystal symmetry. Second-rank field tensors such as stress and strain possess certain intrinsic symmetry, but their components are unaffected by the symmetry of the crystal. On the other hand, property tensors, which may relate two or more field tensors and hence possess their intrinsic symmetry, will also acquire the symmetry of the crystal within which the property is evinced. Thus, property tensors may possess a higher symmetry than that possessed by the crystal. When the components representing a given property tensor vary with crystallographic direction, the crystal is said to be anisotropic with respect to that property. Conversely, if the components of a given property tensor are invariant with crystallographic direction, the crystal is said to be isotropic with respect to that particular property. A crystal may possess partial isotropy with respect to a given property if, for example, the components of the property are invariant with direction in a particular crystallographic plane but vary with direction out of that plane. The term crystal symmetry, as used above, refers not to the atomic structure but to the morphology or macroscopic symmetry of the crystal. During the natural growth of some crystals, the planes of highest atomic density have a propensity to form the external faces of the crystal. A naturally occurring quartz crystal is a good example. The special relationship between these faces produces a symmetry that forms the basis of classification of crystals into 32 conventional symmetry classes called point groups. Thus, each of the 32 point groups defines a symmetry class. It is the point group symmetry (i.e., macroscopic symmetry) of a crystal that imposes certain limitations on the relationships between different components of a macroscopic tensor property. For magnetic

38 tensor properties of solids

crystals, the atomic magnetic spin moments, viewed collectively over the crystal, become important in symmetry considerations. This leads to the formation of the 90 magnetic point groups. There are, however, certain microscopic symmetry elements that take place at the atomic level and that are not possible in a point group, conventional or magnetic. Several symmetry operations at the atomic level are used to classify the microscopic symmetry elements in a three-dimensional space lattice, and these are called a space group. There are 230 conventional space groups and 1651 magnetocrystalline space groups, and every crystal must belong to one or more of these groups. We will not further consider space groups, conventional or magnetic, since they fall outside the scope of this text.

3.2

MACROSCOPIC CRYSTAL SYMMETRY AND SYMMETRY TRANSFORMATIONS

There are two fundamental macroscopic symmetry operations that can be performed at a point to generate all 32 point groups representing the 32 crystal classes. These two operations are rotation and center of symmetry. We will consider these in some detail along with the appropriate symmetry transforms and then develop the symbology used to designate the 32 point groups.

3.2.1 Permissible Rotations When a perfect crystal can be brought into congruence with itself by a rotation about an axis, it is said to possess a proper rotation axis of symmetry. One-, two-, three-, four-, and sixfold rotation axes are permissible as expressed by φ = 2π / n, where n = 1, 2, 3, 4, or 6. These permissible rotations are presented in Table 3.1 and are often referred to as monad, diad, triad, tetrad, and hexad axes of rotation, respectively. Rotations for n = 5, 7, ... are not permissible.

3.2.2 Center of Symmetry Taking the origin of coordinates as the center of symmetry, this operation consists of moving each point (x, y, z) to a position (−x, −y, −z) as shown in Figure 3.1. This represents an inversion of axes through the origin of coordinates and is expressed by the transformation matrix (aij) = −(δij), where (δij ) is the unitary matrix. Note that in tensor subscript notation, δij is called the Kronecker delta previously discussed in Section 2.6.3.

TABLE 3.1: Permissible rotations to bring a perfect crystal into self-congruence n

1

2

3

4

6

Rotation, φ = 2π / n

φ = 360°

φ = 180°

φ = 120°

φ = 90°

φ = 60°

Crystal Systems, Symmetry Elements, and Symmetry Transformations 39

x3 z -y

x

x1

-x x2

y -z

FIGURE 3.1: Coordinate axes showing a center of symmetry.

The two operations, an n-fold proper rotation and a center of symmetry, may be combined to produce rotoinversion axes designated by x¯= 1¯, 2¯, 3¯, 4¯, or ¯6. The rotoinversion operation is one of n-fold rotation followed by inversion through a center of coordinates. If the transformation matrices for these two operations are a1 and a2 (= −δij), respectively, then the resultant transformation matrix is a = a2a1 = (−δij)a1 = −a1. A twofold rotoinversion axis of symmetry, ¯2 , is identical to a reflection across a mirror plane (sometimes called a plane of symmetry) lying perpendicular to the ¯2 axis. This is illustrated in Figure 3.2, where the symbol commonly used to designate a plane of symmetry is m ( = 2¯ ). As an example, the rotoinversion transformation matrix representing a reflection across the mirror plane x1, x2 is

180o

Mirror Plane End

FIGURE 3.2: Graphical illustration of a twofold rotoinversion axis of symmetry.

0 1 0

0 0 , −1

Begin

0 1 0 = 0 1 0

0 −1 0 0 −1 0 0 −1 0 = 0 −1 0 0 0 −1 0 1 0

−1 0 0 −1 0 0

a = −( δij )

(3.1)

40 tensor properties of solids

which is obvious from an inspection of Figure 3.2. Here, the first and second matrices represent a center of symmetry and a 180° rotation about the 0x3 axis, respectively—the order is immaterial. Remember that the entries (1’s, −1's, and 0's in this case) in a transformation matrix represent the direction cosines as illustrated in Figure 2.1. Other combinations of the two fundamental symmetry elements are possible and are designated by certain symbology. An n-fold rotoinversion axis lying in a plane of symmetry is designated − as X m = n¯m. An n-fold rotation axis of symmetry perpendicular to a plane of symmetry is designated as X/m = n/m. As an example, consider a fourfold rotation axis of symmetry about 0x3 lying normal to the x1, x2 plane of symmetry. This symmetry operation designated as 4/m(= 42¯), has a transformation matrix

0 0 , −1

0 0 1 0 = −1 0 1 0 0

1 0 0

0 0 0 −1 −1 0

0 1 0

1 a= 0 0

(3.2)

TABLE 3.2: Symmetry transformation symbology used to identify the 32 point groups X

An n-fold rotation axis of symmetry

− X

An n-fold rotoinversion axis of symmetry

m

Plane of symmetry or mirror plane

X/m

Rotation axis with one mirror plane normal to it

X2

Rotation axis with a diad normal to it

− X 2

Rotoinversion axis with a diad normal to it

Xm

Rotation axis with one mirror plane parallel to it

− Xm

Rotoinversion axis with one mirror plane parallel to it

Xmm

Rotation axis with one mirror plane parallel to it*

X/mmm

Rotation axis with one mirror plane normal to it and one mirror plane parallel to it*

* The last element in three- and four-element forms such as Xmm and X/mmm is usually unnecessary to generate the group (see Table 3.6 for examples).

Crystal Systems, Symmetry Elements, and Symmetry Transformations 41

and the 4/m point group would be generated by repeated operations represented by the above transformation matrix product. The symbology used to identify the 32 point groups is presented in Table 3.2, where X and n are interchangeable, and all rotations are taken to be CCW (positive rotations).

3.3

SPACE LATTICES, UNIT CELLS, CRYSTALLOGRAPHIC PLANES, AND DIRECTIONS—MILLER INDICES

A crystal is defined as a special arrangement of atoms that repeats itself periodically in three dimensions. If this periodicity is precise and if it is continuous ad infinitum, the crystal is said to be perfect. Of course, real crystals cannot be perfect because they have finite bounds (free surfaces) and contain internal imperfections such as impurities, vacancies, dislocations, and usually subboundaries. We will treat crystals as being of finite dimensions but without internal defects. The atomic arrangement in a crystal is conveniently represented as a three-dimensional network of straight lines called a space lattice. The intersections of lines are points of the space lattice that may represent the residence of a single atom or a group of atoms distributed in some fashion about the point. There are 14 space lattices called Bravais lattices into which all crystal structures must fall. Each space lattice has some convenient set of axes that is conventionally used with it. Six different systems of axes are commonly used in crystallography. Each set of lattice axes 0x, 0y, 0z → → → represents the directions along which the primitive translation vectors a , b , c lie as illustrated in Figure 3.3. The six different systems of axes define the six crystal systems into which fall the 14 Bravais lattices and hence all the crystal structures possible. These are presented in Table 3.3 together with the unit cell axes and angles, the lattice symbols, and the minimum symmetry elements required for

z

c β

a

α

b

y

γ

x FIGURE 3.3: General space lattice showing the primitive translation vectors and angles.

42 tensor properties of solids

membership in each system. The lattice symbols P, F, I, C, and R are the Hermann–Mauguin notation for primitive (P), face-centered (F), body-centered (I), base-centered (C), and rhombohedral (R) unit cells. Thus, a given crystal system may exist as more than one Bravais lattice. For example, the orthorhombic crystal system exists in primitive, face-centered, body-centered, and base-centered crystal structures. The space lattice is then generated by the translation vector →

→

→

→

T = ma + pb + q c ,

(3.3)

where m, p, and q are integers. The totality of all such translation operations for all values of m, p, and q is called the translation group of the crystal. The magnitudes (a, b, and c) of primitive transla→ → → tion vectors a , b , c are called the lattice parameters, which, together with the lattice angles (α, β, γ ), define the unit cell of a crystal. Before continuing with the subject of macroscopic crystal symmetry elements and symmetry transformations, it will be instructive to review the notation for describing crystallographic planes and directions. Shown in Figure 3.4 are the generalized Miller and Miller–Bravais indices for planes and directions for the six crystal systems in Table 3.3 where the hexagonal and trigonal systems are treated together. Here, referring to Figure 3.4(a), the Miller indices for the plane (hkl ) are the reciprocals of the intercepts (1 / ix , 1 / iy , 1 / iz ). For example, if the intercepts are (ix = 1, iy = 1, iz = 1), then

z

z

(hkl) Plane

iz

ix x

(a) Miller Indices for all crystal systems

[UVTW]

y'

[uvw] Direction

iy

(hkil) Plane

y

Direction

120o

x

o

12 0

y

(b) Miller-Bravais indices for hexagonal and trigonal crystal systems

FIGURE 3.4: Notation for description of planes and directions showing Miller indices for all crystal systems and the Miller–Bravais indices for the hexagonal and trigonal crystal systems.

Crystal Systems, Symmetry Elements, and Symmetry Transformations 43

TABLE 3.3: The 14 Bravais lattices showing the conventional unit cell axes and angles together with their lattice symbols and minimum symmetry elements Crystal system

Unit cell axes and angles

Lattice symbols

Minimum symmetry elements

Triclinic

a ≠ b ≠ c ; α ≠ β ≠ γ

P

1 (or ¯ 1 )

Monoclinic

a ≠ b ≠ c ; α = γ = 90° ≠ β

P, C

2 (or ¯ 2 )

Orthorhombic

a ≠ b ≠ c ; α = β = γ = 90°

P, F, I, C

222 (or ¯ 2 2¯ 2¯)

Tetragonal

a = b ≠ c ; α = β = γ = 90°

P, I

4 (or 4¯ )

Trigonal and

a = b ≠ c ; α = β = 90°; γ = 120°

R, P

3 (or ¯ 3 ); 6 (or ¯ 6 )

a = b = c ; α = β = γ = 90°

P, F, I

4 triads along

hexagonal Cubic

taking the reciprocals of the intercepts gives (111) for the plane. As a second example, if the intercepts are (ix = 1, iy = 1/2, iz = 1/3) along axes 0x, 0y, and 0z, respectively, then the Miller indices for the plane would be (1, 2, 3). For the hexagonal and trigonal crystal systems represented in Figure 3.4(b), the i index in (hkil ) is determined by i = −(h + k) but is sometimes replaced by a dot as (hk.l ). The Miller indices for direction [uvw] are found by “walking” along all axes, x, y, and z in turn, from origin to the end of the lattice vector. Referring to Figure 3.3, one would measure distances along x, y, and z axes in units of a, b, and c, respectively, or their fractions. As an example, and again referring to Figure 3.3, a lattice vector represented by a, b, c would be designated by [111], or a lattice vector (1/2)a, −b, 0 in the x–y plane would be designated as [1/2, 1¯, 0] or clearing fractions [1, 2¯ , 0]. Referring to Figure 3.4(b), the same direction in the hexagonal and trigonal systems would be designated as [UVTW ] = [1, ¯2 , 1, 0], where T = −(U + V ). In the cubic system, for which a = b = c, any direction [uvw] is perpendicular to the plane (hkl ) of the same indices. Planes of the form are designated as {hkl} and {hkil }, whereas the directions of the form are indicated as 〈uvw〉 and 〈UVTW 〉. The four index forms apply specifically to the hexagonal and trigonal systems. The number of non-parallel planes of the form {hkl } is found by multiplying [permutation term] × [sign term]/2. For example {123} has [3!][23]/2 = 24 non-parallel planes of this form. Directions of the form 〈123〉 also have 24 nonparallel directions of that form.

44 tensor properties of solids

TABLE 3.4: The 32 conventional point groups showing crystal system, group number, and the international short symmetry notation Crystal system

Group number

International (short) notation

Triclinic

1

1

2

|| ¯1 ||

3

2

4

m

5

|| 2/m ||

6

222

7

mm2

8

||mmm||

9

4

10

4¯

11

|| 4 /m ||

12

422

13

4mm

14

4¯ 2m

15

|| 4 /mmm ||

Monoclinic

Orthorhombic

Tetragonal

Crystal Systems, Symmetry Elements, and Symmetry Transformations 45

TABLE 3.4: (continued) Crystal system

Group number

International (short) notation

Trigonal (rhombohedral)

16

3

17

|| 3¯ ||

18

32

19

3m

20

|| 3¯m ||

21

6

22

6¯

23

|| 6/m ||

24

622

25

6mm

26

¯6 m2

27

|| 6/mmm ||

28

23

29

|| m3 ||

30

432

31

4¯ 3m

32

|| m3m ||

Hexagonal

Cubic (isometric)

46 tensor properties of solids

3.4

THE MACROSCOPIC SYMMETRY OF CRYSTALS AND THE 32 CONVENTIONAL POINT GROUPS

The 32 conventional point groups are listed in Table 3.4 in the order of increasing symmetry. The symbols used to represent the symmetry elements characteristic of each crystal class belong to the Hermann–Mauguin international short system. There are two other systems used for this purpose. They are the full symbol notation and Schoenflies symbols; neither of which will be used in this text. The 11 point groups, designated by the symbol || X || in the seven crystal systems, each possess a center of symmetry and meet the requirements for complete (maximum) symmetry allowable for classification in that system. These 11 point groups are called the holohedral groups. Finally, it should be noted that a given point group is generated by the repeated symmetry operations required by the elements of that group. This fact will be important in later developments. A point group that contains a center of symmetry is called centrosymmetrical. A group contains a center of symmetry if the product of the transformation matrices, representing the symmetry elements of the group, becomes −(δij ), where (δij ) is the unitary matrix. As an example, the group 2/m has the following transformation matrix

0 cos(pπ) 0

0 0 , 1

0 cos(pπ) 0 0 −1 0

0 1 0

1 0 0

(3.4)

where p is an integer representing the repeated twofold rotation operation and π = 180°. Clearly, cos( pπ) = −1 for p = ±1, ±3, ±5... , and the transformation for 2/m above becomes –(δij), proving that 2/m contains a center of symmetry and is represented by || 2/m || in Table 3.4.

3.5

NEUMANN’S PRINCIPLE AND ITS APPLICATION TO TENSOR PROPERTIES

Basic and most important to a discussion of the effect of crystal symmetry on the tensor properties of crystals is Neumann’s principle, which states, The symmetry elements of any physical property of a crystal must include all the symmetry elements of the point group of the crystal. This means that the component of a tensor representing a property must remain invariant under a transformation of coordinates governed by a symmetry operation valid for the point group of the crystal. Mathematically, this is represented as

Tijk... = Tijk....

(3.5)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 47

TABLE 3.5: The 10 possible generating matrices are shown for both the s and σ forms

0 −1

0

Center of symmetry, −1 0 0 – s (1) = (1 ) = 0 −1 0

Direct inspection method: 1→ −1, 2→ −2, 3→ −3 Twofold CCW rotation about y, −1 0 0 s (2) = (2y) = 0 1 0

0 −1

0

Direct inspection method: 1→ −1, 2→2, 3→ −3 Twofold CCW rotation about z, −1 0 0 (3) s = (2z) = 0 −1 0

1

0

0

Direct inspection method: 1→ −1, 2→ −2, 3→3 Reflection plane ⊥ to x, −1 0 0 (4) s = (m ⊥ x) = 0 1 0

0

1

0

Direct inspection method: 1→ −1, 2→2, 3→3 Reflection plane ⊥ to y, 1 0 0 (5) s = (m ⊥ y) = 0 −1 0 1

0

0

Direct inspection method: 1→1, 2→ −2, 3→3

1 0 0 σ (1) = 0 0 0

0

0

0

0

1

0

0

0

0 1 0 0 0 0 1 0 0 0 0 1 0 0 0 0

0

0 0 =I 0 0 1

~=I σ −1 = σ

I is the identity (unit) matrix

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (2 ) = 0 0 0 −1 0 0 0 0 0 0 1 0 0 0 0 0 0 −1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (3 ) = 0 0 0 −1 0 0 0 0 0 0 −1 0 0 0 0 0 0 1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (4 ) = 0 0 0 1 0 0 0 0 0 0 −1 0 0 0 0 0 0 −1

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (5 ) = 0 0 0 −1 0 0 0 0 0 0 1 0 0 0 0 0 0 −1

~ σ −1 = σ

48 tensor properties of solids

TABLE 3.5: (continued)

0 −1

0

Direct inspection method: 1→1, 2→2, 3→ −3 Threefold CCW rotation about z, −1/2 3/2 0 (7) s = (3z) = − 3/2 −1/2 0

0

1

0

Direct inspection method: not applicable Fourfold CCW rotation about x, 1 0 0 (8) s = (4x) = 0 0 1

0

−1

0

Direct inspection method: 1→1, 2→3, 3→ −2 Fourfold CCW rotation about z, 0 1 0 (9) s = (4z) = −1 0 0

0

1

0

Direct inspection method: 1→2, 2→ −1, 3→3 Cyclic interchange of xi, 0 1 0 s(10) = (3[111] ) = 0 0 1 0

0

1

σ (7) =

1/4

3/4

0

0

0

3/4

1/4

0

0

0

0 0 0 3/4 −

Direct inspection method: 1→2, 2→3, 3→1

0 0 0 3/4

1 0 0 0 −1/2 − 3/2 0 3/2 −1/2 0 0 0

− 3/2 3/2 0 0 0 −1/2

To form σ −1. interchange − 3 and 3

1 0 0 0 0 0 0 0 1 0 0 0 0 1 0 0 0 0 σ (8) = 0 0 0 −1 0 0 0 0 0 0 0 −1 0 0 0 0 1 0

~ σ −1 = σ

0 1 0 0 0 0 1 0 0 0 0 0 0 0 1 0 0 0 σ (9 ) = 0 0 0 0 −1 0 0 0 0 1 0 0 0 0 0 0 0 −1

~ σ −1 = σ

0 1 0 0 0 0 0 1 0 0 1 0 0 0 0 = 0 0 0 0 1 0 0 0 0 0 0 0 0 1 0

~ σ −1 = σ

~ σ −1 = σ

1 0 0 0 0 0 0 1 0 0 0 0 0 0 1 0 0 0 σ (6) = 0 0 0 −1 0 0 0 0 0 0 −1 0 0 0 0 0 0 1

Reflection plane ⊥ to z, 1 0 0 s(6) = (m ⊥ z) = 0 1 0

σ (10)

0

0 0 0 1 0

Crystal Systems, Symmetry Elements, and Symmetry Transformations 49

If, on the other hand, a particular component of a tensor changes sign after such a transformation of coordinates, the component must vanish for that crystal in accordance with Neumann’s principle. Mathematically, this is expressed as

Tijk... = −Tijk... = 0

(3.6)

Application of Neumann’s principle to property tensors requires the use of transformation laws for tensors. The transformation laws for both polar and axial property tensors must be valid for any symmetry operation permissible by a given point group. If s represents a symmetry operator, that is, the transformation matrix of a symmetry operation valid for a particular point group, then the generalized transformation laws become

Tijk... = simsjnsko ...Tmno

(3.7)

Tijk... = |s | simsjnsko ...Tmno

(3.8)

for polar property tensors and

for axial tensors, where |s| is the determinant of the symmetry operator (see Section 2.4). For a given crystal class, there will be as many sets of equations for each property tensor as there are symmetry operations valid for the point group of that class. However, the number of operators derived from these symmetry operations can be reduced considerably to some minimum number required to generate the point group. These are called generation operators, which result from the 10 (s) generating matrices given in Table 3.5. The σ generating matrices are the quadratic forms of the s matrices and are applicable only to symmetrical property tensors as represented by ~ (0)= I are Eq. (2.22) in Section 2.2.5. We note here that s(0) = (1) = (δij), σ (0) = I, and [σ (0)]−1 = σ identity (unit) matrices. The minimum number of generating matrices (derived from the 10 generating matrices in Table 3.5) required for each of the 32 point groups are given in Table 3.6. The point groups are designated by using the international short-form symbology as used in Table 3.4. The generating matrices will be used to determine the nonzero components of a given property tensor as required for a particular point group and in accordance with the appropriate transformation law. The symbol || X || appearing in Table 3.6 is used to designate the holohedral group defined earlier. The minimum generating matrices can also be used to generate the stereograms for the 32 point groups (see Endnotes). The work required for simplifying the components of a given tensor can be greatly reduced by recognizing that a tensor of rank r transforms like the products of r coordinates of a point. For example, the center-of-symmetry operator s(1) = (−δij ) requires that

50 tensor properties of solids

TABLE 3.6: Minimum generating matrices for the 32 point groups showing the 11 centrosymmetrical crystal classes designated by || X || Crystal system Triclinic

Monoclinic

Orthorhombic

Tetragonal

International Minimum symbol generating (short form) matrices 1

s(0)

|| 1¯ ||

s(1)

2

s(2)

m

s(5)

|| 2/m ||

s(2), s(5)

222

s(2), s(3)

mm2

s(3), s(5)

|| mmm ||

s(4), s(5), s(6)

4

s(9)

4¯

s(11)

|| 4/m ||

s(6), s(9)

422

s(12), s(9)

4mm

s(4), s(9)

¯4 2m

s(12), s(11)

|| 4/mmm ||

s(4), s(6), s(9)

(4 ¯ z) = s(1) . s(9) = s(11), (2x) = s(1) . s(4) = s(12)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 51

TABLE 3.6: (continued) Crystal system Trigonal

Hexagonal

Cubic

International Minimum symbol generating (short form) matrices 3

s(7)

|| 3¯ ||

s(13)

32

s(12), s(7)

3m

s(4), s(7)

|| 3¯m ||

s(4), s(13)

6

s(14)

6¯

s(15)

|| 6/m ||

s(6), s(14)

622

s(12), s(14)

6mm

s(4), s(14)

¯6 2m

s(4), s(15)

|| 6/mmm ||

s(4), s(6), s(14)

23

s(12), s(10)

|| m3 ||

s(4), s(10)

432

s(8), s(10)

¯4 3m

s(16), s(10)

|| m3m ||

s(4), s(10), s(17)

(3 ¯ z) = s(1) . s(7) = s(13), (6z) = s(3) . s(7) = s(14) (6 ¯ z) = s(1) . s(14) = s(15), (4 ¯x) = s(1) . s(8) = s(16)

m ⊥ (110) = s(4) . s(9) = s17

52 tensor properties of solids

→ −1 → −2 → −3

1 x2 → −x2 or 2 x3 → −x3 3

x1 → −x1

(3.9)

This means that for a polar property tensor of odd rank, any combination of subscripts will result in T ′ = −T = 0 in accordance with Neumann’s principle. Similarly, for an axial property tensor of even rank, any combination of subscripts will result in T ′ = −T = 0 also in accordance with Neumann’s principle. This process of simplification is called the method of direct inspection and is applicable to all point groups except those in the trigonal and hexagonal crystal systems. For a particular crystal class in these two systems, it is necessary to operate on a property tensor with each generating matrix in turn. The use of the quadratic generation operators is then recommended, especially for property tensors of rank greater than two. Note that throughout this text, the notation for crystallographic axes will adhere to the accepted convention x1 = x, x2 = y, and x3 = z in accordance with Figure 3.1.

3.6

APPLICATION OF NEUMANN’S PRINCIPLE TO SYMMETRICAL SECOND-RANK PROPERTY TENSORS

The macroscopic symmetry of a given crystal can dramatically affect the number of nonzero components of a property tensor that are permitted to exist in that crystal. This is easily demonstrated by applying Neumann’s principle to a symmetrical second-rank property tensor Sij , which may repre sent any of several properties to be studied in subsequent chapters. Typical examples are the dielectric susceptibility and thermal expansion coefficient. We begin with the triclinic crystal system and continue in the direction of increasing symmetry to the cubic system. For this purpose, use will be made of the generation matrices for the 11 holohedral point groups in Table 3.6—those possessing a center of symmetry and the necessary generating matrices for complete symmetry. As we progress from the triclinic to cubic system, use will be made of the method of direct inspection except for the trigonal and hexagonal systems as indicated earlier. 1. Triclinic system: Because all symmetrical second-rank property tensors are centrosymmetrical, they cannot be made null by the center-of symmetry operation. The symmetry transformation becomes

(1)

S11 S12 S31 S' = s S˜s = S = S12 S22 S23 S31 S23 S33 (1)

(3.10)

leaving the property Sij unchanged, with all six independent components needed to repre sent it.

Crystal Systems, Symmetry Elements, and Symmetry Transformations 53 (2)

2. Monoclinic system: The monoclinic system requires use of the generation operators s and s(5) via holohedral group || 2/m ||. Beginning with s(2), S′ transforms as

0 0 −1

0 1 0

S11 S12 S31 −1 S12 S22 S23 0 S31 S23 S33 0 S31 −S23 . S33

−1 0 0 0 1 0 0 −1 0 S11 −S12 S22 = Sym.

S' = s (2)S s˜ (2) =

(3.11)

Applying Neumann’s principle requires that S12 = S23 = 0, giving the result

Sym.

S31 0 , S33

0 S2

S11

S=

(3.12)

where S22 = S2 is a principal component along 0x2 = 0y. Application of operator s(5) leaves the result of Eq. (3.12) unchanged. The same result could have been obtained with greater ease by using the direct inspection method. For example, the use of generating matrix s(2) in Table 3.5 gives → −1 → 2 → −3

2 3

1

or

x1 → −x ′1 s(2) → x2 → x ′2 x3 → −x ′3

(3.13)

It now follows that components having a single 1 or single 3 subscript (but not both) must be zero in accordance with Neumann’s principle, that is, S23 = S12 = 0 (all others must remain nonzero), which is applicable to the three classes of the monoclinic crystal system. 3. Orthorhombic system: The holohedral group || mmm || has the generation matrices s(4), s(5), and s(6), which cover all classes of the orthorhombic system. From Table 3.5, these three operators are given by

→ 1 → 2 . → −3

s → 2 3

1 → 1 (6) → −2 s → 2 → 3 3

1

(5)

s → 2 3

→ −1 → 2 → 3

1

(4)

(3.14)

Taken separately and using the direct inspection method together with Neumann’s principle, the generation matrices s(4), s(5), and s(6) require all components having a single 1, a single

54 tensor properties of solids

2, or a single 3 be zero. Thus, S23 = S31= S12 = 0, with all others being nonzero. Therefore, S is now represented by

0 0 . S3

0 0 S1 S2 0 = S33 Sym.

0 S22 0

S11 S= 0 0

(3.15)

The arrays in Eq. (3.15) apply to all crystal classes of the orthorhombic system. The second- rank property components S1, S2, and S3 are the principal components along the crystallographic axes 0x = [100], 0y = [010], and 0z = [001], respectively. 4. Tetragonal system: The holohedral group || 4 /mmm || has the generating matrices s(4), s(6), and s(9), of which s(4) and s(6) have previously been used for the orthorhombic crystal system, and operator s(5) leaves these results unchanged. Then, applying the operator s(9) from Table 3.5 to the results of the orthorhombic system requires, by the direct inspection method, that

→ 2 → −1 . → 3

x1 → x ′2 1 s(9) → x2 → −x ′1 or 2 x3 → x ′3 3

(3.16)

The results are S31 = S32 = −S31 = 0 and S11 = S22 = S1 in accord with Neumann’s principle. This means that the property tensor Sij is everywhere isotropic in the x, y (001) plane. Thus, the components of Sij for all point groups of the tetragonal crystal system are represented by the array 0 0 . S3

Sym.

0 S1

S1

S=

(3.17)

5. Trigonal and hexagonal systems: The holohedral groups || 3¯m || and || 6 /mmm || contain generating operators s(1), s(3), s(4), s(6), and s(7). The application of the operators s(1), s(3), s(4), and s(6) to the tensor Sij will leave unchanged the results obtained for the tetragonal systems. Therefore, there remains only the application of the operator s(7). Because the method of direct inspection is not applicable here, we must perform the transformation given by

S ′ = s(7)S s~(7) = σ (7)S .

(3.18)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 55

But this transformation can be given more conveniently by using the quadratic transformation 0 0 − 3/2 S1 S1 3/2 S2 0 0 S1 S3 0 0 0 S3 = . −1/2 − 3/2 0 0 0 0 0 3/2 −1/2 0 0 0 −1/2 0 0

0 0 1 0 0 0

1/4 3/4 3/4 1/4 0 0 0 0 0 0 3/4 − 3/4

S ′ = σ (7)S =

(3.19)

This indicates that the components of Sij for all point groups of the trigonal and hexagonal crystal systems are the same as those for the tetragonal system. Consequently, these three systems may be treated as a single group with respect to symmetrical second-rank tensor properties. They are often called the optically uniaxial crystal systems. 6. Cubic system: The holohedral group || m3m || contains generation operators s(4), s(9), and s(10), all but s(10), of which have been applied to the previous, less symmetrical systems. So there now remains the application of the generation operator s(10), to the results obtained for the tetragonal, trigonal, and hexagonal systems. The method of direct inspection, which is again applicable, requires that

or

32

→ → →

2 3 . 1

1

→ x2 → x3 →

x′2 x′3 x′1

s

x1 →

(10)

(3.20)

Then by application of Neumann’s principle there results

S1 = S2 = S3 = S,

(3.21)

meaning that any cubic crystal system is isotropic with respect to any symmetrical second-rank property tensor. To summarize, the effect of crystal symmetry on properties that are represented by symmetrical second-rank tensors is given in Table 3.7. The effect of crystal symmetry on other tensor properties will be given at the time the individual properties are considered. This is especially desirable for the property tensors of higher rank because they often possess unique inherent symmetry. This is particularly true for the axial and axial–magnetic property tensors for which both axial and magnetic symmetry must be considered.

56 tensor properties of solids

TABLE 3.7: Effect of crystal symmetry on symmetrical second-rank tensor properties

0 S2

Sym.

S33

0 S1

Sym.

Cubic

s (4), s (9), s (10)

S

S3 0 S

0

Sym.

0 0 S

0

S1

s (1), s (3), s (4), s (6), s (7), s (9)

S3

Tetragonal, trigonal, and hexagonal

0

Sym.

0

0 S2

0

S1

S31

S33

s (4), s (5), s (6)

S 11

S23

Orthorhombic

Sym.

S31

s (2), s (5)

S12 S22

Monoclinic

S11

s (1)

Triclinic

Independent components of the property matrix

System

Holohedral generating matrices

3.7 EFFECT OF NEUMANN’S PRINCIPLE ON THE 11 CENTROSYMMETRICAL CRYSTAL CLASSES With reference to Table 3.6, it is clear that each of the 11 holohedral groups, those designated by || X ||, contain the center-of-symmetry operator s (1) = (−δij), which requires that the symmetry transformations of (3.9) be applied to any crystal system that contains a center of symmetry. As a result, Neumann’s principle requires that for all centrosymmetrical crystal classes

for axial tensors of even rank

for polar tensors of odd rank

T ′= −T = 0 ⇒

.

(3.22)

Crystal Systems, Symmetry Elements, and Symmetry Transformations 57

Thus, all 11 of the centrosymmetrical crystal classes, those that contain a center-of-symmetry, will be lacking in odd-rank polar tensor properties and even-rank axial tensor properties. For example, the piezoelectric tensor dikl , included in Eq. (2.54), is a polar third-rank tensor property whose property components vanish for any of the 11 centrosymmetrical (holohedral) classes designated by || X || in Tables 3.4 and 3.6. Another example is the pyroelectric coefficient defined by ∆Pi = Pi ∆T, where the three components of pi are null for any of the 11 centrosymmetrical crystal classes. All axial and axial–magnetic tensor properties of even rank will be lacking property components for any of the centrosymmetrical crystal classes. The 90 magnetic point groups come into play only for magnetic and axial–magnetic tensor properties of odd rank, further reducing the number of existing components over those required strictly by conventional symmetry arguments.

3.8 LONGITUDINAL AND TRANSVERSE EFFECTS FOR SYMMETRICAL SECOND-RANK PROPERTY TENSORS Use of either the longitudinal or transverse effects, or both, offers a convenient and practical means of measuring the components of symmetrical second-rank property tensors. To demonstrate these effects, it will be helpful to consider the symmetrical second-rank tensor as being a property relating a cause parameter q to an effect parameter p according to pi pj Sij = q = q = Sji . j i

(3.23)

Referring to Figure 2.1, with the transformation matrix represented as

a11 a12 a13 l1 l2 l3 a = a21 a22 a23 = m1 m2 m3 a31 a32 a33 n1 n2 n3

(3.24)

for convenience, the generalized transformation law for longitudinal and transverse effects becomes

m1 m2 m3

n1 n2 . n3

l1 l2 l3

S31 S23 S33

S12 l1 l2 l3 S11 ~ S' = aSa = m1 m2 m3 S22 n1 n2 n3 Sym.

(3.25)

Equation (3.25) is valid for any crystal system in which the property Sij is manifest. We will now explore the effect of crystal symmetry on the longitudinal and transverse effects. 1. Triclinic system: For the triclinic system, no restrictions are placed on the orientation of the reference axes. If the effect parameter p is sensed along the 0x′1 when the cause parameter q is applied in that same direction, the longitudinal effect for the triclinic system is given by

58 tensor properties of solids

S12 S22

S11

S31 l1 l2 l3 . S23 . l2 S33 l3 Sym. = l12 S11 + l22 S22 + l32 S33 + 2l2 l3 S23+ 2l3 l1 S31+ 2l1l2 S12.

p'1 S'11 = q = l1 '1

(3.26)

Here, the longitudinal effect is simply the magnitude of S measured along some arbitrary direction 0x′1. Similarly, if p is sensed along 0x′1 when q is applied along 0x′2 , or vice versa, the transverse effect given by

S11

S31 m1 S23 . m2 S33 m3 Sym. = l1m1S11 + l2m2S22 + l3m3S33 + (l2m3 + l3m2)S23 +

S12 S22

(l3m1 + l1m3)S31 + (l1m2 + l2m1)S12

l3 .

l2

p'1 p'2 S'12 = q = q = l1 '2 '1

(3.27)

is also applicable to the triclinic crystal system. Thus, to measure all six independent components of Sij , six independent measurements must be made using either the longitudinal effect or transverse effect or some suitable combination thereof. The six resulting equations must then be solved simultaneously to obtain the six components. 2. Monoclinic system: Applied to the monoclinic crystal system, Eqs. (3.26) and (3.27) for the triclinic system can be simplified to the extent that S23 = S12 = 0, as indicated in Table 3.7. All other terms in thee expressions remain the same, with S22 = S2 = S[010] being the principal component along 0x2 = 0y = [010]. Four independent measurements, using either the longitudinal or transverse effects or some combination of them, will yield four independent equations from which the four independent components of Sij can be obtained. Note that the magnitude of the property S′11 measured along the axis of symmetry 0x2 = 0y is the principal component S2. 3. Orthorhombic system: The longitudinal and transverse effects can be put into special forms for the orthorhombic crystal system when we note that S23 = S31 = S12 = 0 and that the principal axes lie along the crystallographic axes. The longitudinal effect now becomes

S 11 ′ = p 1′ / q 1′ = l 12S 1 + l 22S 2 + l 32S 3 2 2 2 S[100] + l [010] S[010] + l [001] S[001], = l [100]

(3.28)

where l〈100〉 are the direction cosines between any direction 0x′1 = [uvw] and the crystallographic (principal) axes, [100], [010], and [001], and S〈100〉 represent the three principal

Crystal Systems, Symmetry Elements, and Symmetry Transformations 59

components along these axes. Similarly, if the direction 0x′2 = [m1, m2, m3] is also taken with respect to the crystallographic axes, the transverse effect for the orthorhombic crystal system is given by

S 12 ′ = p 1′ / q 2′ = p 2′ / q 1′ = l1m1S 11 + l2m2S 22 + l3m3S 33 = l[100] m[100]S[100] + l[010]m[010]S[010] + l[001]m[001]S[001]

(3.29)

Thus, knowing the orientation of the principal axes, three independent measurements using either the longitudinal effect or transverse effect or both, will yield the principal values S1, S2, and S3. 4. Tetragonal, trigonal, and hexagonal systems: For the optically uniaxial crystal systems (tetragonal, trigonal, and hexagonal) the longitudinal effect requires measurement of the two independent components, S1 and S3, along any two arbitrary, but different, directions (one direction must be out of the (001) or (0001) plane). Accordingly, the longitudinal effect is established from Eq. (3.28) as

2 2 2 S 11 ′ = p 1′ / q 1′ = (l [100] + l [010] )S[100] + l [001] S[001] 2 2 = (1 - l [001])S[100] + l [001]S[001]

(3.30)

since now S[100] = S[010] due to the isotrophy of property S in the (001) or (0001) plane for the optically uniazial crystal systems. Defining the Eulerian angles θ and φ, as shown in Figure 3.5, the longitudinal effect takes the form S 11 ′ = S⊥sin2φ + S||cos2 φ

z = [001] [uvw]

φ y = [010]

θ x = [100] FIGURE 3.5: Arbitrary direction [uvw] expressed in terms of the Eulerian angles φ and θ.

(3.31)

60 tensor properties of solids

independent of θ. Here S⊥ = S〈uv 0〉 is the magnitude of the property along any direction 〈uv 0〉 perpendicular to the [001], and S|| = S[001] is the magnitude of the property parallel to the [001] direction. Consequently, the magnitude of the property in any direction [uvw] = 0x′1 depends only on the angle φ and the values S⊥ and S||. For the trigonal and hexagonal crystal systems, the longitudinal effect may be represented alternatively as

S 11 ′ = S〈UV T 0〉sin2φ + S[0001]cos2 φ

(3.32)

for measurement in any direction 0x′1 = [UV TW]. The transverse effect for the optically uniaxial crystal systems is established from Eq (3.29) noting again that S[100] = S[010] = S⊥ and S[001] = S||. Therefore, by knowing the direction cosines for directions 0x1′ = [l1, l2, l3] and 0x2′ = [m1, m2, m3] with respect to the crystallographic axes, the transverse effect can be measured. As always, the transverse effect is more difficult to measure than the longitudinal effect. 5. Cubic system: For the cubic system, the magnitude of the property S is the same in all directions, that is, it is isotropic relative to the property S and requires only one measurement of its magnitude in any direction. • • • •

61

chapter 4

Generalized Thermostatics and the Systematic Correlation of Physical Properties 4.1 Energy Representations and the Criteria for Thermodynamic Equilibrium In classical thermodynamics, the first law is expressed as the change in internal energy of a closed system given by

dU = d−Q + d−W,

where d−Q is the thermal energy (heat) transferred to the system and d−W is the external work done on the system. Here, d−Q and d−W are inexact differentials called Pfaffians—they are path-dependent. For a closed solid-phase system, the infinitesimal change in internal energy is given by the first and second laws of thermodynamics as _ dU = d Q +

_

_

Σi dWi = T dS + dW

_ _ _ + dWMag.+ dWMech.+ dWChem.

Elect.

(4.1)

in which d−Q = TdS is the infinitesimal reversible heat absorbed by the solid-phase system at an absolute temperature T, and dS is the infinitesimal entropy change associated with the absorbed heat d−Q. Σd−W is the sum of all infinitesimal reversible work (electrical, magnetic, mechanical and i

i

chemical) done on the solid-phase system by the surroundings. Each work term in Eq. (4.1) is represented by the product of a particular intensive parameter and an infinitesimal change in its conjugate extensive parameter. In crystalline materials, the atoms are essentially immobile compared to the gaseous (or liquid) state. This complicates the energy representation. For example, in classical PVT thermodynamics, pressure P is an adequate intensive parameter for gases, but it is not adequate to describe the effect of applying surface forces to a solid. Similarly, volume V, used as the extensive parameter for gases, must be replaced by reference volume times strain V0e for solids. Thus, –PdV work in the classical sense (for gases) must be replaced by

62 tensor properties of solids

Table 4.1: Intensive and extensive parameters for a solid-state system and their SI units Intensive Parameters

Extensive Parameters

T — Temperature (°K)

S — Entropy ( J/°K)

E — Electric field intensity (V/m)

Pˆ — Total electric dipole moment (Cm)

B — Magnetic flux density (N / A · m = tesla, T)

I — Total magnetic dipole moment (Am2)

s — Stress (N/m2)

V0e — Strain times reference state volume (m3)

m —Chemical potential ( J/mol)

N — Mole number

elastic strain energy sd (V0e) for the case of solids. Furthermore, the fact that solids can develop a net polarization or magnetization adds additional complications to the energy representation— electrical and magnetic work terms must be added. The intensive and extensive parameters that best describe the equilibrium tensor properties of crystals are presented in Table 4.1 along with their SI units. Note that the magnetic intensive parameter is the magnetic flux density B = m0 H measured in the absence of the crystal system (m0 is the permeability in a vacuum and H is the magnetic field strength). Using these parameters, the total infinitesimal change in internal energy for a solid-phase system is given by

dU = T dS + E dPˆ + B dI + σ d (ε V0 ) + µ d N

(4.2)

in agreement with the respective work terms given in Eq. (4.1). From Euler’s theorem on homogeneous first-order forms, the corresponding Euler relation is given by

U = T S + EPˆ + BI + σ (ε V0 ) + µ N .

(4.3)

The Euler relation is a thermodynamic potential seen to combined first and second laws of thermodynamics in terms of the product of conjugate parameters (in energy units of Joules, J ) given in Table 4.1. The Euler relation will later be used in the generation of other useful thermodynamic potentials for a closed solid-phase system of one component (dN = 0). Differentiating Eq. (4.3) gives the result dU = T dS + S d T + E d Pˆ + Pˆ d E + B dI + I dB + σ d (ε V0 ) + (ε V0 ) d σ + µ d N +N d µ ,

Generalized Thermostatics and correlation of Physical properties 63

which compared to Eq. (4.2) requires that

S d T + Pˆ d E + I dB + (ε V0 ) dσ + N d µ = 0

(4.4)

Equation (4.4) is the general form of Gibbs-Duhem equation for a solid-phase system of a single component (d N = 0). The concepts of equilibrium and spontaneous (irreversible) processes are best understood in terms of the thermodynamic potentials G and F called the Gibbs and Helmholtz free energies, respectively. The extended Gibbs free energy for a single component solid-phase system is defined as

G ≡ µ N = U − TS − E Pˆ − BI − σ (ε V0 ),

(4.5)

which follows from the Euler relation. This potential is the Legendre transform of U that simulta- neously replaces S by T, Pˆ by E, I by B and eV0 by s as the independent variables. Differentiating Eq. (4.5) for a closed solid-phase system of one component and introducing Eq. (4.2) gives the infinitesimal change in Gibbs free energy

dG = − S dT − Pˆ d E − I d B − (ε V0 ) dσ

(4.6)

In actual experimental situations, it is often a simple matter to hold the intensive parameters constant. When this is done, that is, when T, E, B, and s are held fixed, the solid-phase system is said to be thermally, electrically, magnetically and mechanically free resulting in

dG = 0

(4.7)

as the criterion for thermodynamic equilibrium. When one or more of the intensive parameters are varied, then

dG < 0 ,

(4.8)

and the process is said to be spontaneous or irreversible. Clearly, the condition dG > 0 applies to a process that will not take place without changing the thermodynamic parameters of the system. The Helmholtz free energy is a thermodynamic potential defined as

F ≡ U − TS .

(4.9)

Thus, the Helmholtz free energy is the Legendre transform that replaces the entropy S by temperature T as the independent variable. Differentiating Eq. (4.9) for a closed solid-phase system of one component and introducing Eq. (4.2) gives the infinitesimal change in the Helmholtz free energy as

d F = − S dT + E d Pˆ + Bd I + σ d(ε V0 )

(4.10)

64 tensor properties of solids

which eliminates the difficult task of holding entropy constant to establish equilibrium but retains the extensive parameters Pˆ, I, and eV0 as the independent variables. Thus, in experimental situations when T, Pˆ, I, and eV0 are held constant, the system is said to be thermally free but electrically, magnetically, and mechanically, clamped. Under these conditions,

d F = 0

(4.11)

as the criterion for thermodynamic equilibrium. It also follows that d F < 0 corresponds to an irreversible or spontaneous thermally free process at constant Pˆ, I, and e, whereas d F > 0 corresponds, to a spontaneous isothermal but electrical, magnetic and mechanical clamped process. Other thermodynamic potentials may also serve usefully as criteria for thermodynamic equilibrium under the appropriate clamped and/or free conditions.

4.1.1 Energy Density Representation In applying thermodynamic arguments to solid-state systems in which the various tensor components must be manipulated, it becomes burdensome to carry the reference volume V0 along with strain to establish the true extensive mechanical parameter. Because the strains are infinitesimal in magnitude, all equations can be divided by the volume of the fiducial or reference state, which is equal to the instantaneous volume V0 of the solid phase. When this is done, the internal energy density and Gibbs free energy density for a closed system of one component (dN = 0) become

d u = dU / V0 = T ds + E d P + B d M + σ d ε

(4.12)

d g = dG / V0 = − s d T − P d E − M d B − ε d σ ,

(4.13)

and

respectively. The extensive parameters are now defined as follows: s = S / V0 = entropy density ( J/°K/m3), P = Pˆ / V0 = total electric dipole moment/unit volume = polarization (C/m2), M = I / V0 = total magnetic dipole moment/unit volume = magnetization (A/m), and e = eV0 / V0 = elastic strain (dimensionless). The criteria for equilibrium still apply but in energy density form, and the Euler relation u = U / V0 and Helmholtz free energy density f ≡ u – Ts follow from the above definitions. By using the energy density representation for simplicity, other thermodynamic potentials, in addition to g and f, can be generated by Legendre transformations of u. Listed in Table 4.2 are the 16 thermodynamic potentials and their differentials for a closed solid-phase system of one component. Some of these will prove to be useful. For example the generalized enthalpy density h, which is given by thermodynamic potential φ5, is used to define the heat capacity of a solid at constant E, B,

Generalized Thermostatics and correlation of Physical properties 65

Table 4.2: The 16 thermodynamic potential densities and their differentials for a closed solid state system of one component Thermodynamic Potentials

Thermodynamic Potential Differentials

φ1 = u − Ts − EP − BM − σε = g

dg=−sdT−PdE−MdB−ε dσ

φ2 = u − Ts − EP − BM

d φ2 = − s d T − P d E − M d B + σ d ε

φ3 = u − Ts − EP − σε

d φ3 = − s d T − P d E + B d M – ε d σ

φ4 = u − Ts − BM − σε

d φ4 = − s d T + E d P − M d B − ε d σ

φ5 = u − EP − BM − σε = h

dh=Tds−PdE−MdB−ε dσ

φ6 = u − Ts − EP

d φ6 = − s d T − P d E + B d M + σ d ε

φ7 = u − Ts − BM

d φ7 = − s d T + E d P − M d B + σ d ε

φ8 = u − Ts − σε

d φ8 = − s d T + E d P + B d M − ε d σ

φ9 = u − EP − BM

d φ9 = T d s − P d E − M d B + σ d ε

φ10 = u − EP − σε

d φ10 = T d s − P d E + B d M − ε d σ

φ11 = u − BM − σε

d φ11 = T d s + E d P − M d B − ε d σ

φ12 = u − Ts

= f

d f = − s d T + P d E + M d B + ε d σ

φ13 = u − EP

d φ13 = T d s − P d E + B d M + σ d ε

φ14 = u − BM

d φ14 = T d s + E d P − M d B + σ d ε

φ15 = u − σε

d φ15 = T d s + E d P + B d M − ε d σ

φ16 = u = u

du=Tds+EdP+BdM+σ dε

and s, which is analogous to CP in the classical sense. Still other potentials, such as φ2, φ3, φ4, and including φ5 are useful in developing Maxwell’s relations for the dependent coupled effects holding certain intensive parameters constant. The reader will note that the differential forms dφi result by differentiating φi followed by introduction of Eq. (4.12), du = T d s + E d P + B d M + σ d ε to complete the Legendre transform of u. For example, differentiating φ13 = u – EP gives dφ 13 = d u − E d P − P d E = T d s + E d P + B d M + σ d ε − E d P − P d E = Td s − P d E + B d M + σ dε

4.2

Thermodynamic Definition of Parameters

Taking any closed solid-state system of one component (d N = 0) in which reversible processes are occurring, the fundamental equation of state becomes u = u (s, Pi , Mi , εij ), where the tensor rank of the

66 tensor properties of solids

extensive parameters is indicated by the number of subscripts. Expanding an infinitesimal change in u in a Taylor series and neglecting the second, and higher-order differential terms, we write the first-order terms of du as

∂u ∂u ∂u d s + dPi + ∂ s P,M,ε ∂ Pi s,M,ε ∂ Mi

du =

∂u d Mi + ∂ε s,P,ε ij

= T d s + Ei d Pi + Bi d Mi + σij dεij (i, j = 1−3).

dεij s,P,Μ (4.14)

By comparing coefficients, we find the following thermodynamic definitions for the intensive parameters by holding certain extensive parameters constant as indicated by the symbols subscripted to the curved brackets: The absolute temperature

(4.15)

∂u ≡T ∂ s P,M,ε

∂u ≡ Ei ∂Pi s,M,ε

The external electric field strength vector

(4.16)

The external magnetic flux density vector

(4.17)

∂u ≡ Bi ∂Mi s,P, ε

The stress tensor.

(4.18)

∂u ∂ε ij

≡ σij s,P,M

In these definitions, T is a scalar and is specified by one component, Ei and Bi are vectors each specified by three components (Bi is axial magnetic in character), and σij is usually a symmetrical secondrank polar tensor (σij = σji ) specified by six components as in Eqs. (2.17) and (2.20). Now, let the letter I represent the intensive parameters (T, Ei , Bi , σij ) and the letter e represent the extensive parameters (s, Pi , Mi , εij ) so that an infinitesimal change in the internal energy density is given in the compact form d u = Im d em

(m = 1–13).

(4.19)

Here, the sequence (T d s + E1 d P1 + E2 d P2 + E3 d P3 + B1 d M1 + B2 d M2 + B3 d M3 + σ1 d ε1 + σ2 d ε 2 + ... σ 6 dε6 )

Generalized Thermostatics and correlation of Physical properties 67

has been written in the form ( I1 d e1 + I2 d e2 + ... + I13 d e13 ), where the stress and strain components have been unfolded according to the matrix scheme of Eq. (2.20) for symmetric second-rank tensors. In a similar manner, the extensive tensor parameters can be defined by using the generalized Gibbs free energy density. For any closed solid-phase system of one component, the fundamental equation of state becomes g = g (T, Ei , Bi , σij ), and we write for the first differential of g ∂g dg = ∂T

E,B,σ

∂g dT + ∂ Ei

∂g d Ei + T,B,σ ∂Bi

d Bi + T,E,σ

∂g ∂σ ij

dσij T,E,B

= − s d T − Pi d Ei − Mi d Bi − εij dσij .

(4.20)

Again, by comparing coefficients there results the following definitions for the extensive parameters of a closed system holding certain intensive parameters constant:

∂g ∂ T E,B,σ

−

≡s

The entropy density

∂g − ≡ Pi The total electric dipole moment per unit volume E ∂ i T,B,σ or (polarization) ∂g − ∂ Bi

(4.22)

≡

Mi The total magnetic dipole moment per unit volume T, E, σ or (magnetization)

∂g − ∂σ ij

(4.21)

≡ εij The strain tensor. T, E, B

(4.23) (4.24)

As with their conjugate intensive parameters, s is a scalar, Pi and Mi are vectors of three components each (Mi is axial magnetic in character), and εij is usually represented as a symmetrical second-rank tensor (εij = εji ) specified by six components as in Eq. (2.20). An infinitesimal change in the Gibbs free energy density may also be represented in the compact form

68 tensor properties of solids

dg = − em dIm

(m = 1 − 13),

(4.25)

where (e1 dI1 + e2 dI2 + ... + e13 dI13) represents the sequence ( s d T + P1 d E 1 + P2 d E 2 + P3 d E 3 + M1 d B1 + M 2 d B 2 + M 3 d B 3 + ε 1d σ 1 + ε 2 d σ 2 + ... ε 6 d σ 6 ). Here again, the stress and strain components have been unfolded according to the scheme given by Eq. (2.20).

4.3

Generalized Compliance and Rigidity Matrices

We now wish to know how the reversible variation of all intensive parameter components affect a given extensive parameter component and vice versa. Consider, as an example, the equation of state for the polarization of a solid-state system of one component as a function of the four intensive parameters given by Pi = Pi(T, Ej , Bj , σkl). In this case, an infinitesimal change in polarization is given by the Taylor series 1 ∂ ∂ ∂ dPi = ∑ dT ∂T + dE k ∂E + dB k ∂B + dσkl n = 1 n! k k ∞

∂ ∂ σkl

n

Pi (T , E , B ,σ ).

(4.26)

Similar Taylor series expansions can also be given for the remaining three equations of state s = s (T , Ek ,Bk , σkl ); Mi = Mi (T , Ek , Bk , σkl )

ε ij = εij (T ,Ek,Bk , σkl ).

(4.27)

Carrying out these Taylor series expansions and accepting only the first-order terms (n = 1), thus neglecting the second- and higher-order differential terms, the infinitesimal changes in the extensive parameters are given by the linear first-order equations:

∂s ∂s ds = dT + ∂ T E,B,σ ∂ Ek ∂P d Pi = i ∂T

E,B,σ

∂ Mi d Mi = ∂T

∂ε dε ij = ij ∂T

∂P dT + i ∂ Ek

E,B,σ

E,B,σ

T,B,σ

∂s d Ek + ∂ Bk

∂P d Ek + i T,B,σ ∂ Bk

T,E,σ

∂ Pi d Bk + T,E,σ ∂σ kl

∂ Mi ∂ Mi dT + dEk + ∂ Ek T,B,σ ∂ Bk

∂ε dT + ij ∂ Ek

T,B,σ

∂ε d Ek + ij ∂ Bk

∂s d Bk + ∂ σkl

T,E,σ

T,E,σ

dσkl T,E,B

dσkl T,E,B

∂ Mi d Bk + ∂ σkl

∂ε d Bk + ij ∂ σkl

dσ kl T,E,B

dσkl . T,E,B

(4.28)

Generalized Thermostatics and correlation of Physical properties 69

The partial derivatives are called the property compliances, where the subscripts indicate those intensive parameters that are held constant. Now, we designate the property compliances by the letter C with the appropriate subscripts and superscripts, such that (∂s / ∂T )E,B,σ = C s,T, (∂s / ∂Ek )T,B,σ = Cks,E, etc., thereby permitting us to set Eqs. (4.28) in the matrix form given by Eq. (4.29). This matrix equation is called the general property compliance matrix for first-order equilibrium properties. The tensor rank of any compliance is indicated by the number of subscripts it has. Thus, it is ε,σ . seen that the tensor rank varies from zero for C s,T to rank 4 for the compliance Cijkl

ds C dP C P,T i= i dMi C M,T i ε,T dεij Cij s,T

Cks,E

Cks,B

CiP,E k

CikP,B

CiM,E k

CiM,B k

Ciεjk,E

Ciεjk,B

Ckls,σ dT CiP,σ kl dEk ⋅ CiM,σ dBk kl ε,σ dσ Cijkl kl

( i, j , k , l = 1 − 3 )

(4.29)

A close inspection of the compliance matrix (4.29) reveals that it is, in reality, a (13 x 13) matrix of tensor components if stress and strain are taken as symmetrical second-rank tensors. This is illustrated in Table 4.3 where the individual property matrices are designated by (r × c), meaning rows by columns. The four principal effects of the property compliance matrix lie along its leading diagonal and are shaded. The off-diagonal compliances represent the coupled (interaction) effects. If we let e represent the extensive parameter components and I represent the intensive parameter components, then the set of linear first-order equations for the compliances in Table 4.3 are expressed in contracted subscript form as

dem = Cmn d In ( m , n = 1 − 13 ),

(4.30)

where it follows that C11 = C s,T = (∂ s / ∂ T )E,B,σ

C12 = C s,E1 = (∂ s / ∂ E1 )T, E

2, E3,B,σ

C29 = CP1, σ2 = (∂P1 / ∂ σ2 )T,E,B,σ ,σ

, σ 1 3 � 6

C46 = CP3, B2 = (∂ P3 / ∂ B2 )T, E, B

1 , B2 , σ

C13,13=C ε6, σ6 = (∂ ε 6 / ∂ σ 6 )T,E,B,σ

,σ ,...σ 1 2 5

(4.31)

70 tensor properties of solids

Table 4.3: Component arrangement of the general compliance matrix emphasizing the principal effects along the leading diagonal (shaded regions), all other being the coupled effects n→

m ↓ 1

s

2 P1 3 P2 P3 4 5 M1 6 M2 7 M3 8 ε1 9 ε2 10 ε 3 11 ε 4 12 ε 5 13 ε 6

1

2

T

E1 E2

3

4

5

E3

B1 B2

6

7

8

9

B3

σ1 σ2

10

11

12

13

σ3

σ4

σ5

σ6

C s,T (0)

C s,E (1 × 3)

C s,B (1× 3)

C s,σ (1 × 6)

C P,T (3 × 1)

C P,E (3 × 3)

C P,B (3 × 3)

C P,σ (3 × 6)

C M,T (3 × 1)

C M,E (3 × 3)

C M,B (3 × 3)

C M,σ (3 × 6)

C ε ,T (6 × 1)

C ε ,E (6 × 3)

C ε ,B (6 × 3)

C ε ,σ (6 × 6)

Thus, a given compliance is a quantity that expresses the rate of change of one particular extensive property component with respect to an intensive property component holding all other intensive parameter components constant. Following the same procedure, the intensive parametric equations of state are

T = T (s ,P,M , ε )

E = E (s , P, M , ε )

B = B (s ,P ,M , ε )

σ = σ (s ,P , M , ε )

(4.32)

From these, there results the following linear first-order equations expressing the infinitesimal changes in intensive parameters as functions of infinitesimal changes in the extensive parameters:

Generalized Thermostatics and correlation of Physical properties 71

dT R dE RE,s i= i dBi RB,s i d σij Riσ,j s

T,s

RkT,P

RkT,M

RiE,P k

RiE,M k

RiE,P k

RikB,M

Riσ,P jk

Rijkσ,Μ

RT,k ε ds REikl,ε dP k ⋅ RiB,klε dMk Rijσ,klε d ε kl

( i, j , k , l = 1 − 3 )

(4.33)

Here, the R matrix is called the general property rigidity matrix for the first-order equilibrium tensor properties. Equations (4.33) can be represented in contracted tensor subscript form as d Im = Rmn d en

(m ,n = 1−13 ),

(4.34)

where it follows that the rigidity and compliance matrices have an inverse relationship given by R = C -1.

(4.35)

The rigidities have the meaning that R11= RT,s = (∂ T / ∂ s )P,M,ε

R46 = RE3,M2 = (∂ E3 / ∂ M2)s,P,M

1,M2 , ε

1

R13,13 = R σ6 , ε6 = (∂σ6 / ∂ε6 )s, P, M, ε

1, ε2, ... ε5.

(4.36) In the above developments, only infinitesimal reversible changes in the intensive and extensive parameters were considered, and all solid-phase systems were assumed closed on their bound- aries. Furthermore, we have suppressed the names of the various property compliances and rigidities until symmetry considerations have been discussed in the next section. Let it suffice for now to say that the properties along the leading diagonals of the general compliance and rigidity matrices each represent four principal effects, whereas the off-diagonal symbols represent the 12 interaction effects often called coupled effects.

4.4

Symmetry of the General Compliance and Rigidity Matrices

The thermodynamic potentials listed in Table 4.2 are functions of thermodynamic properties of a given solid, and each of the thermodynamic properties has only one definite value for any given

72 tensor properties of solids

state of the solid. A thermodynamic property is, therefore, any quantity that depends on the state of the solid and that is independent of the path taken to reach that state. Such quantities are called state functions and form exact differentials. For the intensive and extensive parameters that are field tensors of rank 1 or 2 (T and s are scalars), the term thermodynamic property refers to an individual component of the tensor. For example, φ = g in Table 4.2 represents the Gibbs free energy density g(T , E , B , σ) = g(T , E1 , E2,E3 , B1 , B2 , B3 , σ1, σ2, ... σ3) in which g is given as function of 13 thermodynamic properties (intensive parameter components). Thus, it follows that although g is intensive in nature, internal energy density u is extensive in nature and all other φi in Table 4.2 are of mixed character. Consider any thermodynamic property ζ( p,q) of a solid that is a function of any other two thermodynamic properties, p and q. Now suppose that the substance is taken from its initial thermodynamic state through a series of states allowing p and q to vary independently in some arbitrary manner and that the process may be either reversible or irreversible. Finally, if the substance is returned to its initial state, we would notice that ∆ ζ = 0 since ζ depends only on the initial and final states, which, in this case, are the same. The independence of path of a given thermodynamic property ζ is expressed mathematically by Green’s theorem in a plane (special case of Stoke’s theorem) given by

∫

∂ς ∂ p

∂ς d p + ∂q

d q

ς ( p, q ) =

∫

C

=

∫

(M d p + N d q ) = − C

C

∫

∂ M ∂N d p d q = 0 − S ∂ q p ∂ p q

(4.37)

for any simple closed path C in a given region R′. It follows, therefore, that

∂ N ∂ 2ς ∂ 2ς ∂M = = = ∂ p ∂ p ∂q ∂ q∂ p ∂ q

(4.38)

if M( p,q) and N( p,q) have continuous derivatives in region R′. Simply stated, the order of differentiation of any thermodynamic property ζ is immaterial. This result is essential in describing the symmetry of the generalized compliance and rigidity matrices from which come the Maxwell relations. It will also be most useful when discussing the symmetry of second- and higher-order tensor properties in subsequent chapters. We now apply Eq. (4.38) to the extended Gibbs free energy density. From Eq. (4.25) for any component, em of an extensive parameter is defined by em = −

∂g . ∂Im

(4.39)

Generalized Thermostatics and correlation of Physical properties 73

Also, its infinitesimal change is related to an infinitesimal change in a component of an intensive parameter given by d em = Cmn d In, where the compliance is defined by

Cmn =

∂ em . ∂In

(4.40)

Because the order of differentiation is immaterial, we have the important result that

∂ em ∂e ∂2 g ∂2 g =− =− = n ∂ In ∂ In ∂Im ∂ Im ∂ In ∂ In

(4.41)

or

Cmn = Cnm .

(4.41a)

The meaning of Eq. (4.41) is straightforward. With reference to Table 4.3, only the principle effects (those along the diagonal and shaded) possesses self-symmetry expressed by

~ ~ ~ CP,E = CP,E, CM,B = CM,B, C ε,σ = C ε,σ ,

meaning that the principle property compliance matrices (of components) taken separately are equal to their transpose. All other (coupled) property compliance matrices are related to the corresponding ones across the leading diagonal according to the Maxwell relations given later in Section 4.5.2. ∼ ∼ ∼ ∼ For example, while C P,B = C M,E, it also follows that C P,B ≠ C P,B and C M,E ≠ C M,E ; or while C P,σ = C ε,E, ∼ ∼ it is clear that C P,σ ≠ C P,σ or C ε,E ≠ C ε,E. Consequently, the 13 × 13 compliance component matrix shown in Table 4.3 is symmetric, about the leading diagonal (within the shaded regions), which reduces the number of independent compliance components from 169 to 91. This type of inherent symmetry is called thermodynamic tensor symmetry since it arises from thermodynamic arguments. It must be remembered that the symmetry expressed by Cmn = Cnm applies only to the tensor components on the leading diagonal of the generalized compliance matrix. By similar reasoning, it follows from Eq. (4.19) that Im =

∂u , ∂ en

(4.42) where an infinitesimal change in any intensive parameter is given by dIm = Rm en. Again applying Green’s theorem in a plane yields the result

∂Im ∂I ∂ 2u ∂ 2u =− = = n ∂ en ∂ en ∂ em ∂ em ∂ en ∂ em

(4.43)

74 tensor properties of solids

or Rmn = Rnm.

(4.43a)

We note that this result could have been deduced from Eq. (4.35). Consequently, the 13 × 13 rigidity component matrix is also symmetric about its leading diagonal thereby reducing the number of independent rigidity components from 169 to 91. It must be understood that the so-called thermodynamic tensor symmetry is in no way associated with the symmetry of the crystal in which the tensor properties may or may not be manifest. Thus, the symmetry expressed by Cmn = Cnm and Rmn = Rnm applies generally to all crystal systems. Operation of the minimum generating matrices given in Table 3.6 and the application of Neumann’s principle given in Section 3.6 for symmetric second-rank tensors may result in a reduction of independent components required to specify the property for that point group. This will be done separately and selectively for the tensor properties as they are discussed in later developments.

4.5

Systematic Enumeration and Correlation of First-Order Tensor Properties— Generalized Maxwell Relations

It is desirable at this point to enumerate and correlate the various properties represented by the general compliance and rigidity matrices given by Eqs. (4.29) and (4.33). To do this, we will begin with the principle effects that lie along the leading diagonal of the general compliance matrix and then proceed to the interaction (coupled) effects that are represented by the off-diagonal compliances. Again, we will assume a single solid-phase system that is closed on its boundaries and that all fields applied to it are infinitesimally small so as to avoid second- and higher-order effects.

4.5.1 Principal Effects The principal properties are those that relate conjugate parameters and are defined as follows:

∂s ≡ (C )E, B, σ , specific heat (Heat capacity per unit volume) ∂ T E, B, σ

TC s,T = T

∂ Pi ≡ ( χik )T , B,σ , dielectric susceptibility tensor ∂ Ek T , B, σ

κ −1 CiPk , E = κ −1 0 0

where κ0 is the permittivity of a vacuum.

(4.44)

(4.45)

Generalized Thermostatics and correlation of Physical properties 75

∂ Mi ≡ (ψik )T , E,σ , magnetic susceptibility tensor ∂Bk T , E,σ

B = µ 0 µ 0CiM, k

(4.46)

where µ0 is the permeability of a vacuum.

∂ε Ciε,jklσ = ij ∂ σ kl

≡ (sijkl )T , E , B , elastic compliance tensor T , E , B

(4.47)

By application of the results of the previous section, we find these principal effects have the following thermodynamic tensor symmetry:

~ ( i , k = 1, 2 ,3 ) or χ = χ

(4.48)

~ ψ ik = ψ ki ( i , k = 1, 2 ,3 ) or ψ = ψ

(4.49)

sijkl = sklij ( i , j , k , l = 1, 2 ,3 ) or smn = snm

(4.50)

χ =χ ik

ki

It follows, therefore, that the two susceptibilities are symmetrical second-rank tensors, whereas the fourth-rank elastic compliance tensor sijkl is symmetric with respect to the interchange of pairs (ij ) and (kl ). It will later be shown that σij and εij are nearly always symmetrical second-rank tensors.

4.5.2 Independent Coupled Effects These coupled effects are represented by the off-diagonal compliances of the general compliance matrix and do not relate conjugate parameters. Consequently, they possess no thermodynamic tensor symmetry in themselves (self symmetry) as did the principal effects. However, since the general compliance component matrix is symmetric about its leading diagonal, there results the following six sets of Maxwell relations (57 in all) describing the six independent coupled effects all of which derive from the thermodynamic potential φ1 = g in Table 4.2. 1. Pyroelectric Effect

∂s ∂E 1 T , E ,E 2

3,B,σ

∂s ∂E 3 T , E 1 ,E

∂P = 1 = ( p1)B,σ ∂ T E,B,σ

2,B, σ

∂P = 3 = ( p3)B, σ ∂ T E,B, σ

(4.51)

76 tensor properties of solids

or, collectively, in matrix notation ~ C sE )T ,B,σ = C PT )E,B,σ = ( p)B,σ

(4.52)

These equations state that the electrocaloric coefficients are numerically equal to the corresponding pyroelectric coefficients, and both are represented by the first-rank polar tensor pk (k = 1,2,3). Thus, Eqs.(4.51) derive from dg = -sdt -PdE -MdB -εdσ, to which we apply Stoke’s theorem to give

[(∂ 2 g / ∂ E∂ T ) = (∂ 2g / ∂ T∂ E)]B,σ

or [(∂ / ∂ E)(∂ g / ∂ T ) = (∂ / ∂ T )(∂ g / ∂ E )]B,σ

where ∂g / ∂T = -s and ∂g / ∂E = -P, thereby yielding Eqs. (4.51) at constant B and σ. 2. Pyromagnetic Effect

∂s ∂M = 1 = ( q1)E,σ ∂B1 T ,E , B ,B ,σ ∂ T E,B,σ 2 3 ∂s ∂M = 3 = ( q3)E,σ ∂B3 T ,E , B1 ,B ,σ ∂ T E,B,σ

2

(4.53)

or, collectively, in matrix notation ~ C sB )T ,E,σ = C M,T)E,B,σ = (q )E,σ .

(4.54)

These equations state that the magnetocaloric coefficients are numerically equal to the corresponding pyromagnetic coefficients, and both are represented by the first-rank tensor qk (k = 1,2,3), which is both axial and magnetic in tensor character. 3. Thermal Expansion

∂s ∂ σ 11 T ,E, B,σ

22…σ 12

∂ ε 11 = (α 11) E,B ∂ T E ,B,σ

=

∂s ∂ σ 12 T ,E, B,σ

∂ ε 12 = (α 12 ) E, B ∂ T E , B ,σ

= …σ 11 31

(4.55)

or, collectively, in matrix notation

~ C sσ )T ,E,B = C ε,T )E,B,σ = (α)E,B

(4.56)

Generalized Thermostatics and correlation of Physical properties 77

which states that the piezocaloric coefficients are numerically equal to the corresponding thermal expansion coefficients and that both are represented by the second-rank polar tensor αik(i,k = 1,2,3). It is assumed that stress, strain and thermal expansion are all symmetric second-rank tensors that are unfolded according to the schemes of Eqs. (2.19) or (2.20). 4. Magnetoelectric susceptibility

∂P 1 ∂M 1 = = (λ 11) T, σ ∂B1 T, E, B2, B3,σ ∂E 1 T, E, B2, B3,σ

∂P 2 ∂M 1 = = (λ 21) T, σ ∂B1 T, E, B , B , σ ∂E 2 T, E ,E , B,σ 2

3

(4.57)

1 3

or, collectively, in matrix notation ~ C PB)T,E,σ = C ME)T,B,σ = (λ)T,σ .

(4.58)

Here, the corresponding coefficients of the direct and converse magnetoelectric susceptibility effects are numerically equal and are represented by the asymmetrical second-rank tensor λik which is axial and magnetic in character. Note that the components have been unfolded according to the following schemes: Tensor notation: S11 Matrix notation: S1

S22

S33

S23

S31

S12

S32

S13

S21

(4.59)

S2

S3

S4

S5

S6

S7

S8

S9

(4.60)

5. Piezoelectric Effect

∂P1 ∂ σ 11 T ,E, B,σ

∂ ε 11 E ∂ 1 T,E

= 22…σ 12

= ( d111)

T ,B

2,E3,B,σ

∂P3 ∂ σ 12 T ,E, B,σ

∂ ε 12 ∂ E3 T, E , E

= 11…σ 31

1

2 ,B, σ

= ( d312)

T ,B

(4.61)

or, collectively, in matrix notation

~ C Pσ)T,E,B = C ε,E )T ,B,σ = (d )T ,B .

(4.62)

78 tensor properties of solids

These equations state that the corresponding 18 components of the direct and converse piezoelectric effects are numerically equal and are represented by the third-rank polar tensor dijkl in the form of Tim given by Eq. (2.30) where the partial inherent symmetry is expressed by dikl = dilk = dim. 6. Piezomagnetic Effect

∂M1 ∂ σ 11 T ,E, B, σ

22…σ12

∂ ε 11 = ( Q111) T ,E ∂ B1 T, E,B ,B ,σ

=

2 3

∂M3 ∂ σ 12 T , E, B,σ

11…σ 31

∂ ε 12 = ( Q312) T ,E ∂ B3 T, E,B ,B ,σ

=

1 2

(4.63)

or, collectively, in matrix notation

~ C Mσ)T, E,B = C ε,B )T , E ,σ = (Q)T , E .

(4.64)

Similar to the piezoelectric effects, the corresponding 18 components of the direct and converse piezomagnetic effects are numerically equal. They are represented by the axial-magnetic third-rank tensor with the partial inherent symmetry Qikl = Qilk = Qim, assuming that stress and strain are symmetric second-rank tensors and are expressed by a tensor of the form given by Eq. (2.30). Thus, of the 16 properties represented by the general compliance matrix, only 10 are independent, 4 principal and 6 coupled effects. The same is true for the general rigidity matrix. It will be left as and exercise for the reader to repeat the above correlation procedure for the rigidities.

4.6 Effect of Measurement Conditions on the First-Order Tensor Properties Frequently, it is desirable to convert property coefficients measured under one set of conditions to those measured under another set of conditions. As an example, ultrasonic wave velocity measurements provide isentropic (thermally clamped) elastic coefficients. However, it may be the isothermal (thermally free) elastic coefficients that are desired. A second, and perhaps most common example is the conversion of heat capacity at constant stress (mechanically free) to heat capacity at constant strain (mechanically clamped) or vice versa. There are many other such examples. The problem of

Generalized Thermostatics and correlation of Physical properties 79

converting property coefficients in the clamped state to those in the free state or vice versa is one, which we shall now consider. Let a clamped compliance be that compliance that is measured holding any one of the extensive parameters (s, P, M, or ε) constant. Also, let a free compliance be one that is measured holding any one of the intensive parameters (T, E, B, or σ) constant. Now, consider any two extensive parameters a = a(α , β) and b = b(α , β) that are functions of any two intensive parameters α and β. From the equations dem = Cmn dIn, we write

∂a ∂a dβ da = dα + α ∂ β ∂β α

(4.65)

∂b ∂b db = d α + ∂ α β ∂β

(4.66)

and

d β . α

Holding b constant and multiplying Eq. (4.66) by (∂β / ∂b)α, we obtain

giving the result

∂β ∂b ∂β ∂b 0 = dα + ∂b ∂ β ∂b α ∂ α β α

d β , α b

∂ β ∂b d β = − dα . ∂b α ∂α β

(4.67)

Introducing Eq. (4.67) into Eq. (4.65) gives

∂a ∂ β ∂b ∂a da = d α − dα . α ∂ ∂β ∂b ∂α α β α β

(4.68)

Now, dividing Eq. (4.68) by dα at constant b leads to the final result or

∂a ∂ β ∂b ∂a ∂a − = − ∂β ∂b ∂α ∂α ∂α α β α β b (C a,α)b − (C a,α )β = −(C a,β )α (Rβ,b )α (C b,α )β

(4.69)

80 tensor properties of solids

in symbolic notation. Equation (4.69) gives the difference between the clamped (C a, a)b and free (C a, a)b compliances and requires that all other intensive parameters γ,δ, and so forth be held constant and that b and b be conjugate parameters. Application of Eq. (4.69) is simply accomplished by selecting the desired compliance through choice of a and a, and the clamped and free conditions through choice of the conjugate parameters b and b. For example, the difference between the mechanically clamped and free heat capacities is obtained by the following choice of parameters

a = s b = ε

α = T

(E, B constant)

β =σ

Introducing these parameters into Eq. (4.69) results in

∂ s ∂ σ ij ∂s ∂s − = − ∂ σ ∂ T ε ∂ T σ ij T ∂ ε kl

∂ ε kl , T ∂ T σ

(4.70)

where E and B are assumed to be held constant. But (∂s / ∂σij)T = (∂εij / ∂T )σ = aj by Maxwell’s relation and (∂σij / ∂εkl )T = (cijkl )T where (cijkl )T is the isothermal elastic stiffness coefficient. From this, we find the difference between the mechanically clamped and free heat capacities to be Cε − Cσ = − Tα ij (c ij k l ) α k l

( i , j , k , l = 1 − 3)

in tensor subscript notation or, alternatively,

Cε − Cσ = − Tα i (c ij ) α j = − T α~ ( c ) α T

T

( i , j = 1 − 6 )

(4.71)

in contracted tensor subscript and conformable matrix notation, respectively. Now suppose we wish to know the difference between the isentropic (constant entropy) and isothermal dielectric susceptibilities. For this purpose the choice of parameters becomes

a = P b = s

α = E β = T

(B constant),

resulting in the equation

∂Pi ∂E j

∂Pi − ∂E s j

= − ∂Pi ∂ T ∂ s ∂ T E ∂ s E ∂Ej T

, T

(4.72)

Generalized Thermostatics and correlation of Physical properties 81

where B and σ are held constant. However, because (∂Pi / ∂T )E = (∂s / Ei)T = pi from Maxwell’s relations, there results (χ ) − (χ ) = −

ij T

ij s

T

κ 0 CE

( i , j = 1 − 3 ),

pi pj

(4.73)

where T (∂s / T )E = CE with B and σ held constant, and pi pj is the dyadic or outer product of the pyroelectric coefficients. The above two examples demonstrate how one could obtain the difference between clamped and free principal effects. However, the difference between clamped and free coupled effects can be obtained with equal ease. As a third example, suppose it is desired to know the difference between the electrically clamped and electrically free coefficients of thermal expansion. For this purpose, the choice of parameters must be

a = ε b = P

α=T

β = E

(B constant),

resulting in the equation

∂ ε ij ∂ ε ij ∂T − ∂T P

∂ε = − ij ∂E E k

∂E k ∂P m ∂P ∂ T . E T m T

(4.74)

But according to Maxwell’s relations, (∂εij / ∂Ek)T = (∂Pk / ∂σij )E = dkij , with the result that

(α ij ) − ( αij) = −κ 0−1 (dkij ) ( χkm)−1 ( pm ) E

P

T,σ

T

σ

(i , j , k , m = 1 − 3 )

in tensor subscript notation or, alternatively,

(αi ) − (αi ) = −κ 0-1 ( dki ) ( χ km) -1 ( pm) P

E

T

T,σ

σ

(i = 1 − 6; k , m = 1 − 3)

(4.75)

or

~ αP − αE = −κ 0−1 dT ( χ −1)T,σ pσ

in conformable matrix notation. Because there are four principal effects each with three ways to vary the clamped and free compliances and six independent coupled effects each with two ways to vary the clamped and free compliances, there are a total of 24 equations of the type illustrated above. These are presented in

82 tensor properties of solids

Table 4.4: Differences between clamped and free first-order property compliances given in conformable matrix order for the principal and coupled effects. Principal Effects

Coupled Effects

}

Q s − QT = −(T / C B ,σ )qσ α~ B}E

(1)

C P − C E = −κ 0 T ~ p ( χ T ) −1 p

(2)

~ (ψ ) −1 q C M − C B = −µ 0−1T q T

(3)

~ c α} Cε − Cσ = − T α E, B T

(15)

(4)

p }B , σ χ − χ T = − (T / κ 0 ) C E p ~

(16)

dM − d B = − µ 0 λσ ( χ E ,σ ) − 1 QE

(17)

α P − α E = −κ 0− 1 d T ( χ T ,σ ) −1 pσ

(18)

~ α M − α B = −µ 0 QT (ψ T ,σ) − 1 qσ

(19)

~ qP − q E = −κ 0−1λT ( χ T , B ) −1 p B

(5)

(13)

B ,σ

}

(14)

E,σ

s

−1 ~ χM − χE = − ( µ 0 / κ 0 )λ (ψ E ) λ

}

T,σ

(6)

~ −1 χε − χσ = −κ o dcE d

(7)

ψs − ψT = − ( µ0 T / C B ) q q~}E ,σ

(8)

~ −1 ψ P − ψ E = − ( µ 0 / κ 0 )λ ( χ B ) λ

}

T, B

}

T, σ

QP − QE = −κ 0− 1 λσ ( χ B ,σ ) − 1 d B

T

ds − d T = −(T / C E ,σ ) pσ ~ p E}B

}

~

T

}

B

}

E

}

qε − qσ = − Q T cT , B α B

pM − p B = − µ 0 λ T ( ψ T , E )

E

~ ψε − ψσ = − µ 0 Q cB Q }T , E

(21)

(10)

~} * ss − sT = −(T / Cσ )α α E,B

(22)

pε − pσ = − dT c T , E α E

(11)

~ sP − sE = − κ 0− 1 d ( χσ ) − 1 d}T , B

(23)

λ s − λ T = − (T / C E , B) p B q~ E

(12)

~ s M − sB = − µ0 Q (ψσ ) −1 Q}

(24)

−1

qE

}

}

B

}

~ λε − λσ = −d B c E, B QE

* Difference between the isentropic (constant entropy density) and isothermal elastic compliances.

σ

}

(20)

(9)

T, E

}

}

T

σ

σ

Generalized Thermostatics and correlation of Physical properties 83

Table 4.4 in conformable matrix order. To use the table, one only needs to replace the symbols by their respective matrices and carry out the multiplication as indicated. The tilde appearing above some of the symbols indicates the transpose of the normal matrix form. This may be illustrated by expanding Eq. (4.75), which is Eq. (17) in Table 4.4 (all at constant B), as follows:

α 1 α 1 d11 α α d 2 2 12 α 3 α 3 1 d13 − = − κ 0 d14 α4 α4 α α d 5 5 15 α6 α6 d16 P E

d21 d22 d23 d24 d25 d26

d31 d32 χ −1 d33 11 χ −1 d34 12 χ −1 d35 31 d36 T

χ −1 12 χ −1 22 χ −1 23

χ −1 p1 31 χ −1 p2 . 23 χ −1 p3 σ 33 T,σ

(4.76)

Keep in mind that crystal symmetry considerations can greatly reduce the number of property components needed for use in equations of the type just given and, as a consequence, greatly reduce the matrix calculation time and effort to obtain a result. The matrix equations in Table 4.4 may be used to obtain order-of-magnitude values for the differences between clamped and free compliances. However, in using any one equation, great care must be exercised in choosing representative magnitudes of the properties. Remember that the values of the components usually differ somewhat within each tensor and that these magnitudes my vary dramatically from crystal to crystal if, in fact, they exist at all by reason of normal crystal and magnetic symmetry. It can be easily verified that the inverse of Eq. (4.69) is

R α, a )β − ( R α, a )b = − (R α, b )b (C α, b )b ( R β , α )b

(4.77)

giving the difference between free and clamped rigidity coefficients. In the case of rigidities, it is required that all other extensive parameters c, d, …, and so forth. be held constant and that b and β be conjugate parameters. This also leads to 24 equations of the type shown in Table 4.4. • • • •

85

chapter 5

The Dependent Coupled Effects and the Interrelationships Between First-Order Tensor Properties— Use of Interaction Diagrams The independent principal and coupled first-order effects are featured in Table 4.3, which gives the component arrangement of the general compliance matrix. The four principal effects are those relating the conjugate parameters along the leading diagonal (the shaded regions) and possess thermodynamic self-symmetry. The six coupled effects are the off-diagonal regions in Table 4.3 and relate intensive parameters to nonconjugate extensive parameters—the opposite being true for the general rigidity matrix. Consequently, off-diagonal effects exhibit no self-symmetry. However, they do possess thermodynamic tensor symmetry expressed by the six Maxwell relations in Section 4.5.2 and by Eqs. (4.41a) and (4.43a). For this reason, they are labeled independent coupled effects.

5.1

THE DEPENDENT COUPLED EFFECTS

Additional coupled effects relating any two intensive parameters (or two extensive parameters) can be defined by suitable choice of the thermodynamic potentials given in Table 4.2 followed by application of Stoke’s theorem (actually Green’s theorem in a plane) discussed in Section 4.4. As an example, suppose it is desired to equate the isothermal elastocaloric coefficient (∂s / ∂ε )T to the isometric thermal stress coefficient (∂σ / ∂T )ε at constant P and B. For this purpose, φ7 in Table 4.2 must be used together with Stoke’s theorem. Thus, for dφ7 = - s d T + E d P – M d B + σ d e, we have

∂ 2φ 7 ∂ 2φ 7 = ∂ ε ∂T ∂ T ∂ ε P ,B

∂ ∂φ ∂ or 7 = ∂ ε ∂ T ∂ T

∂φ 7 ∂ ε

, P ,B

86 Tensor properties of solids

with the result that ∂s ∂ε ij

T,P ,B

∂σ = − ij ∂T

( )

= t ij P ,B,ε

P ,B

There are many other examples of dependent coupled effects. In fact, an examination of Table 4.2 will indicate that there are four sets of clamped and/or free conditions for each of the six dependent coupled effects and their inverse, leading to a total of 48 equations of the type exemplified above. Thus, the choice of the thermodynamic potential used to obtain a given Maxwell relation will depend not only on the particular coupled effect involved but on what parameters are desired to be held constant. For the sake of illustration here, let us require that all effects be defined in such a way that only the intensive parameters are held constant. By using just four thermodynamic potentials φ2, φ3, φ4, and φ5, the following six Maxwell relations, representing the six additional coupled effects, are given in the order of increasing tensor rank.

∂ Pi ∂s

∂s ∂ M i

∂s ∂ε ij

∂ Mj ∂ P i

E,B,σ

∂εjk ∂ P i

∂T = − ∂ Ei

T ,E,σ

T,E,B

∂εjk ∂ M i

B,σ

s ,B,σ

∂B = − i ∂T

= (ηi )

(from φ3)

(5.2)

∂σ = − ij ∂T

= t ij

( )

(from φ2)

(5.3)

( )

(from φ4)

(5.4)

( )

(from φ4)

(5.5)

(from φ3)

(5.6)

E,σ

E ,M,σ

E,B,ε

E,B

∂E = − i = υij ∂ Bj T ,P ,σ T ,B,σ

T ,B,σ

T ,E,σ

(from φ5) (5.1)

= ( hi )

∂ Ei = − ∂σ jk

= εijk T,P ,B

∂ Bi = − ∂σ jk

T ,σ

T ,B

( )

= mijk T,E,M

T,E

The inverse of each of the above relations is readily obtained from a different thermodynamic potential chosen from the same group φ2, φ3, φ4, and φ5. For example, (hi-1)B,σ results from φ4.

Dependent Coupled Effects 87

5.2

INTERRELATIONSHIP BETWEEN FIRST-ORDER PROPERTIES—USE OF INTERACTION DIAGRAMS

An inspection of the general interaction diagram in Figure 1.1 reveals the important fact that the six interaction effects in Eqs. (5.1)–(5.6) are not independent effects because each can be expressed in terms of the first-order properties defined in Section 4.5. To illustrate, consider the interaction diagram in Figure 5.1 representing (hi)B,σ in Eq. (5.1) for which the arrows point toward the dependent variable. From Figure 5.1, there results the equation

∂ T ∂ T ∂ s = ∂ Ei ∂ s ∂ Ei

or

− ( hi )

B,σ

B,σ

T = σ pi C B,σ

(5.7)

giving an additional expression for the dependant pyroelectric effect vector, all at constant B and σ. But it is easily verified that three other interaction diagrams shown in Figure 5.2 can also be used to describe hi , leading to the three additional equations that follow, all at constant B and σ. −hi = κ 0 p−j 1 χ ji = qj−1 λ ji = α jk−1 d jki B,σ

(5.8) Similarly, the interaction diagram shown in Figure 5.3 represents the Maxwell relation in Eq. (5.4) for the dependent coupled effect -νij = (∂Ei / ∂Bj)P. From this diagram, there results the equation −ν j = p−1 q i j T , σ i

(5.9)

at constant T and σ and involving the outer or dyadic product pi-1qj . However, it is clear that three other equations for νij can be derived from the three interaction diagrams given in Figure 5.4. Three additional equations are −1 λ−1 λ = µ−1 − νij = κ −1 ψ = d i−1kl Qklj 0 χ ik kj 0 ik kj

(5.10)

all at constant T and σ. T/Cρ

T

s

−h p E FIGURE 5.1: Interaction diagram for dependent coupled effect h in Eq. (5.1) at constant B and σ.

88 Tensor properties of solids

T

T –1

p

−h E

κ 0χ

T

−h P

−h

q–1

E

α–1

E

λ

M

d

ε

FIGURE 5.2: Additional interaction diagrams representing the dependent coupled effect h in Eq (5.1), all at constant B and σ.

Following the same procedure, the four expressions for each of the remaining four dependent coupled effects are readily obtained. These, together with those illustrated previously, are given by the following six sets of equations all given in conformable matrix order:

~ − h = (T /Cσ ) p = κ 0 χ p−1 = λ q−1 = dα −1

(B,σ constant)

(5.11)

− η = (Cσ / T ) q−1 = λ−1 p = µ0ψ −1 q = Q−1α

(E,σ constant)

(5.12)

~ ~ − t = (Cσ / T )α −1 = d −1 p = Q−1 q = s−1α

(E, B constant)

(5.13)

~ − ν = p−1 q~ = κ 0−1 χ −1λ = µ0−1 λ−1ψ = d −1 Q

(T,σ constant)

(5.14)

~ = κ −1χ −1d = λ −1Q = d −1 s − ε = p−1α 0

(T, B constant)

(5.15)

− m = q−1 α~ = λ−1 d = µ0ψ −1 Q = Q−1s

(T, E constant)

(5.16)

The various tensor properties are used in the above six sets of equations to represent the dependent coupled effects defined by Eqs. (5.1)–(5.6) in Section 5.1. The tilde (~) appearing above some of p–1

s

E q

−υ B

FIGURE 5.3: Interaction diagram for dependent coupled effect υ in Eq. (5.4) at constant T and σ.

Dependent Coupled Effects 89

E

−υ

(κ 0χ)–1

P

E

λ–1

−υ

λ B

E

B

ψ /µ 0

−υ M

d –1

B

Q

ε

FIGURE 5.4: Additional interaction diagrams representing the dependent coupled effect υ in Eq (5.4), all at constant T and σ.

the property symbols indicates the transpose of the normal matrix form of the tensor. The normal matrix dimensions (rows × columns) for first- and third-rank tensors are (3 × 1) and (3 × 6), respectively. The normal matrix dimensions for a second-rank tensor property are either (3 × 3) or (6 × 1), the latter being the column form of symmetrical second-rank tensor properties such as α, χ and ψ, all of which are polar in character. As defined by Eqs. (4.57) in Section 4.5, the magnetoelectric susceptibility λ is an asymmetrical axial–magnetic second-rank tensor and has normal matrix dimensions of (3 × 3). However, unfolded according to arrays given by Eqs. (4.59) and (4.60), it would be represented as a (9 × 1) column matrix with axial character. Because the properties q, λ, and Q are axial–magnetic (first-, second-, and third-rank tensors, respectively), the dependent coupled effects η, ν, and m are also axial–magnetic in tensor character. The three remaining dependent coupled effects are polar tensors. The six sets of equations, Eqs. (5.11) to (5.16), have some important uses. First they can be used to obtain the components for any dependent coupled tensor property from known components of the more common first-order properties defined in Section 4.5. As an example, suppose it is desired to know the six components of the isometric thermal stress coefficient tij given by Eqs. (5.13) and determined at constant E and B fields subjected to a particular crystal. If the heat capacity Cσ and coefficients for thermal expansion αij are known for the crystal, as they commonly are, or if the piezoelectric moduli d and the pyroelectric coefficients p are known, then Eqs. (5.13) give two alternatives for the determination of tij at constant E and B.

t1 t 2 t C − 3 = σ t 4 T t 5 t 6

α −1 d −1 11 1 −1 −1 α d 2 21 α −1 d −1 3 31 −1 = −1 α d 4 41 α −1 d −1 5 −1 51 −1 α 6 d 61

−1 d 12 d −1 22 −1 d 32 −1 d 42 −1 d 52 −1 d 62

−1 d 13 −1 d 23 p 1 d −1 33 p −1 2 d 43 p −1 3 d 53 d −1 63

(5.17)

90 Tensor properties of solids

~ Here, it should be understood that quantities such as d -1 represent the component inverse (reciprocal) of its transpose, a two-stage operation from the normal (3 × 6) form. There are many other such examples, including the inverse of the six dependent coupled effects given by Eqs. (5.11)–(5.16). For example, with reference to Eq. (5.3), the components of the effect (∂Ti / ∂σij)s , which describes the adiabatic application of stress, can be obtained by taking the inverse of Eq. (5.17) to give (∂Ti / ∂σij)s = -(T / Cσ)αij all at constant E and B. These same results can also be obtained from the application of Stoke’s theorem to the generalized enthalpy, φ5 = h given in Table 4.2, followed by the appropriate interaction diagram. Another important use of the six sets of equations, Eqs. (5.11)–(5.16), is to interrelate the various first-order effects. Suppose, as a typical example, it is desired to find the components of the magnetoelectric susceptibility λ for a particular crystal under conditions of constant T and σ. If the components of the dielectric susceptibility χ, those of the piezoelectric coefficient d, and those of the piezomagnetic coefficient Q are all known for a particular crystal, Eqs. (5.14) yield the result ~ κ −1 χ−1 λ = d −1 Q 0

(5.18)

Then, solving for λ gives

χ χ d −1 χ 11 11 31 12 −1 λ = κ 0 χ χ χ d 21 23 22 12 χ χ χ d −1 31 31 33 23

−1 d 12 d −1 22 −1 d 32

d −1 13 d −1 23 d −1 33

d −1 14 d −1 24 −1 d 34

−1 d 15 d −1 25 d −1 35

Q11 Q −1 21 d 16 Q31 d −1 26 Q 41 d −1 36 Q 51 Q61

Q12 Q22 Q32 Q42 Q52 Q62

Q13 Q23 Q33 Q43 Q53 Q63

(5.19)

where λ is given generally as an asymmetrical (3 × 3) matrix. If, however, all components of the four effects are known, then Eq. (5.18) could be used to check the internal consistency of the tensor properties involved. This internal consistency check can be used on other interrelated first-order effects.

5.3

THE GRÜNEISEN TENSOR

There are other interaction effects that may be deduced from the interaction diagram in Figure 1.1, and the Grüneisen tensor is one such example. The Grüneisen parameter can be used to show that the quantity (Cε)-1cα remains constant as the temperature T is changed. In its classical form, the Grüneisen parameter is represented by the relation

∂P γ = −V ∂ U V

(5.20)

Dependent Coupled Effects 91

Here, P is the pressure, U is the internal energy, and V is the volume, which is held constant. This equation may be written in a more general form, applicable to crystal systems, if -P is replaced by σij, dU is replaced by Vdu, and V is replaced by strain to give the Grüneisen tensor as

∂σ γ = ij . ij ∂ u ε

(5.21)

But in the absence of any polarization and magnetization (P and M are zero under constant E and B) and at constant strain, such that no mechanical work is done, we recognize that du = Tds for any process in which reversible heat is absorbed by the system. Therefore, Eq. (5.21) becomes

γ = ij

1 ∂σ ij , =γ ji T ∂s ε

(5.22)

indicating that the Grüneisen tensor is proportional to the inverse of the isometric piezocaloric coefficient αij-1 (see Eqs. (4.55)), which is symmetrical. Shown in Figure 5.5 is the interaction diagram that is descriptive of the Grüneisen parameter as presented in Eq. (5.22). Here, as before, the arrows point toward the dependent variable. From the diagram, there results the tensor equation (note that the T ’s cancel)

γ ij =

1 ∂σ ij = ( 1 /Cε ) cijkl α kl T ∂ s ε

(5.23)

all taken at constant E, B, and ε, and where Cε represents the heat capacity at constant strain, αkl is the thermal expansion tensor, and cij represents the elastic stiffness moduli. The properties Cε, αkl, and cijkl can all be obtained in the region of zero strain, P and M, which satisfies the condition of constant strain, and constant E and B.

T

T/C ε

s

α−1 α

σ

c

ε

FIGURE 5.5: Interaction diagram descriptive of the Grüneisen parameter.

92 Tensor properties of solids

Equation (5.23) may be represented in matrix form by

γ i = (Cε )−1 cij α j

(5.24)

or in expanded form shown in Eq. (5.25). This holds generally for any of the seven crystal systems with the proper choice of cij and αj,.

γ 1 c11 c12 c13 γ c 22 c 23 2 γ 3 c33 −1 = (Cε ) γ 4 γ Sym 5 γ 6

c14 c 24 c34 c 44

c15 c 25 c 35 c 45 c 55

c16 α 1 c 26 α 2 c 36 α 3 c 46 α 4 c 56 α 5 c66 α 6

(5.25)

Of particular interest is the Grüneisen tensor specified for the cubic crystal system. See Section 6.2.5 and Table 6.3 for cubic elastic stiffness moduli. In expanded form, we can write

γ 1 γ 2 γ 1 γ = 3 = 0 Cε 0 0

c 11 c12 c 12 0 c 11 c 12 0 c11 0 c 44 Sym.

0 0 0 0 c44

0 α 1 1 0 α 0 α α (c11 + 2c12) 1 = , 0 0 Cε 0 0 0 0 c 44 0 0

(5.26)

giving the six components of γ . From Eq. (5.26), it follows that the Grüneisen invariant is

γ=

αK γ 1 α (c 11 + 2c 12) α = = = 3Cε 3 3Cε ( s 11 + 2 s 12) Cε

(5.27)

which is the classical result, with K = (c11 + 2c12) / 3 being the bulk elastic modulus for the cubic crystal system. The quantity K is also the reciprocal of the volume compressibility. Because of its close relationship with stress (or strain), the Grüneisen parameter may be decomposed into spherical and deviatoric components given by where γij* = λij - γ is the Grüneisen deviator.

γ ij = γ δ ij + γ i*j

(5.28)

Dependent Coupled Effects 93

There are other ways of representing the Grüneisen parameter as can be seen from five of the six dependent coupled effects given by Eqs. (5.11)–(5.13), (5.15), and (5.16). Keep in mind from Figure 5.5 that the Grüneisen tensor is the inverse of the piezocaloric coefficient, αij-1. However, most of these other expressions involve axial–magnetic and/or first-rank property tensors that greatly restrict their application in obtaining the components of γij for many crystals. Eqs. (5.11) and (5.13) would appear to be the most useful as alternative means of representing the Grüneisen tensor. • • • •

95

chapter 6

Third- and Fourth-Rank Tensor Properties—Symmetry Considerations Before we can discuss the second- and higher-order effects presented in the next chapter, it is necessary to lay a proper foundation for that discussion. The best means of accomplishing this is to revisit the third- and fourth-rank tensor properties defined earlier in Section 4.5. We do this by considering, as good examples, the piezoelectric and elastic effects.

6.1 DIRECT AND CONVERSE PIEZOELECTRIC EFFECTS Beyond mere definitions as in Eqs. (4.61) and (4.62), little was said about the direct or converse piezoelectric coefficient. It is important that these subjects be covered at this time because they illustrate the typical symmetry and transformation characteristics displayed by several other thirdrank polar tensor properties.

6.1.1 Direct Piezoelectric Effect When a stress σij is applied to certain crystals, they will develop a total electric dipole moment per unit volume ( polarization) Pi proportional to that stress as represented in tensor subscript notation by

Pi = dijkσjk

(i, j, k = 1 - 3)

(6.1)

The effect represented by Eq. (6.1) is called the direct piezoelectric effect, and dijk are the piezoelectric moduli. Thus, dijk is a third-rank polar tensor property relating a vector to a second-rank tensor, hence, a vector-tensor property. If only “pure” stresses (no body torques) are applied, then σjk = σkj , which allows dijk = dikj = dim and permits us to write the direct piezoelectric effect in the contracted form

Pi = dimσm

(i = 1-3; m = 1- 6),

(6.2)

96 tensor properties of solids

thereby reducing the number of independent components of dijk from 27 to 18 according to Eq. (2.30). Thus, to convert between tensor subscript notation and matrix notation, the stress components become

σ 1 σ6 σ2 ↔ Sym.

σ5 σ4 σ3

σ 11 σ 12 σ 31 σ22 σ23 Sym. σ33

.

(6.3)

However, because stress is a symmetric second-rank tensor σjk = σjk , we follow the tensor-to-matrix conversion rule (recommended in “Standards on Piezoelectric Crystals,” see Endnotes)

d ijk = d im 2d ijk = dim

for

m =1− 3

for

m = 4 − 6

(6.4)

to avoid the appearance of factors of 2 in Eq. (6.2) in terms for which m = 4, 5, and 6. As a result, we represent Eq. (6.2) as P = d:σ or in matrix notation as P = dσ.

(6.5)

Recall that the double dot (:) indicates a double contraction product as in Eq. (2.47). In expanded form, the three components of P in Eq. (6.5) can be written in the conformable matrix array form given by

P1 P = 2 P3

d 11 d 21 d 31

d12

d13

d14

d15

d 22

d 23

d 24

d 25

d32

d 33

d 34

d 35

σ1 σ d16 2 σ d 26 3 σ d 36 4 σ 5 σ6 .

(6.6)

Here, σ1, σ2, and σ3 are the tensile stresses (positive by convention), and σ4, σ5, and σ6 are shear stresses, with the understanding that σ23 = σ32 = σ4, σ31 = σ13 = σ5, and σ12 = σ21= σ6. Shown in Table 6.1 are five common stress arrays. Note that for hydrostatic pressure p = -σ applied on each of the axis normals. The transformation law for piezoelectric moduli, d, can now be established. First, let P = dσ be true relative to the “old” axes and let P ′ = d ′σ ′ hold relative to a “new” set of axes. Then, because P and σ transform as P ′ = aP and σ ′ = ασ or σ = α −1 σ ′, respectively, it follows that

Third- and Fourth-Rank Tensor Properties 97

TABLE 6.1: Sample stress arrays assuming a symmetric stress tensor σij = σji Uniaxial stress

Biaxial stress

Hydrostatic pressure

Pure shear stress

σ1 0 0 0 0 Sym. 0

0 0 σ1 σ2 0 0 Sym.

0 0 − σ −σ 0 − σ Sym.

− σ 0 0 0 σ 0 0 0 σ 0 = 0 0 Sym. Sym.

P ′ = aP = adσ = adα −1σ ′ = d′σ ′

from which we conclude that

d′ = adα −1,

(6.7)

where α is the quadratic transformation form as presented in Eq. (2.22). Equation (6.7) is the appropriate transformation law for the piezoelectric moduli and is identical to Eq. (2.31), assuming ∼. that stress is a symmetrical second-rank field tensor, σ = σ

6.1.2 Converse Piezoelectric Effect When an arbitrarily oriented electric field Ei is applied to a piezoelectric crystal, the shape of the crystal changes slightly, that is, a strain is produced that is proportional to the electric field strength. This is the converse piezoelectric effect expressed by

εjk = dijkEi

(i, j, k = 1-3).

(6.8)

As a result, Eq. (6.8) is succinctly represented by ε = d ⋅ E or simply as

~ ε = dE

(6.9)

in conformable matrix form. The single dot (⋅) indicates a single contraction product as in Eq. (2.46). The converse piezoelectric effect is also called the first-order electrostrictive effect, and dijk are the first-order electrostrictive moduli. From Eqs. (4.61) and (4.62), it is clear that the direct and converse piezoelectric moduli are numerically equal.

98 tensor properties of solids

Because strain is usually a symmetrical second-rank tensor, εjk = εjk, the tensor symmetry for dijk becomes dijk = dikj = dim, which permits Eq. (6.8) to be written as

εm = dimEi

(i = 1 - 3; m = 1 - 6).

(6.10)

∼ The transpose of d, expressed as d in Eq. (6.9), indicates that its rows and columns of the normal form in Eq. (2.30) must be interchanged to a 6 × 3 matrix if the product of Eq. (6.9) is to be conformable. Thus, Eq. (6.9) is written in extended matrix form as

ε1 ε 2 ε3 = ε4 ε 5 ε 6

d11 d 12 d 13 d 14 d 15 d 16

d 31

d 21

E d 33 1 ~ E = d E. d 34 2 E 3 d 35 d 36

d 22

d 32

d 23 d 24 d 25 d 26

(6.11)

Equation (6.11) is valid because the symmetric part of the strain tensor εjk, defined by Eq. (2.17), is

εjk =

1 2

( εjk + ε kj ) ,

(6.12)

which, in turn, permits the strain matrix to be given by

ε11 Sym.

ε12 ε22

ε 11 ε23 = ε33 Sym. ε31

1 2

(ε 12 + ε21 )

1 2

ε22

1 2

(ε 31 + ε 13 )

(ε 23 + ε 32 ) . ε 33

(6.13)

The tensor-to-matrix conversion scheme for strain now becomes

ε11 Sym.

ε12 ε22

ε1 ε23 → Sym. ε33 ε31

1 2

ε6

ε2

1 2 1 2

ε5

ε4 ,

ε 3

(6.14)

where ε1, ε2, and ε3 are the elastic tensile strains or stretches, and the three remaining, ε4, ε5, and ε6, are the elastic shear strains. As a result of the conversion scheme of Eq. (6.14), the shear strain components of Eq. (6.10) will have factors of ½ on both sides of the equations that cancel. This

Third- and Fourth-Rank Tensor Properties 99

permits Eq. (6.11) to be written in simple two-subscript form exclusive of the factors of 2 in the shear components that would otherwise be present. As it turns out, matrix shear strain is identical to engineering shear strain (i.e., ε4 = γyz, ε5 = γzx, and ε6 = γxy ). The antisymmetrical part of εjk is the axial second-rank tensor given by ϖjk = − 21 (εjk − εkj) which is the rotation resulting from elastic shear. The transformation law for converse piezoelectric moduli, d, is now established in a manner ∼ similar to that for the direct effect given earlier. First, let ε = d E be true relative to the “old” axes and ∼ let ε ′= d ′E ′ hold relative to a “new” set of axes. Now, because ε and E transform as ε ′= α∼ -1ε and ∼ ∼ ∼ E ′ = aE or E = a∼E ′ (a-1 = a∼ ), respectively, it follows that ε ′ = α∼ -1ε = α∼ -1 d E = α∼ -1 d a∼ E ′ = d ′E ′, from which we conclude that ~ ~−1 ~ ~ d′=α d a .

(6.15)

∼ -1ε, results from the tensor-to-matrix converThe transformation for matrix shear strain, ε′ = α sion rule given by Eq. (6.14). Note that α∼ -1 requires two separate operations because α∼ ≠ α -1 in general.

6.1.3 Crystal Symmetry Considerations The method of direct inspection can be used to determine the effect of crystal symmetry on the components of the third-rank tensor properties. To do this, the full tensor subscript notation must be used and then only on crystal systems other than the trigonal and hexagonal crystal systems as explained in Section 3.6. Application of Neumann’s principle to the direct (or converse) piezoelectric moduli, dijk, results in dijk = dijk d = − = 0 .. dijk ijk

(6.16)

For example, all holohedral crystal systems, those represented as Xin Table 3.6, are centrosymmetrical, and as a result, dijk = −dijk = 0. Thus, the 11 centrosymmetrical crystal groups will be lacking in all piezoelectric moduli. To illustrate, we apply Neumann’s principle to the 222 crystal group. By using Table 3.6, we observe that the 222 group requires the use of generating matrices s(2) and s(3). From Table 3.5, the transform of axes are given in compact form according to (2)

s

1 → −1 1 → −1 (3) → 2 → 2 and and s → 2 → −2 3 → −3 3 → 3

(6.17)

100 tensor properties of solids

and are applied in any sequence. Applying s(2) first, it is clear that dijk = 0 for all moduli containing an odd number of 1’s and/or 3’s. Application of s (3) requires that dijk = 0 for all moduli for which there is an odd number of 1’s and/or 2’s. Therefore, the only moduli to survive are those containing all three, 1, 2, and 3 in any order. As a result, the array of piezoelectric moduli becomes

d 111 d 122 d 133 d 123 d 131 d 112 d 211 d 222 d 233 d 223 d 231 d 212 d 311 d 322 d 333 d 323 d 331 d 312 ⇓

0 0 0 0 d 14 0 0 0 0 0 d 123 0 0 0 0 0 d 0 = 0 0 0 0 d 25 0 231 0 0 0 0 0 d 312 0 0 0 0 0 d 36

(6.18)

in both three- and two-suffix notation. Application of Neumann’s principle to the trigonal or hexagonal crystal systems requires the “brute-force” method involving Eq. (6.7) for all threefold and sixfold rotations.

6.1.4 Brute-Force Method for the Trigonal and Hexagonal Classes— The Piezoelectric Moduli 1. If generating matrices other than s(7) are involved in the particular crystal class, apply them first each in turn by using the method of direct inspection to obtain a simplified array of the moduli. 2. By using the appropriate transformation law, for example, Eq. (6.7), complete the matrix calculations with the generating matrices s(7) and σ ( 7) to obtain a set of equations for the new property moduli. 3. As a final sep, equate each old modulus with the new and solve the resulting equations simultaneously for the moduli appropriate for the given crystal class. As an example, let us apply Neumann’s principle to the hexagonal class 6. From Table 3.6, we see that this requires the application of generating matrices s(3) ⋅ s(7) = s(14). To simplify the calculations, it is advantageous to apply s(3) first, then follow with s(7) as required by the brute-force method. From generating matrices given by Eq. (6.17), application of s(3) allows the dijk to survive only for moduli with an odd number of 3’s, a total number of eight independent moduli. When this is done, application of s(7) to the piezoelectric transformation law given by Eq. (6.7) takes the form

Third- and Fourth-Rank Tensor Properties 101

[dijk] s

s(7)

3 − 12 2 d′ = 3 1 − 2 − 2 0 0

0 0 1

(3)

(σ (7)) −1

0 0 d 123 d 131 0 0 0 0 d 223 d 231 0 0 d 311 d 322 d 333 0 0 d 312

41 43 0 0 0 − 43

3 2

3 4

0

0

0

1 4

0

0 1

0 0

0 − 23 0 0

0

0

− 12

0

0 −

3 4

0

3 2

0

3 2

0

− 12

0

0

− 12

. (6.19)

When the matrix multiplication operations of Eq. (6.19) are carried out, there result the following equations relating the old moduli to the new moduli: d123 =

d 123 4

−

3 1 −d 3 d223 − 131 + d231 3 4 2 2 2

d131 =

1 −d123 3 + d223 2 2 2

d223 =

d 3 1 d123 + 223 − 4 4 2

d231 =

1 2

3+

d131 4

−

3 d 4 231

− 3 d d131 − 231 3 2 2

− 3 d d123 − 223 2 2

3+

d 3 d131 231 4 4

d311 = d322 =

d311 4

+

3 3 d − d 4 322 4 312

d 3 3 d311 + 322 + d 4 4 4 312

d333 = d333 d312 =

d 3 3 d311 − d322 − 312 2 2 2

Solving these eight equations simultaneously gives the following class 6 piezoelectric moduli in both three- and two-suffix notation where the eight independent moduli in Eq. (6.19) have been reduced to four in Eq. (6.20).

0 0 d123 d131 0 0 0 0 d 14 0 0 0 d 131 −d 123 0 = 0 0 0 d 15 0 d 311 d 311 d 333 0 0 0 d31 d31 d33 0

d 15 0 −d 14 0 0 0

(6.20)

From Table 3.6, we note that the generating matrices for class 622 are s(12) and s(14). Because the moduli arrays of Eq. (6.20) result from the application of s(14), there remains only the application of s(12) = s(1) ⋅ s(4) to the three-suffix form of Eq. (6.20) to obtain the moduli for class 622. From Table 3.5 for s(12) and using the method of direct inspection, it is clear that the only moduli to survive

102 tensor properties of solids

are those for which an odd number of 1’s exists. Thus, d131 = d311 = d333 = 0, resulting in the array for class 622 given by 0 0 0 0 0 d14 0 0 0 d123 0 0 0 0 −d123 0 = 0 0 0 0 0 0 0 0 0 0 0 0 0 0

0 0 . 0

0 − d14 0

(6.21)

Continuing on to class 6mm, we see from Table 3.6 that the generation matrices required for this crystal class are s(3), s(4), and s(7). So there remains only the application of s(4) in Table 3.5 to the three-suffix result of matrix arrays (6.20). When this is done, the only moduli to survive are those for which an even number of 1’s or no 1’s exist. Thus, d123 = 0 in arrays (6.19) resulting in the moduli arrays for class 6mm given by 0 0 0 d131 0 0 0 0 0 0 0 0 d131 0 0 = 0 0 0 d15 0 0 0 d 31 d 31 d 33 0 d 311 d 311 d 333 0

0 0 0

d15 0 0

(6.22)

By applying similar analyses to the 32 crystal classes, there result the matrices for the direct and converse piezoelectric moduli given in Table 6.2 where dijk = 0 for all centrosymmetrical classes. TABLE 6.2: Piezoelectric moduli for both the direct and converse effects Triclinic

Class 1 d 11 d 12 d 21 d 22 d 31 d 32

d 13

d 14

d 23 d 24 d 33

d 34

d 15

d 16

d 25 d 26 d 35 d 36

Class 1 centrosymmetrical, dijk = 0 Monoclinic Class 2 (2 x2)

0 d21 0

0

0

d 14

0

d 22

d23

0

d 25

0

0

d34

0

Class m (m ⊥ x2) d 16

0 d 36

d 11 d 12 0 0 d 31 d 32

Class 2 / m centrosymmetrical, dijk = 0

d 13 0 d 33

0

d 15

d24 0 0 d 35

0

d 26 0

Third- and Fourth-Rank Tensor Properties 103

TABLE 6.2: (continued) Orthorhombic Class 222

Class 2mm 0 0 0 0 d 31 d 32

0

0

d 15

0

d 24

0

d 33

0

0

0

0 0 0 0 0 0 0 0 0

0 0

d 14

0

0

0

d25

0

0

0 d36

Class mmm centrosymmetrical, dijk = 0 Tetragonal _ Class 4

Class 4 0 0 0 0 0 0 d 31 d 31 d 33

d14 d 15 0

d 15 0 −d 14 0 0 0

0 0 0 0 d 31 −d 31

0

0

0

0 d 36

d 14 d 15 −d 15 d 14 0 0 0

Class 4 / m centrosymmetrical, dijk = 0 _ Class 42m

Class 4mm

0 0 d31

0

0

0

0

d 31 d 33

0 d 15 0

0 0 0 0 0 0 0 0 0

d15 0 0 0 0 0 Class 422

0 0 0 0 0 0 0 0 0

d 14 0 0

0

0

−d 14 0 0 0

Class 4 / mmm centrosymmetrical, dijk = 0

d 14

0

0

0

d 14

0

0

0 d 36

104 tensor properties of solids

TABLE 6.2: (continued) Trigonal Class

Class 3

d 11 − d 22 d 31

−d 11

d 22 d 31

0 0 d 33

d 14 d 15 0

d 15 _ d 14 0

0 − d22 d31

_ 2d 22

−2d 11 0

3m

(m ⊥ x1)

0

0

0

d15

−2d 22

d 22

0

0

0

d31

d 33

d 15 0

0

0

Class 3 centrosymmetrical, dijk = 0 Class 32 (quartz)

d 11 0 0

−d 11 0 0

0

d 14 0 0 0 0

0 − d 14 0

0

− 2d 11

0

Class 3 m centrosymmetrical, dijk = 0 Hexagonal

_ Class 6

Class 6 0 0 0 0 0 0 d 31 d 31 d 33

d 14 d 15 0

d 15 0 −d 14 0 0 0

d 11 −d 22 0

_d

11

d 22 0

0 0 0 _ 2d 22 0 0 0 _ 2 d 11 0 0 0 0

Class 6 centrosymmetrical, dijk = 0 Class 6mm (same as 4mm )

0 0 d31

0

0

0

d 15

0

0

d 15

0

d 31 d 33

0

0

Class 622 (same as 422)

0

0 0 0 0 0 0 0 0 0

0 0 _ Class 62m

d 11 −d 11 0 0 0 0

0 0 0

0

0 0 0

−2 d 11

0 0 0

0

Class 6 mmm centrosymmetrical, dijk = 0

d 14 0 0

0

0

−d 14 0 0 0

Third- and Fourth-Rank Tensor Properties 105

TABLE 6.2: (continued) Cubic

_ Class 23 and 4 3m

0 0 0 0 0 0 0 0 0

Class 432

d 14

0

0

0

d 14

0

0

0 d 14

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

Class m3 centrosymmetrical, dijk = 0 Class m3m centrosymmetrical, dijk = 0

To demonstrate the use of the piezoelectric moduli in Table 6.2, we will work a couple of problems involving quartz, which belongs to the crystal class 32. Consider the direct piezoelectric effect represented by Eq. (6.2) as applied to class 32 and the application of normal and shear stresses. Shown in Figure 6.1(a) is the array of piezoelectric moduli for class 32 together with the corresponding polarization and stress components. In Figure 6.1(b) is the stereogram for class 32 giving the x1 and x2 axes in the (0001) plane with its normal along the threefold (optic) axis, x3. Clearly, there are only two independent piezoelastic moduli, d11 and d14. Referring to Figure 6.1 for quartz, a polarization P1 can be produced along the x1 direction under the following conditions: 1. By a tensile stress σ1 applied along the x1, resulting in P1 = d11σ1, where P2 = P3 = 0. 2. By a compressive stress σ2 applied along x1, resulting in P1 = -d11σ2 where P2 = P3 = 0. 3. By a shear stress σ4 = σ23, resulting in P1 = d14σ4, where P2 = P3 = 0. Normal

Shear

{ { σ1

σ2

σ3 σ4

σ5

σ6

P1 d11 –d11 0 d14 0 Along x1 0 d = P2 0 0 0 0 –d14 –2d11 Along x2 P3 0 0 0 0 0 0 Along x3

(a)

y' z,x3 y x2 x,x1

(b)

FIGURE 6.1: (a) Piezoelectric moduli for quartz (class 32) and the corresponding polarization and stress components. (b) Stereogram for class 32.

106 tensor properties of solids

A polarization P2 along x2 can be produced only by negative shear stresses σ31 and σ12 giving P2 = -d14σ31 and P2 = -2d11σ12, where for both P1 = P3 = 0. From Figure 6.1(a), it is evident that a polarization P3 along x3 is not possible under any set of conditions.

6.1.5 Longitudinal Piezoelectric Effect The polarization can be found in an arbitrary direction P1′ according to P1′ = d 111 ′ σ11′ = d 11 ′ σ 1′.

(6.23)

Here, d1′1, measures the longitudinal piezoelectric effect in the x1x2 plane, meaning the charge per unit area on the surface of a plate divided by the force per unit area applied normal to that surface, which is in the 0x3 direction. To find d1′1, we will need to find α -1 by making use of the equations σ = ∼a σ ′a = α -1σ ′, which are the inverse of Eqs. (2.21) and (2.22). Recall that the stress tensor is a symmetric second-rank tensor. Once α -1 is known, then d1′1, can be found from the transformation equation d ′ = adα -1, where a given moduli array is chosen from Table 6.2. As an example, we will find d1′1 for a quartz crystal. Shown in Figure 6.2 is the longitudinal direction 0x′1 and direction cosines relative to a set of coordinate axes such that lie in the (0001) plane of a quartz crystal. Thus, as required, the surface of the crystal must conform to the point group symmetry. Because a polarization cannot be produced alone 0x3, a direction 0x′1 out of the x1x2 plane will produce a polarization only due to the projection of 0x′1 onto the x1x2 plane. Thus, we are entitled, but not required, to set a13 = l3 = 0, not shown in Figure 6.2. To facilitate the calculations, we will make the following transformation simplifications: a11 = l1, a12 = l2, a13 = l3, with mi and ni used for the remaining direction cosines following Eq. (3.24). First, we will find α -1 as follows:

l1 σ =a%σ ′a = l2 l 3

m1 m2 m3

l2 n1 σ 1′ 0 0 l1 n2 0 0 0 m1 m2 n3 0 0 0 n1 n2

l3 l 12 m3 = l1 l2 n l l 3

3 1

l1 l2 l22 l2 l3

l3 l1 l2 l3 σ 1′ . l 2 3

(6.24)

Then, reconfiguring yields the result

σ1 σ2 σ σ = 3= σ4 σ 5 σ6

l12 2 l2 l2 3 l2 l3 l l 3 1 l1 l2

0

0

0

0

0 σ 1′

0

0

0

0

0

0

0

0

0 0 0 0

0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

−1 = α σ′ .

(6.25)

Third- and Fourth-Rank Tensor Properties 107

x2 x'2

x'1

cos–1�2 90 o - θ θ

x3

cos–1�1

x1

0

FIGURE 6.2: Longitudinal direction x1 relative to a set of coordinate axes, where x1 and x2 lie in the (0001) plane of crystal class 32.

Now with α-1 known, we will set up the matrix equation for d ′ = ada-1 where d is the class 32 array obtained from Table 6.2. Thus, there results l1 l2 d ′ = m1 m2 n 1 n 2 l1d11 = m1d11 n1d 11

l 3 d 11 −d 11 0 d 14 m3 0 0 0 0 n 3 0 0 0 0 − l1d11 0 l1d14 −m1d11 0 m1d14 − n1d 11 0 n1d 14

− l2 d14 −m2 d14 − n2d 14

0 −d14 0

0 −2d 11 α −1 = a d α − 1 0

−2l 2 d11 −2m2 d 11 −2n2 d 11

l 12 l 22 l 32 l 2 l3 l3 l1 l1l 2

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 . 0 0 0 0 (6.26)

0 0 0 0 0 0

Therefore, d11′ = l13 d11 − l1 l22 d11 + l1 l2 l3 d14 − l1 l2 l3 d14 − 2 l1 l22 d11

= l13 d11 − 3 l1 l22 d11 = l1 ( l12 − 3 l22 ) d11 ,

(6.27)

which is seen to depend only on d11. Furthermore, from Figure 6.2, it follows that l1 = cosθ and l2 = cos(90° - θ) = sinθ. Therefore, with the help of trigonometric identities, we find d11′ = d11 cos θ (cos2 θ − 3 sin2 θ )

= d11 cos θ (cos2 θ + 3 cos2 θ − 3)

= d11 ( 4 cos3 θ − 3 cosθ ) = d11 cos 3θ .

(6.28)

The result d1′1 = d11 cos 3θ forms a three-petal (each almond shaped) rosette in the (0001) plane, indicating that the polarization is a maximum along the directions x, y, and y ′ spaced 120° apart (see Figure 6.1(b)) and that it is zero at 60° intervals between the x, y , and y ′ directions.

108 tensor properties of solids

6.1.6 Transverse Piezoelectric Effect A similar procedure to that used for the longitudinal piezoelectric effect can be used for the transverse piezoelectric effect. However, the calculations are necessarily made more complex because the direction cosines li , mj , and nk (i, j, k = 1, 2, 3) will, in general, be involved. To demonstrate, let us set up the equations σ = a∼σ ′ a = α -1 σ ′ for the case of a shear stress σ 6 ′ = σ12′ applied to a quartz crystal relative to axes x′1 and x′2 . The results become

l1 σ = a% σ ′ a = l2 l3

m1 m2 m3

n1 0 σ6′ n2 σ6′ 0 n3 0 0

σ 1 0 σ 0 2 σ 0 σ = 3 = σ 4 0 σ 5 0 σ 6 0

0 0 0 0 0 0

l2 0 l1 0 m3 m3 0 n3 n3 0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

l3 2 l1 m1 m3 = n3 Sym.

l1m2 + l2 m1 2 l2 m2

2l 1m 1 0 2l2m 2 0 2l3m 3 0 −1 = α σ′ l2m 3 + l3m 2 0 l3m 1 + l1m 3 0 l1m 2 + l2m 1 σ 6′

l3 m1 + l1m3 l2m3 + l3m2 σ ′ 2 l3 m3

(6.29)

Knowing α -1 permits us to evaluate d ′ = ad α -1, which will be more complex to evaluate than in the case of the longitudinal effect given by Eqs. (6.26), (6.27), and (6.28).

6.2 ELASTICITY The concept of elasticity can best be understood by considering a one-dimensional lattice shown in Figure 6.3. Here, the equilibrium condition is demonstrated in Figure 6.3(a), where the lattice parameter is given by a0. Then, if a tensile force is applied along the 0x direction the atoms are displaced by an amount l = a - a0 to an atom separation of a as in Figure 6.3(b). At a state of equia0

a f

(a)

f (b)

FIGURE 6.3: A one-dimensional lattice. (a) Atoms at equilibrium with lattice parameter a0. (b) Atoms reversibly displaced after the application of a tensile force f along the 0x direction.

Third- and Fourth-Rank Tensor Properties 109

+ Binding Energy 0 E(l)

a0

l

_

(dE/dl) l

=0=

0 Position of stability

Attraction

Force

f(l) 0

Repulsion

l f=0

FIGURE 6.4: Binding energy and tensile force showing position of stability in a one-dimensional lattice.

librium, the force f0 would represent a short-ranged attractive force between atoms along 0x where the lattice parameter between atoms is maintained at a0. The binding energy of the atoms in the one-dimensional lattice is a function of the atom displacement l and is shown in Figure 6.4. Here, at static equilibrium, the minimum in the energy curve occurs at (dE / dl )l = 0 = 0,

(6.30)

for which the applied tensile force f = 0 and where a = a0. So, as f → 0, a position of stability between the atoms is approached. Of course, the force f can be either a tensile force r a compressive force. The convention followed in this text is as follows:

If

f > 0

tensile

a > a0 and

l>0

If

f < 0

compressive

a < a0 and

l < 0.

In any case, the cohesive force between atoms is a reversible function of displacement.

110 tensor properties of solids

6.2.1 Hooke’s Law Assuming that the elastic strain energy E is everywhere a continuous function of displacement l, we can expand E in a Maclaurin series about the state of displacement l = 0, there results

1 d2E dE l + 2 2 dl d l (0)

E ( l ) = E0 +

2 .. . l + . (0)

(6.31)

For very small l, small linear strains exist, and applying Eq. (6.30), we have

E ( l ) ≅ E0 +

1 d2E

l 2 + .... 2 d l 2 (0)

(6.32)

Taking the derivative of Eq. (6.32) with respect to displacement l leads to Hooke’s law given as

f =

d E(l ) dl

d2 E l =Y⋅l, 2 d l (0)

=

(6.33)

where

d2 E = Young's Modulus. Y = 2 d l (0)

(6.34)

Here, Young’s modulus (d2 E / dl 2) is the curvature of the E(l ) versus l curve in Figure 6.4. Thus, the sharper the minimum in the E(l ) versus l curve, the greater will be the Young’s modulus, Y, and vice versa.

6.2.2 Bulk Elastic Behavior Up to this point, we have dealt with a one-dimensional lattice to express the simplest form of Hooke’s law. Now we must move to bulk elastic representations that have practical application. To expand the one-dimensions model to bulk elastic behavior require summing all individual elastic deformations between atoms (neighbors, next nearest neighbors, etc.) taken over all directions in the crystal. Clearly, ∑i( fi = Yli ) applied in this manner would be an impossible task. This apparent dilemma can be overcome by making the following transformations:

f ⇒ σ = stress l ⇒ ε = strain.

(6.35)

Now, the two alternative forms of Hooke’s law may be expressed in terms of the new parameters, σ and ε, as

Third- and Fourth-Rank Tensor Properties 111

σ = c ε , ε = sσ

(6.36)

where

c = E lastic stiffness coefficient (N/m2) S

= E lastic compliance coefficient = c −1.

(6.36a)

Following the developments given in Section 6.1 with regard to stress and strain, we can express Hooke’s law σ = cε in tensor and matrix form, respectively, as

σij = cijkl εkl

(i, j, k, l = 1 - 3)

(6.37)

(m, n = 1 - 6).

(6.38)

and

σm = cmn εn

Here, the first and last suffix pairs of cijkl permit the cmn coefficients to be unfolded according to the following scheme.

Tensor Notation 11 22 33 23, 32 31, 13 12, 21 Matrix Notation 1 2 3 4 5 6

(6.39)

Then, by thermodynamic arguments presented in Section 4.4, we can write

cmn = cnm.

(6.40)

In expanded matrix form, Eq. (6.38) becomes

σ 1 c11 c12 c13 σ c 22 c23 2 σ3 c33 = σ 4 σ Sym. 5 σ 6

c14 c24 c34 c44

c15 c 25 c35 c45 c55

c16 ε1 c26 ε 2 c36 ε 3 ⋅ c46 ε 4 c56 ε5 c66 ε6

(6.41)

where, as before in Section 6.1, σ1, σ2, and σ3 are the tensile stresses (positive by convention) and σ4, σ5, and σ6 are shear stresses, with the understanding that σ23 = σ32 = σ4, σ31 = σ13 = σ5, and σ12 = σ21 = σ6. With the convention used in Eq. (6.14), the strains ε1, ε2 and ε3 are the elastic tensile strains or stretches, and the three remaining, ε4, ε5 and ε6, are the elastic shear strains.

112 tensor properties of solids

The alternative form of Hooke’s law ε = sσ is presented in the tensor form as

εij = sijkl σkl ,

(6.42)

which represents nine equations each with nine terms—a total of 81 sijkl coefficients. Equation (6.42) can be represented in the simplified matrix form

εm = smnσn

(m, n = 1 - 6),

(6.43)

provided that 2’s and 4’s are introduced into the definitions of simn according to the following: sijkl = smn when m and n are 1, 2, or 3 2sijkl = smn when either m and n are 4, 5, or 6 4sijkl = smn when either m and n are 4, 5, or 6. These definitions avoid the appearance of the 2’s and 4’s in Eq. (6.42), thereby making the simplified matrix form possible. Note that in the case of Eq. (6.38), no introductions of 2’s and 4’s were necessary to allow Eq. (6.41). By the thermodynamic arguments presented in Section 4.4, we can write smn = snm ,

(6.44)

giving the expanded matrix form of Eq. (6.43) as

ε 1 s11 s12 s13 ε s22 s23 2 ε3 s33 = ε 4 ε Sym. 5 ε 6

s14 s24 s34 s44

s15 s16 σ1 s25 s26 σ 2 s35 s36 σ3 ⋅ s45 s46 σ4 s55 s56 σ5 s66 σ6

(6.45)

6.2.3 Transformation Laws The transformation laws for the elastic stiffness coefficients and elastic compliances are easily determined by using matrix notation together with the quadratic transformation matrix, α. The reader may find it helpful to review Section 6.1 because it pertains to the transformation laws for the direct and converse piezoelectric effects. Beginning with the stiffness coefficients, the procedure is as follows: Let σ = cε be true relative to the “old” axes and let σ ′ = c ′ε ′ hold relative to the “new” axes. Stress transforms to the “new” axes as

Third- and Fourth-Rank Tensor Properties 113

σ ′ = ασ. Then referring to the developments leading to Eq. (6.15), the strain transforms to the new ∼ -1ε or ε = α ∼ ε ′. Therefore, it follows that σ ′ = ασ = αcε = αcα ∼ ε′ = c ′ε ′, or finally, axes as ε ′ = α ~ . c ′ = α cα

(6.46)

A procedure similar to that for the stiffness coefficients is followed for the elastic compliance coefficients. Let ε = sσ and ε ′ = s ′σ ′ be valid for the old and new axes, respectively. From the pre ∼ -1ε = α∼ -1 sσ = α∼ -1 sα -1σ ′ = s ′σ ′ from which results ceding, σ = α -1σ ′, such that we can write ε ′ = α ~ −1 sα −1 s′ = α ,

(6.47)

∼ . Here, α∼ -1 is the transpose of the inverse of α, two operations. where it is understood that α -1 ≠ α

6.2.4 Elastic Strain Energy Density Referring to the thermodynamic potentials in Table 4.2, the elastic strain energy density can be given by

df = dw = σi dεi = ci j εj dεi

(i, j = 1 − 6)

(6.48)

or

−dg = εi dσi = si j σj dσi

(i, j = 1 − 6)

(6.49)

for a reversible, isothermal deformation in the absence of all electrical and magnetic fields and their conjugate effects. For a linear elastic solid under these conditions, σi dεi = εi dσi. Making use of the substitution property of the Kronecker delta dij (see Section 2.6.3), there results εj = dij εi permitting Eq. (6.48) to be integrated for the elastic strain energy density

wElastic = =

∫ ci

j

1

2

( δij εi ) dεi =

cij εi εj =

1

2

1

2

cij ( δij ε i2 ) + C

σi εi

(i = 1 − 6),

(6.50)

where the constant of integration C = 0 because welastic = 0 if εiεj = 0. For the total strain energy, Eq. (6.50) must be integrated over the volume of the deformed crystal,

ETotal =

∫V σi εi dV .

(6.51)

6.2.5 Effect of Crystal Symmetry Because the procedure to be followed here is similar to that used in Section 6.1 for the piezoelectric moduli, the reader may find it useful to review that material. First of all, it should be recalled that all

114 tensor properties of solids

polar tensors of even rank are “centrosymmetrical.” This means that by Neumann’s principle, their property coefficients are left unchanged by the transformation operation of a center of symmetry. The procedure to be followed for property coefficients of polar fourth-rank tensor properties is as follows: 1. Use the method of direct inspection for all crystal classes for which the s generating matrices, other than s(7), are required as indicated in Table 3.6. This method provides the easiest means of obtaining the independent coefficients of polar fourth-rank tensors. The 10 possible generating matrices are given in Table 3.5 for both s and quadratic σ forms. In applying the direct inspection method to the two suffix coefficient arrays in Eqs. (6.41) and (6.45), the four suffix notation they represent must be kept in mind. Remember that it is actually the four suffix notation to which the method of direct inspection is applied via the tensor/matrix notation of Eq. (6.39). 2. The brute-force method must be used in applying the generating matrix σ(7) to the trigonal and hexagonal crystal systems of polar fourth-rank tensor properties. However, if generating matrices other than s(7) are involved in the particular crystal class, apply them first each in turn by using the method of direct inspection to obtain a simplified array of the moduli. By using the appropriate transformation law, c ′ = α c α∼ or ∼-1sα -1, complete the matrix calculations with the generating matrix σ (7), together s ′ = α with its inverse and transpose as needed, to obtain a set of equations for the new property moduli. As a final step, equate each of the old moduli with the new and solve the resulting set of equations simultaneously for the moduli appropriate for the given crystal class. It is strongly recommended that application of the brute-force method be computer assisted. As an example, let us apply the method of direct inspection to the centrosymmetrical cubic crystal class ||m3|| having the generating (s) matrices s(4) and s(10) given in Table 3.6 and their respective generation operators provided in Table 3.5. Referring to the tensor/matrix suffix notations of Eq. (6.39), we apply the transformation of axes for the generating matrices s(4) and s(10) as follows:

s

(4)

− 1 0 0 = (m ⊥ x) = 0 1 0 0 0 1

Direct inspection method: 1 → -1, 2 → 2, 3 → 3. This means that all c stiffness moduli in Eq. (6.41) containing a single 5 or single 6 (but not containing both) are zero. As examples, c15 = c1131 = 0, c25 = c2231 = 0, c46 = c2312 = 0, and so forth, for a total of eight vanishing coefficients. Application of s(10) then follows accordingly:

Third- and Fourth-Rank Tensor Properties 115

s

(10)

0 1 0 = ( 3[111] ) = 0 0 1 1 0 0

Direct inspection method: 1 → 2, 2 → 3, 3 → 1 and 4 → 5, 5 → 6, 6 → 4. Together with s(4), this means that c16 = c24 = c2223 = 0, c36 = c14 = c1123 = 0, and so forth. Also, c11 = c22 = c33, c44 = c55 = c66 , and c12 = c23 = c31. If, for class ||m3m||, the transformation of axes for s(4) and s(9) together with that for s(10) is applied to the remainder of the cubic classes, the results are found to be the same as above. Thus, the elastic stiffness and compliance coefficients for all classes of the cubic system are given by the following arrays in which there are three independent coefficients, c11, c12 , c44, and s11 , s22 , s44:

c11 c =

c12

c12

0

0

0

s12

s12

0

0

c11

c12

0

0

0

s11

s12

0

0

c11

0

0

0

s11

0

0

c44

0

0

s44

0

c44

0

Sym.

c44

s11 and s =

Sym.

s44

0

0 0 0 s44 0

Continuing in this way, the independent elastic stiffness coefficients are identified for the remainder of the seven crystal systems and are presented in Table 6.3. The case of an isotropic solid is added for completeness and will be considered separately below as an extension of the cubic crystal system. TABLE 6.3: The independent elastic stiffness coefficients for the seven crystal systems with the addition of the case for the isotropic solid Triclinic

c 11

c 12

1, 1 c 13 c 14

c 15

c 16

c 22

c 23

c24

c 25

c33

c 34

c 35 c 36

c44

c 45

Sym.

c55

c 26

c46

c 56 c66

116 tensor properties of solids

TABLE 6.3: (continued) Monoclinic m, 2, 2 / m for diad parallel to x2 c 11 c 12 c 13 0 c 15 0

c 22

c 23

0

c 25

0

c 33

0

c 35

0

c 44

0

c 46

Sym.

c55

0

c 66 Orthorhombic 2mm, 222, mmm c 12 c 13 0 0

c 11 c 22 c 23 c 33 Sym. _ 4, 4, 4 / m c 13 0 0

c 11 c 12 c 11 c 13 c 33 Sym.

0

0

0

0

c 44

0 c 44

0

0

0 0

0

0

0

c 44

0

0 0

Tetragonal c 16 − c 16

0 0 0 c 66

c 55

c 66 _ 4mm, 42m, 422, 4 / mmm 0 c 11 c 12 c13 0 0

c 11

Sym.

c 13

0

0

0

c 33

0

0

0

c 44

0

0

c 44

0 c 66

Third- and Fourth-Rank Tensor Properties 117

TABLE 6.3: (continued) Trigonal

_ 3, 3

c 11 c 12 c 13 c 11 c 13 c 33 Sym.

c 14

−c 14 0 c44

−c 25 c25 0 0 c 44

c 11

0 0 (c 25 ) (c14 ) 1 ( c 11 − c12 ) 2 0

{

_ 3m, 32, 3m

}

c 12

c 13

c 14

0

c 11

c 13

− c14

0

0

0

c 44

0

c 33 Sym.

c 44

( c25 ) → 2s25 , ( c14 ) → − 2s 14

{

}

1 ( c11 − c 12) → 2 (s11 − s12 ) 2

Hexagonal _ _ 6, 6, 6 / m , 6mm, 622, 62m, 6 / mmm 0 c 11 c 12 c 13 0 0

c 11

c 13

0

0

c 33

0

0

c 44

0

Sym.

c 44

0 0 0 1 ( c11 − c12) 2 0

{

}

Cubic _ 23, m3 , 432, 432, m3m , c 11 c 12 c 12 0 0 0 c11 c 12 0 0 0

c 11 Sym.

0

0

0

c 44

0

0 0

c 44

c 44

0 0 0 c ( 14 ) 1 (c 11 − c 12 ) 2 0

{

}

118 tensor properties of solids

TABLE 6.3: (continued) Isotropic

c 11

c 12

c 12

0

0

c 11

c 12

0

0

c 11

0

0

{

1 ( c11 − c12) 2

}

Sym.

{

0

{

0 0 0 0 1 (c 11 − c 12 ) 2 0

1 (c 11 − c12) 2

}

}

{

}

1 (c 11 − c 12 ) → 2( s11 − s12 ) 2

The classes to which a given coefficient array belongs are indicated above the array. Note that the elastic compliance coefficients sij are obtained from the elastic stuffiness coefficients by replacing c by s except where noted by parentheses and braces {x}.

6.2.6 Homogeneous Elastically Isotropic Solids Consider the ′ = σ 6′ to the cubic system, where x′1 , = [110] _ application of a pure shear stress σ 12 ′ = σ 21 and x′2 , = [1 10] as shown by the 45° rotation in Figure 6.5. In the absence of all other stresses, σ ′1 = σ 2′ = σ 3′ = σ ′4 = σ 5′ = 0, the stress tensor transforms as the inverse of Eq. (2.13) or x3, z 450

x2' x2, y

x1, x FIGURE 6.5: Rotation of 45° about the z axis.

x1'

Third- and Fourth-Rank Tensor Properties 119

1 2 a σ ′ a = 1 2 σ =~ 0

−1

2

1

2 0

0 0

0 1

σ6′

0 σ 6′ 1 0

2

1

2

0 − 1 2 1 2 0 0 0

0 0

0

0 = 1

− 1 0 0 0 1 0 σ ′ 6 0 0 0

(6.52) Introducing the results of Eq. (6.52) into Eq. (6.43) for the cubic system yields

s11 εm′ = smn σn′ =

s12

s12

0

0

0 − 1

s11

s12

0

0

0

s11

0

0

0

s44

0

0

s44

0

Sym.

s44

1 0 0 0 0

− ( s11 − s12 ) (s − s ) 11 12 0 σ 6′ = σ 6′ 0 0 0

(6.53)

Then, transforming shear strain to the new axes gives

εi′j = aikajl ε kl or ε12 ′ = a11a21ε 11 + a12a22ε 22 = −ε 11/2 + ε 22 /2.

Therefore, by Eq. (6.53), we have ε′12 = [(s11 - s12) / 2 + (s11 - s12) / 2] σ′12 = (s11 - s12) σ′12 where use of the matrix-to-tensor strain conversion of Eq. (6.14) yields the results

ε 6′ = 2ε 12 ′ = 2(s11 − s12)σ 6′ = s44σ 6′ or s44 = 2(s11 − s12)

(6.54)

as the necessary and sufficient condition for elastic isotropy, in agreement with Table 6.3. Obviously, the application of any other pure shear stress, σ′4 or σ′5 , would lead to the same result. Let us now compare the elastically isotropic compliance array in Table 6.3 with those frequently found in engineering textbooks:

ε1 ε 2 ε3 = ε4 ε 5 ε6

s11

s12

s12

0

0

0

s11

s12

0

0

0

s11

0

0

0

2 ( s11 − s12 )

0

0

2 ( s11 − s12 )

0

Sym.

2 ( s11 −

σ1 σ 2 σ3 σ 4 σ 5 s12 ) σ6

(6.55)

120 tensor properties of solids

ε 1 ε 2 ε 3 = ε 4 ε 5 ε 6

1 / Y

− ν /Y

− ν /Y

1 /Y

− ν /Y 1 /Y

Sym.

0

0

0 σ1

0

0

0

σ2 0 σ3 0 0 1/G 0 0 σ4 1/G 0 σ5 1 / G σ6

(6.56)

A comparison of Eqs. (6.55) and (6.56) indicates the following relationships: s12 = −ν / Y

s11 = 1 / Y

and 2(s11 − s12) = 1 / G,

(6.57)

where Y is Young’s modulus, ν is Poisson’s ratio, and G is thes modulus of rigidity with the combined relation, derived from Eq. (6.57), given by G = Y / {2(1 + ν)} .

(6.58)

Here, Y is a measure of the elongation of an elastically isotropic solid under tension, and ν is a measure of the transverse contraction (at right angles to the elongation). The rigidity modulus measures the stuffiness to shear.

6.2.7 Young’s Modulus in a Particular Direction Consider a bar-shaped crystal of axis 0x1′, along which is applied a unit tensile stress σ 1′ as shown in Figure 6.6.

σ1'

x3 x1'

x3' x2'

x2 x1

(a)

(b)

FIGURE 6.6: (a) Application of a unit tensile stress to a crystal rod along the 0x1′ direction. (b) Orientation of the rod axis 0x′1 relative to reference axes 0xi.

Third- and Fourth-Rank Tensor Properties 121

From Eq. (6.57), Young’s modulus can be defined in the 0x direction ′ as 1 s′11 = 1 / Y = ε 1′ / σ 1′

(6.59)

′ of the rod such that where it is understood that σ 1′ is a unit tensile stress applied along the 0x axis 1 σ 2′ = σ 3′ = σ 4′ = σ 5′ = σ 6′ = 0. Referring to Figure 2.1, let the direction cosines for 0x in ′ Figure 6.6(b) 1 relative to reference axes 0xi be represented as follows: a11 = l1, a12 = l2, and a13 = l3. Then, s′11 is found for any crystal system by Eq. (6.47), which is ~ −1 s α −1 s′ = α

(6.60)

where α-1 is found from σ = a∼σ ′ a = α -1 σ ′ as in Eq. (6.25). Proceeding, having determined α -1, we apply Eq. (6.60) to the cubic system to give l 12 l 22 0 0 0 0 s′ = 0 0 0 0 0 0

or

l 32 l2 l3 0 0 0 0 0 0 0 0 0 0

l3 l 1 0 0 0 0 0

l1 l2 s11 0 0 0 0 0

s12 s11

s12 s12 s11

0 0 0 s44

Sym.

0 0 0 0 s44

0 0 0 0 0 s44

l12 l22 l32 l2 l 3 l 3 l1 l1 l2

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

s′11 = s11(l 14 + l 24 + l 34 ) + s44(l 22 l 32 + l 32 l 12 + l 12 l 22 ) + 2s12(l 22 l 32 + l 32 l 12 + l 12 l 22 ).

But (l 41 + l 42 + l 43 ) = (l 21 + l 22 + l 23 ) -2(l 22 l 23 + l 23 l 21 + l 21 l 22) which, when introduced into the equation for s′11, yields the well-known result

′ = s11

1 = s11 + { s44 − 2 ( s11 − s12 )} Y

(l

2 2 l + l32 l12 2 3

)

+ l12 l22 ,

′ [uvw], such that which is not isotropic. Now, as examples, let 0x = 1

l1 = u / u 2 + v 2 + w 2 , l2 = v / u 2 + v 2 + w 2 , l3 = w / u 2 + v 2 + w 2

where ( l22l 32 + l 23 l 21 + l 21 l 22 ) = (u 2v 2 + v 2 w 2 + w 2u 2 ) (u 2 + v 2 + w 2 ) which is always positive.

(6.61)

122 tensor properties of solids

Along (l 22 l 23 + l 23 l 21 + l 21 l 22 ) = 0 and Y = 1/ s11 = Ymin ′ ) / 3 ; Y = Ymax . Along (l 22 l 23 + l 23 l 21 + l 21 l 22 ) = 1/ 3 and 1 / Y = s11 + ( s44 − s44 Also, because (s44 − s4′4) = 3(Y -1 − Y -1), then

−1 −1 −1 −1 Y = Y + 3 (Y − Y ).

(6.62)

The results for other crystal systems can be found in Nye cited in Endnotes.

6.2.8 Shear Modulus and Poisson’s Ratio The analysis for the shear modulus follows in a similar manner to that for Young’s Modulus. Con′ the 0x direction ′ on a plane whose normal is the 0x′2 sider the application of a shear stress σ in 6 1 direction. Thus, we define 1 = ε 6′ . G σ 6′ (6.63) The method of solution is the same as for Young’s modulus, namely, s′ = α∼ -1 sα -1, where α -1 is found from σ = a∼ σ ′a and σ = α -1σ ′. After simplifying the result, the rigidity modulus is

2 2 2 2 2 2 1 G = s44 − 2 {( s44 − 2( s11 −s12 )} (a11 a21 + a12 a22 + a13 a33 ) ,

(6.64)

which is easily seen not to be isotropic. If we take [uvw] = 0x1′ and [hkl ] = 0x′2, then

(a112 a212 + a122 a222 + a132 a332 ) = {(uh)2 + (vk) 2 + (wl )2 }

(u 2 + v 2 + w 2 )( h 2 + k 2 + l 2 )

Poisson’s ratio, defined as v = −ε2′ / ε1′ = −ε3′ / ε1′, is more difficult to obtain by using the procedure above. However, knowing Y and G, it is easily found from Eq. (6.58) to be

ν = Y / 2 G − 1. • • • •

(6.65)

123

chapter 7

Second- and Higher-Order Effects— Symmetry Considerations First, as we move into a discussion of the second- and higher-order effects, it quickly becomes apparent that their number is far too large for a detailed inclusion in this text. However, we will give specific examples, for instructional purposes, and then provide a generalized approach to their development. Second, it is often the case that the second-order effects do not depend strongly on the magnitudes of the intensive and extensive parameters and may be regarded as weak correction terms (if they exist at all) to the first-order effects under a given set of small intensive or extensive fields. Remember that the first-order effects were developed under the assumption of infinitesimally small fields. However, some second-order effects may actually dominate the first-order effects particularly under field strengths that are not infinitesimally small. If the second-order effects are but weak correction terms to the first-order effects, then it is safe to say that the third- and higher-order effects may be disregarded as we do in our treatment.

7.1 ELECTROSTRICTION AND MORPHIC EFFECTS

~ Recall that the piezoelectric moduli were given earlier by Eq. (4.62) as C P, σ )T,E,B = C ε,E )T,B,σ = dT, B . Here, the converse piezoelectric effect is the first-order electrostriction effect expressed in integrated tensor form as

εij = dijk Ek = εji ,

(7.1)

which applies for very small electric fields and very small stresses and strains all at constant T, B, and σ. At large stresses and strains, quadratic (second-order) terms must be introduced. To do this, we can expand dijk in a Taylor series to give

∂d 1 ∂ 2dijk dijk = dijk0 + ijk E E + …, El + 2 ∂El ∂Em T , B,σ l m ∂ El T , B,σ

(7.2)

0 is the value for dijk at infinitesimal field strength. Introducing Eq. (7.2) into Eq. (7.1) gives where dijk the result

124 tensor properties of solids

{

}

E + … Ek , (7.3) ijkl l 0 where the third-rank tensor terms γijkl El + ... are the correction terms to dijk proportional to field strength and that must conform to both tensor and crystal symmetry. 0 vanish for the 11 centrosymmetrical crystal classes given in All electrostrictive moduli dijk Table 3.4. However, the correction terms γijkl El + ... are not centrosymmetrical and can create new electrostrictive moduli proportional to the field strength E and a strain proportional to E 2. These new moduli create what is called a morphic effect. Thus, an electrostrictive effect in a centrosymmetrical class can exist but only as a morphic effect. 0 + γ εij = dijk

7.1.1 Symmetry and Transformation Considerations of Fourth-Rank Tensors Given the second-order electrostrictive effect from Eq. (7.3),

εij = γ ijkl El Ek ,

xxx(7.4)

it follows that the symmetry for γ becomes

γ

ijkl

=γ

jikl

=γ

ijlk

=γ

jilk

=γ

mn

,

(7.5)

since strain is commonly taken to be symmetrical, εij = εji. Therefore, we can write

εm = γmn (EE )n or ε = γ ( EE )

where

γmn ≠ γnm .

(7.6)

Now, the transformation law for γ can be determined in matrix form from Eqs. (6.46), (7.5), and (7.6) as follows: First, we recognize that all principal compliance and rigidity effects, respectively, those along the leading diagonals in Eqs. (4.29) and (4.33), exhibit thermodynamic symmetry as illustrated by Eqs. (4.48) to (4.50). Accordingly, the elastic stiffness tensor cijkl (a property rigidity) is symmetrical to the extent that cmn = cnm, which derives from the fact that both stress and strain are taken to be symmetrical ∼ , where a is the second-rank tensors. Thus, cijkl transforms in matrix notation as in Eq. (6.46) or c ′ = a c a quadratic transformation form discussed in Section 2.2. In matrix notation, we can write that σ = cε with respect to the “old” set of axes 0xi and that σ ′ = c ′ε ′ with respect to the “new” set of axes 0xi′ . Now, with appropriate substitutions we write

∼ε′ = acε σ ′ = aσ = c ′ε ′ = ac a

Solving for ε ′ by acknowledging the transformation for the dyadic EE and using Eq. (7.6), there results

∼ -1 ε and ε ′ = a

(EE)′ = a(EE) or

(EE) = a -1(EE)′

∼ -1ε = a ∼ -1γ (EE) = a ∼ -1γa -1 (EE)′ = γ (EE)′, resulting in the transformation form Therefore, ε ′ = a

Second- and Higher-Order Effects—Symmetry Considerations 125

~−1γ α −1, γ ′ =α

(7.7)

which transforms exactly like the elastic compliance coefficient, s ′ = a∼ -1 sa -1 given in Eq. (6.47).

7.2

GENERALIZED DEVELOPMENT OF THE SECOND-ORDER EFFECTS

Let the intensive parameters be represented by a , β , γ, ... and their conjugate extensive parameters represented by a, b, c, ... , such that the state equations for the extensive parameters are a = a (α ,β ,γ , …)b ,c , ... b = b (α ,β ,γ , …)a ,c , ... �

�

(7.8)

Similarly, the state equations for the intensive parameters are

α = α (a ,b, c , …)β , γ , … β = β ( a , b, c , …)α, γ , … �

�

(7.9)

We now expand each state equation in Eqs. (7.8) in a differential Taylor’s series with the result

∞ 1

∂ ∂ ∂ … n d a (α ,β ,γ , …) d d + + + α β γ ∂α b, c,… ∂β ∂γ n=1 n !

da = ∑

∞ 1

∂ ∂ ∂ … n b (α ,β ,γ , …) dα + dβ + dγ + a, c,… ∂α ∂β ∂γ n=1 n !

db = ∑

M

M

(7.10)

Similarly, the Taylor series expansion of the intensive state equations in (7.9) become

∞ 1 ∂ ∂ ∂ … n c d d a b d + + +

dα = ∑ n =1

n!

∂a

∂b

∂c

α (a , b , c ,…)

β ,γ ,…

∞ 1

∂ ∂ ∂ … n + db + dc + d a ∂a ∂b ∂c n =1 n !

dβ = ∑

M

β (a , b, c, …)

α ,γ ,…

M

(7.11)

Now, for the sake of illustration, consider any two intensive parameters α and β and their corresponding (conjugate) extensive parameters a and b with all other extensive parameters held

126 tensor properties of solids

constant, i.e., γ,δ, ... = constant. Then, if Eqs. (7.10) apply to the compliance effects as in Eq. (4.26), we can use Taylor’s expansions to evaluate the integrals ∫da and ∫db, giving

∆ a = (C

a,α

)β ∆α + (C

1 ∂ (C )α ∆β + 2 ∂α

)β

1 ∂ (C 2 ∂α

)β

a, α

a, β

∆ b = (C b, α )β ∆ α + (C b , β)α ∆β +

b,α

( ∆α )

2

1 ∂ (C + 2 ∂β

)α

1 ∂ (C 2 ∂β

)α

a, β

b, β

( ∆α )2 +

( ∆β )2 + …

(7.12)

(∆β )2 + …,

(7.13)

where now ∆α = α - α and ∆b = b - b, indicating that the Taylor series (7.12) and (7.13) are to be evaluated around initial values α0 and b0 that become vanishingly small. After differentiating Eqs. (7.12) and (7.13), there results

d a = (C a, α)β d α + (C a, β)α d β +

d b = (C

)β dα + (C )α dβ +

b ,α

b, β

∂ (C a, α)β ∂α ∂ (C b, α )β ∂α

α dα +

α dα +

∂ (C a,β )α ∂β ∂ (C b,β )α ∂β

β d β + …

(7.14)

β dβ + …,

(7.15)

where use was made of

d l im (∆α )2 = 2 α dα and d l im (∆β ) 2 = 2 β dβ . α → 0 β → 0 0

(7.16)

0

If only the first- and second-order effects are considered, Eqs. (7.14) and (7.15) can be represented approximately in the matrix form ∂ C a, α (C a, α)β + α ∂α β d a d b = b, α C b,α + α ∂ C ( ) ∂α β β

a,β ∂ C a,β (C )α + β ∂β α dα . dβ b, β ∂ C b, β (C )α + β ∂β α

(7.17)

Here, other second-order terms such as ∂ 2a / ∂α∂β and ∂ 2b / ∂α∂β together with the third- and higher-order terms have been neglected. We will revisit the issue of first- and second-order terms later when we consider the phenomenological development of the optical effects. Assuming that Eqs. (7.17) are a valid approximate representation of the extensive differentials da and db as functions of the intensive α and β, then an interesting and useful relationship between the second-order terms can be derived. Since from the application of Stoke’s theorem in Eq. (4.38), we established the symmetrical nature of the compliance effects given by Cmn = Cnm , it

Second- and Higher-Order Effects—Symmetry Considerations 127

follows that a symmetrical relationship can also be established between the second-order effects in Eqs. (7.17). Thus,

(C a, β )α = ∂∂βa

permits

α

∂b = = (C b, α )β ∂α

∂ (C b,β) ∂ C a, β ∂ ∂b α = = ∂β ∂α ∂ β β α ∂ β α α

and

∂ (C a, α) ∂ C b, α β ∂ ∂a = = β ∂ α β ∂ ∂ ∂ α α β β α

(7.18)

β

(7.19)

(7.20)

because the order of differentiation is immaterial. The meaning of (∂(Cb,β)α/∂α)β in Eq. (7.19) is that Cb,β is evaluated at constant α and that its change with α is evaluated at constant β. The expressions in Eqs. (7.19) and (7.20) are second-order Maxwell relations. Introducing these expressions into Eqs. (7.17) gives the results ∂ (C b, β) a, β α (C )α + β β ∂ α dα . dβ ∂ C b,β b, β (C )α + β ∂β α (7.21) By thermodynamic symmetry, the Maxwell relations lead to the equality of cross (bracketed) terms a, α (C a, α ) + α ∂ C β ∂α β d a = db ∂ C a, α ) β C b, α + α ( )β ∂β ( α

∂ (C a, α) ∂ (C b,β )α β b, , = (C α)β + α β α ∂ α ∂ β

(C a,β )α + β

(7.22)

where it follows that ∂ (C a, α ) ∂ (C b,β )α β = β α . ∂α β ∂β α

(7.23)

Note that the expressions in Eq. (7.23) result from the symmetry expressed by Eq. (7.18) and that the second-order cross terms in Eqs. (7.21), (7.22), and (7.23) are no longer multiplied by an intensive parameter that is not held constant as in the case of Eqs. (7.17).

128 tensor properties of solids

Consider the use of Eqs. (7.21) to develop the first- and second-order electrostrictive effects as was done in Section 7.1, but from a different approach. To do this, we select the following extensive and intensive parameters:

Equations (7.21) now become

a = ε = b P

ε, σ (C ε,σ ) + σ ∂ C E ∂ E E d ε d P = ∂ (C ε, σ ) E (C P , σ ) E + σ ∂E σ

α = σ . β = E ∂ (C P,E )σ ε,E (C )σ + E E σ ∂ dσ , d E P, E P, E ∂C (C )σ + E ∂ E σ T ,B

(7.24)

(7.25)

where it is understood that T and B are held constant. By thermodynamics symmetry, the cross (braced) terms are equal giving the results

(

C ε,E

)σ

∂ (C P, E )σ ∂ (C ε, σ) E , P,σ + E = (C ) E + σ ∂σ E ∂ σ E

(7.26)

where it follows that

∂ (C P , E ) ∂ (C ε, σ) σ E , = σ E ∂σ E E ∂ σ

(7.27)

because (C ε,E)σ = (CP,σ)E . The compliances CP,E and C ε,σ are defined by Eqs. (4.45) and (4.47), respectively. Written in tensor notation, Eq. (7.27) becomes

∂χ j ∂s κ 0 i E l = ijkl σlm = ψ ijk . ∂σ kl E ∂ Em σ

(7.28)

What Eq. (7.28) indicates is that the components of the polar third-rank tensor ψijk on left side of the equation are numerical equal to those on the right side or vice versa. However, the frequency of the E and σ field changes must be the same if the equality of Eq. (7.28) is to be valid. As another approach to the evaluation of second-order effects, consider the application of the parameter selection in Eq. (7.24) to Eqs. (7.17) expressed as

Second- and Higher-Order Effects—Symmetry Considerations 129

,σ ∂ C ε ,σ ε ,E ∂ C ε ,E C + E (C ε )E + σ ( ) ∂ E σ ∂σ E σ dε dσ . d P = dE E P , , P σ P,σ ∂ C P , E ∂ C (C ) + σ (C )σ + E E ∂σ E ∂ E σ

(7.29)

The first- and second-order converse piezoelectric (electrostrictive) effects are represented by the equation for dε under constant stress σ given in tensor notation by ∂ d jk dε ij = ( dijk)σ dEk + i Ek d El ∂El σ

or in integrated form

{

ε ij = d ijk + γ ijkl E l

}

σ

Ek ,

(7.30)

which is the same as Eq. (7.3). Here, dijk are the converse piezoelectric moduli or the first-order electrostrictive moduli, and γijkl are second-order electrostrictive moduli. In conformable matrix form, ∼ q. (7.30) is given by ε = d E + λ(EE c ), where (EE c ) is the self-conjugate (dyadic) product of electric fields. In expanded matrix form, the strain matrix of Eq. (7.30) becomes

ε 1 d 11 ε d 2 12 ε 3 d 13 = ε 4 d 14 ε d 15 5 ε 6 d 16

d 21 d 22 d 23 d 24 d 25 d 26

d 31 γ 11 γ d 32 E 21 d 33 1 γ 31 E + d 34 2 γ 41 E d 35 3 γ 51 d 36 γ 61

γ 12 γ 22 γ 32 γ 42 γ 52 γ 62

γ 13 γ 23 γ 33 γ 43 γ 53 γ 63

γ 14 γ 24 γ 34 γ 44 γ 54 γ 64

γ 15 γ 25 γ 35 γ 45 γ 55 γ 65

γ 16 E E 1 1 γ 26 E2 E 2 γ 36 E3 E 3 γ 46 E2 E 3 γ 56 E3 E 1 γ 66 E1 E 2

(7.31)

where it is recalled from Section 7.1 that γmn ≠ γnm.

7.3

PHENOMENOLOGICAL DEVELOPMENT OF THE OPTICAL EFFECTS

In the presence of external fields, the dielectric constant (relative permittivity) Kij = κij / κ0 and, hence, the refractive index of a crystal may change. For example, in the presence of an external electric field, an isotropic solid may become optically anisotropic, a uniaxial crystal may become biaxial, and so forth. The effect of the external electric field on the optical symmetry of the crystal is commonly

130 tensor properties of solids

called the electro-optical effect. Similar effects are obtained by the application of other external fields such as magnetic, stress, and temperature changes. The corresponding effects are referred to as magneto-optical, piezo-optical, and thermo-optical effects, respectively. There are several ways to phenomenologically develop the previously mentioned optical effects. For example, we could expand the relative permittivity tensor, Kij in a power series as a function of electric field E, magnetic field H, and stress σ. Two of the coefficients resulting from this expansion would be called the electro-optical and piezo-optical coefficients. Alternatively, we could expand the electric field strength E as a function of the polarization P, magnetic flux density B, and strain ε,thereby obtaining the electro-optical, magneto-optical, and elasto-optical coefficients, and so forth, the choice being arbitrary and a matter of convenience. For our purposes, we will choose as the dependent variable the dielectric impermeability tensor defined as

(

)

Bij = K i−1j = κ 0 ∂Ei / ∂ Dj = Bji ,

(7.32)

→ → → where Dj is the electric flux density given vectorially as D = κ0E + P . The refractive index of a crystal is specified generally by an ellipsoid called the indicatrix whose coefficients at optical frequencies are the components of the dielectric impermeability tensor Bij given by Bijxixj =1. Expansion of the dielectric impermeability in a Taylor’s series about the state of a reference temperature T 0, zero electric field, zero magnetic flux density, and zero stress yields

∞ 1

n

∂ ∂ ∂ ∂ 0 (T − T 0 ) + Ek + Bl + σmn Bij (T , 0 , 0 ,0 ) ∂ ∂ ∂ n ! T E B ∂ σ n= 0 k l mn

Bij ( T , Ek , Bl , σmn ) = ∑

∂ Bij ∂ Bij ∂ B ij ∂ Bij = Bij (T 0 , 0, 0, 0) + ∆ T + E + B + ∂E k ∂B l ∂σ σ mn ∂ T l k mn

+

(7.33)

2 2 ∂ 2 B ij ∂ 2B ij ∂ Bij 1 ∂ Bij 2 B E B ∆ T + E + + ( ) l p σmn σqr 2 ! ∂ T 2 ∂ Ek ∂ Eo k o ∂Bl ∂ Bp ∂ σmn σqr

2 2 2 2 ∂ B ij ∂ Bij ∂ B ij ∂ Bij +2 Ek ∆ T + 2 ∂ T ∂ B Bl ∆ T + 2 ∂T ∂σ σ mn ∆T + 2 ∂ E B Ek Bl ∂ T ∂ Ek k l mn l 2 2 ∂ Bij ∂ Bij E σ 2 +2 + Bl σmn + …. k mn ∂ Ek∂σmn ∂ Bl σ mn

(7.34)

Second- and Higher-Order Effects—Symmetry Considerations 131

Here, Bij (T 0,0,0,0) and all coefficients (in parentheses) are evaluated at a reference temperature T 0 and at zero electric field, zero magnetic field, and zero stress. We now develop phenomenologically the 14 linear and quadratic optical effects expressed in Eq. (7.34). ∂ Bij = tij = linear thermo-optical effect ∂ T (T 0,0 ,0 ,0 ) 1 2

∂ 2Bij = T j = quadratic thermo-optical effect ∂T 2 (T 0,0 ,0 ,0 ) i

∂ Bij ∂ E

k (T 0,0 ,0 ,0 )

1 2

l

= fijl = linear magneto-optical (Faraday) effect (T 0,0 ,0 ,0 )

∂ 2Bij = Fijlp = quadratic magneto-optical (Cotton–Mouton) effect ∂Bl ∂Bp (T 0,0 ,0 ,0 )

∂ Bij ∂σ mn 1 2

∂ 2Bij = Rijko = quadratic electro-optical (Kerr) effect ∂ E ∂E k o (T 0,0 ,0 ,0 )

∂ Bij ∂ B 1 2

= rijk = linear electro-optical effect

= π ijmn = linear piezo-optical effect (T 0,0 ,0 ,0 )

∂ 2Bij = Πijmnqr = quadratic piezo-optical effect ∂ σ mnσ qr (T 0,0 ,0 ,0 )

∂ 2Bij ∂T ∂E k ∂ 2Bij ∂T ∂B l

) = thermoelectro-optical effect = ri(T jk (T 0,0 ,0 ,0 )

= f jl(T ) = thermomagneto-optical effect i (T 0,0 ,0 ,0 )

∂ 2Bij ∂ T∂σ mn

= π i(Tjmn) = thermopiezo-optical effect (T 0,0 ,0 ,0 )

132 tensor properties of solids

∂ 2Bij ∂E B k l

∂ 2Bij ∂ E ∂σ k mn

(T 0,0 ,0 ,0 )

∂ 2Bij ∂B σ l mn

= mijkl = magnetoelectro-optical effect

(T 0,0 ,0 ,0 )

= zijkmn = piezoelectro-optical effect

= wijlmn = piezomagneto-optical effect. (T 0,0 ,0 ,0 )

Only a few of these effects have been experimentally investigated and their tensor rank and symmetry considered. In what follows, we will briefly examine a few of the more common effects.

7.3.1 Electro-Optical Effects The linear and quadratic electro-optical effects can be obtained by applying very small electric fields to a crystal at constant reference temperature T 0 and zero magnetic field and stress. The Taylor’s series expansion of the dielectric impermeability tensor reduces to

2 ∂ Bij ∂ Bij 1 Bij (Ek ) = Bij ( 0) + E + 2 Ek Eo + L ∂Ek k ∂Ek ∂Eo

(7.35)

∆Bij = rijk Ek + Rijko Ek Eo + �.

(7.36)

or

where rijk and Rijko represent the linear and quadratic electro-optical effects, respectively. The coefficients rijk, which describe the linear electro-optical effect in crystals, form a polar nonmagnetic third-rank tensor with symmetry rijk = rjik = rmk such that the linear electro-optical effect can be written as

∆Bm = rmk Ek

( m = 1 − 6; k = 1 − 3) .

(7.37)

In simplified notation, Eq. (7.37) can be expressed as ∆B = r ⋅ E or simply as ∆B = r∼ E in conformable matrix form. Thus, the matrix representation of Eq. (7.37) is the same as the converse piezoelectric effect given by Eq. (6.11). with ε replaced by ∆B and d replaced by r. Because rijk and dijk are both third-rank polar tensors, the symmetry restrictions on their coefficients must be the same. Thus, rijk = 0 for all 11 centrosymmetrical crystal classes and the rmk for the linear electro-optical moduli are the same as those in Table 6.2 if the transpose of each array is taken with the subscripts mk reversed as in Eqs. (6.10) and (6.11). Remember that the d moduli arrays in Table 6.2 are given in normal form.

Second- and Higher-Order Effects—Symmetry Considerations 133

Because the linear electro-optical effect is possible only in piezoelectric crystals, the presence of an externally applied electric field will produce a slight change in the shape of the crystal by the converse piezoelectric effect. The change in crystal shape results in the elasto-optical effect, to be considered in Section 7.3.2. As a result, the electro-optical effect will consist of two components: 1) the true (primary) linear electro-optical effect and 2) the false (secondary) linear electro-optical effect. Combined, these effects are given by ∆Bij = rijkEk = rijk∗ E k + pij lm εlm,

(7.38) rijk* are the true electro-optical coefficients and pijlm are the elasto-optical coefficients. The where elasto-optical coefficients are related to the linear piezo-optical coefficients, as in Eqs. (7.50), by

pijlm = π ijrs crslm

and

π ijlm = pijrs Srslm ,

(7.39)

where c and s represent the elastic stiffness and elastic compliance moduli of a crystal, respectively. Equation (7.38) can be cast into an alternative form by using Eq. (6.8), yielding

∆Bij = (ri∗jk + pijlm dklm ) E k

or

∆Bm = (rm∗k + pmr dkr )Ek ,

(7.40)

so that the product pd appears as a correction factor for the true linear electro-optical effect. At high-field frequencies, the pd correction factor is usually much smaller than the true linear electrooptical effect, but at low frequencies, it can become relatively important. The quadratic electro-optical effect, or Kerr effect, is represented by the coefficients Rijko in Eq. (7.36), which is a polar nonmagnetic fourth-rank tensor. Thus, contrary to the linear electro-optical effect, the quadratic effect may exist in all crystal classes. From its definition ∂ 2Bij / ∂Ek∂Eo there exists symmetry in the subscript pairs (i, j ) and (k, o) permitting the Kerr coefficients to be represented in either form ∆Bij = RijkoEk Eo or

∆Bm = Rmn En2

(m, n = 1 − 6),

and

Rmn ≠ Rnm .

(7.41)

R 16 E1 E 1 R 26 E2 E 2 R 36 E3 E 3 . . R 46 E2 E 3 R 56 E3 E 1 R66 E1 E 2

(7.42)

In expanded matrix form, Eq. (7.41) becomes

∆B1 R 11 ∆B R 2 21 ∆B3 R 31 = ∆B4 R 41 ∆B5 R 51 ∆B6 R 61

R 12 R 22 R 32 R 42 R 52

R 13 R 23 R 33 R 43 R 53

R 14 R 24 R 34 R44 R 54

R 62 R 63 R 64

R 15 R 25 R 35 R 45 R 55 R 65

134 tensor properties of solids

Here, the Rmn coefficients are related to the Rijko coefficients by the rules: Rmn = Rijko if n = 1 - 3, and Rmn = 2Rijko if n = 4 - 6. The restrictions imposed by crystal symmetry on the coefficients Rmn are exactly the same as those imposed on the linear piezo-optical coefficients considered in Section 7.3.2. As in the case of the linear electro-optical effect, the quadratic effect will normally contain two parts: 1) the true (primary) quadratic electro-optical effect and 2) the false (secondary) quadratic electro-optical effect. This can be expressed as

∆Bij = Rijko Ek Eo = Ri∗jko Ek Eo + pijlm εlm,

(7.43)

where R are * the coefficients for the true quadratic electro-optical effect and pijlm are the compoijko nents for the elasto-optical effect. Equation (7.43) can be cast into an alternative form by use of second-order electrostrictive coefficients given in Eq. (7.4). When this is done, Eq. (7.43) becomes

∗ ∆Bij = ( Rijko + pijlm γlmko )Ek Eo ,

(7.44)

where now the pγ product appears as a correction to the true quadratic electro-optical (Kerr) effect. The pγ correction factor is usually weak but can become important in some ferroelectric crystals.

7.3.2 Piezo-Optical and Elasto-Optical Effects The linear and quadratic piezo-optical effects can be obtained by applying small stress components to a crystal at a reference temperature T 0 under zero magnetic and electrical field conditions. The Taylor’s series expansion of the dielectric impermeability tensor in Eq. (7.34) reduces to ∂ 2Bij ∂Bij 1 σ Bij (σmn ) = Bij ( 0) + + σmnσqr + � 2 ∂σmn mn ∂ σmnσqr or

∆Bij = πijmnσmn + Πijmnqrσmn σ qr + L ,

(7.45)

where πijmn and ∏ijmnqr represent the linear and quadratic piezo-optical coefficients, respectively. The coefficients πijmn represent a polar fourth-rank tensor with partial symmetry implied by Bij and σmn thereby permitting the linear effect to be presented in reduced suffix notation as

∆Bo = π op σ p

( o, p = 1 − 6 )

and

π op ≠ π po

(7.46)

Second- and Higher-Order Effects—Symmetry Considerations 135

or in expanded matrix form ∆B1 π 11 ∆B π 2 21 ∆B3 π 31 = ∆B4 π 41 ∆B5 π 51 ∆B6 π 61

π 13 π 14 π 15 π 16 σ 1 π 23 π 24 π 25 π 26 σ 2 π 33 π 34 π 35 π 36 σ 3 . , π 43 π 44 π 45 π 46 σ 4 π 53 π 54 π 55 π 56 σ 5 π 63 π 64 π 65 π 66 σ 6

π 12 π 22 π 32 π 42 π 52 π 62

(7.47)

The elasto-optical coefficients can be obtained in a similar manner by expressing the impermeability tensor as functions of the strain components of the crystal, as in Eq. (7.43), to give ∆Bij = pijlm ε lm ( i , j, m , n = 1 − 3) (7.48) or in reduced suffix notation

∆Bo = pop εp

(o, p = 1 − 6)

and

pop ≠ ppo

(7.49)

Now, Pop = Pijlm for all o and p with no factors of 2 or 1 2 present. The elasto-optical and piezo- optical coefficients are related through the elastic moduli c and s, respectively, by the equations

∂B ∂σq pop = o = πoq cqp ∂σq ∂εp

and

∂Bo ∂ε p πoq = = pop spq . ∂εp ∂σq

(7.50)

The effect of crystal symmetry on the piezo-optical coefficients πoq can be determined by applying the direct inspection method to all crystal classes except the trigonal and hexagonal systems for which the “brute-force” method must be used. Thus, for the trigonal and hexagonal systems, the transformation equation must be used:

π ′ = απα −1.

(7.51)

which also applies to the quadratic electro-optical coefficients R given in Eq. (7.42). Note that Eq. (7.51) derives from B ′ = αB = απσ = απα-1σ ′ = π ′σ ′ because B = πσ applies to the old axes 0xi , whereas B ′ = π ′σ ′ applies to the new axes 0xi′ . Here, the linear quadratic electro-optical coefficients Rmn will be affected by crystal symmetry exactly as will be πmn . Shown in Table 7.1 are the piezo-optical coefficients πmn for the seven crystal systems and the isotropic solid with the understanding that πij ≠ πji. This table can also be applied to the elasto-optical coefficients with some minor changes.

136 tensor properties of solids

7.3.3 Piezo-Optical Effect in Cubic Crystals Under Uniaxial Tension

Consider the application of a uniaxial stress on a cubic crystal of the class 4− 32, 432 or m3m. For any direction of stress, the matrix equation Eq. (7.46) becomes 0 π π π 12 0 ∆ B 0 0 σ1 B B − 1 11 12 1 ∆B B − B 0 π π 11 π 12 0 0 0 σ 2 12 2 2 ∆B3 B3 − B 0 π 12 π 12 π 11 0 0 0 σ 3 = = . , 0 0 π 44 0 0 σ 4 ∆B4 B4 0 ∆B5 B 0 0 0 0 π 44 0 σ 5 5 0 0 0 0 π 44 σ 6 ∆B6 B6 0 (7.52) where B 0 is the reference dielectric impermeability defined by the indicatrix sphere for the undeformed crystal in the absence of temperature, electric, and magnetic fields

x2 x2 x2 B 0 ( x12 + x22 + x32 ) = 01 2 + 02 2 + 03 2 = 1 (n ) (n ) (n )

(7.53)

because B 0 = 1(n0)2. Here, n0 is the refractive index in the absence of all external fields. Now, let a uniaxial tensile stress σ2 be applied along the 0x2 direction, with 0x1 and 0x3 being the other cubic unit cell axes. Because ∆B4 = ∆B5 = ∆B6 = 0, Eq. (7.52) reduces to

∆B1 = π12σ2 ∆B2 = π11σ 2 ∆B 3 = π12σ 2 .

(7.54)

The changes in the three principal refractive indices can be determined by noting, for example, that Bi = 1 / ni2. Then, after differentiation, there results ∆Bi = -(2 / ni3 )∆ni = Bi = Bi0 0 (s. in units of Energy/l 3tT ),

(8.13)

where l is length (e.g., meter, m), t is time (e.g., second, s), and T is temperature (e.g., °K) as in the SI system of units for which energy is given in joules, (1 W = 1 J/s). Thus, we take entropy density production as the time variation of unrecoverable work per unit volume per unit temperature inside the system and whose quadratic form must be positive definite. In general, we assert the requirements that s. = 0 (reversible process) s. > 0 (irreversible process) s. < 0 (a process that cannot occur without altering the system conditions).

8.5

PROPER CHOICE OF PARAMETERS

The entropy production criterion allows for some latitude of “proper choice” for the fluxes J α and affinities X α. Thus, authors may differ in their choice for the fluxes and affinities. We will consider the conjugate parameters for the flow of electrical current, entropy (heat), and matter as they relate to reciprocal Ohm’s, Fourier’s, and Fick’s laws, respectively, given in Section 8.1. But in doing this, we will require that the product of the conjugate parameters each have the units of entropy density production s., that is, s. in SI units of Energy / l 3tT as in Eq. (8.13). 1. Flow of electronic charge: J 1 = Jin = −Jie /e = Electron flux (in units of no. electrons/l 2t ),

transport properties and irreversible thermodynamics 153

where J e is the charged electron flux in the direction of the electrostatic potential gradient. The affinity (force) is given by – – µ ∇µ X 1 = ∇i = i (in units of Energy/lT ), T T

( )(

)

where

µ− = µc + eφ

(8.14)

is the electrochemical potential (total energy per particle, also called the Fermi level in the equilibrium state), µc is the chemical potential per particle, eφ is the electrostatic potential per particle, and e is the charge on the particle assumed to be a positive test charge equal to + | e | = 1.60 × 10−19 C. Thus, the inner product of the conjugate parameters for the flow of electronic charge gives the entropy density production per particle as

(

− µ

T

(

s· = − J ni ∇i

(in units of Energy/l 3tT ),

(8.15)

which will later be shown to satisfy the corresponding reciprocity relations. Be aware of the fact that we are using the positive current convention and that high electrostatic potential is more positive than low electrostatic potential. Thus, Jin is always in a direction counter to the electrostatic potential gradient, which is from low potential to high potential. 2. Flow of entropy or heat: J 2 = Jis = Entropy flux (in units of Energy/l 2t)

(

∇i T (in units of l −1). T =− T The inner product of the conjugate parameters for the flow of entropy yields the entropy production as

(

1

(

s· = J si T ∇i

1

(

X 2 = T ∇i

3 T (in units of Energy/l tT ),

(8.16)

which will be shown to satisfy the corresponding reciprocity relations. Alternatively, for our purpose, because J q = T J s, the conjugate parameters become

X 2 = ∇i

(

1

T

(

and

J 2 = Jjq = Heat flux (in units of Energy /l 2t ) =−

∇i T (in units of (lT )−1, T 2

154 tensor properties of solids

which gives the entropy density production 1

(

(

s· = J qi ∇i

T

(in units of Energy/l 3tT ),

(8.17)

3. Flow of matter (uncharged single component): J 3 = J m = Matter flux (in units of mole number N /l 2t )

µ X 3 = ∇i c

= T

∇i µc

(in units of Energy/lT ).

T

Here, the mole number N is defined as the actual number of the diffusing species divided by Avogadro’s number. The inner product of the conjugate parameters for the flow of uncharged mass (kg-moles) counter to the concentration gradient of one component gives the entropy density production as

µ s· = − J mi ∇i c

(in units of Energy/l 3tT ),

T

(8.18)

which will also be shown to satisfy the corresponding reciprocity relations. Combining Eqs. (8.15), (8.17), and (8.18) yields the total entropy density production for all three processes as

s· =

∑i Ji

α

µ Xiα = − Jin ∇i

+ J q ∇ 1 − J m ∇ µc , i i T i i T

T

(8.19)

which are each represented in units of Energy/l 3tT ). Thus, the phenomenological relations for the three types of flow can be written in the following matrix forms

− Jin q Ji − J m i

=

Li11j Li12j 21 22 Li j Li j L 31 L 32 ij ij

( µ T ) Li23 ∇j (1 T ) . j ∇ ( µ T ) Li33 c j j Li13j ∇j

(8.20)

Here, diagonal Lijαα are the principal phenomenological coefficients and the Lijαβ are the cross or interference coefficients. Onsager’s reciprocity theorem permits the following relationships between the phenomenological coefficients in the absence of a magnetic field ~ ~ Liβα = Ljαβ or Lβα = Lαβ for α ≠ β but Lβα ≠ Lαβ, that is, Lijαβ ≠ Ljαβ j i i and ~ Liαα = Ljαα or Lαα = Lαα for α = β. j i

transport properties and irreversible thermodynamics 155

Thus, only the Lijαα are self-symmetrical. The reciprocal relations are best illustrated for a three-dimensional system in which only electric current and heat flow occurs. Accordingly, Eqs. (8.20) now become

− J1n n − J2 − J n q3 J1 Jq 2 J3q

11 L11 11 L12 L11 = 31 L12 11 L12 12 12 L13

11 L12

11 L31

12 L11

12 L12

∇1 L12 13

11 L22 11 L23 12 L21 12 L22 12 L23

11 L23 11 L33 12 L31 12 L32 12 L33

12 L21 12 L31 L22 11 22 L12 22 L31

L12 22 12 L32 22 L12 22 L22 22 L23

L12 23 L12 33 22 L31 22 L23 22 L33

( ) ( ) ( ) , µ

T

µ ∇2 T ∇ µ T ⋅ 3 1 ∇1 ( T) ∇ ( 1 T) 2 1 ∇3 ( T )

(8.21)

11 11 22 22 21 12 12 12 where L = L˜ , L = L˜ , and L = L˜ , meaning that Lij21 = Lji12, but L ≠ L˜ .

8.5.1 Further Restrictions on the Phenomenological Coefficients Relating the entropy production given in Equation (8.13) to the phenomenological coefficients provides a first step in formalizing a unified theory of the cross (interaction) effects as they relate to the conjugate effects for linear, first-order, irreversible processes. For conditions under which Eq. (8.10) is valid, the quadratic form of the entropy production as given earlier is s⋅ =

∑L

αβ

X α X β > 0,

(8.22)

αβ

which is positive definite and implies that the matrix of phenomenological coefficients Lαβ also be positive definite. For this to be so requires that that determinant of the Lαβ matrix and all of its minors be positive definite. Take, for example, a two-flow process involving a two-dimensional matrix Lαβ given by

J 1 L11 2 = 21 J L

12

L12 X 1

, L22 X 2

(8.23)

21

where L = L according to Onsager’s principle. The necessary and sufficient condition for Eq. (8.23) to be positive definite is that the 2 × 2 determinant of Lαβ be positive definite. Thus,

L11

L12

L21

L22

= L11 L22 − (L12) 2 > 0.

(8.24)

Generally, the diagonal coefficients Lαα > 0 (i.e., are positive), but the Lαβ coefficients can be positive or negative. Applying Eq. (8.13) to the flow of electric charge and heat given in Eq. (8.20), we would write the entropy production for any two-flow process as

156 tensor properties of solids

s· =

∑L

αβ

(

X α X β = L αα X α X α + 2 Lαβ X α X β + Lββ X β X β

αβ

) > 0

(8.25)

or specifically for the flow of electric charge and heat

2

2

µ µ 1 1 + 2 L12 ∇ ⋅ ∇ + L22 ∇ > 0, T T T T

s· = L11 ∇

(8.26)

where each of the quadratic terms is given in units of Energy/l 3tT. Now back to Eq. (8.23), the value of the 2 × 2 determinant given by Eq. (8.24) requires that L11L22 > (L12)2,

(8.27)

which must be valid if the Lαβ matrix is to obey Onsager’s reciprocal relations L12 = L21. Note that L11L22 and (L12)2 both have units of T 2(l . t)−2 for the flow of electric charge and heat.

8.6 FLOW OF ELECTRONIC CHARGE AND HEAT— THE CONDUCTIVITIES A basic postulate in irreversible thermodynamics states that “every observed flux depends on all the affinities (driving forces) applied.” This means that the electronic and heat fluxes must depend on their conjugate affinities as well as the cross affinities. Thus, the flow of electrons not only transport charge but also heat (recall what Joule heat is when electric current flows through a resistor). The flow of mass in this case is considered negligible. With these concepts in mind, consider the simultaneous flow of electron current and heat in a system whose phenomenological equations for the thermoelectric effects are from Eq. (8.20) given by

(

+ L12 ∇ j ij

1

T

Jiq = Lj12i ∇j µ + Li22 ∇j j T

(

1

T

(

µ − Jin = L11 ∇ ij j

(

T

(8.28) (8.29)

The phenomenological coefficients Lij in Eqs. (8.28) and (8.29) can now be related to the familiar conductivities σij and kij. We begin with the electrical conductivity σij , which is defined as the electric current density −eJin per unit potential gradient ∇φ = ∇µ−/e in an isothermal system, the latter being essentially an electromotive force because ∇µc = 0, giving ∇µ− = e ∇φ. Therefore, under isothermal conditions, Eq. (8.28) becomes − Jin = Li11j

(

1

(

11 T ∇j µ = eLij

∇j φ T

for ∇T = 0

transport properties and irreversible thermodynamics 157

and

σ ij ≡

− eJin ∇j φ

= e 2 Li11j / T = σji ,

(8.30)

which indicates symmetry of the electrical conductivity, σij = σji because Lij11 Lji11 . Thus, the electrical conductivity is a symmetrical second-rank tensor with the component array given by Eq. (2.17). Solving for Lij11 in Eq. (8.30) gives Li11 = Tσij /e 2. j

(8.31)

Next, we turn to the heat conductivity defined as the heat current density per unit temperature gradient for zero electric current, J n = 0. For this purpose, Eqs. (8.28) and (8.29) become

µ 0 = Li11 ∇j j

− L12 ∇j T ij T 2

(8.32)

T

and

− L22 ∇ ∇j T . 2 j j i T T

µ Jiq = Lj12 ∇j i

µ Solving for ∇ j

(8.33)

in Eq. (8.32) gives, with subscripts excluded for simplicity, T µ ( 11)−1 12 ∇ T L ∇ = L , for J n = 0 T 2 T

which when substituted into Eq. (8.33) yields 12

(L11)−1 L12 − L22

{

{~L

(

(

Jq =

∇T T 2 .

(8.34)

The thermal conductivity tensor, defined as the heat current density − Jiq per unit temperature gradient ∇jT, now becomes

kij = −

Jiq ∇j T

=

1 T

2

{L

22 ij

}=L

( Li11j ) Li12j − Lj12 i −1

11 22 Lij

ij

− ( L12) 2

Li11j T 2

=

| DL | Li11j T 2

,

(8.35)

~ where by Eq. (8.11) Lji12 = Lij12 = L12, and | DL | > 0 is the determinant of the phenomenological coef~ ficients. Here, (L12)2 is a symmetrical square matrix often represented as L12L12 in matrix symbology. Because L11, L22, and (L12)2 are all symmetrical square matrices, we are permitted to state that

kij = kji

(8.36)

158 tensor properties of solids

~ ~ ~~ ~ t Thus, kij = kji if (L12 (L11)−1 L12) = L12 (L11)−1 L12, which it does since (ABC )t = (C B A ) or in this ~ ~ case, (A B −1A )t = A B −1A. A potential problem with this has been pointed out by Casimir in Nye’s Physical Properties of Crystals (see Endnotes). Only if the antisymmetrical part of kij (see Eq. (2.16)) is negligibly small or unobservable can Eq. (8.36) be justified. Given the validity of Eq. (8.36), the component array for kij as a symmetrical second-rank tensor is given by Eq. (2.17). Solving for Lij22 in Eq. (8.35) and introducing Eq. (8.31) yields the results Lij22 = (L12)

2

(Li11j )−1 + kij T 2 = e

(L12 )2 (σ )−1 + T 2 k . ij ij

2

T

(8.37)

We can now write Eqs. (8.28) and (8.29) in terms of the conductivities σij and kij by introducing the expressions for Lij11 and Lij22 in Eqs. (8.31) and (8.37) with the results

T σ ij − Jin = 2 e

(

µ 1 ∇j + Li12j ∇j T T

(

(

2 + T 2 k + e (L12)2 (σ ) −1 ∇ 1 , j T ij ij T T

µ Jiq = Lj12i ∇j

(8.38)

(

(8.39)

~ where (L12)2 = Lji12Lij12 = L12L12. Equations (8.38) and (8.39) give the generalized force–flux expressions for the dual flows of electricity and heat in an anisotropic solid both in terms of the conductivities σij and kij and the cross-coupled phenomenological coefficient Lij12 yet to be determined in Section 9.1. By dropping the subscripts i and j, these equations can be applied to the one-dimensional flow of electricity and heat in a homogeneous isotropic wire or rod. We end this section by defining thermal resistivity tensor rij as the inverse of the thermal conductivity tensor. Following Eq. (2.35), the inverse of kij is rij given by rij = −

or in matrix notation r = k−1. ( kij ) −1 =

∇i T Jjq

|Mji | | kij |

( − 1)(i + j )

(8.40)

= rij = rji ,

(8.41)

where | Mji | is the ji th minor of | kij |, indicating that any individual component of rij is not the simple reciprocal of kij component. The same reasoning applies to the relationship between the electrical conductivity σij and resistivity ρij expressed by (σij)−1 = ρij . • • • •

159

chapt e r 9

Thermoelectric, Piezothermoelectric, and Diffusive Effects in Solids In previous sections, we dealt mainly with the conduction of electricity and heat as two separate processes. This was done to formalize the conductivity definitions and define the phenomenological coefficients Lij11 and Lij22 in terms of the proper conductivities σij and kij . Now we will consider the simultaneous flow of electricity and heat usually referred to as the thermoelectric effects or, more specifically, the Seebeck, Peltier, and Thomson effects. In doing this, we will recognize that the irreversible processes involved interfere with one another. Thus, we will have to take into account the cross coupled or interference effects by making use of the developments given in Section 8.4. To simplify the treatment given here, we will begin with the isotropic case and then move to the generalized case of the anisotropic solids. In fact, it will be instructive to switch back and forth between the isotropic and anisotropic nomenclature as needed.

9.1

SEEBECK EFFECT (THERMOCOUPLE EFFECT)

The Seebeck effect is defined as the production of an open-circuit voltage or thermoelectric electromotive force between two dissimilar conductors held at different temperatures under conditions of J n = 0. This is, of course, the means by which one can measure a temperature difference by means of a calibrated thermocouple. The physical picture of the thermocouple is illustrated in Figure 9.1 where an ideal capacitor is placed in a circuit that consists of the two dissimilar conducting wires A and B attached to large heat reservoirs held at high and low temperatures designated as TH and TL. The presence of the ideal capacitor ensures that J n = 0. The potential difference ∆φ is the thermoelectric voltage difference between high and low potential measured across the capacitor held at the reference temperature T0. High potential is taken as being more positive than low potential. From Eq. (8.32), with subscripts removed and with ∇µc = 0, we have

∇ µ = e ∇φ =

L12 TL11

∇ T .

(9.1)

In a continuous conducting media, the absolute thermoelectric power ∑ is defined generally as the electrostatic potential gradient per unit temperature gradient when J n = 0. However, in the case of

160 tensor properties of solids A

TL (3)

T0

B

(4)

(2)

B

TH

(1)

∆φ = φ 1 – φ 4

FIGURE 9.1: Thermocouple setup showing two dissimilar metals A and B joined at junctions that are maintained at different temperature TH and TL. Figure 9.1, there can be no temperature gradient across the open circuit of the ideal capacitor. Thus, the absolute thermoelectric power ∑ must be defined as the change in electrostatic voltage potential per unit change in temperature relative to the heat reservoirs. Thus, by using Eqs. (9.1) and (8.31), we have

∑≡

∇φ ∇T

12

=

L

11

eTL

12

=

eL 2

T σ

in units of (V/°K)

(9.2)

in terms of L12 and σ. Solving for L12 then gives the result L12 =

T 2σ ∑. e

(9.3)

From Figure 9.1, because there is no temperature gradient across the capacitor held at temperature T 0, we can sum the electrostatic potential differences as

∆φ = φ 1 − φ4 = (φ1 − φ2 ) + (φ2 − φ3 ) + (φ3 − φ4 ) =

∫

=

∫

T0

TH TH TL

∑ B dT +

∫

TH

TL

∑ A dT +

∫

TL

T0

∑ B dT

(∑ A − ∑ B ) dT .

Therefore, the resulting absolute thermoelectric power for the thermocouple becomes

∑AB =

L12 = A 11 ∆T eTLA

∆φAB

L12 − B 11 eTLB

=∑ −∑ A B

(9.4)

In tensor notation, we write Eq. (9.2) applied to an anisotropic medium as since Lij12 ≠ Lji12.

( Li11j )−1 ∇i φ L12 ij ∑ij = = ≠∑ ji ∇j T eT

(9.5)

Thermoelectric, Piezothermoelectric, and diffusive effects 161

By introducing Eq. (9.3) into Eqs. (8.38) and (8.39), we can cast these thermoelectric equations into forms containing physically measurable quantities (σ, k, and ∑) as they apply to a thermoelectric junction composed of two different isotropic conductors. When this is done, the results are, excluding subscripts,

(

Tσ µ T 2σ ∑ 1 ∇ + e ∇ T 2 T e

(

(9.6)

T2σ ∑ µ ∇ + T 2 k + T σ ∑2 ∇ 1 . e T T

(

Jq =

(

− Jn =

µ between Eqs. (9.6) and (9.7), there results T e2 J n eΣ ∇ µ = − + ∇T . T Tσ T

(9.7)

Then, by eliminating ∇

(9.8)

Finally, by introducing Eq. (9.8) into Eq. (9.7) with ∇(1/T ) = −∇T /T 2 and with a little algebra, Eq. (9.7) can be written in the useful alternative form J q = –eT ∑ J n − k∇T = TJ s

(9.9)

which provides another definition for the thermoelectric power given by

∑≡−

1 Jq

Js = , eT J n ∇T = 0 J e ∇T = 0

(9.10)

where J n = −J e /e and J q = T J s.

TABLE 9.1: Effect of crystal symmetry on ∑ij for the tetragonal, trigonal, and hexagonal systems, all others being the same as in Table 3.7 except that ∑ij ≠ ∑ji Classes

Classes

− − 4, 4 , || 4/m ||, 3, || 3 || − 6, 6 , || 6/m ||

− − 4mm, 4 2m, 422, || 4/mmm ||, 3m, 32, || 3 m || || − 6 m2 ||, 6mm, 622, || 6 /mmm ||

∑11 −∑ 12 0

∑12 ∑11 0

0

0 ∑ 33

∑11 0 0

0

∑11 0

0

∑ 33 0

162 tensor properties of solids

To apply Eqs. (9.6) and (9.7) to an anisotropic solid, one need only reinstall the subscripts and take into account the affect of crystal symmetry on the property tensors—all of which are second-rank tensors but only ∑ij is nonsymmetrical. The effect of crystal symmetry on the ∑ij components follows Table 3.7 for Sij with the following changes: 1) crystal systems are the same as Sij except that ∑ij ≠ ∑ji and 2) the uniaxial group of tetragonal, trigonal, and hexagonal systems is given as in Table 9.1.

9.2

PELTIER EFFECT (THERMOELECTRIC HEATER/REFRIGERATOR EFFECT)

The Peltier effect is defined as the evolution or absorption of heat accompanying the flow of electric current across an isothermal junction between two dissimilar conductors or semiconductors. That is, when J n flows across a junction, heat must be removed or added continuously to maintain the junction at constant temperature, T. This is illustrated in Figure 9.2. Because ∇T = 0 at the junction (the junction is at constant T ), Eq. (9.9) applies as J q = –eT ∑ J n = TJ s .

(9.11)

J Aq − J Bq = –eT ( ∑A − ∑B ) J n = –eT ∑AB J n ,

(9.12)

Then the difference in heat flow is

where ∑AB is the thermoelectric power of the AB junction. Heat evolved Constant T junction

A

(J

(J q)A > (J q)B

Jn B (J q)B

q) A

(J q)A < (J q)B Heat absorbed

FIGURE 9.2: Schematic illustrating the Peltier effect.

Thermoelectric, Piezothermoelectric, and diffusive effects 163

By definition, the Peltier coefficient ∏ is the heat that must be removed from the isothermal junction AB per unit electric current flux from conductor A to conductor B as depicted in Figure 9.2. This is expressed by J Bq − JAq = T ∑AB , ΠAB ≡ (9.13) n eJ ∇T = 0

giving the relationship between the Peltier and Seebeck (thermoelectric power) coefficients. Equation (9.13) is known as the first Kelvin relation. Thus, if ( J Aq − J B q ) > 0, heat must be issued from the isothermal junction AB to the surroundings (thermoelectric heating). Or if ( J Aq − J B q ) < 0, heat must be supplied to (absorbed by) the isothermal junction from the surroundings (thermoelectric cooling) as illustrated in Figure 9.2. In tensor notation, applicable to anisotropic crystals, the Peltier and Seebeck coefficients are related according to ∏ij = T ∑ij ≠ ∏ji since ∑ij ≠ ∑ji ,

(9.14)

where the effect of crystal symmetry for ∏ij is the same as that for ∑ij given in Table 9.1. It should be noted that the developments presented by Eqs. (9.11), (9.12), and (9.13) apply to homogeneous isotropic conducting materials.

9.3

THOMSON EFFECT

Consider a homogeneous conducting rod of uniform cross section that has established a steadystate heat flow J q in the absence of an electric current. Assume that the surroundings are heat reservoirs having the same temperature distribution as the rod. Now, if an electric current J n is allowed to flow through this material, heat must be emitted to or absorbed from the surroundings

φ + ∆φ

Thomson Heat Heat Reservoir

T+∆T

∇φ ∇T

Jn Jq

Jn' J q' ∆x

Heat Reservoir Thomson Heat

FIGURE 9.3: Schematic illustrating the Thomson effect in a homogenous rod element ∆x of a constant cross section carrying heat and electric currents and surrounded by heat reservoirs.

164 tensor properties of solids

to maintain the steady temperature distribution. This is what is called the Thomson effect (after Sir William Thomson, who later became Lord Kelvin), and the heat that is exchanged in this process is called the Thomson heat as depicted by the closed system in Figure 9.3. Whether the Thomson heat is emitted to or absorbed from the surroundings depends on the direction and magnitude of the electric current relative to the heat flow. We now establish an energy flow balance given by fluxes Jiu = Jiq + µ− Jin ,

(9.15)

− is the total energy carried per particle. Thus, as where Jiu is the total energy flow along the rod and µ the electric current flows through the conducting rod, any change in the total energy flow must be supplied by a Thomson heat interchange with the surroundings. Introducing Eq. (9.9) into (9.15) yields

Jiu = –eT ∑ji Jjn − kij∇jT + µ− Jin = (eT ∑ji + δji µ− ) Jjn − kij∇jT ,

(9.16)

where the substitution property of the Kronecker delta δji has been used (see Section 2.6.3). The rate at which energy is interchanged between the rod element and the surroundings in Figure 9.3 is the divergence (Section 2.6.2) of Eq. (9.16) represented by

∇i Jiu = –eT ∇i ( Jjn ∑ji ) – (e ∑ji ∇iT – δji∇i µ− ) Jjn − ∇i (kij∇jT ).

(9.17)

But from Eq. (9.8)

µ ∇j µ = T ∇j

= − e 2J nσ −1+ e ∑ ∇ T ji i i ji T

(9.18)

or

−1

e 2σji Jin = (e ∑ji∇iT − δji ∇i µ )

(9.19)

because δji∇i µ− = ∇j µ−. Introducing Eq. (9.19) into Eq. (9.17) yields

∇i Jiu = − eT ∇i ( Jjn ∑ji ) − e 2 ρji Jin Jj n − ∇i ( kij ∇j T ) , Thermoelectric heat

Joule heat

(9.20)

Conduction

where σij−1 = ρij and e 2ρji Jin Jjn is the Joule (I 2R) heat that is generated by current flow through a conductor even in the absence of a temperature gradient. But for the steady-state conditions, J n = 0 and ∇ . J n = 0, it follows that ∇ . J u must vanish. If we set ∇ . J n = 0 and ∇ . J u = 0, we have

{∇i ( k i ∇ T )} j

j

∇ ⋅J n = 0 ∇ ⋅J u = 0

= 0 ,

Thermoelectric, Piezothermoelectric, and diffusive effects 165

which gives the result

∇i Jiu = − eT ∇i ( Jjn Σj ) − e 2 ρji Jin Jjn . i Thermoelectric heat

(9.21)

Joule heat

We now note that the thermoelectric power ∑ji is a function of the local temperature represented as ∇i ∑ji / ∇iT = ∂ ∑ji / ∂T, which allows

∂ Σji ∇i Σj = i ∂T

∇i T .

(9.22)

Introducing Eq. (9.22) into Eq. (9.21) yields ∇i Jiu = − T

∂ Σji ∂T

∇i T e Jjn − e 2 ρji Jin Jjn Joule heat

T homson heat

= − τ ji ∇i T e Jjn − e 2 ρji Jin Jjn T homson heat

(9.23)

Joule heat

Here,

τ ji = T

∂ Σji ∂T

≠ τ ij

(9.24)

is the Thomson heat coefficient, which is seen to be an asymmetrical second-rank tensor where the effect of crystal symmetry follows that for ∑ji ≠ ∑ij in Table 9.1. Equation (9.24) is known as the second Kelvin relation. Thus, the Thomson heat is the heat evolved or absorbed per unit volume per unit time depending on the direction and magnitude of the current Jin relative to the Joule heat it produces. The Thomson coefficient is usually (but not always) defined as positive if heat must be added to (absorbed by) the element in Figure 9.3 so as to maintain the steady-state temperature distribution in the element. Notice that the Thomson heat (proportional to J n) changes sign when the current density is reversed but that the Joule heat does not because it is proportional to the square of the current density. The foregoing results apply generally to an anisotropic conducting material. However, they can be applied to homogeneous isotropic conductors or semiconductors by dropping subscripts except for a suffix indicating a specific direction along which the heat effects are generated. When this is done, for example, Eq. (9.23) becomes

∇ J u = − τ ∇ T e J n − e 2 ρ ( J n )2 . T homson heat

Joule heat

(9.25)

166 tensor properties of solids

This single direction would apply to one-dimensional flow in the longitudinal direction of the conducting rod (e.g., the x direction). In the isotropic case, the Thomson coefficient is given by the known isotropic value for τ when substituted for the S cubic (diagonal) values presented in Table 3.7.

9.4

PIEZOTHERMOELECTRIC AND ELASTOTHERMOELECTRIC EFFECTS

From what we have learned so far in this chapter, the thermoelectric power tensor ∑ij is fundamental to a general description of the three thermoelectric effects discussed in Sections 9.1, 9.2, and 9.3. However, in practical experimental situations, both temperature and stress variation of the thermoelectric power may be involved. Assuming that ∑ij is everywhere, a continuous function of temperature and stress and that its derivatives with respect to temperature T and stress σkl are real, we may expand ∑ij in a Taylor’s series about the state of reference temperature T0 and zero applied stress (neglecting gravitational forces and body torques). When this is done, we have 1

n

∑ij (T , σ kl ) = ∑ (T − T0 ) + σ kl ∑ j (T0 , 0 ) n = 0 n! ∂T ∂ σ kl i ∂ Σij ∂ Σij = ∑ij (T0 , 0 ) + ( T − T ) + 0 ∂σ T ∂ ( T0 , 0 ) kl ∞

+

2 1 ∂ Σij

2! ∂ T 2

∂

∂

∂ 2 Σij ( T − T 0) + 2 ∂ T∂ σ kl ( T0 , 0 )

∂ 2 Σij + ∂σ ∂σ op kl

2

σ kl σ op ( T0 , 0 )

(T

σ kl 0

, 0)

( T − T 0 )σ kl ( T0 , 0 )

+…,

(9.26)

where ∑ij (T0, 0) and all coefficients (in parentheses) are evaluated at temperature T0 and zero stress. Assuming that all measurements are to be conducted at a reference temperature of T = T0 and that all second- and higher-order terms in stress can be neglected, Eq. (9.26) becomes

∂Σ ∆∑ij = ∑ij (T0 , σ kl ) − ∑ij (T0 , 0 ) = ij ∂ σ kl

(T

σ kl = ∏ijkl σ kl , 0

, 0)

(9.27)

Thermoelectric, Piezothermoelectric, and diffusive effects 167

where ∏ijkl is a fourth-rank polar tensor called the piezothermoelectric power tensor, not to be confused with the Peltier coefficient ∏. Because σkl is symmetrical but ∆∑ij is not, then ∏ijkl = ∏ijlk or ∆∑i = ∏ij σj (i = 1 − 9; j = 1 − 6)

(9.28)

in matrix subscript notation. Thus ∏ij in Eq. (9.28) is completely specified by 54 independent coefficients for the triclinic crystal system given by

∆Σ1 ∆Σ 2 ∆Σ3 ∆Σ4 ∆Σ = 5 ∆Σ 6 ∆Σ 7 ∆Σ 8 ∆Σ 9

∏11 ∏ 21 ∏31 ∏ 41 ∏ 51 ∏61 ∏ 71 ∏81 ∏ 91

∏12

∏13

∏14

∏15

∏16

∏ 22

∏ 23

∏24

∏ 25

∏26

∏ 32

∏33

∏34

∏35

∏36

∏ 42

∏ 43

∏44

∏ 45

∏ 46

∏ 52

∏53

∏54

∏ 55

∏56

∏ 62

∏ 63

∏64

∏ 65

∏66

∏ 72

∏ 73

∏74

∏ 75

∏76

∏82

∏83

∏84

∏85

∏86

∏ 92

∏93

∏94

∏95

∏96

σ 1 σ 2 σ 3 σ 4 σ 5 σ 6

(9.29)

The transformation law for the piezothermoelectric power tensor ∏ is easily determined from the transformation laws for stress and thermoelectric power. These transformation laws are σ ′ = ασ or σ = α−1σ ′, as given in Section 6.1.1, and ∑ is ∑′ = β∑, where α is the quadratic transformation form for symmetrical second-rank polar tensors and β is the general quadratic transformation form for asymmetrical second-rank polar tensors. If ∑′ = ∏′σ ′ relative to coordinate axes 0x′ and ∑ = ∏σ relative to axes 0x, then it follows that ∑′ = β∑ = β∏σ = β∏α −1σ ′ = ∏′σ ′

or

∏′ = β∏α −1

(9.30)

↔

in matrix symbolic notation. The quadratic transformation form β is given by Eq. (9.31), where it is divided into nine 3 × 3 submatrices (numbered in parentheses), 4 of which are replicated as indicated by the symbols ↔ and . Eq. (9.31) can be deduced from that of α given by Eq. (2.22).

168 tensor properties of solids (1) 2 a 212 a 213 a 11 a2 a 222 a 223 21 a 232 a 233 a 231 (4) a21 a31 a22 a32 a23 a33 β = a a 31 11 a32 a12 a33 a13 a11 a21 a12 a22 a13 a23 (7) (4) b (7)

(2)

a13 a11

a11 a12

a12 a23

a23 a21

a21 a 22

a32 a33

a33 a31

a31 a 32

a22 a33

a21 a33

a21 a32

a23 a32

a12 a33

a11 a33

a11 a32

a13 a32

a12 a23

a11 a23

a11 a22

a13 a22

(5)

(8)

(2) ↔ (3) (6) a23 a31 a22 a31 a13 a31 a12 a31 a13 a21 a12 a21 (9) (5) ↔ (9) (3)

a12 a13

(6) ↔ (8)

(9.31)

The variation in thermoelectric power with strain can also be established. For this purpose, Eq. (9.27) is altered to give

∂ Σij ∂εmn ∆Σij = ∂ εmn ∂ σkl

σkl = Εijmn smnkl σkl

(9.32)

or

∆Σi = Εik skj σj = Εik εk

(9.33)

in matrix subscript notation. Here Eik = (∂∑i /∂εk ) is a polar fourth-rank tensor called the elastothermoelectric power tensor and skj is the elastic compliance tensor given by Eq. (4.47). By comparing Eqs. (9.28) and (9.33), the piezothermoelectric and elastothermoelectric power coefficients can be related by reciprocity

∏ ij = Eikskj

(9.34)

Eij = ∏ ik ckj ,

(9.35)

or its inverse

where ckj is the elastic stiffness modulus given by c = s−1 as deduced from Eq. (6.36a) and thermodynamic symmetry discussed in Section 4.4. The transformation law for the elastothermoelectric power tensor E is easily found from the ~ −1ε or ε = α ~ ε ′ transformation laws for strain and thermoelectric power. Strain transforms as ε ′ = α (see Section 6.1.2) and ∑ transforms as ∑′ = β∑. Because from Eq. (9.33) ∑ = Esσ = Eε relative to coordinate axes 0xi and ∑′ = E′ε′ relative to axes 0xi′, it follows that

~ ε ′ = E′ε′ ∑′ = β ∑ = β Eε = β Eα

Thermoelectric, Piezothermoelectric, and diffusive effects 169

or

~ E′ = β Eα

(9.36)

all in matrix notation. A complete description of the first-order piezothermoelectric and elastothermoelectric properties must necessarily include the piezo- and elasto-Seebeck, Peltier, and Thomson effects. From Eq. (9.24) in contracted subscript form and using Eqs. (9.28) and (9.34), there results

τi = T

∂ Σi ∂T

∂ ∏ij ∂Ε s σj = T ik kj ∂T ∂T

= T

σj ,

(9.37)

giving the Thomson effect in terms of the piezothermoelectric and elastothermoelectric coefficients. Here, it has been assumed that all thermal stresses are absent and that the tensor character and aelotropism of ∏ and E are the same. The anisotropy of the piezothermoelectric and elastothermoelectric coefficients ∏ and E is determined by the standard methods emphasized in this text. Consider the ∏ array in Eq. (9.29), which applies to the triclinic crystal system. The anisotropy of all crystal systems, other than the trigonal and hexagonal, can be determined by the method of direct inspection as was done for the piezoelectric moduli in Section 6.1.3. For the trigonal and hexagonal crystal systems, the “bruteforce” method described in Section 6.1.4 must be used. Remember that the generalized quadratic transformation form β must be used together with α in Eqs. (9.30) and (9.36) when applying the brute-force method. For the coefficient arrays of ∏ and E, see Tinder in Endnotes, Section VII.

9.5

PIEZORESISTANCE EFFECT (STRAIN GAUGE EFFECT)

The application of a mechanical stress can significantly change the electrical resistivity of a given conducting medium. The calibrated sensitivity of piezoresistive elements made from metal or semiconductor thin wires are used as gauges to measure the surface strains resulting from a stressed solid member to which the strain gauges are firmly attached. The strain gauges can be aligned with specific crystallographic axes for meaningful measurements. Such measurements are usually in the form of a fractional change in the resistance associated with elongation or contraction of the piezoresistive elements. For cubic crystals, the piezoresistive sensitivity is similar to that discussed for Young’s modulus in Section 6.2.7. To determine the tensor nature of the piezoresistance effect, we can expand the resistivity tensor ρij in a Taylor’s series about the state of reference temperature T0 and zero applied stress (neglecting gravitational forces and body torques) much the same as in the previous section for the

170 tensor properties of solids

piezothermoelectric effect. Here again, we assume that ρij is everywhere a continuous function of temperature and stress and that its derivatives with respect to temperature T and stress σkl are real. The resulting expansion is ∞

ρij (T , σkl ) = ∑

n=0

1

∂

n!

∂T

( T − T0 )

∂ ρij = ρij (T0 , 0 ) + ∂T +

2! ∂T 2

+

∂ 2 ρij

∂σ ∂σ kl op

ρij (T0 , 0 )

+ σkl

∂ σkl

∂ ρij ( T − T ) + 0 ∂σ ( T0 , 0 ) kl

2 1 ∂ ρij

n

∂

∂ 2 ρij (T − T0 ) + 2 ∂ T∂ σ kl ( T0 , 0 ) 2

σkl σop ( T0 , 0 )

σkl ( T0 , 0 )

(T − T0 ) σkl ( T0 , 0 )

+ L,

(9.38)

where ρij (T0, 0) and all tensor coefficients (in parentheses) are evaluated at temperature T0 and zero stress. Notice that the second-order effects, ∂ 2ρij / ∂ T∂σkl and ∂ 2ρij / ∂σkl ∂σop, represent the piezothermoresistive and quadratic piezoresistive effects, respectively. There will be no further discussion of the second-order effects, the remainder of which are self-explanatory. Assuming that all measurements are to be conducted at a reference temperature of T = T0 and that all second- and higher-order terms in stress can be neglected, Eq. (9.38) becomes

∂ ρij ∆ ρij = ρij (T0 , σ kl ) − ρij (T0 , 0 ) = ∂ σkl

σkl = Ρijkl σkl , ( T0 , 0 )

(9.39)

where Pijkl is a fourth-rank polar tensor called the piezoresistance tensor. Because both ρij and σkl are symmetrical second-rank tensors, we can write

∆ρi = Pijσj (i = 1 − 6; j = 1 − 6),

(9.40)

where it is understood that Pij ≠ Pji . Thus, the piezoresistance tensor transforms the same as the linear piezo-optical coefficients given by Eq. (7.51) and is affected by crystal symmetry the same as presented in Table 7.1.

Thermoelectric, Piezothermoelectric, and diffusive effects 171

9.6

ELECTRODIFFUSIVE AND THERMODIFFUSIVE EFFECTS

There are two other two-flow processes that derive from Eqs. (8.20) and that are worthwhile mentioning, the electrodiffusive and thermodiffusive effects. These are represented as follows.

µ T

− J n = L11∇

13 µc + L ∇ T

µ µ − J = L ∇ + L33 ∇ c T T m

Electrodiffusive effects

31

1 23 µ c + L ∇ T T

(9.41)

J q = L22 ∇

µ 1 − J = L32 ∇ + L33 ∇ c T T

Thermodiffusive effects

m

(9.42)

The reader has already been introduced to the phenomenological developments of the thermoelectric effects in some detail including the application of Onsager’s reciprocity principle as applied to the phenomenological coefficients given in Eqs. (8.20). The interaction effects in Eqs.(8.20) can be complex considering that charged matter (electrons, holes, ions) can carry charge, heat, and mass at the same time and that different species can influence other species. Although it is not our intention to explore the electrodiffusive and thermodiffusive effects in detail, a short discussion of the diffusive effects is necessary when dealing with the coupled effects in Eqs. (9.41) and (9.42).

9.6.1 Multiple Diffusing Species In dealing with diffusion of matter, one must understand that several species could be diffusing simultaneous and that the different species may not all be independent. Thus, the flow of one species may influence the flow of another. The entropy density production associated only with the simultaneous diffusion of several species in the absence of an electrostatic field potential gradient (∇φ = 0) and temperature gradient is from Eq. (8.19)

s& = − ∑ Jim ∇ i

µi

,

T

(9.43)

where Jim is the mass flux of the ith species and µi is the chemical potential for the i th species. From this we can generalize Fick’s law in the modified form of Eq. (8.8) and under isothermal conditions as the sum of diffusing species given by

Jim = − ∑ j

Lij T

∇ Nj = − ∑ Dij ∇ Nj ( x ). j

(9.44)

172 tensor properties of solids

Here, Nj (x) is the concentration (mole number) of the j th component at any position in Cartesian space of the medium in which the diffusion is occurring. The problem now remains to relate the phenomenological coefficient L ij with the physically measurable diffusion constant D ij . This requires the use of Gibbs–Duhem relation, Eq. (4.4) under constant temperature, electric, magnetic, and stress fields together with the use of chemical thermodynamics as applied to the condensed state. For example, at constant T, E, B, and σ, the Gibbs–Duhem relation for a non-independent, two-species system and for arbitrary dx, is expressed as N1 d µ1 + N2 d µ2 = N1∇µ1 + N2∇µ2 = 0,

(9.45)

where N1 is the mole number concentration of the (dilute) diffusing species and N2 >> N1 is the mole number concentration of the host medium. Because diffusion flows do not produce a volume change, it follows that →

→

J 1v1 + J 2v2 = 0,

(9.46)

where vi is the partial molar volume of the species i. Now, by introducing Eqs. (9.45) and (9.46) into (9.43), the isothermal entropy density production for the two-component system becomes

r ∇µ r ∇µ r N r ∇µ1 N v r ∇µ 1 1 2 (9.47) s& = − J1 ⋅ − J2 ⋅ = − J1 − 1 J2 ⋅ = − 1 + 1 1 J1 ⋅ T T N2 T N2 v 2 T

in vector notation. With the information in Eq. (9.47), Eqs. (9.44) and (9.45) combine to give the linear force flux equation for the diffusing species as

r N v J1 = − L11 1 + 1 1 N2 v2

µ1 ∇ = − D11 ∇ N1 . T

(9.48)

But ∇µ1/∇N1 = (∂µ1 / ∂N1), which allows

r N v 1 J1 = − L11 1 + 1 1 T N2 v2

resulting in L11 =

∂ µ1 ∂ N1

D11T

v N 1 + 1 1 v2 N2

∂ µ1 ∂N1

since v1N1

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close